# cif

formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4401
b: 11.4401
c: 11.4401
alpha: 90
beta: 90
gamma: 90
cell_volume: 1497.233
crystal_density: 3.577
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: sLsHAAAAAABg4xYA8P39/w==
atoms_y: wF0AAAAAAAAAAAAAyBYDAA==
atoms_z: AFUPAAAAAABAQg8AyFsJAA==
atoms_occupancy: QEIPAAAJPQAACT0AAAk9AA==
atoms_u_iso: QDgAAKAtAAAoKAAA2DsAAA==
atoms_aniso_label: ["Al", "Si", "O"]
atoms_aniso_u11: +A6yAKA7jQDwYd8A
atoms_aniso_u22: +A6yADi0pACg2QcB
atoms_aniso_u33: +A6yADi0pABQ4tYA
atoms_aniso_u12: YJ4BAAAAAADw3OL/
atoms_aniso_u13: YJ4BAAAAAABo5SoA
atoms_aniso_u23: YJ4BAAAAAADIVAsA
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 96.7 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAABAAAAAAAAQACAAAAgAgBACAAAQBAAAAIBAIAAgICAgIEAAAgQIEECBABBAAhBBACCCEEIIAgCEIIQCEAAhEIhCARCAgAIiIBABEAAREBEAIAAEAAABAAAAAAAAASAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4425
b: 11.4425
c: 11.4425
alpha: 90
beta: 90
gamma: 90
cell_volume: 1498.176
crystal_density: 3.575
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAUP39/w==
atoms_y: AAAAAAAAAAAAAAAAgBMDAA==
atoms_z: QEIPAAAAAABAQg8AaFwJAA==
atoms_occupancy: 0
atoms_u_iso: YFQAAJgrAAC4KQAAoDwAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 122.3 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQACAAAAgAgBACAAAQBAAAAIBAIAAgICAgIEAAAgQIEECCABBABBBBACCCEEIQAgCEIIQCEAAiEIhCAREAgARCICABEAAREBEAIAAEAAABAAAAAAAAASAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4450
b: 11.4450
c: 11.4450
alpha: 90
beta: 90
gamma: 90
cell_volume: 1499.158
crystal_density: 3.572
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAsPz9/w==
atoms_y: AAAAAAAAAAAAAAAAiBUDAA==
atoms_z: QEIPAAAAAABAQg8AcF4JAA==
atoms_occupancy: 0
atoms_u_iso: cGcAAPgvAADILQAA8EEAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 173.7 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQACAAAAgBABACAAAQBAAAAIBAIAAgICAgIEAAAgQIEECCABBABBBBACCEEIIQAgCEIIgCEAAiEIhEAhEAgARCICABEAAREBEAIAAEAAABAAAAAAAAAiAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4508
b: 11.4508
c: 11.4508
alpha: 90
beta: 90
gamma: 90
cell_volume: 1501.438
crystal_density: 3.567
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYA6Pv9/w==
atoms_y: AAAAAAAAAAAAAAAACBMDAA==
atoms_z: QEIPAAAAAABAQg8ACF0JAA==
atoms_occupancy: 0
atoms_u_iso: aHkAAAA3AACIMQAAwEkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 223.3 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQACAAABABABACAAAQCAAAAIBAIAAgICAgQEAAAgQIIECCABBABBBBACEEEIIQBACEIQgCEABCEQhEAhEAgAREICACIAAiICIAQAAIAAACAAAAAAAAAkAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4548
b: 11.4548
c: 11.4548
alpha: 90
beta: 90
gamma: 90
cell_volume: 1503.012
crystal_density: 3.563
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAKP39/w==
atoms_y: AAAAAAAAAAAAAAAAIBQDAA==
atoms_z: QEIPAAAAAABAQg8A4FwJAA==
atoms_occupancy: 0
atoms_u_iso: yIwAAFg+AAAgOgAAYFQAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 273.6 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABABACAAAgCAAAAIBAQAAgICAgQEAAAgQIIECCACBABBCCACEEIIQQBACEIQgCEABCEQiEAiEBAAhEQEACIAAiICIAQAAIAAACAAAAAAAABEAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4572
b: 11.4572
c: 11.4572
alpha: 90
beta: 90
gamma: 90
cell_volume: 1503.957
crystal_density: 3.561
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAEPz9/w==
atoms_y: AAAAAAAAAAAAAAAAYBADAA==
atoms_z: QEIPAAAAAABAQg8AQFwJAA==
atoms_occupancy: 0
atoms_u_iso: eJYAABBAAABgOwAAOFkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 295 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABABACAAAgCAAAAIBAQAAgICAgQEAAAgQIIEECACBABBCCACEEIIQgBACEIQgCIABEIQiIBCIBAAhEQEACIAAiIEQAQAAIAAACAAAAAAAABEAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4592
b: 11.4592
c: 11.4592
alpha: 90
beta: 90
gamma: 90
cell_volume: 1504.745
crystal_density: 3.559
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAOPz9/w==
atoms_y: AAAAAAAAAAAAAAAAmA8DAA==
atoms_z: QEIPAAAAAABAQg8AgF0JAA==
atoms_occupancy: 0
atoms_u_iso: aKEAADhFAACwQAAAyF8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 322.8 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABABAEAAAgCAAAAIBAQAAgICBAQIAAAgQQIEEEACCACBCCACEEIIQgBACEIRACIABEIQiIBCIBAAhEQEACIAAiIEQAQAAQAAAEAAAAAAAABEAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4641
b: 11.4641
c: 11.4641
alpha: 90
beta: 90
gamma: 90
cell_volume: 1506.676
crystal_density: 3.554
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYA6Pv9/w==
atoms_y: AAAAAAAAAAAAAAAA0A4DAA==
atoms_z: QEIPAAAAAABAQg8AmF4JAA==
atoms_occupancy: 0
atoms_u_iso: MLYAAKBLAACwRQAAAGkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 373.5 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABABAEAAAgCAAAAIBAQAAgIEBAQIAAAggQIEEEACCACCCCAEEEIIQgBAEIQhAEIACEIhCIBCIBAAiEgEAEQABEQEQAQAAQAAAEAAAAAAAABEAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4690
b: 11.4690
c: 11.4690
alpha: 90
beta: 90
gamma: 90
cell_volume: 1508.609
crystal_density: 3.550
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYA+Pr9/w==
atoms_y: AAAAAAAAAAAAAAAAEBADAA==
atoms_z: QEIPAAAAAABAQg8AGGEJAA==
atoms_occupancy: 0
atoms_u_iso: CMoAAGhWAACITwAAGHQAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 423.3 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABACAEAAAgCAAAAICAQABAQEBAQIAABAgQIIEEACCACCCCAEEIIQQgBAEIQhAEIACEIhEIBEIBAAiIgEAEQABEQEQAgAAQAAAIAAAAAAAABIAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4730
b: 11.4730
c: 11.4730
alpha: 90
beta: 90
gamma: 90
cell_volume: 1510.188
crystal_density: 3.546
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYA+Pr9/w==
atoms_y: AAAAAAAAAAAAAAAAGA0DAA==
atoms_z: QEIPAAAAAABAQg8AYF8JAA==
atoms_occupancy: 0
atoms_u_iso: 6N8AAFhcAAAAVQAAgH8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 472.6 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABACAEAAAgCAAAAQCAQABAQEBAgIAABAgQIIEEACCACCCCAEEIIQQgCAEIQhAEIACEQhEIBEICABEIgIAEQABEQEQAgAAQAAAIAAAAAAAABIAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4801
b: 11.4801
c: 11.4801
alpha: 90
beta: 90
gamma: 90
cell_volume: 1512.993
crystal_density: 3.540
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAWPr9/w==
atoms_y: AAAAAAAAAAAAAAAAOAsDAA==
atoms_z: QEIPAAAAAABAQg8AqF0JAA==
atoms_occupancy: 0
atoms_u_iso: mO4AAHBiAADAWAAAoIcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 523.0 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABACAEAAAgCAAAAQCAQABAQEBAgQAABAgQQIIEAEEACEEEAIIIQQggCAIQQhAIQACIQiEQCEQCABEQgIAIgACIgIgAgAAQAAAIAAAAAAAACQAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4848
b: 11.4848
c: 11.4848
alpha: 90
beta: 90
gamma: 90
cell_volume: 1514.852
crystal_density: 3.535
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAuPn9/w==
atoms_y: AAAAAAAAAAAAAAAAcAoDAA==
atoms_z: QEIPAAAAAABAQg8AiF8JAA==
atoms_occupancy: 0
atoms_u_iso: 4AABADhoAADwXwAAsJAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 572.9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABABACAEAAAgCAAAAQCAgABAQEBAgQAABBAQQIIEAEEACEEEAIIQQghACAIQhCAIQAEIRCEQCEQEABERAQAIgACIgIgBAAAgAAAIAAAAAAAAEQAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4893
b: 11.4893
c: 11.4893
alpha: 90
beta: 90
gamma: 90
cell_volume: 1516.634
crystal_density: 3.531
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAuPn9/w==
atoms_y: AAAAAAAAAAAAAAAA8AcDAA==
atoms_z: QEIPAAAAAABAQg8A2F8JAA==
atoms_occupancy: 0
atoms_u_iso: GBQBACBxAADgZQAA8JsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 622.9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAQAEAAABACACAEAAAgEAAAAQCAgABAQECAgQAACBAgQQIIAEEAEEEEAIIQQghAEAIQhCAIQAEIRCIQCIQEACERAQAIgACIgJABAAAgAAAIAAAAAAAAEgAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.4960
b: 11.4960
c: 11.4960
alpha: 90
beta: 90
gamma: 90
cell_volume: 1519.289
crystal_density: 3.525
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAMPr9/w==
atoms_y: AAAAAAAAAAAAAAAAQAgDAA==
atoms_z: QEIPAAAAAABAQg8AYF8JAA==
atoms_occupancy: 0
atoms_u_iso: kCgBAMh4AACoawAAgKcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 672.9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAgAEAAACACACAEAABAEAAAAQCAgABAQECAgQAACBAgQQIIAEEAEEEIAIIQghBAEAIQhCAIgAEQhEIQCIgEACISAQARAACRARACAABAAAAQAAAAAAAAIgAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5023
b: 11.5023
c: 11.5023
alpha: 90
beta: 90
gamma: 90
cell_volume: 1521.788
crystal_density: 3.519
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAyPj9/w==
atoms_y: AAAAAAAAAAAAAAAASAUDAA==
atoms_z: QEIPAAAAAABAQg8AiF8JAA==
atoms_occupancy: 0
atoms_u_iso: kEEBAOiAAADYcgAAKLQAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 723.0 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAAgAEAAACACACAEAABAEAAAAQCAgABAQICAgQAACBAggQIIAIEAEEIIAIQQghCAEAQhCCAQgAIQiEQgEQgEACIiAQARAAERARACAABAAAAgAAAAAAAAJAAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5078
b: 11.5078
c: 11.5078
alpha: 90
beta: 90
gamma: 90
cell_volume: 1523.972
crystal_density: 3.514
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAGPn9/w==
atoms_y: AAAAAAAAAAAAAAAA+AQDAA==
atoms_z: QEIPAAAAAABAQg8AeGAJAA==
atoms_occupancy: 0
atoms_u_iso: UFQBAFiJAADoewAAeL4AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 773.1 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAAgAIAAACACACAIAABAEAAAAQEAgACAgICBAQAACBAggQQIAIIAIIIIAQQQghCAEAQhCEAQgAIRCEQgEQgIAEIiAgAhAAERAiACAACAAAAgAAAAAAAAJAAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5136
b: 11.5136
c: 11.5136
alpha: 90
beta: 90
gamma: 90
cell_volume: 1526.277
crystal_density: 3.509
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAsPf9/w==
atoms_y: AAAAAAAAAAAAAAAAyP0CAA==
atoms_z: QEIPAAAAAABAQg8AMGIJAA==
atoms_occupancy: 0
atoms_u_iso: IGYBAKCRAACgfQAA8MgAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 823.1 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAAgAIAAACACAEAIAABAEAAAAgEAgACAgICBAgAACBBAgQQIAIIAIIIIAQQghBCAIAQhCEAggAIhCIRAIRAIAERCAgAiAAIiAiAEAACAAABAAAAAAAAAJAAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5195
b: 11.5195
c: 11.5195
alpha: 90
beta: 90
gamma: 90
cell_volume: 1528.625
crystal_density: 3.503
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAePj9/w==
atoms_y: AAAAAAAAAAAAAAAA8AIDAA==
atoms_z: QEIPAAAAAABAQg8A2F8JAA==
atoms_occupancy: 0
atoms_u_iso: +HkBALCaAAAwiQAAONYAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 873.1 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAAgAIAAACACAEAIAABAEAAAAgEAgACAgIEBAgAAECBAggQQAIIAIIIIAQghBCCAIAhBCIAhAAQhEIRAIRAIAIREAgAiAAIiAkAEAACAAABAAAAAAAAASAAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5244
b: 11.5244
c: 11.5244
alpha: 90
beta: 90
gamma: 90
cell_volume: 1530.576
crystal_density: 3.499
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAAPj9/w==
atoms_y: AAAAAAAAAAAAAAAAsAEDAA==
atoms_z: QEIPAAAAAABAQg8A8GAJAA==
atoms_occupancy: 0
atoms_u_iso: cIkBANCiAADgkgAAiOAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 922.9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAAgAIAAACACAEAIAABAIAAAAgEBAACAgIEBAgAAECBAgggQAIQAIQQQAQghBCEAIAhCEIAhAAQhEIhAIhAQAIhEBAAiAAJEBEAIAACAAABAAAAAAAAASAAAAAAAAAAAAAAAAAA==


formula: Mg3 Al2 Si3 O12
compound: Synthetic
formula_title: <missing>
a: 11.5291
b: 11.5291
c: 11.5291
alpha: 90
beta: 90
gamma: 90
cell_volume: 1532.450
crystal_density: 3.495
atoms_sites: ["Mg", "Al", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAyPj9/w==
atoms_y: AAAAAAAAAAAAAAAAsAEDAA==
atoms_z: QEIPAAAAAABAQg8A8GAJAA==
atoms_occupancy: 0
atoms_u_iso: eJoBAEioAADomQAAEOoAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Static disorders of atoms and experimental determination of Debye temperature in
 pyrope: Low- and high-temperature single-crystal X-ray diffraction study
 Note: T = 972.9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAACAAAAAAAAgAIAAACACAEAIAACAIAAAAgEBAACAgQECAgAAECBBAggQAQQAIQQQAQhBCCEAQAhCEIAiAAQiEIhAIiAQAIiEBABEAAREBEAIAAEAAABAAAAAAAAAkAAAAAAAAAAAAAAAAAA==


formula: Pb2 S2 C O6
compound: Trentini mine, Mount Naro, Vicenza Province, Veneto, Italy
formula_title: <missing>
a: 16.320
b: 8.7616
c: 4.5809
alpha: 90
beta: 90
gamma: 90
cell_volume: 655.020
crystal_density: 5.948
atoms_sites: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_x: WEoIAHAwAACghCsAwMgDANDTEAAw2QAA4GkLACAENgA=
atoms_y: iLkdAEBCDwBAQg8AQEIPAGAGJgBgxgYAQEIPAEBCDwA=
atoms_z: IKgjACA2BADgnhcAgIkyACCUHgDgUQ8AgK4XAKCzOAA=
atoms_occupancy: 0
atoms_u_iso: 0EwBAMDaAADgKAEAIEgBACBIAQAgSAEAYGcBAIA4AQA=
atoms_aniso_label: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_aniso_u11: IBYBAGDqAABAnAAAgD4AAGBnAQCAOAEAwNQBACDLAAA=
atoms_aniso_u22: 0DMBAOAoAQCAOAEAAHECAIC1AQAgSAEAgDgBAKCGAQA=
atoms_aniso_u33: EJ4BAAB9AADA1AEAgDgBAIC7AABgZwEAgDgBAIA4AQA=
atoms_aniso_u12: YPD//wAAAAAAAAAAAAAAACDX/v+gDwAAAAAAAAAAAAA=
atoms_aniso_u13: kOj//2Bz///AY///AH0AAIC7AAAAg///wGP//yDR//8=
atoms_aniso_u23: 8PH//wAAAAAAAAAAAAAAACBU///A4P//AAAAAAAAAAA=
pub_title:
 Fassinaite, Pb22+(S2O3)(CO3), the first mineral with coexisting
 thiosulphate and carbonate groups: description and crystal structure
 Note: Sample ID FAS-01

qdat:
AAAAAAAAAAAABAAAAEAAAAADADUQJBAAQCIkIAcIIREgVKaHAmKrmZMhaeFFC5yU48fIX3x2RXSWeufHgN5TGr23RmH3983uVrV53Xn4/u9H9lz+dhtzc9f/2dv9+fmu+38neqzu6fP/9P90p9PkXef3m5luxkxldz1/k1==


formula: Pb2 S2 C O6
compound: Erasmus adit, Schwarzleo District, Leogang, Salzburg, Austria
formula_title: <missing>
a: 16.343
b: 8.760
c: 4.592
alpha: 90
beta: 90
gamma: 90
cell_volume: 657.412
crystal_density: 5.926
atoms_sites: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_x: eEgIAKAoAADQfCsAYKYDALDQEAAw2QAAIFcLANAINgA=
atoms_y: QLYdAEBCDwBAQg8AQEIPADD1JQBg3wYAQEIPAEBCDwA=
atoms_z: 4KEjAOBhBABg4xYAQGoyACCUHgAAIw8A4J4XAFCfOAA=
atoms_occupancy: 0
atoms_u_iso: 8DYBACDLAADA2gAA4CgBAAB3AQDgKAEAwFcBAIAfAQA=
atoms_aniso_label: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_aniso_u11: EAgBAECcAABAnAAAgLsAAMBXAQAA+gAAoIYBAOCrAAA=
atoms_aniso_u22: wCUBAKAJAQCAOAEAoAMCAECWAQBgZwEAAHcBAAB3AQA=
atoms_aniso_u33: cHUBAIC7AACAuwAA4KsAAGBnAQCgCQEAoAkBAIA4AQA=
atoms_aniso_u12: 0O7//wAAAAAAAAAAAAAAAECi///A4P//AAAAAAAAAAA=
atoms_aniso_u13: 0O7//4DB///gsf//gD4AAAB9AADgsf//wNoAAMDg//8=
atoms_aniso_u23: wPn//wAAAAAAAAAAAAAAAOA0//8gTgAAAAAAAAAAAAA=
pub_title:
 Fassinaite, Pb22+(S2O3)(CO3), the first mineral with coexisting
 thiosulphate and carbonate groups: description and crystal structure
 Note: Sample ID FAS-02

qdat:
AAAAAAAAAAAABAAAAEAAAAADACUQJBAAQCIkIAUIIREgqKqLBGLPO6MicsJKD5kUo0vIruTWjumkdeefgLySG2++TMN2/avWea37+vK5fc+L/x3+7i/6///+fZO797NP/u9//7rev/e+8/+63k3wk99m6jU/jNlT129v3r==


formula: Pb2 S2 C O6
compound: Friedrich-Christian mine, Schapbach, Black Forest,
formula_title: <missing>
a: 16.326
b: 8.773
c: 4.583
alpha: 90
beta: 90
gamma: 90
cell_volume: 656.414
crystal_density: 5.935
atoms_sites: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_x: iEwIAOAuAAAwbSsAwK8DAGDVEACg1wAAAG0LANAINgA=
atoms_y: iLkdAEBCDwBAQg8AQEIPADDcJQBgxgYAQEIPAEBCDwA=
atoms_z: wKgjAOB6BAAgxBYA4HkyAMCjHgCAYQ8AQAwYAMCdOAA=
atoms_occupancy: 0
atoms_u_iso: UEABADDyAACgCQEAIEgBAOClAQDgKAEAgLUBANAzAQA=
atoms_aniso_label: ["Pb", "S1", "C", "O1", "O2", "O3", "O4", "S2"]
atoms_aniso_u11: oCIBACDLAAAgywAAAPoAAGBnAQDgKAEAIEICAKAJAQA=
atoms_aniso_u22: MCQBAMDaAABAGQEA4KUBAOClAQBg6gAAwNQBACBIAQA=
atoms_aniso_u33: IHoBAOAoAQCAOAEA4CgBAAD0AQDAVwEAQBkBACBIAQA=
atoms_aniso_u12: 0O7//wAAAAAAAAAAAAAAAECi///gsf//AAAAAAAAAAA=
atoms_aniso_u13: 0O7//2Dw///AXQAAYG0AAKCMAACAwf//4KsAAIDB//8=
atoms_aniso_u23: EPX//wAAAAAAAAAAAAAAAIBE//9AHwAAAAAAAAAAAAA=
pub_title:
 Fassinaite, Pb22+(S2O3)(CO3), the first mineral with coexisting
 thiosulphate and carbonate groups: description and crystal structure
 Note: Sample ID FAS-03
 Baden-Wurttemberg, Germany

qdat:
AAAAAAAAAAAABAAAAEAAAAADADUQJBAAQCIkIA0IIREgpK6HAmKtuaUhaeJGC5kV40uIfbR2TeSmWubPgP5TE6/fTGN75tXudTr7mtu5bN+H5p3ufB/1d+6+u/9v07G/t24vb3m92be/1f/prafIuefvtpn/RMjKun7/l5==


formula: Ag.985 Cu.005
compound: northeast USSR
pub_title: Native silver and its new structural modifications Note: sample DV-300, known as silver 4H
formula_title: <missing>
a: 2.88
b: 2.88
c: 9.62
alpha: 90
beta: 90
gamma: 120
cell_volume: 69.102
crystal_density: 5.124
atoms_sites: ["Ag", "Cu", "Fe", "Cr", "Ni"]
atoms_x: VVgUAFVYFABVWBQAVVgUAFVYFAA=
atoms_y: q7AoAKuwKACrsCgAq7AoAKuwKAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_occupancy: cCY8AOBHAACQAQAAkAEAAJABAAA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAAAAAAgMAAAIAAAAAQAAAAAAEAAAAIAACAAACAABACAAAAAAjACwAAQAAACACCAAgAAAAAMABAAiAcABCAAIAgACAAgBBgAgAIBAAEAAAQgAAEAgQAAFAwBEAEAIBAAABA==


formula: Ag.985 Cu.005
compound: northeast USSR
pub_title: Native silver and its new structural modifications Note: Sample DV-300
formula_title: <missing>
a: 4.084
b: 4.084
c: 4.084
alpha: 90
beta: 90
gamma: 90
cell_volume: 68.117
crystal_density: 10.396
atoms_sites: ["Ag", "Cu", "Fe", "Cr", "Ni"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_occupancy: cCY8AOBHAACQAQAAkAEAAJABAAA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAIAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAgAABAAAAAAAAAAAAAEAAAAAAAABAACAAAAAAAAAACAAAAAAAIAAAAAAAAAAAgAAAAACABAAAAAAAAQAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Crystal structure of dense nanocrystalline BaTiO3 ceramics Note: phase T (tetragonal)
formula_title: BaTiO3
a: 3.9988
b: 3.9988
c: 4.0222
alpha: 90
beta: 90
gamma: 90
cell_volume: 64.317
crystal_density: 6.021
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgCAhB4AgIQeAA==
atoms_y: AAAAAICEHgCAhB4AAAAAAA==
atoms_z: AAAAAFClHgDwEP//oE8fAA==
atoms_occupancy: 0
atoms_u_iso: gPYLAEAZAQCgCQEA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAABgAAAAAAAIAAAAAAoAAAAAEAAAABQAAAAAAAABQAAAUAAALAAAFAAAEAAAgAADAAAAAARAACgAFwABQACwAAgAGAAAABQASABuAJgAAAJACIAAACQCIAuAKgRwAQFcAACG==


formula: Ba Ti O3
compound: Synthetic
pub_title: Crystal structure of dense nanocrystalline BaTiO3 ceramics Note: phase O (orthorhombic)
formula_title: <missing>
a: 4.0094
b: 5.6214
c: 5.6386
alpha: 90
beta: 90
gamma: 90
cell_volume: 127.085
crystal_density: 6.094
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAACAhB4A0O0tAA==
atoms_z: AAAAAMAgHwBA6B0AQCQtAA==
atoms_occupancy: 0
atoms_u_iso: AL4KAAD6AAAgvwIAgLUBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAA4AAAAAAAMAAAAAASAAAAADAAAAAcAAAAAAAAAcAAANgAACYAADQAABgAAKgAB8AAAAAEQAA8AB3AAdAAlABOAB4AAAAdAC+AXQBWAAAB/ARwAAAMQPYC6BeBVgBgvwAAI==


formula: Ba Ti O3
compound: Synthetic
pub_title: Neutron diffraction study of orthorhombic BaTiO3 Note: orthorhombic structure
formula_title: <missing>
a: 3.990
b: 5.669
c: 5.682
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.523
crystal_density: 6.026
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAIHEPAA==
atoms_z: AAAAAMAgHwBA6B0AIHcOAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAAUAAAAAMAAAAAwAAAAAAAADgAAAOAAAEgAAHgAAGAAA8AADgAAAAAIgAHgADoADwADIAHwALAAAABoAOwA/AHoAAAPoByAAAJgDeA/AOgFkCAB2AAAx==


formula: Ba Ti O3
compound: Synthetic
pub_title: Neutron diffraction study of orthorhombic BaTiO3 Note: tetragonal structure
formula_title: BaTiO3
a: 3.986
b: 3.986
c: 4.026
alpha: 90
beta: 90
gamma: 90
cell_volume: 63.966
crystal_density: 6.054
atoms_sites: ["Ba", "Ti", "OI", "OII1"]
atoms_x: AAAAAICEHgCAhB4AgIQeAA==
atoms_y: AAAAAICEHgCAhB4AAAAAAA==
atoms_z: AAAAAKAsEACgmP7/gGcOAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAwAAAAAAAIAAAAAAkAAAAAKAAAAAoAAAAAAAAAoAAAmAAAIgAAEgAACAAAkAACwAAAAAggAKoAEsAAkAEMAEYACgAAABEAlACVgIkAAARoCDAAABECJAmIIoRGQBIjAACA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 15 K
formula_title: BaTiO3
a: 4.00360
b: 4.00360
c: 4.00360
alpha: 89.839
beta: 89.839
gamma: 89.839
cell_volume: 64.172
crystal_density: 6.034
atoms_sites: ["Ba", "Ti", "O"]
atoms_x: AAAAAIC8HQDQLh8A
atoms_y: AAAAAIC8HQDQLh8A
atoms_z: AAAAAIC8HQCQLQEA
atoms_occupancy: 0
atoms_u_iso: kOj//8ArAABAHwAA
atoms_aniso_label: ["Ba", "Ti", "O"]
atoms_aniso_u11: kOj//8ArAADwIwAA
atoms_aniso_u22: kOj//8ArAADwIwAA
atoms_aniso_u33: kOj//8ArAADgFQAA
atoms_aniso_u12: 8L///2AJAABABgAA
atoms_aniso_u13: 8L///2AJAADwCgAA
atoms_aniso_u23: 8L///2AJAADwCgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAEAAAAAgAAAAAAAABAAAAMAAAAAAACAAAAAAAAAACAAAAAAAAAGAABAAAAABAACAAAAAAABAAAAAoAFAAAAFAAQAAABAAAAAAEAFAAABgAAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 20 K
formula_title: BaTiO3
a: 4.0036
b: 4.0036
c: 4.0036
alpha: 89.840
beta: 89.840
gamma: 89.840
cell_volume: 64.172
crystal_density: 6.034
atoms_sites: ["Ba", "Ti", "O"]
atoms_x: AAAAAADJHQDAOR8A
atoms_y: AAAAAADJHQDAOR8A
atoms_z: AAAAAADJHQCwMAEA
atoms_occupancy: 0
atoms_u_iso: 0O7//xAnAAAgHAAA
atoms_aniso_label: ["Ba", "Ti", "O"]
atoms_aniso_u11: 0O7//xAnAACQGgAA
atoms_aniso_u22: 0O7//xAnAACQGgAA
atoms_aniso_u33: 0O7//xAnAACwHQAA
atoms_aniso_u12: 0Lz//5ABAACQAQAA
atoms_aniso_u13: 0Lz//5ABAABABgAA
atoms_aniso_u23: 0Lz//5ABAABABgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAEAAAAAgAAAAAAAABAAAAMAAAAAAACAAAAAAAAAACAAAAAAAAAGAABAAAAABAACAAAAAAABAAAAAoAFAAAAFAAQAAABAAAAAAEAFAAAAgAAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 40 K
formula_title: BaTiO3
a: 4.0035
b: 4.0035
c: 4.0035
alpha: 89.843
beta: 89.843
gamma: 89.843
cell_volume: 64.167
crystal_density: 6.035
atoms_sites: ["Ba", "Ti", "O"]
atoms_x: AAAAAHCVHQAADh8A
atoms_y: AAAAAHCVHQAADh8A
atoms_z: AAAAAHCVHQDwHQEA
atoms_occupancy: 0
atoms_u_iso: IOr//7AdAADAKwAA
atoms_aniso_label: ["Ba", "Ti", "O"]
atoms_aniso_u11: IOr//7AdAADwPAAA
atoms_aniso_u22: IOr//7AdAADwPAAA
atoms_aniso_u33: IOr//7AdAACADAAA
atoms_aniso_u12: EMP//zD4//8gAwAA
atoms_aniso_u13: EMP//zD4//8AGQAA
atoms_aniso_u23: EMP//zD4//8AGQAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAEAAAAAgAAAAAAAABAAAAMAAAAAAACAAAAAAAAAACAAAAAAAAAGAABAAAAABAACAAAAAAABAAAAAYAFAAAAFAAQAAABAAAAAAEAFAAAAgAAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 70 K
formula_title: BaTiO3
a: 4.0042
b: 4.0042
c: 4.0042
alpha: 89.837
beta: 89.837
gamma: 89.837
cell_volume: 64.201
crystal_density: 6.032
atoms_sites: ["Ba", "Ti", "O"]
atoms_x: AAAAAFCSHQDgCh8A
atoms_y: AAAAAFCSHQDgCh8A
atoms_z: AAAAAFCSHQBwEQEA
atoms_occupancy: 0
atoms_u_iso: QO3//+AVAABQLQAA
atoms_aniso_label: ["Ba", "Ti", "O"]
atoms_aniso_u11: QO3//zACAABAOAAA
atoms_aniso_u22: QO3//zACAABAOAAA
atoms_aniso_u33: QO3//zACAAAAGQAA
atoms_aniso_u12: 0Lz//8D5//+gDwAA
atoms_aniso_u13: 0Lz//8D5///gFQAA
atoms_aniso_u23: 0Lz//8D5///gFQAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAIAAAABAAAAAAAAABAAAAMAAAAAAACAAAAAAAAAACAAAAAAAAAGAABAAAAABAACAAAAAAABAAAAAoAGAAAAFAAgAAABAAAAAAEAFAAABgAAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 150 K
formula_title: BaTiO3
a: 4.0057
b: 4.0057
c: 4.0057
alpha: 89.846
beta: 89.846
gamma: 89.846
cell_volume: 64.273
crystal_density: 6.025
atoms_sites: ["Ba", "Ti", "O"]
atoms_x: AAAAAACwHQDQFR8A
atoms_y: AAAAAACwHQDQFR8A
atoms_z: AAAAAACwHQDQGgEA
atoms_occupancy: 0
atoms_u_iso: wBIAACA1AADAKwAA
atoms_aniso_label: ["Ba", "Ti", "O"]
atoms_aniso_u11: wBIAALA2AAAQQAAA
atoms_aniso_u22: wBIAALA2AAAQQAAA
atoms_aniso_u33: wBIAALA2AABgCQAA
atoms_aniso_u12: 8Kb//8Dg//9ABgAA
atoms_aniso_u13: 8Kb//8Dg//+gDwAA
atoms_aniso_u23: 8Kb//8Dg//+gDwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAAAAAAAIAAAABAAAAAAAAABAAAAMAAAAAAACAAAAAAAAAACAAAAAAAAAGAACAAAAABAACAAAAAAABAAAAAwAKAAAAGAAgAAACAAAAAAEAFAAABgAAAA==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 190 K
formula_title: <missing>
a: 3.9828
b: 5.6745
c: 5.6946
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.700
crystal_density: 6.018
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAkKEPAA==
atoms_z: AAAAACCOHwCg2B0AuCkPAA==
atoms_occupancy: 0
atoms_u_iso: EA4AAKAoAAAASwAAECcAAA==
atoms_aniso_label: ["Ba", "Ti", "O1", "O2"]
atoms_aniso_u11: oEEAALAdAADAXQAAsB0AAA==
atoms_aniso_u22: QIMAAOAuAAAQQAAAEA4AAA==
atoms_aniso_u33: IJkAAMArAAAwQwAA4EcAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAADIAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAAUAAAAAYAAAAB4AAAAAAAAFgAAAZAAAMgAAKwAAGAACUAALwAAAAAQQANgAOsAJwAKIAOQAXAAAACsAukD6gOmAAAXIFjAAASgGrCuhEwRhOAHmgAEg==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 210 K
formula_title: <missing>
a: 3.9806
b: 5.6710
c: 5.6904
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.455
crystal_density: 6.029
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAkKEPAA==
atoms_z: AAAAAPBjHwCg2B0AKCgPAA==
atoms_occupancy: 0
atoms_u_iso: wBIAALBPAADwVQAAcDAAAA==
atoms_aniso_label: ["Ba", "Ti", "O1", "O2"]
atoms_aniso_u11: ADIAAHAwAACQZQAAYCIAAA==
atoms_aniso_u22: gKIAAJBMAAAAMgAAYAkAAA==
atoms_aniso_u33: 0J0AABByAABAagAAAGQAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAA8CMAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAASAAAAAYAAAAB4AAAAAAAADQAAAdAAAMQAAGQAAGAABKAAHwAAAAAIQAGgAPUAFwALEAKQALAAAACkAZUD+QOiAAAbkDxAAAJQCtBfgmYJRGADyQACw==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 230 K
formula_title: <missing>
a: 3.9841
b: 5.6741
c: 5.6916
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.665
crystal_density: 6.019
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAAIcPAA==
atoms_z: AAAAAPD/HgAQCR4AuCQPAA==
atoms_occupancy: 0
atoms_u_iso: ABJ6AKBzAAAASwAAADIAAA==
atoms_aniso_label: ["Ba", "Ti", "O1", "O2"]
atoms_aniso_u11: oEEAANAHAAAwdQAAwBIAAA==
atoms_aniso_u22: EFkAABCLAABwMAAAoEEAAA==
atoms_aniso_u33: sJoAAADIAADwPAAAoEEAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAoA8AAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAAUAAAAAIAAAABwAAAAAAAAFgAAAZAAAMgAAGgAAGAABEAAHwAAAAAQQANgAOsAFwAKIAOAALAAAACsAiED6gOkAAAfIFiAAASgGrC/AkwZiGAFmgACg==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 250 K
formula_title: <missing>
a: 3.9855
b: 5.6738
c: 5.6903
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.674
crystal_density: 6.019
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAA8KoPAA==
atoms_z: AAAAAEBGHwCgvx0AcCsPAA==
atoms_occupancy: 0
atoms_u_iso: EA4AACBnAAAwXAAAoEEAAA==
atoms_aniso_label: ["Ba", "Ti", "O1", "O2"]
atoms_aniso_u11: UEYAACA1AABAagAAYCIAAA==
atoms_aniso_u22: IIAAAICJAAAwQwAAcDAAAA==
atoms_aniso_u33: kAEAADB1AAAgZwAAoHMAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAYDsAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAAUAAAAAYAAAABwAAAAAAAADgAAAdAAAMgAAGgAAGAABEAAHgAAAAAQgAFgAOoAFwAKIAOQAKAAAACsAaID+gOkAAAfIDiAAAKgCqBfAkgJiGADngACg==


formula: Ba Ti O3
compound: Synthetic
pub_title: Structures of the ferroelectric phases of barium titanate Note: T = 270 K
formula_title: <missing>
a: 3.9874
b: 5.6751
c: 5.6901
alpha: 90
beta: 90
gamma: 90
cell_volume: 128.761
crystal_density: 6.015
atoms_sites: ["Ba", "Ti", "O1", "O2"]
atoms_x: AAAAAICEHgAAAAAAgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAAKAPAA==
atoms_z: AAAAAJCMHwCgeRgAYCwPAA==
atoms_occupancy: 0
atoms_u_iso: IBwAACA1AABgVAAAYDsAAA==
atoms_aniso_label: ["Ba", "Ti", "O1", "O2"]
atoms_aniso_u11: kEwAAKAoAABwSQAAMCoAAA==
atoms_aniso_u22: oKUAAKBBAADAXQAAECcAAA==
atoms_aniso_u33: QJwAALA2AADwVQAAcGIAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAcDAAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAABgAAAAAAAYAAAAAAUAAAAAYAAAABwAAAAAAAADgAAAZAAAMgAAGgAAEAABUAAHgAAAAAQgANgAOoAFgAKIAOQAOAAAACoAaoD/AOsAAAfIDiAAAKgCuB3AkgLkGADnAACg==


formula: Fe Cl2
compound: <missing>
pub_title: The structure of FeCl2 at high pressures Note: P = 1.04 kbar
formula_title: <missing>
a: 3.598
b: 3.598
c: 17.481
alpha: 90
beta: 90
gamma: 120
cell_volume: 195.983
crystal_density: 3.222
atoms_sites: ["Fe", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAGCQDwA=
atoms_occupancy: 0
atoms_u_iso: qNkAAAgVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAQCgAAAAIAAAgAAAAAAADAAAAUABAAAAAAEOAAIAEAAAAAYAAEAAAAAASgAgBAAAAIABgIAAAAwAAAAAAIAIBAAALAEBAAAIAIAAAEwCBAABACAAACwEEAAIAwgAAQAAAAQAA==


formula: Fe Cl2
compound: <missing>
pub_title: The structure of FeCl2 at high pressures Note: P = 3.15 kbar
formula_title: <missing>
a: 3.592
b: 3.592
c: 17.384
alpha: 90
beta: 90
gamma: 120
cell_volume: 194.246
crystal_density: 3.251
atoms_sites: ["Fe", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAACCKDwA=
atoms_occupancy: 0
atoms_u_iso: gO0AAIDtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAQCQAAAAIAAAQAAAAAAAAwAAAJAAgAAAAAEGgAEABAAAAAGAABAAAAAAJIAIAgAAAEAAwCAAAAMAAAAAACACAgAAEgBAgAAEACAAABUBAgAAQAgAABMCCAACAMIAAGAAAAEAA==


formula: Fe Cl2
compound: <missing>
pub_title: The structure of FeCl2 at high pressures Note: P = 5.70 kbar
formula_title: <missing>
a: 3.589
b: 3.589
c: 17.260
alpha: 90
beta: 90
gamma: 120
cell_volume: 192.539
crystal_density: 3.280
atoms_sites: ["Fe", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAGB3DwA=
atoms_occupancy: 0
atoms_u_iso: gO0AADABAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAAQBIAAAAEAAAIAAAAAAAASAAAIgAQAAAAACGIACABAAAAACgAAgAAAAAIiAIAQAAABAAUCAAAAFAAAAAABACAQAACoBAQAADABAAABJAgQAAIAQAAApBAgABAGEAADAAAABAA==


formula: Fe Cl2
compound: <missing>
pub_title: The structure of FeCl2 at high pressures Note: P = 5.97 kbar
formula_title: <missing>
a: 3.585
b: 3.585
c: 5.735
alpha: 90
beta: 90
gamma: 120
cell_volume: 63.833
crystal_density: 3.297
atoms_sites: ["Fe", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAGCWDgA=
atoms_occupancy: 0
atoms_u_iso: MAEBAKjZAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAAAAEAIAAAAAAAAAACAAAABAAAEAAQAAIAAABBAAAgAACAAAkAAAAABAAAAoAEAAEIAIAQBACAAEIEAAAECoBAQAAAIgRAAjCgAAQIAAYBACEJAAEEQAYRAEgIEDBIBAQgBi4A==


formula: Sn2.56 Fe.43 S6 Pb2.01
compound: San Jose, Bolivia
pub_title: The crystal structure of franckeite, Pb21.7Sn9.3Fe4.0Sb8.1S56.9
formula_title: <missing>
a: 5.805
b: 5.856
c: 17.338
alpha: 94.97
beta: 88.45
gamma: 89.94
cell_volume: 586.955
crystal_density: 5.300
atoms_sites: ["Sn1", "Fe1", "S1", "Pb2", "Sn2", "Pb3", "Sn3", "S2", "S3"]
atoms_x: QEIPAEBCDwAglxEAiAAnAIgAJwDI3AoAyNwKADDCCADQOwgA
atoms_y: QEIPAEBCDwBgDCUAOEE7ADhBOwAoBzoAKAc6ANDqOgBw3xkA
atoms_z: AAAAAAAAAAAwDAUAWN7x/1je8f+w0ub/sNLm/8DD7/+AV+f/
atoms_occupancy: QMoiAMA+GgAACT0AgCotAIDeDwCgLBAAYNwsAAAJPQAACT0A
atoms_u_iso: sJQBALCUAQBA2wIAkCcCAJAnAgCQJwIAkCcCACApAgDAZAMA
atoms_aniso_label: ["Sn1", "Fe1", "S1", "Pb2", "Sn2", "Pb3", "Sn3", "S2", "S3"]
atoms_aniso_u11: 0C0CANAtAgBAfgUAUKQBAFCkAQDA1AEAwNQBAHBDAQBAigMA
atoms_aniso_u22: IIAAACCAAADA8wAAUNYBAFDWAQCg6gEAoOoBAMBwAQBAhAQA
atoms_aniso_u33: gBkCAIAZAgDgIgIAQPQCAED0AgAwtAIAMLQCACC5AwCgAwIA
atoms_aniso_u12: QAYAAEAGAACgDwAAgPP//4Dz//9QeAAAUHgAAMArAACASv7/
atoms_aniso_u13: IIAAACCAAADAXQAAAAAAAAAAAAAQWQAAEFkAADBDAABwSQAA
atoms_aniso_u23: 0AcAANAHAADwCgAAoA8AAKAPAACwTwAAsE8AABAnAADgsf//
qdat:
AAAAAAgAAAAAQAAAAAxEAEEAIIKACBIJAABBdBBA5i2gIyEMUgPNCZazS8rjL4hOvoOHYDIXb5vf2Oo2/k38EpkiVJe2/1b3O53ezflP631Ob/7z1O++Wfma9nLl/jv+03/fX7zP+dumZI6fe/6v3af8vpvu/r9xu298+/==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.5142
b: 5.6634
c: 7.88162
alpha: 90
beta: 90
gamma: 90
cell_volume: 246.136
crystal_density: 5.580
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: WDr//wAAAACQDwYAMKUqAA==
atoms_y: EBUDAICEHgBgWxwAwDwSAA==
atoms_z: QEIPAICEHgBAQg8AgCwDAA==
atoms_occupancy: 0
atoms_u_iso: kG8AAFA8AADAdgAAyG4AAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: 4FEAAHgyAACIiwAA4FEAAA==
atoms_aniso_u22: iIYAABhMAACorAAAaGAAAA==
atoms_aniso_u33: kHQAACA1AAA4MQAAWJ0AAA==
atoms_aniso_u12: sPD//1AAAACo8///yL///w==
atoms_aniso_u13: AAAAAKAAAAAAAAAA0CUAAA==
atoms_aniso_u23: AAAAANACAAAAAAAAcMf//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 0.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAABQAAEAACAACAAAAkgAQAIC4EIBAJAAAwCgEikIQIBAKMINM0BEpAggkU/anAkR0ncNOlQgSktrCiijvVWmLItmrs6jFZ/XQomL/2/9mfTtBMT1v2VdH9702/1zu3vZ0262u/frb9a7+69N8Z==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.5043
b: 5.6558
c: 7.8687
alpha: 90
beta: 90
gamma: 90
cell_volume: 244.962
crystal_density: 5.607
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: 0DX//wAAAACQKAYA0JsqAA==
atoms_y: EBUDAICEHgCAXhwA0DESAA==
atoms_z: QEIPAICEHgBAQg8AYCkDAA==
atoms_occupancy: 0
atoms_u_iso: eG4AAOg6AADYcgAAuHQAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: +GsAAPgvAAAo5gAAOBMAAA==
atoms_aniso_u22: wGcAAKAyAADIQQAAgMUAAA==
atoms_aniso_u33: oHgAAGA2AAAQMQAAWIQAAA==
atoms_aniso_u12: MPP//0ABAACo8///SMz//w==
atoms_aniso_u13: AAAAALD///8AAAAAqCUAAA==
atoms_aniso_u23: AAAAAMgAAAAAAAAA2Nz//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 0.738 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAABQAACAACAACAAAAigAIAIC4CEAgIgAAQBQESSMQEAgFGEMm6AiogQQSKvVSgSI6TqHmkoQJUW1hRRRn6r1FEUyU2dhjc9/oUTj97b2yrtqjCJ73/r7j7auVP6573z8XftP6tm/f/nXr/3v9m==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.4952
b: 5.6486
c: 7.8561
alpha: 90
beta: 90
gamma: 90
cell_volume: 243.855
crystal_density: 5.632
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: oDj//wAAAACQKAYAoIoqAA==
atoms_y: UBsDAICEHgBQTRwAsEcSAA==
atoms_z: QEIPAICEHgBAQg8AICMDAA==
atoms_occupancy: 0
atoms_u_iso: AG4AAFA8AACwfAAAuHQAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: AG4AANA5AAAglAAA6BcAAA==
atoms_aniso_u22: GGoAAAhIAACQnAAAkJwAAA==
atoms_aniso_u33: 2HIAAEAzAABwRAAA8KoAAA==
atoms_aniso_u12: eAAAALD///+IGAAAoNj//w==
atoms_aniso_u13: AAAAAGD///8AAAAA6BcAAA==
atoms_aniso_u23: AAAAAHADAAAAAAAA6Or//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 1.50 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAABIAACAACAABAAAAiQAIAIBsCEAgEgAAYBQCRKEIEAQElEGWZASUQQIRKdsrgRIdJtFzSUIEqLcwoooz1W6iiLXK3O4x2dduNJy//vbZV21JRE977Td43rvHm8+93d9Pa/n3/7/vXyXu3z7vR==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.4824
b: 5.6384
c: 7.8387
alpha: 90
beta: 90
gamma: 90
cell_volume: 242.310
crystal_density: 5.668
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: cDb//wAAAADAIAYAkJUqAA==
atoms_y: sCQDAICEHgAQRxwA8DQSAA==
atoms_z: QEIPAICEHgBAQg8A4DUDAA==
atoms_occupancy: 0
atoms_u_iso: 6GcAALg4AAAIYQAA0HAAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: WGYAAJA4AACAkwAA6HYAAA==
atoms_aniso_u22: oGQAAChBAADIbgAAoFUAAA==
atoms_aniso_u33: eG4AACAwAAA4HQAAaH4AAA==
atoms_aniso_u12: CAcAAMgAAABYBwAAGM///w==
atoms_aniso_u13: AAAAAFAAAAAAAAAAcAMAAA==
atoms_aniso_u23: AAAAALgBAAAAAAAAeOf//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 2.61 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAABIAACAABAABAAAASQAEAEBcBCAQEQAAMAoCJJCICAQCjCFLOgQqIIEElL1UwEkUo+ipoqECVltUMUUJ+q9RYlmzP2sIXN99HkY1+796p9t0YyNe/9f6fe1xZ/Pve+PmXvl/9mv79q169/f/0==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.4676
b: 5.6267
c: 7.8186
alpha: 90
beta: 90
gamma: 90
cell_volume: 240.536
crystal_density: 5.710
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: 2DL//wAAAABgMAYA8IUqAA==
atoms_y: 0CcDAICEHgAwYxwAQEkSAA==
atoms_z: QEIPAICEHgBAQg8AgCwDAA==
atoms_occupancy: 0
atoms_u_iso: KGkAACg3AAAwTQAA8GQAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: CGEAAMA6AADoPwAAsF4AAA==
atoms_aniso_u22: UG4AADg7AABQjAAAqFIAAA==
atoms_aniso_u33: +GsAAPgvAAAQHQAAyH0AAA==
atoms_aniso_u12: QPf///AAAACo+P//SOD//w==
atoms_aniso_u13: AAAAAFAAAAAAAAAA4BAAAA==
atoms_aniso_u23: AAAAANACAAAAAAAA+Pj//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 3.94 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAoAABAABAAAgAAARIACAEAuBCAQCIAAEAkBEkhEBAIBRhClnQElEICCRn6qYCKHSfRUqSiBGx/uFHKGdq1UmRTZ25+GNzvtRpGV/u/aqf7dGEjbv5L/n+t8afz53vjNVb+vddv///Nfvdvu9==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.4538
b: 5.6162
c: 7.8006
alpha: 90
beta: 90
gamma: 90
cell_volume: 238.930
crystal_density: 5.749
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: oDj//wAAAADgIwYAUHYqAA==
atoms_y: gCwDAICEHgCwVhwAcFoSAA==
atoms_z: QEIPAICEHgBAQg8AwDIDAA==
atoms_occupancy: 0
atoms_u_iso: uGUAAMA1AAAIYQAAEFkAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: QGUAALBAAAAooAAAAFAAAA==
atoms_aniso_u22: WGYAADAvAABYPgAAgCUAAA==
atoms_aniso_u33: oGQAABAxAAAwSAAAYJUAAA==
atoms_aniso_u12: UOf//1AAAADI5///SOX//w==
atoms_aniso_u13: AAAAAJj+//8AAAAA4BAAAA==
atoms_aniso_u23: AAAAABgBAAAAAAAAiPX//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 5.18 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAkAABAAAgAAgAAAIoACACArAhAIBEAAGASAkSRiAgEAowhSzoEKiCBBIx9UsBEjpHYWNJQgjY1yijihG07aJElWZ6vBCp/6cajldrP2qvv3hDR/7+yvRe9bFl899yZ7dLunv/+7nrTP3zV3f==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.44480
b: 5.60887
c: 7.78906
alpha: 90
beta: 90
gamma: 90
cell_volume: 237.871
crystal_density: 5.774
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: sDL//wAAAAAwOAYA4HcqAA==
atoms_y: ADkDAICEHgCgSBwAkEQSAA==
atoms_z: QEIPAICEHgBAQg8A0EADAA==
atoms_occupancy: 0
atoms_u_iso: 0GsAANA5AADYaAAA4GoAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: +GsAAKg+AADAhQAAoGkAAA==
atoms_aniso_u22: MGEAAHg3AAAIegAAsEUAAA==
atoms_aniso_u33: iHcAAMg3AACAPgAAEJAAAA==
atoms_aniso_u12: SOr//wAAAADw4v//GN7//w==
atoms_aniso_u13: AAAAALgBAAAAAAAAAAoAAA==
atoms_aniso_u23: AAAAAKAAAAAAAAAAeN3//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 5.98 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAkAABAAAgAAgAAAIkABABAXAggEBEAADAKASRQyAQCAkYgypoCJhCBAkZ6qmAih0j0TOkogRsezhRzhnattEkWrU/Wwhs1/uNQyu937WX/rwgo/b3J38/9dhvePuduc6X/zvtv/dr53rdpu7==


formula: Ca Sn O3
compound: Synthetic
formula_title: <missing>
a: 5.43626
b: 5.60235
c: 7.77743
alpha: 90
beta: 90
gamma: 90
cell_volume: 236.868
crystal_density: 5.799
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: 4Cr//wAAAABwPgYAkHwqAA==
atoms_y: ADkDAICEHgDwXBwAUD4SAA==
atoms_z: QEIPAICEHgBAQg8A4DUDAA==
atoms_occupancy: 0
atoms_u_iso: uGAAAFg5AAAAXwAA8GQAAA==
atoms_aniso_label: ["Ca", "Sn", "O1", "O2"]
atoms_aniso_u11: QFsAAIA+AADIqgAAiE8AAA==
atoms_aniso_u22: 4GoAACg8AACITwAAiFQAAA==
atoms_aniso_u33: 0FwAANgxAACYIQAA6IoAAA==
atoms_aniso_u12: iPD//0ABAAB48f//aNn//w==
atoms_aniso_u13: AAAAALAEAAAAAAAAAAoAAA==
atoms_aniso_u23: AAAAAFAAAAAAAAAAsPX//w==
pub_title:
 Tilting and distortion of CaSnO3 perovskite to 7 GPa determined from
 single-crystal X-ray diffraction
 Note: P = 6.73 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAkAAAgAAgAAQAAAIkABABAVAggEAiAADAJASJIxAQBAUUQpZ0CFRCAgkY9pTAiRST6KnSoQI6PZow5wxpW2iRKVmerQQuf/nGoZXe75rJ/t0YUXu/kv2fvTo93H3+XGVr3l///fd+6Zzd+u/==


formula: Cu As S
compound: Grube Gabe Gottes near Sainte-Marie-aux-Mines, France
pub_title: The crystal structure of lautite and of sinnerite, a new mineral from the Lengenbach Quarry
formula_title: <missing>
a: 11.356
b: 3.754
c: 5.453
alpha: 90
beta: 90
gamma: 90
cell_volume: 232.464
crystal_density: 4.873
atoms_sites: ["Cu", "As", "S"]
atoms_x: QJIKACDkAACwEwoA
atoms_y: QEIPAEBCDwDAxi0A
atoms_z: ILkDAAB8FQCg3TEA
atoms_occupancy: 0
atoms_u_iso: oJ8BAAgVAQD4xQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAEAAIAAAACAAAAAAHAQBAMEACCCAAIIIAhAAIApAQNC0BgBjQTKMCQABRBQRYFhTSoRDTMHIGREUHWqeHTR4jxqRMEWilRGUSPWGkts4yaS8D77uIrwaaF7jSO0bQzeLvqd4a1biLKrYJv4LGL63r==


formula: Na1.11 Ca.65 Bi.15 Ta2 O6 F
compound: Quixaba, Paraiba, Brazil
pub_title: Fluornatromicrolite, (Na,Ca,Bi)2Ta2O6F, a new mineral species from Quixaba, Paraiba, Brazil
formula_title: <missing>
a: 10.4451
b: 10.4451
c: 10.4451
alpha: 90
beta: 90
gamma: 90
cell_volume: 1139.562
crystal_density: 6.526
atoms_sites: ["Na", "Ca", "Bi", "Ta", "O", "F"]
atoms_x: AAAAAAAAAAAAAAAAgIQeAMDX9P8goQcA
atoms_y: AAAAAAAAAAAAAAAAgIQeACChBwAgoQcA
atoms_z: AAAAAAAAAAAAAAAAgIQeACChBwAgoQcA
atoms_occupancy: 4N8hACDWEwDgkwQAAAk9AAAJPQAACT0A
atoms_u_iso: wFECAMBRAgDAUQIA0OgAAPAdAQDgpQEA
atoms_aniso_label: ["Na", "Ca", "Bi", "Ta", "O", "F"]
atoms_aniso_u11: wFECAMBRAgDAUQIA0OgAAIA4AQDgpQEA
atoms_aniso_u22: wFECAMBRAgDAUQIA0OgAAKAJAQDgpQEA
atoms_aniso_u33: wFECAMBRAgDAUQIA0OgAAKAJAQDgpQEA
atoms_aniso_u12: 4Gb//+Bm///gZv//wPT//wAAAAAAAAAA
atoms_aniso_u13: 4Gb//+Bm///gZv//wPT//wAAAAAAAAAA
atoms_aniso_u23: 4Gb//+Bm///gZv//wPT//8BdAAAAAAAA
qdat:
AAAAAAAAAAgAAAQAAIAAgAIAEAAAIAgCAICAQEAAQIECBAggAQQQgAhACCEIQhAIQhEIgERCIiAiIgIgRESJASJIkCRJEgiSCQRSJQSSSQEkkhKQUJJSgpSkKUJCpAgSpQiVQKVIIRQkBhQRAkIKAAJEgAgARAQAAARAAA==


formula: Cu Fe S2
compound: Palabora mine, South Africa
formula_title: <missing>
a: 5.2900
b: 5.2900
c: 10.4217
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.642
crystal_density: 4.180
atoms_sites: ["Cu", "Fe", "S"]
atoms_x: AAAAAAAAAADA5A8A
atoms_y: AAAAAAAAAABAQg8A
atoms_z: AAAAAICEHgAgoQcA
atoms_occupancy: 0
atoms_u_iso: kPsAAJCXAABAgwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The low-temperature and high-pressure thermoelastic and
 structural properties of chalcopyrite, CuFeS2
 T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAEAgAAEQAAAAIAAAAAAAEgAoAAAQACAABGgAgAAggIAAFAQIAQQAAJoFEAAkAABAQgETBAsIAASSABghAAUAVKiBFQAQYASAgckAQQAYBAliJmIIkAIJALAmgAqgEIBKEKJAE==


formula: Cu Fe S2
compound: Palabora mine, South Africa
formula_title: <missing>
a: 5.28563
b: 5.28563
c: 10.41917
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.090
crystal_density: 4.188
atoms_sites: ["Cu", "Fe", "S"]
atoms_x: AAAAAAAAAACQbw8A
atoms_y: AAAAAAAAAABAQg8A
atoms_z: AAAAAICEHgAgoQcA
atoms_occupancy: 0
atoms_u_iso: AEsAAJBMAADQUgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The low-temperature and high-pressure thermoelastic and
 structural properties of chalcopyrite, CuFeS2
 T = 4.2 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAEAgAACQAAAAEAAAAAAAEgAkAAAIAAAABGgAgAAQQAAAFAQIAIQAAEoDCAAUAABAIgEKgAkIAARKABghAAQALFiAlAAQMAJAQKkAIQAMBAlQElEEiAMFALAWQAlQCEApCGMgC==


formula: Ca Sn O3
compound: Synthetic
pub_title: The ASnO3 (A = Ca, Sr) perovskites
formula_title: <missing>
a: 5.532
b: 5.681
c: 7.906
alpha: 90
beta: 90
gamma: 90
cell_volume: 248.464
crystal_density: 5.528
atoms_sites: ["Ca", "Sn", "O1", "O2"]
atoms_x: UDP//wAAAAAgEQYAAK0qAA==
atoms_y: UBsDAICEHgDwKhwA0DESAA==
atoms_z: QEIPAAAAAABAQg8AICMDAA==
atoms_occupancy: 0
atoms_u_iso: MHUAALA2AABgbQAAYG0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAACQAAEAAEAAEAAABJAAQAQFwIQCASAABgFARFIQgQCAUYQqboCKiBBCJK9laCJCydo2qTBApS2sGOKO/VaYsi2auzqMVnttCiUr+67Uare0Iye9+7/4+17lT+ufV83NW3T/37drfrjfv3xvnX==


formula: Sr Sn O3
compound: Synthetic
pub_title: The ASnO3 (A = Ca, Sr) perovskites
formula_title: SrSnO3
a: 5.707
b: 5.707
c: 8.064
alpha: 90
beta: 90
gamma: 90
cell_volume: 262.643
crystal_density: 6.432
atoms_sites: ["Sr", "Sn", "O1", "O2"]
atoms_x: 8PH//wAAAAAAfgQAwIcrAA==
atoms_y: wMEAAICEHgAA4h0A0GkRAA==
atoms_z: QEIPAAAAAABAQg8AAD8CAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAgAAgABAAAACAAgAgAgAgBAEAABgEAgEAgEBAAGBAQEAAgQAMGCBBhAgAwwQQwwQBBDCCEIAwhCAIQBCMQzCARCMREAxEYiICMRARARERMwMiRIwBkTIgRJgiDJESINEmiCRNNgkiCQ2T==


formula: Mn.88 Fe.09 (Ta1.72 Nb.28) O6
compound: Brazil
formula_title: <missing>
a: 14.3196
b: 5.7413
c: 5.0624
alpha: 90
beta: 90
gamma: 90
cell_volume: 416.196
crystal_density: 7.766
atoms_sites: ["Mn", "Fe", "Ta", "Nb", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAg4AkAIOAJAOAKBgDgkhkAoO8uAA==
atoms_y: YPUTAGD1EwBADwsAQA8LAMA5BgDgBAcAwLAHAA==
atoms_z: QEIPAEBCDwBgWS0AYFktAOAWBAAAZQQA4AoGAA==
atoms_occupancy: ALY1AEB+BQCAfTQAgIsIAAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and structure of the orthorhombic
 (Fe,Mn)(Ta,Nb)2O6 family of compounds
 Note: Sample Mn0.88Fe0.09Ta1.72Nb0.28O6

qdat:
AAAAAAAAAAAAAACAAAACAAAAAAAAEQAQAAAIEAAIRIkBIBDMAAKRABISAgUoKAEgCZYAIgUqo0spQS0hKWGh4ziXZCVGJHClhOwkcaOtMKiKGvObcNYS5pSjWiCY5jvPldTzLI4luc7kUy2Sy0/el+tLbN2u9dqy82d6Ov==


formula: Fe (Nb1.2 Ta.8) O6
compound: Brazil
formula_title: <missing>
a: 14.2737
b: 5.73543
c: 5.0554
alpha: 90
beta: 90
gamma: 90
cell_volume: 413.864
crystal_density: 6.549
atoms_sites: ["Fe", "Nb", "Ta", "O1", "O2", "O3"]
atoms_x: AAAAACDgCQAg4AkAANwFAECDGQAgsS4A
atoms_y: YHIUAODsCgDg7AoAwLYGAMC2BgDAtgYA
atoms_z: QEIPAABpLQAAaS0AgKkDAMBFBAAA4gQA
atoms_occupancy: AAk9AACfJAAAahgAAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and structure of the orthorhombic
 (Fe,Mn)(Ta,Nb)2O6 family of compounds
 Note: Sample Fe(Ta0.4Nb0.6)2O6

qdat:
AAAAAAAAAAAAAACAAAACAAAAAAAAGIAIAAAIEAAIIkiAkBBKAAJQgAkbAQKkNAEQBUoAEwSV08epQJqgjMjw8bxHMhPDEzDVwncSONHUVPxFDVXP2KsJc455lRDEc51n6vp532WSzPbrHY5HY/ffL+r1u7GzflnYKmNtGz==


formula: Na6 S2 O8 Cl F
compound: not provided
formula_title: <missing>
a: 10.071
b: 10.071
c: 10.071
alpha: 90
beta: 90
gamma: 90
cell_volume: 1021.452
crystal_density: 2.500
atoms_sites: ["Na", "S", "O", "Cl", "F"]
atoms_x: gJ8NAEBCDwDwGQoAgIQeAAAAAAA=
atoms_y: AAAAAEBCDwDwGQoAgIQeAAAAAAA=
atoms_z: AAAAAEBCDwDwGQoAgIQeAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: kDwBACCyAAAwAQEA4CgBAKjZAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The size, atomic charges, and motion of the sulfate radical of
 symmetry -43m in the crystal of sulfohalite, Na6ClF(SO4)2

qdat:
AAAAAAAAAAAAAAAAAAgABAAAAAAAAIAAAAEAgAAAACAAAIEAAAAgAAgAAABAAEIAABAAQgAAgAIgABABAAAQASAAQAiAAgCIAEAQABAEgAgEgAAEgAgIACAkAICgBAgAQEAACQBAoAAkAAQAQAAgEAAgBAAAAgABAAQAAA==


formula: Pb F2
compound: Synthetic
pub_title: Synthesis and characterization of mixed fluorides with PbF2 and ScF3
formula_title: <missing>
a: 5.9397
b: 5.9397
c: 5.9397
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.553
crystal_density: 7.772
atoms_sites: ["Pb", "F"]
atoms_x: AAAAAEBCDwA=
atoms_y: AAAAAEBCDwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAIAAAAAAAAAAAAABAAAAAAAAEAAgAAAAAAAAEAAAAABABAAAAAAAIAAAACAAAAAAACAAAAIBAAAAAEAAACAgAAAAQAABAQAAAAgAAIAAAAAgAAIEAAACAACCAAACAACCAAAI==


formula: Pb F2
compound: Kupol'noe deposit, Sarychev range, Sakha Republic, Russian Federation
pub_title: Fluorocronite, the natural analogue of beta-PbF2, from the Sakha Republic, Russian Federation
formula_title: <missing>
a: 5.9306
b: 5.9306
c: 5.9306
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.591
crystal_density: 7.808
atoms_sites: ["Pb", "F"]
atoms_x: AAAAAEBCDwA=
atoms_y: AAAAAEBCDwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAIAAAAAAAAAAAAAAgAAAAAAAEAAQAAAAAAAACAAAAAAgAgAAAAAAEAAAACAAAAAAABAAAAEAgAAAACAAABAQAAAAIAAAQIAAAAQAACAAAAAIAAEEAAABAABBAAAAgABBAAAC==


formula: Fe Br2
compound: Synthetic
pub_title: Neutron diffraction investigations of the magnetic ordering in FeBr2, CoBr2, FeCl2, and CoCl2
formula_title: FeBr2
a: 3.772
b: 3.772
c: 6.223
alpha: 90
beta: 90
gamma: 120
cell_volume: 76.679
crystal_density: 4.670
atoms_sites: ["Fe", "Br"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAACAAQAAAAAAAAAEAAAEAAAAEAAgBAAAAAgIIAAAAIAAgAAAAAEAAQAEQAAgIAAAAQCCABhAAABgACAAgIAAQhJAGIAgAAAQBAJQBEASAABAMBAAiAUBBEASEgMBIAAAAAbAREk==


formula: Co Br2
compound: Synthetic
pub_title: Neutron diffraction investigations of the magnetic ordering in FeBr2, CoBr2, FeCl2, and CoCl2
formula_title: CoBr2
a: 3.728
b: 3.728
c: 6.169
alpha: 90
beta: 90
gamma: 120
cell_volume: 74.250
crystal_density: 4.892
atoms_sites: ["Co", "Br"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgACAAAAAAAAAAgAABAAAAAQACAIAAAACAhAAAAAQABAAAAAAEABAAEQABAIAAAAIBBABAgAABAABAAICAAIITADCAYAAAEAQBMAQQJAAAIBAEAEECgCCICGCAgQQAAAABsBh==


formula: Fe Cl2
compound: Synthetic
pub_title: Neutron diffraction investigations of the magnetic ordering in FeBr2, CoBr2, FeCl2, and CoCl2
formula_title: <missing>
a: 3.603
b: 3.603
c: 17.536
alpha: 90
beta: 90
gamma: 120
cell_volume: 197.147
crystal_density: 3.203
atoms_sites: ["Fe", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAHCFDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAgDAAAAAQAAAgAAAAAAACAAAAYABAAAAAAIcAAQAEAAAAAQAAIAAAAAAlAAgCAAAAQADAIAAABgAAAAAAQAICAAASAICAAAgAgAAAJAIEAACAEAAALAQIAAgBBAAAgAAABAAA==


formula: Co Cl2
compound: Synthetic
pub_title: Neutron diffraction investigations of the magnetic ordering in FeBr2, CoBr2, FeCl2, and CoCl2
formula_title: CoCl2
a: 3.553
b: 3.553
c: 17.359
alpha: 90
beta: 90
gamma: 120
cell_volume: 189.778
crystal_density: 3.408
atoms_sites: ["Co", "Cl"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAOCcDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAAEAQAAAACAAAEAAAAAAAAYAAAAgACAAAAAAIYAAQAEAAAAAwAAEAAAAAARgAQAgAAAEAAwCAAAAIAAAAAACABAIAABIAgIAABABAAAAKAIEAAEAIAAAFgIEAAIAggAAQAAAAQ==


formula: Hg I
compound: Synthetic
pub_title: Redetermination of Hg2I2
formula_title: <missing>
a: 4.8974
b: 4.8974
c: 11.649
alpha: 90
beta: 90
gamma: 90
cell_volume: 279.396
crystal_density: 7.786
atoms_sites: ["Hg", "I"]
atoms_x: AAAAAAAAAAA=
atoms_y: AAAAAAAAAAA=
atoms_z: MMkGAGASFQA=
atoms_occupancy: 0
atoms_u_iso: 8JoBAHBDAQA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: QCwCAHCnAQA=
atoms_aniso_u22: QCwCAHCnAQA=
atoms_aniso_u33: 4HkAAHB7AAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAgAAAAQAAAAAAQAAAIQgAAAAABAAAIgCBAAAAhBAAAAEBAQBCECBCoAgAAAECogAiACAEEICJCAVAhCAKCkAQQIAEAIIhMDEABFgAICAiICSAwCIFKQFIQJESAUhIADUEgQAAqQwSQUyAogEApJCA==


formula: Ta2 Fe O6
compound: Synthetic
pub_title: Hochtemperatursynthese und Kristallchemie der Oxotantalate Cr2+0.761Ta2.095O6 und FeTa2O6
formula_title: <missing>
a: 4.7595
b: 4.7595
c: 9.201
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.429
crystal_density: 8.186
atoms_sites: ["Ta", "Fe", "O1", "O2"]
atoms_x: AAAAAAAAAACg7hEA0BITAA==
atoms_y: AAAAAAAAAACg7hEA0BITAA==
atoms_z: wDAUAAAAAABQtRMAAAAAAA==
atoms_occupancy: 0
atoms_u_iso: AH0AAAB9AABgZwEAwFcBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAABABAAAAAAQAQAAAAEACAAAgEQAAUEAAAQQAAABAgQYBAIgICEgAQIwAkAIQQGQYEIQgBDsIOgAQmI4A0AFTBAwIIqIdHESAIkhDRiJkhGgNmIMmJ4BjCWUJojREsITkMIkgAUimJaRcRSBYS==


formula: Ta2.033 Cr.755 O6
compound: Synthetic
pub_title: Hochtemperatursynthese und Kristallchemie der Oxotantalate Cr2+0.761Ta2.095O6 und FeTa2O6
formula_title: Cr0.761Ta2.095O6
a: 4.7476
b: 4.750
c: 10.405
alpha: 90
beta: 117.152
gamma: 90
cell_volume: 208.786
crystal_density: 8.003
atoms_sites: ["Ta1", "Cr2", "Ta2", "O1", "O2", "O3"]
atoms_x: YEAUAAAAAAAAAAAAoKglACBjOwDgvBIA
atoms_y: cAc9AAAAAAAAAAAAYAESAIBzDADA6xIA
atoms_z: YEAUAAAAAAAAAAAAwOUTAEDdCgCgDwAA
atoms_occupancy: wJA2AOAULgAg9A4AAAk9AAAJPQAACT0A
atoms_u_iso: 4KsAAEAZAQBAGQEAQBkBAEAZAQAgywAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAACAQAAAAEAEAAAQUQAAEKAAAYiAAABCAAQEAIxAAiqAIKgAkAAQgSRwQEgQhGmQaFCAqAUDUAxdEEwEJBoU+KcAMEaFUCNgBMgIUQsLhSDvkIRFPmNI0CDKY8iiAyi6cqEJzZIpJ==


formula: Ge Al2 O6 H2
compound: Synthetic
pub_title: Crystal structure of dialuminium dihydroxogermanate, Al2GeO4(OH)2
formula_title: <missing>
a: 9.107
b: 8.551
c: 4.804
alpha: 90
beta: 90
gamma: 90
cell_volume: 374.106
crystal_density: 3.987
atoms_sites: ["Ge", "Al", "O1", "O2", "O3", "O-H4"]
atoms_x: +D38/wAbCABQvQEAEBgPAFCw//9AKQ8A
atoms_y: QEIPAIDVBABAQg8AQEIPAMA/BQCgEAQA
atoms_z: MK0YAJBX+v+AQO//gMIDANAEDQCQz+b/
atoms_occupancy: 0
atoms_u_iso: IDwDAMBRAgDAUQIAwFECAMBRAgDAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAgGggEAAACACiAAAAAhACKQQiCEohIYARiEgZACEDJEq+UgsrCYcwh8lWChyGKrYT43cc89GH5jq2qjl23WXU5Wn+Z+1vuu+b73Xf1buV//2/77+e/9/y+fuXfb2c9e19tr372ffvZ7zytv9==


formula: B O2 H
compound: Synthetic
pub_title: The monoclinic and cubic phases of metaboric acid (precise redeterminations)
formula_title: <missing>
a: 8.8811
b: 8.8811
c: 8.8811
alpha: 90
beta: 90
gamma: 90
cell_volume: 700.487
crystal_density: 2.493
atoms_sites: ["B", "O1", "O2", "H"]
atoms_x: SMgrAAgvMgBY1jAAMJw4AA==
atoms_y: SFkxACCEOAAgwSgAgHE2AA==
atoms_z: sHcjAIhfJwAAaSMAsO8oAA==
atoms_occupancy: 0
atoms_u_iso: ABJ6AAASegAAEnoA4CICAA==
atoms_aniso_label: ["B", "O1", "O2"]
atoms_aniso_u11: yEEAAHA6AADgVgAA
atoms_aniso_u22: +D4AABgzAAAANwAA
atoms_aniso_u33: CD4AAKBaAAB4NwAA
atoms_aniso_u12: 8AAAAIgEAADwDwAA
atoms_aniso_u13: cAMAALjy///gBgAA
atoms_aniso_u23: 2P///7Dw//84BAAA
qdat:
AAAAAAAAAAAAAAAACAAAAAACAAIABAAAAIAAAIAABAEAQAAQCAgACAgIABAgQAAEEACACCBCCAEEEAQQgCEIAhCAQBEARAIhAJCAiEhEQEREiICJECIESBEgREkSAJEkgSQBIElIkEkkkEkBIJKAQCQkhBCiAISQIAUIQF==


formula: Na2 Ca S2 O8
compound: Chinchon (Madrid), Spain
pub_title: The crystal structure of glauberite, CaNa2(SO4)2
formula_title: <missing>
a: 10.158
b: 8.333
c: 8.551
alpha: 90
beta: 112.333
gamma: 90
cell_volume: 669.521
crystal_density: 2.760
atoms_sites: ["Na", "Ca", "S", "O1", "O2", "O3", "O4"]
atoms_x: 0BkWAAAAAACQPhMAIOAJADCTFACwdBcAUNUWAA==
atoms_y: YFsDAADoAwCgcREA8L0QALCfFAAQ9wcAoCgZAA==
atoms_z: 0KQDAEBCDwBgFBMAcLEQADCjCQDAPRYAMOwaAA==
atoms_occupancy: 0
atoms_u_iso: gEIBAOhsAADobAAAIFMAAABfAABokgAAUKAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAABAAAAAIBAQEAIAAAACBCEAAYCAJACABiACIUggAwBwXFAAURjghYAMDeOiGIEYSmvVgalyKEaQIx7Kw05BxJdUYo1cx35EttFbpB5u6/bPcS8T/3c/mb0fda/LL5bu8Ze8QqD/5xpS+pZmwfFm/H7x==


formula: Pb Fe1.98 Zn.75 Cu.27 Al.09 S2 O14 H6
compound: Mikawa mine, Niigata Prefecture, Japan
formula_title: <missing>
a: 7.3028
b: 7.3028
c: 17.0517
alpha: 90
beta: 90
gamma: 120
cell_volume: 787.548
crystal_density: 4.305
atoms_sites: ["Pb", "FeM", "ZnM", "CuM", "AlM", "S", "O1", "O2", "O-H"]
atoms_x: AAAAAICEHgCAhB4AgIQeAICEHgAAAAAAAAAAAHB4DQDA+wcA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAJCH8v9ABPj/
atoms_z: AAAAAICEHgCAhB4AgIQeAICEHgCQJRMAYNcYADAK/f9w5wcA
atoms_occupancy: AAk9AIBIKABAQg8AQH4FAMDUAQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: OCACAKAjAACgIwAAoCMAAKAjAABgFgIAYDsAAGA7AAAwAQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Study of Zn-bearing beaverite Pb(Fe2Zn)(SO4)2(OH)6
 obtained from Mikawa mine, Niigata Prefecture, Japan

qdat:
AAAAAAAAAAAAAAAAACEACAAAAAAACCAAAChIBAAAAQAAQUiAACQBAkIIAIAQopICEBEYQBCAE0IFQIkiAAEioCoJsAIgJrBIISAIFmIqEoggCVCIhCCA1IkUkBAKChJIAVIWCgRCuBIoAK0aVgkPhyaCFOQQRAknCkAWgp==


formula: Cu3 V2 O11 H6
compound: <missing>
pub_title: Crystal structure of volborthite Cu3(OH)2V2O7*2H2O
formula_title: <missing>
a: 10.60
b: 5.86
c: 7.21
alpha: 90
beta: 95.08
gamma: 90
cell_volume: 446.097
crystal_density: 3.533
atoms_sites: ["Cu1", "Cu2", "V", "O1", "O2", "O3", "O-H", "Wat"]
atoms_x: AAAAAEBCDwAARh4AAAAAAKDxBACgDhUAQGYJAADECQA=
atoms_y: AAAAAEBCDwAAAAAAgIQeAEBCDwAAAAAAAAAAAAAAAAA=
atoms_z: AAAAAAAAAAAAoA8AgIQeAEDdCgAgGAkAAMIzAEB3GwA=
atoms_occupancy: 0
atoms_u_iso: CBUBAAgVAQAIFQEACBUBAAgVAQAIFQEACBUBAAgVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAEAAAABEAAAACAAAQAAAACCKACCBAAGgAQgASAYCIEBOBIEAaeSAAAAEoUWjoYJFYAKMTgjBQp+gJC6I09mUIw4OE0Bc/VWSgYTd4JDuN7JiMqWWssK8moe2+VFzNr6ZotyI9yPtWXt2+lqtkuTOx9enR==


formula: La.67 Nb2 O6
compound: Synthetic
formula_title: La.67Nb2O6
a: 3.9105
b: 3.9197
c: 7.9142
alpha: 90
beta: 90
gamma: 90
cell_volume: 121.309
crystal_density: 5.132
atoms_sites: ["La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAICEHgCAhB4AgIQeAICEHgAAAAAA
atoms_y: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4A
atoms_z: AAAAAKD6DwAAAAAAgIQeAOBLEABgnA0A
atoms_occupancy: wOQoAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: La2/3-x Na3x Nb2O6 synthesized at 1350 deg C
 Note: x = 0

qdat:
AAAAAAAAAAAAAQAAAAAAAAAAAAHAABAAAAAAADACgAAAAAQBAAAAAkBwAAALAYAAAsWAAAALAAAaRAAJYUABO+AAmUAAKMAD0IALkAABYBB+gS4wFsoAk4GuUG2AB/wAGAXILbct/SFuAayX1Q+AAcKfGuDfqiqD7wfrP0==


formula: (La.52 Na.48) Nb2 O6
compound: Synthetic
formula_title: La.5Na.5Nb2O6
a: 3.921
b: 3.923
c: 7.8651
alpha: 90
beta: 90
gamma: 90
cell_volume: 120.982
crystal_density: 5.011
atoms_sites: ["La", "Na", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAACAhB4AgIQeAICEHgCAhB4AAAAAAA==
atoms_y: AAAAAAAAAACAhB4AgIQeAICEHgAAAAAAgIQeAA==
atoms_z: AAAAAAAAAACwiw8AAAAAAICEHgBgEw8AIPQOAA==
atoms_occupancy: AL0fAABMHQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: La2/3-x Na3x Nb2O6 synthesized at 1350 deg C
 Note: x = .16

qdat:
AAAAAAAAAAAAAIAAAAAAAAAAAACAABAAAAAAADAAgAAAAAQAgAAAAMAgAAAGAQAAAIGAAAADAAAMGAABwQAAcMAAMMAAIcAAYwADCAAAQAFGABzgA4gAYwAZwAZAAzAACADYAfwBzALIADgGYAyAAQBkAbAOQDkA/ANgNw==


formula: La.17 Na1.5 Nb2 O6
compound: Synthetic
formula_title: <missing>
a: 5.5189
b: 5.5458
c: 15.6313
alpha: 90
beta: 90
gamma: 90
cell_volume: 478.423
crystal_density: 4.719
atoms_sites: ["La1", "Na1", "Na2", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: gFsQAIBbEABAQg8AoDIPAIAqLQAANQwAgA0dAGDqAAA=
atoms_y: QEIPAEBCDwCguw0AoHgtAEBCDwAgnzEAICMcAKCMAAA=
atoms_z: AAAAAAAAAABAQg8A4JoHAAAAAABAQg8AIBgJAMAzBwA=
atoms_occupancy: QGAKAICEHgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: La2/3-x Na3x Nb2O6 synthesized at 1350 deg C
 Note: x = .5, La.17Na1.5Nb2O6

qdat:
AAAAAAAAAAAAAIAAAAAgAAAQAABCAAgABEAAABoAwAJAMANAIA0AAEgYBwMD4UAwAGggeGAQwaAFzhU4eELAH3DzihBwDjHnPyNAsxrj9SAdjpeo4Pr/6+8Hzf3AULt/Lzw+Vv9+f//2bF0b8pPT2f6//9/7++yfr37//f==


formula: La.09 Na1.74 Nb2 O6
compound: Synthetic
formula_title: <missing>
a: 5.5100
b: 5.5563
c: 15.5670
alpha: 90
beta: 90
gamma: 90
cell_volume: 476.587
crystal_density: 4.659
atoms_sites: ["La1", "Na1", "Na2", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: wP0PAMD9DwBgHw0AwIAPAMBVKwBAQg8AgJAcACDLAAA=
atoms_y: QEIPAEBCDwCA6g0AIDotAEBCDwBA/y4AwLsaAKAPAAA=
atoms_z: AAAAAAAAAABAQg8AAJ4HAAAAAABAQg8AwKQJACAkBwA=
atoms_occupancy: QH4FAIAqLQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: La2/3-x Na3x Nb2O6 synthesized at 1350 deg C
 Note: x = .58, La.09Na1.74Nb2O6

qdat:
AAAAAAAAAAAAAEAAAAAgAAAIAABCAAgAAkAAACoAoAagOANgEA0AAFwUAwOC4UA4AHQofHgooVgL86tcrENgH8hyThRYCUnn7xdhenV9RzArp5do0br147rN59ugzL3Ppn1mGvt+3//rZIsf/Q9vse5O/fO23d2/+ff9vS==


formula: Na Nb O3
compound: Synthetic
formula_title: <missing>
a: 5.5007
b: 5.5621
c: 15.5373
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.371
crystal_density: 4.580
atoms_sites: ["Na1", "Na2", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: IPoNACD6DQCwcg8AwGEpACAADQAgHR0A4CICAA==
atoms_y: QEIPAKA+DQAA0ywAQEIPAEB8LwCgZxsAwFcBAA==
atoms_z: AAAAAEBCDwCwogcAAAAAAEBCDwBgNwkAoOUGAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: La2/3-x Na3x Nb2O6 synthesized at 1350 deg C
 Note: x = .66, Na2Nb2O6

qdat:
AAAAAAAAAAAAAEAAAAAgAAAIAABiAAgAAkAAACwAsAWgOALgEAsAAFwUAQGC8SA8AFoYWmgskVgK0anWrkVgK8xcLRpcCcn1648yanLtZzg7lobku617+vZ5997xoz/Kw27lH7nr3/v9t4mqbocv8b/V9+/tj/a6/2//Xr==


formula: Nd.67 Nb2 O6
compound: Synthetic
formula_title: Nd.67Nb2O6
a: 3.8809
b: 3.9049
c: 7.8380
alpha: 90
beta: 90
gamma: 90
cell_volume: 118.781
crystal_density: 5.291
atoms_sites: ["Nd", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAICEHgCAhB4AgIQeAICEHgAAAAAA
atoms_y: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4A
atoms_z: AAAAANDyDwAAAAAAgIQeAIDkDgCAZw4A
atoms_occupancy: wOQoAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: Nd2/3-x Na3x Nb2O6 synthesized at 1330 deg C
 Note: x = 0

qdat:
AAAAAAAAAAAAAIAAAAAAAAAAAADgAAwAAAAAABgAoAAAAAEAYAAAAGgKAAAB4GAAAChoAAAA4AACxIAAekgAFboACpoAAlQAH5gAewAAFgBJpAXYgF9QCzQD1oD+AD8gARAXQDfsO9Qs1ANQ/5H+AB+EzBeA/2PZB/Ufy9==


formula: (Nd.52 Na.48) Nb2 O6
compound: Synthetic
formula_title: Nd.5Na.5Nb2O6
a: 3.8972
b: 3.9086
c: 7.8057
alpha: 90
beta: 90
gamma: 90
cell_volume: 118.901
crystal_density: 5.137
atoms_sites: ["Nd", "Na", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAACAhB4AgIQeAICEHgCAhB4AAAAAAA==
atoms_y: AAAAAAAAAACAhB4AgIQeAICEHgAAAAAAgIQeAA==
atoms_z: AAAAAAAAAABAjQ8AAAAAAICEHgDg1A4AQMUOAA==
atoms_occupancy: AL0fAABMHQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: Nd2/3-x Na3x Nb2O6 synthesized at 1330 deg C
 Note: x = .16

qdat:
AAAAAAAAAAAAAEAAAAAAAAAAAABAAAgAAAAAAAgAQAAAAAEAIAAAAGAYAAAAgEAAADAwAAAAYAABggAAOGAABhgABhwAAhgADCAAMIAADAAc4AHOADnABnABzABzABGAAUAMQA7gD+AVwAHAO4D2ABwD8A6AfwDUB+Avgf==


formula: Nd.09 Na1.74 Nb2 O6
compound: Synthetic
formula_title: <missing>
a: 5.5100
b: 5.5563
c: 15.5670
alpha: 90
beta: 90
gamma: 90
cell_volume: 476.587
crystal_density: 4.666
atoms_sites: ["Nd1", "Na1", "Na2", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: 4FEPAOBRDwBAyw0A4FEPAKATKQAgfQ0AQHEcACDFAQA=
atoms_y: QEIPAEBCDwDAjA0A0AwtAEBCDwBg0C4AwDgbAIA4AQA=
atoms_z: AAAAAAAAAABAQg8AAJ4HAAAAAABAQg8AoFYJACAkBwA=
atoms_occupancy: QH4FAIAqLQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: Nb2/3-x Na3x Nb2O6 synthesized at 1330 deg C
 Note: x = .58, Nd.09Na1.74Nb2O6

qdat:
AAAAAAAAAAAAAEAAAAAgAAAIAABCAAgAAkAAACoAoAagOANgEA0AAFwUAwOC4UA4AHQofHgooVgL86tcrENgH8hyThRYCUnn7xdhenV9RzArp5do0br147rN59ugzL3Ppn1mGvt+3//rZIsf/Q9vse5O/fO23d2/+ff9vS==


formula: Nd.05 Na1.86 Nb2 O6
compound: Synthetic
formula_title: <missing>
a: 5.5018
b: 5.5598
c: 15.5510
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.688
crystal_density: 4.633
atoms_sites: ["Nd1", "Na1", "Na2", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: YJYOAGCWDgBgnA0AgGEPAGBxKQAArA0AAM8cAAD0AQA=
atoms_y: QEIPAEBCDwDAjA0AcOosAEBCDwDgDi8AwLsaAKAJAQA=
atoms_z: AAAAAAAAAABAQg8AMJYHAAAAAABAQg8A0IAJAOAEBwA=
atoms_occupancy: QA0DAIB9NAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural and dielectric properties of solid solutions of
 sodium niobate in lanthanum and neodymium niobates
 Note: Nb2/3-x Na3x Nb2O6 synthesized at 1330 deg C
 Note: x = .62, Nd.05Na1.86Nb2O6

qdat:
AAAAAAAAAAAAAEAAAAAgAAAIAABiAAgAAkAAACoAoAWgOALgEAsAAFwUAQGC8SA8AHwoXGgYkVgK0anWrkVgG8x8bRpcCcl165dRanPtZjA7po7ku797+vZt89/xZz/K42zlF7Xbv/v1t42baoct+b/d9fvuh+67/e//17==


formula: Na Nb O3
compound: Synthetic
formula_title: <missing>
a: 5.566
b: 15.520
c: 5.506
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.632
crystal_density: 4.578
atoms_sites: ["Na1", "Na2", "Nb1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAMC6LwAgnRAAQEIPAKA4DgAA9AEA4IAcAA==
atoms_y: AAAAAEBCDwDgswcAAAAAAEBCDwCAiwgAwLYGAA==
atoms_z: 4NQOAGCWDgBgqQ8AAI4SAGCoCwAAtyAAwPU6AA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Na1", "Na2", "Nb1", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: SFsCAPDSAACQMwAACBsAAAgWAACwEwAAIOQAAA==
atoms_aniso_u22: IFcBAHCFAABATAAAMDkAAEBMAACAmAAAcIUAAA==
atoms_aniso_u33: mJkAANCsAAAoNwAAmNUAAJiZAAA4TwAAICsAAA==
atoms_aniso_u12: yN3//wAAAACI6///iOv//wAAAABYGwAAsDYAAA==
atoms_aniso_u13: AAAAAODA//8o+///AAAAABAdAAAIEQAAuBoAAA==
atoms_aniso_u23: AAAAAAAAAABo8v//AAAAAAAAAAC4BgAAmA0AAA==
pub_title:
 The structure of sodium niobate at room temperature,
 and the problem of reliability in pseudosymmetric structures

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAAAiAAgABkAAACyAsAGgOALgEAtAAE4cFQmAsiFcAJoUnOwsmUwK0M/W/oXgPcz09hpcCcu7zxVy6XP9ZrBzt45p/fbburS793+xxzXfx9TnPLu7vff75xsqbw190z+n/9u/H9zzuvf/v1==


formula: Nb Na O3
compound: Synthetic
formula_title: <missing>
a: 5.571
b: 7.766
c: 5.513
alpha: 90
beta: 90
gamma: 90
cell_volume: 238.517
crystal_density: 4.564
atoms_sites: ["Nb", "Na", "Na", "O1", "O2", "O3", "O4"]
atoms_x: kAUQAEDYDwCwyhEAELQOAJDGDQCwzAAAYAL9/w==
atoms_y: QEIPAAAAAACAhB4AAAAAAICEHgBgBxEA0GgNAA==
atoms_z: IA0PABCpLQBwuCwAQBETAIDECwCALSAAgDICAA==
atoms_occupancy: 0
atoms_u_iso: QB8AACBOAAAAXgEA0FIAANA5AACAHwEAUF8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The polar phase of NaNbO3: a combined study by powder diffraction,
 solid-state NMR and first-principles calculations
 Note: this is a polymorph of lueshite

qdat:
AAAAAAAAAAAAAEAAAABAAAAYAAAgAAgABgAAACgAsAIAWAMAEAwAAEgUIQuBQkEgAJgkmLgAsYARoYufKoRwVZhlc5QYEUut7jaimvKsRjBDO1/7lSpX9Wijr7/1+mf3E2qMvfd6/+f2xI3f7u7bsz6xzd/3V+/5a67u//==


formula: Nb Na O3
compound: Synthetic
formula_title: <missing>
a: 5.5679
b: 15.5156
c: 5.5029
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.392
crystal_density: 4.580
atoms_sites: ["Nb1", "Na1", "Na2", "O1", "O2", "O3", "O4"]
atoms_x: kIIQAMDGLQAgqy8AQEIPAAApDgCghgEAANUbAA==
atoms_y: cIMHAAAAAABAQg8AAAAAAEBCDwAgmwgAIKcGAA==
atoms_z: YBMPAKCvDwDAgA8AAI4SAID8CgAgiCAAgM39/w==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Nb1", "Na1", "Na2", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: OE8AANDFAADQxQAAgO0AAIDtAADAdgAAwHYAAA==
atoms_aniso_u22: mIoAALg8AQC4PAEAILIAACCyAACA7QAAgO0AAA==
atoms_aniso_u33: OE8AAPjFAAD4xQAAgO0AAIDtAADAdgAAwHYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 Neutron powder profile refinement of ferroelectric and
 antiferroelectric crystal structures: sodium niobate at 22 deg C

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAAAiAAgABkAAACyAsAGgPALgEAtAAE4cJYmAsiFcAJoUmuwsmUwM0N/V9oVgPcz8tRpcEcu7TR1S6nP9dzBzl45l/vXz+tRr93+xpzffw9THPTu7vfv7VwtKbo1707u338+7H2zTev/7vz==


formula: Na Nb O3
compound: Synthetic
formula_title: <missing>
a: 5.5625
b: 15.5495
c: 5.5138
alpha: 90
beta: 90
gamma: 90
cell_volume: 476.911
crystal_density: 4.565
atoms_sites: ["Na1", "Na2", "Nb1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAGBZLQDwww8AQEIPACCpDgDwJAQA8AUeAA==
atoms_y: AAAAAEBCDwDAsAcAAAAAAEBCDwDQhggA4LkGAA==
atoms_z: QEgOAACmDgDgBg8AYPsSABAXCwCwOCEAEEb//w==
atoms_occupancy: 0
atoms_u_iso: 0OgAANDoAACAPgAA0GsAANBrAADQawAA0GsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A new series of oxygen-deficient perovskites in the NaTixNb1-xO3-.05x
 system: synthesis, crystal chemistry, and energetics
 Note: x = 0.00

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAAAmAAgABkAAAC0AoAKgOAOgEA2AAFwUFwsB4UE8ALwonPg4sVgL8YtcvIXgL9j1VhRYE0+7PjXislP9RuA3vxbJ8+7v47Sb5//hSTmfRvllvPPvv/72zJ8v2h7N82rd+7c/n/r9c67v+1==


formula: Na (Nb.95 Ti.05) O2.975
compound: Synthetic
formula_title: <missing>
a: 5.5528
b: 15.5597
c: 5.5140
alpha: 90
beta: 90
gamma: 90
cell_volume: 476.409
crystal_density: 4.496
atoms_sites: ["Na1", "Na2", "Nb1", "Ti1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAMBJLQBg2w8AYNsPAEBCDwDQKg8AMEQEAEAzHgA=
atoms_y: AAAAAEBCDwCwuwcAsLsHAAAAAABAQg8AMHcIACCnBgA=
atoms_z: wAkOAAAjDwBwvQ4AcL0OAAD4EQBA9goAECkhAADt/v8=
atoms_occupancy: AAk9AAAJPQDA+zkAQA0DABAEPAAACT0AEAQ8AAAJPQA=
atoms_u_iso: 0AEBANABAQBQRgAAUEYAANBrAADQawAA0GsAANBrAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A new series of oxygen-deficient perovskites in the NaTixNb1-xO3-.05x
 system: synthesis, crystal chemistry, and energetics
 Note: x = 0.05

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAAAiAAgABkAAACsAoAJgOANgEA2AAFwUEwUA4UC8AHQoXHgYsXgH6Y88rELgH9hzShx4CSv3HyvheXP7ZbA/r5bo8a338rqP5/rgyLnbp1om+nlf/v/r5I8V+x1v8+5u/+e23drbWfff/W==


formula: Na (Nb.9 Ti.1) O2.95
compound: Synthetic
formula_title: <missing>
a: 5.5428
b: 15.5632
c: 5.5094
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.261
crystal_density: 4.433
atoms_sites: ["Na1", "Na2", "Nb1", "Ti1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAECILQBA8Q8AQPEPAEBCDwDQdQ8AQLwDAJAuHgA=
atoms_y: AAAAAEBCDwDQpQcA0KUHAAAAAABAQg8AUGEIABCABgA=
atoms_z: gOQOAACgDwBglg4AYJYOAADMEADwlgoAEPcgAGCS/v8=
atoms_occupancy: AAk9AAAJPQCA7jYAgBoGALAAOwAACT0AsAA7AAAJPQA=
atoms_u_iso: oHMAAKBzAABwSQAAcEkAACBnAAAgZwAAIGcAACBnAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A new series of oxygen-deficient perovskites in the NaTixNb1-xO3-.05x
 system: synthesis, crystal chemistry, and energetics
 Note: x = 0.1

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAAAiAAgABkAAABsAYAFgOANgEAaAADwMC4OA8MB8AFwYXHgYYPgD5YacXkHgFahxxgw4BSnnj5XguVm59vAWq0tUeP9f+d3H5//wbF1vk20TXy2/v3/l7ivO7U252e8/3fP77d8m5rfv//==


formula: Na (Nb.85 Ti.15) O2.925
compound: Synthetic
formula_title: <missing>
a: 5.5396
b: 15.5705
c: 5.5087
alpha: 90
beta: 90
gamma: 90
cell_volume: 475.149
crystal_density: 4.360
atoms_sites: ["Na1", "Na2", "Nb1", "Ti1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAABpLQCg4Q8AoOEPAEBCDwBgXg8AoHoDAFD2HQA=
atoms_y: AAAAAEBCDwBApAcAQKQHAAAAAABAQg8AoFwIAACLBgA=
atoms_z: wIYOAMCADwAQgg4AEIIOAABoEACwdwoAgNwgAOCF/v8=
atoms_occupancy: AAk9AAAJPQBA4TMAwCcJAMD7OQAACT0AwPs5AAAJPQA=
atoms_u_iso: oIwAAKCMAADgLgAA4C4AAKBzAACgcwAAoHMAAKBzAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A new series of oxygen-deficient perovskites in the NaTixNb1-xO3-.05x
 system: synthesis, crystal chemistry, and energetics
 Note: x = 0.15

qdat:
AAAAAAAAAAAAAEAAAABAgAAYAABCAAgABkAAABsAYAFgOANgEAaAADwMC4OA8MB4ADwYPDgYYPgD5YacPkHgDah5xgwoBSn3j5XguVn59rgep0vUeL9X6d/D5v/wJF1/kt8bPzf/r3/1/jvG7MS5ee832vNu3P8l9vf/+/==


formula: Na (Nb.8 Ti.2) O2.9
compound: Synthetic
formula_title: <missing>
a: 5.5303
b: 15.5677
c: 5.5072
alpha: 90
beta: 90
gamma: 90
cell_volume: 474.137
crystal_density: 4.295
atoms_sites: ["Na1", "Na2", "Nb1", "Ti1", "O1", "O2", "O3", "O4"]
atoms_x: wMYtAKB4LQCg4Q8AoOEPAEBCDwBAWw8AMGMDAKDYHQA=
atoms_y: AAAAAEBCDwAQrAcAEKwHAAAAAABAQg8AYFYIANCSBgA=
atoms_z: QMUOAACgDwCgnA4AoJwOAJBQEADAhQoA4OUgACBz/v8=
atoms_occupancy: AAk9AAAJPQAA1DAAADUMAND2OAAACT0A0PY4AAAJPQA=
atoms_u_iso: wNoAAMDaAACgWgAAoFoAAPCHAADwhwAA8IcAAPCHAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A new series of oxygen-deficient perovskites in the NaTixNb1-xO3-.05x
 system: synthesis, crystal chemistry, and energetics
 Note: x = 0.2

qdat:
AAAAAAAAAAAAAEAAAAAgQAAYAABCAAgABkAAABmAYAFgGAEgEAaAADQMB4OA8KBcADwYPDgMYFgC44OcPiDgB5w5wwwYBZjzh1HgOMu47ngOYynqODrP+7vB8m9wNC3fy08Pn7bfj79tfw2TfqT4/Xen7v02dOuT579e/d==


formula: Cu Ni Sb2
compound: Zlatoja Hora (Gold Hill) deposit, Middle Urals, Russia
pub_title: Crystal structure of a new mineral CuNiSb2
formula_title: <missing>
a: 4.0510
b: 4.051
c: 5.1382
alpha: 90
beta: 90
gamma: 120
cell_volume: 73.024
crystal_density: 8.317
atoms_sites: ["Cu", "Ni", "Sb"]
atoms_x: AAAAAAAAAABVWBQA
atoms_y: AAAAAAAAAACrsCgA
atoms_z: AAAAAICEHgBwfxAA
atoms_occupancy: 0
atoms_u_iso: 6GIAAOhiAABgOwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAIAAAAAAAABAAAAAAQAAABAAAAAAAAAECAAAEAAACAQAQABAAgAAAIAAAAAAggEAAAEBABEABAAAAEAIBAhAIAIQCIEAQAEIQAAQIQQIBABQABAgCCAQipAIAAACCEWAAQRCGAECgIggQYIBwAR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim1_q0, untreated
formula_title: <missing>
a: 4.7533
b: 4.7533
c: 9.2876
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.843
crystal_density: 7.950
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABgfhIA8GYSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABgfhIA8GYSAA==
atoms_z: AAAAAAAAAABYUhQAWFIUAFhSFAAAAAAAgEMUAA==
atoms_occupancy: gJwaAIBsIgBANhEAINsnAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIoEAJiACFAAQVAAkAESAkihAJAQCRsgmQEQ4E4KkBhYIRAISSgtMkYAoC0ZwI5CSSgl5IYVC0EzRwLQ9NYh0EF0WZEgBGmUmxY7C8CwS==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim5_q0, untreated
formula_title: <missing>
a: 4.7533
b: 4.7533
c: 9.2773
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.610
crystal_density: 7.958
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACQjxIAEDgSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACQjxIAEDgSAA==
atoms_z: AAAAAAAAAABoTBQAaEwUAGhMFAAAAAAAgCoUAA==
atoms_occupancy: gPsfAIANHQDAhg4AoIoqAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACFAAQMgAkAERAkiggJAQCJsgWQEQ0E4GUBh4IQgISSQtMkUAYC0ZQIZCSagl4oYXC0E7IoLI9FYQ0GFUVZEgBGiUmxY5C2BwR==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7554
b: 4.7554
c: 9.2281
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.683
crystal_density: 7.996
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACAzBIA8AISAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACAzBIA8AISAA==
atoms_z: AAAAAAAAAADoPxQA6D8UAOg/FAAAAAAA0NoTAA==
atoms_occupancy: YNwsAKAsEACADggA4AIxAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim5_q1, treated at 750 C for 30 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgIQAAMEAAAQgAAABBAIYCAIgQCEgAQJQAkAEQQEQwIIQQBBkIGQAwqEYBkAJWCBQEISINOMSAKCyDSCLEhGgJcIMVQ4BTEcKI4jKIsEhSMYlgAUiWNxaKh6AoR==


formula: Fe1.001 Ta1.869 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim9_q0, untreated
formula_title: <missing>
a: 4.7531
b: 4.7531
c: 9.2873
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.818
crystal_density: 7.949
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABAYhIAkF0SAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABAYhIAkF0SAA==
atoms_z: AAAAAAAAAAAgUxQAIFMUACBTFAAAAAAAADcUAA==
atoms_occupancy: 4IwaACB8IgDgRREAgMsnAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIoEAJiACFAAQVAAkAESAkihAJAQCRsgmQEQ4E4KUBhYIRAISSQtMkYAoC0ZwI5CSSgl5IYVC0EzRoLQ9NYh0EF0WZEgBGmUmxY7C0CwS==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7475
b: 4.7475
c: 9.2690
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.912
crystal_density: 7.987
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADQfBIAcEESAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADQfBIAcEESAA==
atoms_z: AAAAAAAAAAA4TxQAOE8UADhPFAAAAAAAkDgUAA==
atoms_occupancy: IB0dAODrHwAg7g8AQCMpAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim9_q1, treated at 700 C for 210 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAQQgAAMCAAAJAAAABCAIYEAIxACCgAIKgAkAEJASRQgEgQBImQWICIsCcCUAxsEIgEJJIUqSMAUBaNYENBJNgS8iMKhSCukYFkOmaIsCBOSslgAjiqUoeOjbAkJ==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7497
b: 4.7497
c: 9.2530
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.744
crystal_density: 7.993
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAQgxIAwDwSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAQgxIAwDwSAA==
atoms_z: AAAAAAAAAAAoSxQAKEsUAChLFAAAAAAAkB8UAA==
atoms_occupancy: oMwfAGA8HQBglg4AAHsqAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim9_q2, treated at 750 C for 120 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAQIQAAMCAAAQgAAABCAIYCAIxACCgAIKgAkAEIgSQwQEgQBFmQOQBQqEUDUAxcEEQEIxIU2KMAMCaFUCFCJNgM0UMKhSBukIFEfikIUDBKKcigASjaMosMhbAoJ==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7504
b: 4.7504
c: 9.2549
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.849
crystal_density: 7.987
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAgkRIAUD4SAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAgkRIAUD4SAA==
atoms_z: AAAAAAAAAABISRQASEkUAEhJFAAAAAAAkAYUAA==
atoms_occupancy: ALEhAABYGwAArA0AYGUrAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim9_q3, treated at 750 C for 180 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgQQAAMCAAAQgAAABCAIYEAIxACCgAIKgAkAEIgSQwQEgQBFmQOQBQqEUDUAxcEEgEJRIU2KMAMCaFUCFCRNgM0UMLhUCukIFEfmkIcCBaK8igAijaUosMhdAoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim14_q0, untreated
formula_title: <missing>
a: 4.7551
b: 4.7551
c: 9.2810
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.852
crystal_density: 7.949
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAQgxIAoFISAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAQgxIAoFISAA==
atoms_z: AAAAAAAAAACATRQAgE0UAIBNFAAAAAAA0CUUAA==
atoms_occupancy: QF8fAMCpHQDg1A4AgDwqAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIoEARiACFAAQVAAoAERAkihAJAQCRsgUQERYE4GkBhYIRAISSgpMkYAoC0awIaCiSApRIYXCoFyQwOQ5NYR4MF0WYFABFGZLhY6DcDQS==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7526
b: 4.7526
c: 9.2501
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.934
crystal_density: 7.984
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABgsBIAEB8SAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABgsBIAEB8SAA==
atoms_z: AAAAAAAAAADgQhQA4EIUAOBCFAAAAAAA8PYTAA==
atoms_occupancy: gDwqAIDMEgBAZgkAIKsvAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim14_q1, treated at 600 C for 20 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgIQAAMEAAAQgAAABCAIYCAIhACEgAQKgAkAEIgSgwQIgQBFkQOQBQsEUDUARUEEgEIyIdaMMAMCWFUEFCROgM0UMTh0C3EILIVnEIcFDaU5CgAmjaUpUNj2AoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim19_q0, untreated
formula_title: <missing>
a: 4.7561
b: 4.7561
c: 9.2748
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.801
crystal_density: 7.951
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACQqBIAsGASAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACQqBIAsGASAA==
atoms_z: AAAAAAAAAADwSxQA8EsUAPBLFAAAAAAAwBcUAA==
atoms_occupancy: AKsiAABeGgAALw0AYOIrAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAUEAAARAAAABEAIYEARhACFAAQUgAoAIRAkiggJAQCJsgUgERYE4GoBh4IRAISSQ5MkYAYE0awIaEiVApwoYWCoFyQwWQtFYQ4MG0VZFABFGYriY7DcDQS==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7516
b: 4.7516
c: 9.2258
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.297
crystal_density: 8.011
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABgsBIAEB8SAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABgsBIAEB8SAA==
atoms_z: AAAAAAAAAABAQhQAQEIUAEBCFAAAAAAAMOQTAA==
atoms_occupancy: oHgtAGCQDwBgwAcAAFExAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim19_q1, treated at 750 C for 40 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgIQAAMCAAAIgAAABBAIICAIgQCCgAIJQAUAEIQGQoIEQQBBmIGQAwmEUB0AIuCBQEIRIMuGKAGCTDSCHiRGgE0MMSw0BriMJEchmEUChaGMjgAKhSM4tNQtA4R==


formula: Fe1.001 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7531
b: 4.7531
c: 9.2219
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.341
crystal_density: 8.011
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACQwRIAEAYSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACQwRIAEAYSAA==
atoms_z: AAAAAAAAAADgPRQA4D0UAOA9FAAAAAAAsL4TAA==
atoms_occupancy: IKsvAOBdDQDAtgYAQGoyAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim19_q2, treated at 750 C for 80 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgIQAAMEAAAQgAAABBAIIBAIgQCEgAIIwAkAEIQGQoIEQQBBkIGQAwmEUA0AJWCBQEISINGEKAJCTDTCHiRGgE0MMTQ0BziMLE0hGEUCRSEMjgAWjSM5VNR1A4R==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim20_q0, untreated
formula_title: <missing>
a: 4.7561
b: 4.7561
c: 9.2880
alpha: 90
beta: 90
gamma: 90
cell_volume: 210.099
crystal_density: 7.940
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADQfBIAcFoSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADQfBIAcFoSAA==
atoms_z: AAAAAAAAAABQUBQAUFAUAFBQFAAAAAAAMC8UAA==
atoms_occupancy: QGsdAMCdHwDgzg8AgEIpAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAUEAAARAAAACEAIoIARiACFAAQVABIAISAkihAJAQERMgkgERoE4MoCjYIRAISShZUkYAoEkawIqEi1ApxIoWCoJ2RQWQpNYh4IK0qqNABFGZNiYqHcDgT==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7547
b: 4.7547
c: 9.2893
alpha: 90
beta: 90
gamma: 90
cell_volume: 210.005
crystal_density: 7.945
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACwYBIAsEcSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACwYBIAsEcSAA==
atoms_z: AAAAAAAAAADIUBQAyFAUAMhQFAAAAAAAsCIUAA==
atoms_occupancy: YDwdAKDMHwCA3g8A4DIpAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q1, treated at 600 C for 5 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAACEAIoIARiACFAAQVABIAESBEihAJAQERsgkQERoE4MoChYIRAISSgtUkYAoC0awIqCSzAlRIYVC0JyRQOQ9NYh4MF0mZNABFGZFhY6G8CwT==


formula: Fe1.001 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7516
b: 4.7516
c: 9.2856
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.647
crystal_density: 7.961
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAgXxIA4D8SAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAgXxIA4D8SAA==
atoms_z: AAAAAAAAAADAThQAwE4UAMBOFAAAAAAA0CUUAA==
atoms_occupancy: 4PcdACARHwBgkA8AoJApAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q2, treated at 600 C for 20 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACFAAQNAAkAEKAiihAJAQCRsgmQEQ0E4KUBhYIQgISSQtsiMAoC0ZQI1CSagl4kYVCUEzIoLIdE0R0EFcTZGgBGjUmw89C2DwR==


formula: Fe1.001 Ta1.869 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7509
b: 4.7509
c: 9.2811
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.484
crystal_density: 7.961
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADgWBIAQEkSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADgWBIAQEkSAA==
atoms_z: AAAAAAAAAADAThQAwE4UAMBOFAAAAAAAECwUAA==
atoms_occupancy: 4HodACCOHwDgzg8AgEIpAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q3, treated at 600 C for 50 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACCgAQMgAkAEJAiihAJAQCRqgWQEQ0E0GUBhUIQgISRQtqiMAoCyZQIVCRagl4kUTCUE7IoHIck0Q8EDcTJGgBGjUmw8dCWBoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7509
b: 4.7509
c: 9.2812
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.486
crystal_density: 7.963
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAgeBIAgDYSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAgeBIAgDYSAA==
atoms_z: AAAAAAAAAAD4TRQA+E0UAPhNFAAAAAAAYCcUAA==
atoms_occupancy: gIQeAICEHgBAQg8AIM8pAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q4, treated at 600 C for 200 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACCgAQMgAkAEJAiihAJAQCRqgWQEQ0E0GUBhUIQgISRQtqiMAoCyZQIVCRagl4kUTCUE7IoHIck0Q8EDcTJGgBGjUmw8dCWBoR==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7506
b: 4.7506
c: 9.2811
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.458
crystal_density: 7.966
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACghBIAwDwSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACghBIAwDwSAA==
atoms_z: AAAAAAAAAADQTRQA0E0UANBNFAAAAAAAICEUAA==
atoms_occupancy: 4HQeACCUHgBAQg8AIM8pAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q5, treated at 600 C for 650 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACCgAQMgAkAEJAiiRAJAQCRqgWQEQ0E0GUBhUIQgISRQtqiMAoC6VQIVCRagV4kUKiUE7IoHIck0Q8GDcTJGgBGjUmo8diWBoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7507
b: 4.7507
c: 9.2794
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.428
crystal_density: 7.965
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABgZRIAsEcSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABgZRIAsEcSAA==
atoms_z: AAAAAAAAAADQTRQA0E0UANBNFAAAAAAAoC0UAA==
atoms_occupancy: wKMeAEBlHgCgMg8AwN4pAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim20_q6, treated at 650 C for 15 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAEABAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIYEAJiACCgAQMgAkAEJAiiRAJAQCJqgWQEQ0E0GUBhUIQgISRQtqiMAoC6NQIVCRagV4kUSiUE7IoHIck0Q8GDcTJGgBGjUmo8dCWBoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim23_q0, untreated
formula_title: <missing>
a: 4.7551
b: 4.7551
c: 9.2818
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.871
crystal_density: 7.949
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADwZhIAkEQSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADwZhIAkEQSAA==
atoms_z: AAAAAAAAAAAITRQACE0UAAhNFAAAAAAAkAYUAA==
atoms_occupancy: QFkgAMCvHADgVw4AgLkqAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAMEAAARAAAABEAIoEARiACFAAQVABIAESAkihAJAQCRsgUQERYE4GoBhYIRAISSgpMkYAoC0awIaCiTApRIYXCoFyQwOQ5NYh4MF0WZFABFGZLhY6DcDQS==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7538
b: 4.7538
c: 9.2193
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.343
crystal_density: 8.007
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABgyRIA0P8RAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABgyRIA0P8RAA==
atoms_z: AAAAAAAAAAAwPhQAMD4UADA+FAAAAAAAgMYTAA==
atoms_occupancy: wLovAEBODQAgpwYAQGoyAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim23_q1, treated at 750 C for 130 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEACAAAgEQAAMEAAAQgAAABBAIIBAIgQCEgAQIwAkAEQQGQYIEQQBBkIGQAQmEUA0AJWCBQEISINGEKAJCTDTCHCRGgE0MMTI0BziMLE0hGEkERSEIjgAUjSM5VJR1A4R==


formula: Fe1.001 Ta1.869 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7571
b: 4.7571
c: 9.2189
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.624
crystal_density: 7.994
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADABBMAoO4RAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADABBMAoO4RAA==
atoms_z: AAAAAAAAAADYOxQA2DsUANg7FAAAAAAAYMMTAA==
atoms_occupancy: IJ8xAOBpCwDAvAUAoFQzAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim23_q2, treated at 750 C for 190 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgEQAAUEAAAQgAAABBAIIBAIgQCEgAQIwAkAIQQEQwIIQQBBkIEgAwqEYAkAJWCBQIISIZGESAJEiCTCLEhEgNUIMVRoBTEcSIoiKIsEjkIIlgAUiUJSaKhaBwR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
pub_title: Structural changes induced by cation ordering in ferrotapiolite Note: Crystal Kim24_q0, untreated
formula_title: <missing>
a: 4.7562
b: 4.7562
c: 9.2910
alpha: 90
beta: 90
gamma: 90
cell_volume: 210.176
crystal_density: 7.937
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACwkhIAEGoSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACwkhIAEGoSAA==
atoms_z: AAAAAAAAAABAURQAQFEUAEBRFAAAAAAAADcUAA==
atoms_occupancy: QPQbAMAUIQBgihAAAIcoAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAEACAAAAAAQAQAAAAEAIAAAgQgAAUEAAARAAAACEAIoIASiACFAAQVABIAISBEihAJAQERMgkgIRoE4MoDDYQRAIUShbUkYAoEkSgIqEi1ApxIwWEoJmRQWQqOYioIK0qqNABFG5NiZqHcHgT==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7499
b: 4.7499
c: 9.2716
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.182
crystal_density: 7.975
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACwkhIAcEESAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACwkhIAcEESAA==
atoms_z: AAAAAAAAAAAwTRQAME0UADBNFAAAAAAAgCoUAA==
atoms_occupancy: gAEfAIAHHgDAAw8AoA0qAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim24_q1, treated at 700 C for 30 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAQQgAAMCAAARAAAABCAIYEAJRACCgAIKgAkAEJAShQgIgQCJqQWQEQ0EUGUAh0IIgERRQUqSMAYCaNYEVCRZgU0kUKiSC7EYFIeksI8CDcTpGgAijSVoscjeAoR==


formula: Fe Ta1.87 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7511
b: 4.7511
c: 9.2648
alpha: 90
beta: 90
gamma: 90
cell_volume: 209.134
crystal_density: 7.977
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABwjBIA8DQSAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABwjBIA8DQSAA==
atoms_z: AAAAAAAAAAAASxQAAEsUAABLFAAAAAAAcBwUAA==
atoms_occupancy: QNYgAMAyHABgGQ4AAPgqAKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim24_q2, treated at 700 C for 120 min

qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAAAAAQAQAAAAEAEAAAgQgAAMEAAARAAAABCAIYEAJhACCgAQKgAkAEJAShQgIgQCFqQWQCQsEUCUAxUEIgERRIcqSMAICaNYENCRKgU0kUTiUC3EYHIemsI8GDcSpGgAmjaVosdjWAoR==


formula: Fe.999 Ta1.871 Nb.13 O6
compound: Kimito, Finland
formula_title: <missing>
a: 4.7561
b: 4.7561
c: 9.2030
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.176
crystal_density: 8.015
atoms_sites: ["Fe(A)", "Ta(A)", "Fe(B)", "Ta(B)", "Nb(B)", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADgBxMAcPYRAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADgBxMAcPYRAA==
atoms_z: AAAAAAAAAABgNhQAYDYUAGA2FAAAAAAAsKUTAA==
atoms_occupancy: oB48AGDqAABgbQAAAKQ4AKD3AwAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural changes induced by cation ordering in ferrotapiolite
 Note: Crystal Kim24_q3, treated at 700 C for 450 min

qdat:
AAAAAAAAAAAAAAAAAAAAAABABAAAAAAQAQAAAAEACAAAgEQAAUEAAAQQAAABAgIIBAIgICEgAQIoAUAIQQGQYEIQQBBkIGgAQmEUA0AFTBAwEIaEVDESAIkRDRhJkhCgNWIMTE4BxiTSI4hJEkELSEMkgAMjSNKZKR5A4R==


formula: Ba B As O5
compound: Synthetic
formula_title: Ba(BAsO)5
a: 7.2666
b: 7.2666
c: 7.1063
alpha: 90
beta: 90
gamma: 120
cell_volume: 324.965
crystal_density: 4.646
atoms_sites: ["Ba", "B", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_x: UMcQAFA8IwBQtCgAYHMxAGC+MQBQuB8AgLAfADClKgA=
atoms_y: YFkUAODtDgCQGfz/kGEJAKCd+f+gvgAA8LXw/0CIFAA=
atoms_z: QGAKAMDR9f9AUQAA0AMJACDV9v8Qdvf/kEgJAHD56/8=
atoms_occupancy: 0
atoms_u_iso: QJwAAMBdAACgjAAAwFcBAADuAgDAVwEAYGECAKCGAQA=
atoms_aniso_label: ["Ba", "B", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: wMEAAECcAABAnAAAgLUBAGDkAQDA2gAAwMgDAMDaAAA=
atoms_aniso_u22: YJ8AAOAuAACAuwAAQJYBAMDaAABAEwIAAHcBAEANAwA=
atoms_aniso_u33: IJkAAEAZAQDwhwAAQBkBAGBPBQDgKAEAAH0AAECWAQA=
atoms_aniso_u12: QGoAAIC7AABgbQAAQBkBAIA+AAAgywAAgD4AAOClAQA=
atoms_aniso_u13: 0CAAAMBdAABABgAAINf+/wD0AQDAY///gMH//2BtAAA=
atoms_aniso_u23: ABkAAIA+AABg8P//oJj+/yDR///A5v7/YPD//2BtAAA=
pub_title:
 Zur Synthese und Kristallstruktur von Bariumboroarsenat Ba(BAsO5) mit
 einem Beitrag uber Bariumorthoarsenat Ba3(AsO4)2

qdat:
AAAAAAAAAAAAAAAACAAAAAQAAAAABAAAIJAAIAAAAQAA0AEQAAgAhgAIACgEgJIACCHCQAAAHEkEQSIRBBEQUhEC4ogIDlUgIQFJBUqJWshQoRWQQiNI2aYsxMFGzTUJoklSfaqKfxLKdCSye/URva16WrHKWQb5a3NU1R==


formula: Ba3 As2 O8
compound: Synthetic
formula_title: Ba3(AsO4)2
a: 5.7672
b: 5.7672
c: 21.1630
alpha: 90
beta: 90
gamma: 120
cell_volume: 609.590
crystal_density: 5.637
atoms_sites: ["Ba1", "Ba2", "As", "O1", "O2"]
atoms_x: AAAAAAAAAABVWBQAEJoKAFVYFAA=
atoms_y: AAAAAAAAAACrsCgA8G4yAKuwKAA=
atoms_z: AAAAAECQDACIfQQAICoGAACc//8=
atoms_occupancy: 0
atoms_u_iso: IMsAAKCMAABgbQAAwFcBAMDUAQA=
atoms_aniso_label: ["Ba1", "Ba2", "As", "O1", "O2"]
atoms_aniso_u11: 0OgAABCLAACAcAAAYGcBAMBRAgA=
atoms_aniso_u22: 0OgAABCLAACAcAAAYGcBAMBRAgA=
atoms_aniso_u33: kH4AAHCUAADgeQAAIMUBAMDaAAA=
atoms_aniso_u12: oHMAALBFAABAOAAAAPoAAOAoAQA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Zur Synthese und Kristallstruktur von Bariumboroarsenat Ba(BAsO5) mit
 einem Beitrag uber Bariumorthoarsenat Ba3(AsO4)2

qdat:
AAAAAAAAAAAAAABAAAAAAEAQAAAABCAAEAAAIAAQEAQQFAJACAAAACICIGBACABADIAAQEAACAYBQgUEAAAQkYQEAAJEiECAQaACCAABAoiCAgoojCAAxTEIAGAQABDCgxAhQGQABDIiABAQAIxQpABMkIAgQAIwAgABki==


formula: Ce B Si O5
compound: Bassano Romano, Viterbo, Italy
pub_title: The refinement of the crystal structure of stillwellite: RE[BSiO5]
formula_title: <missing>
a: 6.844
b: 6.844
c: 6.700
alpha: 90
beta: 90
gamma: 120
cell_volume: 271.785
crystal_density: 4.747
atoms_sites: ["Ce", "B", "Si", "O1", "O2", "O3", "O4", "O5"]
atoms_x: UNIjAPASBwBwiiMAwI4VANCNCwDAeSUAIKYbAFCYAwA=
atoms_y: 4OP//4AfAQBg1///oBIMAOAaFAAAGh0AYHYkADB8AwA=
atoms_z: UNwyAMB8MQDgZRQAgH00APDtCABwqQkAQOcyANBuJQA=
atoms_occupancy: 0
atoms_u_iso: IJkAANCdAADAqAAAAJYAABDvAABAzgAA4N0AAODEAAA=
atoms_aniso_label: ["Ce", "B", "Si", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: wFgAAMBiAAAokQAAQBAAABhlAADIFAAAQH4AAECNAAA=
atoms_aniso_u22: 8EsAAEAaAADIXwAAcDUAAJCcAAAQgQAAyIcAAGBFAAA=
atoms_aniso_u33: AEYAAHBsAADoSQAAgHUAADhZAADAewAAAEsAAMhGAAA=
atoms_aniso_u12: 6DUAACAcAABgYwAA0Pj//5ApAACYCAAAmDUAACgeAAA=
atoms_aniso_u13: qP3//3gZAADAOgAAmPn//9D9//9Q7P//KOf//yjs//8=
atoms_aniso_u23: 4AEAAGgQAACgBQAA2Mj//4AHAACw////UPb///gHAAA=
qdat:
AAAAAAAAAAAAAAAAACAAAAACAAAAAACAAAIJAACAAAACAADQAIQAAgAIwACAAUASAiQACCDhIAAAAokQQgkQhCBEIKQhAWJEAgOaxAIwDIgWSiNlkKChEsghkNIrKqLMLAoyNNQRgkkyad1Dj2JZQ0JFo914Q9y58k645x==


formula: Nd B Si O5
compound: Synthetic
pub_title: Crystal structure and vibrational spectra studies of stillwellite compounds NdBSiO5
formula_title: <missing>
a: 6.8035
b: 6.8035
c: 6.6487
alpha: 90
beta: 90
gamma: 120
cell_volume: 266.521
crystal_density: 4.918
atoms_sites: ["Nd", "B", "Si", "O1", "O2", "O3"]
atoms_x: cGIZALA9NQCQfhkAQAsUADD/GwDA5v7/
atoms_y: AAAAAAAAAAAAAAAAMHcIAHDyMwDQwwIA
atoms_z: VVgUAFVYFADI3DIA0E47AEAGAACw5yEA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQCAhB4A
atoms_u_iso: kCkAAMgsAQBYQwAA2McAADgDAQCwfAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAABAAAAACAAAAAABAAAEEQABAAAAAgAAsAEEAAIACKAAQAFAEQEiAAQQUJAAAAGCiCEEiEIIIRBRCIC84QCA5ykAjAMSBUyEzTYUJGMyBCIWRaZMuYTAx0qVQjRJGSr9TGlaJRJoFGpW2UYmzemlmtZ==


formula: La B Si O5
compound: Synthetic
pub_title: Crystal structure of LaBSiO5
formula_title: <missing>
a: 6.874
b: 6.874
c: 6.717
alpha: 90
beta: 90
gamma: 120
cell_volume: 274.869
crystal_density: 4.672
atoms_sites: ["La", "B", "Si", "O1", "O2", "O3", "O4", "O5", "O5*"]
atoms_x: 2K4oANADIgCrsCgAANMTAECqHwBAPjEA4HwMAMDrKwAgwysA
atoms_y: sFQtAHBOFABwsi0AUJMIAFAcIAAgG/z/8JIsALCGFADgMxQA
atoms_z: gIQeAKBQCgBAUQAAoOALAGDsCAAwIAoAMLYKAODCEQAQ/AIA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AIBmIwCAohkA
atoms_u_iso: wE4AAIDtAAAoSwAA2HIAALB8AAAYsAAAKKoAAKh6AADAdgAA
atoms_aniso_label: ["La", "B", "Si", "O1", "O2", "O3", "O4", "O5", "O5'"]
atoms_aniso_u11: cDoAADBcAADwVQAA4GAAAPCHAABAzgAAoAkBAGBtAADgqwAA
atoms_aniso_u22: qEgAAPCHAABgOwAAcGIAAJBMAADQawAAsGgAAECcAACAuwAA
atoms_aniso_u33: OGMAAKADAgCAVwAAwHYAAPCgAAAAfQAA0IQAACBOAABAHwAA
atoms_aniso_u12: cBwAANBSAADAKwAAkBoAALA2AADAEgAAgFcAAOAuAABgbQAA
atoms_aniso_u13: mAMAAGBtAACwBAAAMN///7A2AADw8f//UPv//8Dg//+gDwAA
atoms_aniso_u23: SAMAACDLAAAgAwAAUBQAAPAKAACw6///UPv//6APAABAHwAA
qdat:
AAAAAAAAAAAAAAAAACAAAAAEAAAAAAEAAAQRAAEAAAACAAFgAQgABAAhgAEAAoBIBIgAEIOCgAAADhJBCCSCEEEQgpBICc4QEBZykBDAUkClUJmmwoSMpkCMQ1DVUx5hIFHSpaBaFIpU9sYW7SKJNBJlL/zGN0rZI5lecW==


formula: Ce B Si O5
compound: Soviet
pub_title: X-ray diffraction study of the atomic structure of stillwellite CeBO[SiO4]
formula_title: <missing>
a: 6.85
b: 6.85
c: 6.70
alpha: 90
beta: 90
gamma: 120
cell_volume: 272.262
crystal_density: 4.739
atoms_sites: ["Ce", "B", "Si", "O1", "O2", "O3", "O4", "O5"]
atoms_x: 4NMjAKDlBgCgtCMA4LAUAODmCwAgaiUAAFIcAOAcAwA=
atoms_y: AAAAAAAAAAAAAAAAQNcLAOCwFAAAUhwAwHklAOAcAwA=
atoms_z: AAAAACBjOwCAhB4AYGcBAMDrEgAAiBMAwNoAACCrLwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAACAAAAACAAAAAAEAAAIJAACAAAACAADQAIQAAgAQwACAAUASAkQACCDBIAAAAwkgQgkghCCEISQiAmKEBAOUxAQwFIgqUiZpsKEhFZAhkNItVKdMLAw2ZOQThJFSapmDn8RZRoJGxr2oxulzol05py==


formula: Ba Cu Si4 O10
compound: Synthetic
pub_title: Refinement of the structure of barium copper silicate BaCu[Si4O10] at 300 K
formula_title: <missing>
a: 7.447
b: 7.447
c: 16.138
alpha: 90
beta: 90
gamma: 90
cell_volume: 894.978
crystal_density: 3.512
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAQXRAA0MwNAADoHADwVwgA
atoms_y: AAAAAICEHgBwhAsA0MwNAEApDwAgMxEA
atoms_z: AAAAAADDBQCgbwkAQEIPAGBWCABA+wUA
atoms_occupancy: 0
atoms_u_iso: QJwAAFB4AAAQcgAAYOQBAAD6AABQ9QAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAgAAAAABAAACAAgAQAAgCAAAAAIhABACEgIEkAAEgAAiQCAyAghURpABsADShIoAUCCUCEwiZJgAcxJgHCCgCgAbKOSoGANZDIQRUQgM6kDosy8DEdEslRwKBWpRgUCxTOg8vuwxMBIG2DBgYEiSZUIFmw==


formula: Cu Ba Si4 O10
compound: Synthetic
pub_title: Structure of BaCuSi4O10
formula_title: <missing>
a: 7.440
b: 7.440
c: 16.097
alpha: 90
beta: 90
gamma: 90
cell_volume: 891.027
crystal_density: 3.528
atoms_sites: ["Cu", "Ba", "Si", "O1", "O2", "O3"]
atoms_x: wMYtAMDGLQDg8jsAsGEvAPCBAQAAnRwA
atoms_y: wMYtAEBCDwBgOvz/EPX//xB+/v+g5QYA
atoms_z: AD36/wAAAADwagkA0FQIAEBCDwBQjAUA
atoms_occupancy: 0
atoms_u_iso: oIwAAIC7AACgjAAAAPoAAGDkAQCgCQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAgAAAAABAAABAAgAQAAgBAAAAAIhABABEgIESAAEgAATIBASAQgqI0gA0ABKhEYAKCBSCCYhMogAKolQDhBQBQAWpGJYDAFUikIIqIgEtSB4USeBiLkeUooFArVIwOBoxbgealQZGASG3BggUEJROqGB64==


formula: Li Ta3 O8
compound: Synthetic
pub_title: Neutron powder diffraction study of the intermediate-temperature form of lithium tantalate
formula_title: <missing>
a: 9.410
b: 11.521
c: 5.0506
alpha: 90
beta: 91.108
gamma: 90
cell_volume: 547.446
crystal_density: 8.223
atoms_sites: ["Li", "Ta1", "Ta2", "O1", "O2", "O3", "O4"]
atoms_x: AAAAALDDDgAAAAAAAJUVALB0FwCwHwgAoDAHAA==
atoms_y: 0JczAEBMBQAAUBQAAIobALD0CgDAohoAoPkLAA==
atoms_z: QEIPANAqDwBAQg8AIMUaAGDqGQCgCgUAYHsGAA==
atoms_occupancy: 0
atoms_u_iso: MAEBAHg3AAB4NwAAaD0AAGg9AABoPQAAaD0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIAAAQAAAIAAIAECEAAAACCYAAACFCQUIBGwABoCAEQIEIhMMiAlCBBEwKLqCAzxAlYAMWuNc5Y8lVAF2m3yBH4j6k1NKxWkv8YPkh0AcS+HCpk4vr4xfAcqybBGTky5oOGbFZCsHcOnRukplDRA09lIx==


formula: Zn2 Si O4
compound: Franklin, New Jersey, USA
pub_title: The crystal structure of willemite Zn2[SiO4]
formula_title: <missing>
a: 13.971
b: 13.971
c: 9.334
alpha: 90
beta: 90
gamma: 120
cell_volume: 1577.805
crystal_density: 4.222
atoms_sites: ["Zn1", "Zn2", "Si", "O1", "O2", "O3", "O4"]
atoms_x: wLELAJC5CwAw+wsAsLsHAHDnBwDAtgYAUFETAA==
atoms_y: 8LwMADAnDQBg7QwA0LkMADCRDABwRg0AcJ8TAA==
atoms_z: QKsjAJAPOADgUQ8AoJoGALAjGACAwC0AUDcPAA==
atoms_occupancy: 0
atoms_u_iso: oIIAAICOAAB4jAAASKgAAFiYAABIngAA8MMAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAQgAAAACAAAgEgAIAgAgSAAJAEKAQEBCyAQSEIggRiATRCAkjIKSJoMGwRSZGpoNrSpYxUMll8ZU674bTsw58a3vhqz2pY/us0EMcutPNYazS4xuTAspUArWEZagWJ4BCEjrEIBCLxCATEBJABAIASQMQ==


formula: Zn2 Si O4
compound: Synthetic
pub_title: Crystal structures of willemite Zn2[SiO4] and its germanium analog Zn2[GeO4]
formula_title: <missing>
a: 8.628
b: 8.628
c: 8.628
alpha: 107.87
beta: 107.87
gamma: 107.87
cell_volume: 521.689
crystal_density: 4.256
atoms_sites: ["Zn1", "Zn2", "Si", "O1", "O2", "O3", "O4"]
atoms_x: oGYwAADQBwDgAxwAoBQUAMB5JQDgQzsAoMAhAA==
atoms_y: QE0iAKC/NgCguw0A4CgBAOC8EgBgACcAIPoNAA==
atoms_z: oH8XAADyKwDgHAMAIFr+/0C/DwAAECcAgGL6/w==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAgAAAACAAAgAIAAAAAAAAgAgAAAAEAAAAIAAEAgAAAEEAAQAAIQEAAABAQAECAAAgECAABCAAgAgAAggAggABACAIAQAhCAIQABAkBEAAggAAiBCgRIJACICBAjAAgIAYQ==


formula: Zn2 Ge O4
compound: Synthetic
pub_title: Crystal structures of willemite Zn2[SiO4] and its germanium analog Zn2[GeO4]
formula_title: Zn2[GeO4]
a: 8.836
b: 8.836
c: 8.836
alpha: 107.7
beta: 107.7
gamma: 107.7
cell_volume: 563.200
crystal_density: 4.730
atoms_sites: ["Zn1", "Zn2", "Ge", "O1", "O2", "O3", "O4"]
atoms_x: wLQwAIAOCACgYRwAIFkTAKAlJgAgYzsA4FYjAA==
atoms_y: QE0iAACwNgAg+g0AIE4AAAALEwCgHycAoDIPAA==
atoms_z: IL4XAOAgLAAAawMAwOz9/wCaEACA0SYAQD37/w==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAgAAAAEAAEABAAAAAAAAIAQAAAACAAAAQAAIBAAAAQgABAAAiAgAAAgQACCAAAQIEAACEACACAACCAEEAAIAgEAIAMxAEIABAkCIACAgACIISAoiIAiAQEJAAgEAEQEAAkB==


formula: Ba Cu Si2 O6
compound: Synthetic
formula_title: <missing>
a: 10.0091
b: 10.0091
c: 22.467
alpha: 90
beta: 90
gamma: 90
cell_volume: 2250.791
crystal_density: 4.167
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAAAAAABQ0RAAwLELAFC8FgCwxBIA
atoms_y: cFg8AEBCDwDw1y0AIA4sACCgNQDQry8A
atoms_z: gIQeAPDjAwCAdzUAYNcxAPhzNABw5gMA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: QM4AABCLAADgeQAAQJwAAAD6AAAAfQAA
atoms_aniso_u22: gLsAAMCPAADQawAAAPoAAGDqAABg6gAA
atoms_aniso_u33: eMMAADDAAADA2gAAoAkBACBCAgDgKAEA
atoms_aniso_u12: AAAAAAAAAAAgAwAAIE4AAIDa//+Awf//
atoms_aniso_u13: 4OP//wAAAACgkv//4C4AACDR//9AHwAA
atoms_aniso_u23: AAAAAAAAAACA8///QB8AAEAfAACAuwAA
pub_title:
 Reinvestigation of the structure of BaCuSi2O6 - evidence for a phase
 transition at high temperature
 Note: T = 293 K

qdat:
AAAAAAAAAAAAAAAAAECAAgABAAAIgCACAgIgAIgAQBBIIJBChhIAEAQAsYgRQihBIUQxGA5EAgkE5KAyQBBCUmIkpEGDIE4UMEBSCNAQiaya4KQqS6wFApLLCEkEYAhD0BQBBEoIgAAgBYCAEABBAQAACAAAAAAAAAAAAA==


formula: Ba Cu Si2 O6
compound: Synthetic
formula_title: BaCuSi2O6
a: 7.1104
b: 7.1104
c: 11.175
alpha: 90
beta: 90
gamma: 90
cell_volume: 564.983
crystal_density: 4.150
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2"]
atoms_x: AAAAAAAAAABA0hAAcL0OAMCxCwA=
atoms_y: gIQeAAAAAABA0hAAgIQeAMCxCwA=
atoms_z: QEIPAEiIBwAAAAAAcHUBABBhBwA=
atoms_occupancy: AAk9AAAJPQAACT0AgIQeAAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Ba", "Cu", "Si", "O1", "O2"]
atoms_aniso_u11: 4HMBAOAoAQDQnQAAoP0CAODqAgA=
atoms_aniso_u22: 4HMBAOAoAQDQnQAAQJwAAODqAgA=
atoms_aniso_u33: oIYBAMBXAQBQpAEA4J8CAMBXAQA=
atoms_aniso_u12: AAAAAAAAAABg8P//AAAAAOC3/v8=
atoms_aniso_u13: AAAAAAAAAAAAAAAAwFcBAEAGAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAEAGAAA=
pub_title:
 Reinvestigation of the structure of BaCuSi2O6 - evidence for a phase
 transition at high temperature
 Note: T = 640 K

qdat:
AAAAAAAAAAAAAAAAAECABAAAAAAAgEACAAQgAEAAACBIASECAQQAIBAAwIAhwFEEIRAoEBhABoQhCJBREEAI4LCJIIcIQTB4gCaTMQGlTJRDBIDgySlFAheqQExiQueipBkCV5TGkgGSSjmSDLSpMAXOmqhQRWCTKDEogw==


formula: Si O2
compound: theoretical
formula_title: <missing>
a: 4.929
b: 4.929
c: 5.319
alpha: 90
beta: 90
gamma: 120
cell_volume: 111.912
crystal_density: 2.675
atoms_sites: ["Si", "O"]
atoms_x: AFIcAMBEGQA=
atoms_y: AAAAAIDYEAA=
atoms_z: AAAAACCnBgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mathematical Modeling of the structures and bulk moduli of TX2 quartz
 and cristobalite structure types, T = C, Si, Ge and X = O, S

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAEAAAAAAAAAAEAAAJAAgAABAAAAAggAAAghAABAAAABEABRAAAAAEEAgAREECABCIABAQAgEgEACIxCAgAEA0BABUQCATAQFAkhhgIJEBCSQgwkAUAIOQUFVEBIMMAQKSIFhRxQi==


formula: Ge O2
compound: theoretical, quartz structure
formula_title: GeO2
a: 5.114
b: 5.114
c: 5.426
alpha: 90
beta: 90
gamma: 120
cell_volume: 122.894
crystal_density: 4.240
atoms_sites: ["Ge", "O"]
atoms_x: QHcbAMDHGAA=
atoms_y: AAAAAIBPEgA=
atoms_z: AAAAAMA/BQA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mathematical Modeling of the structures and bulk moduli of TX2 quartz
 and cristobalite structure types, T = C, Si, Ge and X = O, S

qdat:
AAAAAAAAAAAAAAAAAAAAAAACAAAAAAEAAAAAAAAAAgAAAIAIAAAgAAAAIBAAAgEAAEAAAABgAECAAAAACBAAQQAMAAEEAECAEAAIIAQgBAAEIAxAEAAgAAQBAAhAIwGABAAiAgARARAAARgTAgAiBkAACIAgQAiBAEAJAk==


formula: C O2
compound: theoretical, quartz structure
formula_title: CO2
a: 4.011
b: 4.011
c: 4.214
alpha: 90
beta: 90
gamma: 120
cell_volume: 58.712
crystal_density: 3.734
atoms_sites: ["C", "O"]
atoms_x: AFgbAICoGAA=
atoms_y: AAAAAECtEgA=
atoms_z: AAAAAKDxBAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mathematical Modeling of the structures and bulk moduli of TX2 quartz
 and cristobalite structure types, T = C, Si, Ge and X = O, S

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAgAAAAAAAAAAAAQAAAABQAIAAAAQAAAAAAgAEAAAQBIAAEAAAAAAEgABgBAAAAAAAREAAICQAEIAACIQAEEAAQAAAFIAIJACJAAAQAMBAAQABKAABgiCAASgiEBEIAKQ==


formula: C S2
compound: theoretical, quartz structure
formula_title: CS2
a: 5.232
b: 5.232
c: 5.307
alpha: 90
beta: 90
gamma: 120
cell_volume: 125.810
crystal_density: 3.015
atoms_sites: ["C", "S"]
atoms_x: YE4aAMDNFwA=
atoms_y: AAAAAMBiFAA=
atoms_z: AAAAAKD9AgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAQAAAAAAIAAAAAAAAAgAAACCQAAAIAAAAAQAAQBQAEIAAAAIAEhAAQAAABgAUIASAAEIAUUAEAAAAFGISAAgkCQhAAEgBEhIEAWOYBAgEgmRQAQJCRAQCAyigiZGgAACJklAEEiQBGQaRgEk==


formula: Si S2
compound: theoretical, quartz structure
formula_title: SiS2
a: 5.894
b: 5.894
c: 5.944
alpha: 90
beta: 90
gamma: 120
cell_volume: 178.826
crystal_density: 2.569
atoms_sites: ["Si", "S"]
atoms_x: gB8aAICuFwA=
atoms_y: AAAAAKCRFAA=
atoms_z: AAAAAICvAgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAEAAAAAAgAAAAAAAEAAACBgAACAAAAAgABAoACgAAAEACiAAgAABQAYgBgABIAUgAgAAAEsFQAEgiQSAAoASFQCEH0AgEIZYsAEBkJAIQNlgJ5ugABB1WABMhAJcaOIWJQgQvqhAnARDRpQV3oQ==


formula: Si O2
compound: theoretical
formula_title: <missing>
a: 4.973
b: 4.973
c: 6.627
alpha: 90
beta: 90
gamma: 90
cell_volume: 163.891
crystal_density: 2.435
atoms_sites: ["Si", "O"]
atoms_x: AAsTAEBIDgA=
atoms_y: AAsTAOCBBwA=
atoms_z: AAAAAAC4CwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAgAAAQEAgAgACABAAAACAAEAAAYAQDEEBCAACABgEBgABQAQCBAIMABoARECQBIAQAIAJEMEEgBiIkFAKIQQEBRCANIkxIDAaRBDAUiCKRyBIgNIjFByIRiUiEYJTAMFR==


formula: Ge O2
compound: theoretical, cristobalite structure
formula_title: GeO2
a: 4.973
b: 4.973
c: 6.627
alpha: 90
beta: 90
gamma: 90
cell_volume: 163.891
crystal_density: 4.240
atoms_sites: ["Ge", "O"]
atoms_x: oBQUAKC7DQA=
atoms_y: oBQUAOB1CQA=
atoms_z: AAAAAIDwDAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAgAAAQEAgAgACABAAAACAAEAAAYAQDEEBCAACABgEBgABQAQCBAIMABoARECQBIAQAIAJEMEEgBiIkEAKIQQEBRCANIkxIDAaRBDAUiCKRyBIgNIjFByIRiUiAYJTAMFR==


formula: C O2
compound: theoretical, cristobalite structure
formula_title: CO2
a: 4.033
b: 4.033
c: 5.097
alpha: 90
beta: 90
gamma: 90
cell_volume: 82.903
crystal_density: 3.526
atoms_sites: ["C", "O"]
atoms_x: gEMUAGCcDQA=
atoms_y: gEMUAODyCQA=
atoms_z: AAAAAAAvDQA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAACAAAAAAAAAAACAAAgAARAAgAACAAAABAAAAQAEAAAAAAGAQASAAAQAgBACABAQAICASBABggAgQAQACQQFgABAAEEAgADBAEEAggQEChAIIGADRAQAAEHCBhBQgQAAQcYO==


formula: C S2
compound: theoretical, cristobalite structure
formula_title: CS2
a: 5.232
b: 5.232
c: 6.126
alpha: 90
beta: 90
gamma: 90
cell_volume: 167.692
crystal_density: 3.016
atoms_sites: ["C", "S"]
atoms_x: QJsVAGCiDAA=
atoms_y: QJsVAGCiDAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAIAIAAAAAAAAAACgAAEJAABAAAAAAAgKAAAAAEIAkQAogAAwAwAAAAxgHEARAABFMAUAQIhEQAIgEgUEKITAwABGQQACQpIUaBBAIUGQICWaRQIiE0GAUELqOCIrWGAGYmY4YEx5oRI05==


formula: Si S2
compound: theoretical, cristobalite structure
formula_title: SiS2
a: 5.888
b: 5.888
c: 6.806
alpha: 90
beta: 90
gamma: 90
cell_volume: 235.954
crystal_density: 2.596
atoms_sites: ["Si", "S"]
atoms_x: IMoVAIBzDAA=
atoms_y: IMoVAMAPDQA=
atoms_z: AAAAAACgDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAEAQAAAAAAAAAEAABDAACAAAAAAEIAAAAEQAIgAmAAQAkAAAEQBIAkAAAkAkAIBICABgSAgCgLAoAAWBACBQaBwUCAENBAKHg4cHBQEPCA4cIFChwIKMBmgA444EKMFHDFjhgjzAjzDjhhmm==


formula: Ba2 Cu Si2 O7
compound: Synthetic
pub_title: Synthesis and structure of a new polymorph Ba2CuSi2O7 Note: known as beta-Ba2CuSi2O7
formula_title: Ba2CuSi2O7
a: 8.284
b: 8.284
c: 5.313
alpha: 90
beta: 90
gamma: 90
cell_volume: 364.603
crystal_density: 4.612
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: 2FQUAAAAAABgPQgAAAAAAMBGCABg0gQA
atoms_y: qC8KAAAAAAAgRxYAgIQeAHA9FgBQ/gsA
atoms_z: sBIfAAAAAABgaTsAwBk1ACDoEAAARTMA
atoms_occupancy: 0
atoms_u_iso: 8JEAABCkAADAdgAA4KsAAOCrAAAgywAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAABACAAAAAICAIAAAgAECAAAEhAAIEEBAECEAQSICUQARIBAQcMUIQgBMACWDJBLJhjJKBEOkIYw0hOUIYiVIaxEpxAcYm5WEYyNzUxQbl2E1Ny/mvR6yk2bB2D4sV5OuaOTt+9gxeNrbYPjW7jyqeb==


formula: Ba Cu2 Si2 O7
compound: Synthetic
formula_title: <missing>
a: 6.86058
b: 13.17507
c: 6.89589
alpha: 90
beta: 90
gamma: 90
cell_volume: 623.310
crystal_density: 4.610
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3", "O4"]
atoms_x: UEz//2CDDQBQRgAA8LoEAHAh9v9gvfv/kAoLAA==
atoms_y: QEIPAEBRAAAQKQgAQEIPAHAACACwDAcAEPYDAA==
atoms_z: YFY6APBhMADA4RwAUC4dAOASJgAw/A8AsFcgAA==
atoms_occupancy: 0
atoms_u_iso: UF4BAEBkAQCgggAA+P3//9iFAQAYzQEA2HIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Spin-1/2 quantum antiferromagnetic chains with tunable superexchange
 interactions found in BaCu2(Si1-xGex)2O7

qdat:
AAAAAAAAAAAAAAABAQAAAEAgAABAIAMFQApgAGKAAGEhgROCzQTEIHBsGTGDGkP8P8E73B8A7Wap9XT3Ipe/hX8tzte7vy7/f/X5/8vfv6F/3//+9W91/d1719f///Vm/9//0z37///sf/+3/3/vf/f/7/9/Pfvf+/3X/7==


formula: Ba Cu2 Ge2 O7
compound: Synthetic
formula_title: BaCu2Ge2O7
a: 7.04765
b: 13.40700
c: 7.02755
alpha: 90
beta: 90
gamma: 90
cell_volume: 664.018
crystal_density: 5.218
atoms_sites: ["Ba", "Cu", "Ge", "O1", "O2", "O3", "O4"]
atoms_x: 4Lf+/8BBDQCwh///cCUGAECA9P9QkPz/AFoKAA==
atoms_y: QEIPAIA+AAAQ9wcAQEIPAEBTCADw+QYAwOcCAA==
atoms_z: UOQ5AMC0MABgvxwAcHwdANCzJgDQYg4A0L4gAA==
atoms_occupancy: 0
atoms_u_iso: uHQAALB8AACoJQAAyA8AAPDDAAAYugAACGEAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Spin-1/2 quantum antiferromagnetic chains with tunable superexchange
 interactions found in BaCu2(Si1-xGex)2O7

qdat:
AAAAAAAAAAAAAAACBAAAAgEAAAQBADCUAOQADDAACBRQJKBzQWEIOCQFGEGOgf07gju4OwHZzMZr+/6M6v4O3a7//9P69e/fP4ea+3usH/f/fvar7f/7f/fX9U/Vy7/9/8x3z/f7b/96393zt97f///X6//79//9//f4t/==


formula: Cu Ba Si4 O10
compound: Wessels mine, Kalahari Manganese Field, South Africa
formula_title: <missing>
a: 7.442
b: 7.442
c: 16.133
alpha: 90
beta: 90
gamma: 90
cell_volume: 893.500
crystal_density: 3.518
atoms_sites: ["Cu", "Ba", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwAgpx8AYAodAMA2LADQqRcA
atoms_y: QEIPAMDGLQBITDkA4I47APD6PADw5QEA
atoms_z: QMQFAAAAAADwbwkAQEIPAEBTCADwggUA
atoms_occupancy: 0
atoms_u_iso: 0J0AAPDSAAAAlgAAMAUCAAAsAQAALAEA
atoms_aniso_label: ["Cu", "Ba", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: 4HkAAKDwAACAiQAAsHUCAECcAADQGgEA
atoms_aniso_u22: 4HkAAKDwAAAwjgAAsHUCAICcAQCwswAA
atoms_aniso_u33: IOQAACCZAABQqgAAwCUBAEBLAQDA1AEA
atoms_aniso_u12: AAAAAAAAAABA7f//UDP//6BaAADw2P//
atoms_aniso_u13: AAAAAAAAAACgDwAAsMwAABD1//8Aav//
atoms_aniso_u23: AAAAAAAAAABw/v//sG7//wDn//+AVwAA
pub_title:
 Effenbergerite, BaCu[Si4O10], a new mineral from the Kalahari Manganese Field,
 South Africa: description and crystal structure

qdat:
AAAAAAAAAAAAAgAAAAABAAABAAgAQAAgCAAAAAIhABACEgIEkAAEgAAiICAyAQgyJVABcABKhEoAcCDSCGoiNJgAepFgGhCgCwAWqOLoDAFYioYQ0IgM6iB4Uy6BiLkalJwHAvZIwKBpRqg2bnwRGAkGrDAgUESRcqMC1Q==


formula: Sr Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.36657
b: 7.36657
c: 15.5844
alpha: 90
beta: 90
gamma: 90
cell_volume: 845.709
crystal_density: 3.326
atoms_sites: ["Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwCgBB8A8JQbAMCgKwBAYxYA
atoms_y: wMYtAEBCDwDwxzgAsOE7AFAUAADAJQEA
atoms_z: AAAAANBmBQCwMgkA0BEPAOD+BwBwRAUA
atoms_occupancy: AAk9AAAJPQAACT0AgIQeAAAJPQAACT0A
atoms_u_iso: gCYEAADiBABgZwEAwEUEAOCTBAAAZQQA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = 0.000

qdat:
AAAAAAAAAAAAAEAAAAAAQAAAQABAEAAEAEAAAAAQYAIAAkBAIIAAICAARoEAJBBEggiQAiwBFiAIAIIRJEB4hIIRgF5AUBIIiAFAHEGIlAiBOQQkRKkFBMggTIukgRJZDkolwqB0MUgkBIZSC0cpBCWBkbEFhoIBRoSoMF==


formula: (Ba.105 Sr.895) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.36858
b: 7.36858
c: 15.6346
alpha: 90
beta: 90
gamma: 90
cell_volume: 848.896
crystal_density: 3.355
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8AkA8fAACKGwCwqysAQHwWAA==
atoms_y: wMYtAMDGLQBAQg8AUNE4AND9OwDAEgAA8DYBAA==
atoms_z: AAAAAAAAAABQcwUAYDcJAHAIDwDQCQgAQEwFAA==
atoms_occupancy: oGgGAGCgNgAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: wMgDAMDIAwCAowQAgLUBACCzBADgEAUAgCAFAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .105

qdat:
AAAAAAAAAAAAAIAAAAAAQAAAQABAEAAEAEAAAAAgQAIAAkBAIQAAIEAAhQIAKBBFAgigAigBFCAQAIQhKEBQhIIVAJRAYBIRCAGAGIGImAkBcgRESLEGBYhAVJMlASRpDJIlgsBkIlAkCIqWCktKCCcDIaEJCwQChoyoUF==


formula: (Ba.193 Sr.807) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.3752
b: 7.3752
c: 15.6902
alpha: 90
beta: 90
gamma: 90
cell_volume: 853.446
crystal_density: 3.371
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8A0BUfAHCIGwDAuSsA8JkWAA==
atoms_y: wMYtAMDGLQBAQg8A0N04AKAePAAwEQAA0EwBAA==
atoms_z: AAAAAAAAAACghwUA8DgJAMADDwDAFAgAEFQFAA==
atoms_occupancy: oMcLAGBBMQAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: QAcEAEAHBADgjQUAgLUBAGDYAwCAowQAoPEEAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .193

qdat:
AAAAAAAAAAAAAIAAAAAAQAAAQACAIAAIAIAAAAAgwAIABIBAQQAAQIAAjgIAcCBFBBHABHACOCAwARhBMEDhCQYmAJhAwCwhEAMAOYKJMBIC4giJESIMCpDAUSZLAkiyHJRNBYDIxJBQGQ0cFlaMEEoGRUYSFAgFCRlQoX==


formula: (Ba.276 Sr.724) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.37735
b: 7.37735
c: 15.7266
alpha: 90
beta: 90
gamma: 90
cell_volume: 855.925
crystal_density: 3.393
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8AEBwfAPB7GwBwvisAAKgWAA==
atoms_y: wMYtAMDGLQBAQg8AEOQ4AFAjPADAEgAAMFYBAA==
atoms_z: AAAAAAAAAADAigUAMD8JAGD6DgAAGwgAwFgFAA==
atoms_occupancy: gNgQAIAwLAAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: AO4CAADuAgCAIAUAwMgDAMC2BgDgCgYAoOsFAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .276

qdat:
AAAAAAAAAAAAAIAAAAAAgAAAQACAIAAIAIAAAAAgwAIADIBAQwAAQIABDgIAYCCFDBGABOACKEBgATBCIIDhEQwsAbhAgCghIAcAOQaRIDQC4hiBEWIYCrCAsSZLAklyGRiWBwDISSCwMRkoJpacEJYEhs4WHAgJERpgwW==


formula: (Ba.402 Sr.598) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.38801
b: 7.38801
c: 15.8265
alpha: 90
beta: 90
gamma: 90
cell_volume: 863.853
crystal_density: 3.410
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8AwDkfALCOGwAQzisAgM0WAA==
atoms_y: wMYtAMDGLQBAQg8A0PY4ADA5PABABgAAYGcBAA==
atoms_z: AAAAAAAAAADwmwUAkEgJAPD7DgAQKQgAsGMFAA==
atoms_occupancy: QIkYAMB/JAAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: AGUEAABlBADAPwUAYN4CAIAUBwCAGgYAwLYGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .402

qdat:
AAAAAAAAAAAAAQAAAAAAgAAAgAEAIAAIAQAAAABCQAQAFICAhgAAggACKAQBwCEKGCcACYAEqEFgAsEEwQGiEhhwAvCDAHCEQAwAVRYiwHAHyDIIRIQwHmMBQmycCSLkMlI4FgOykYHAZF5weV04ITgZDZAwYGAkIiVBA1==


formula: (Ba.492 Sr.508) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.38813
b: 7.38813
c: 15.8516
alpha: 90
beta: 90
gamma: 90
cell_volume: 865.251
crystal_density: 3.439
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8AYEkfAKCZGwCw3SsAEOgWAA==
atoms_y: wMYtAMDGLQBAQg8A4AQ5ALBFPACwBAAAIHoBAA==
atoms_z: AAAAAAAAAAAwogUAIEoJAID9DgBQLwgA0GYFAA==
atoms_occupancy: gAceAIABHwAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: IDAFACAwBQDgjQUAgK8CAKDlBgDAvAUAwDkGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .492

qdat:
AAAAAAAAAAAAAQAAAAAAgAAAgAEAIAAIAQAAAABCQAQAFICAigAAhAACOAQBwEEKKCoAC4AFqEGgAsEFwQGiEhhgAvCHAFCEgBwAVRYjwHAGyDIIRIQgNmUBwmyUCSPkclI4FAfSk4LA5J5weV04ITgZDbAwYGAkYiVBA5==


formula: (Ba.636 Sr.364) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.4030
b: 7.4030
c: 15.9357
alpha: 90
beta: 90
gamma: 90
cell_volume: 873.347
crystal_density: 3.461
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8A4FUfACCmGwCw9isA0BMXAA==
atoms_y: wMYtAMDGLQBAQg8AMBk5ADBrPADwCgAAIJMBAA==
atoms_z: AAAAAAAAAAAQuAUAYFAJAPD7DgDwPggAoG4FAA==
atoms_occupancy: gNEmAIA3FgAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: IKcGACCnBgBA9QYAAHECAICjBACgdAQAgBoGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .636

qdat:
AAAAAAAAAAAAAQAAAAAAgAAAgAIAIAAQAgAAAACEgAQASQCBFAABEAAEUAgCgEISSGoAGgANYIVABwQVgQWERFCAB+EaAcEJADABrExFAMAekMRhCwjATZIDhbJQFI+Q5SjgUB7KjgYDiblB5VThiOBEPOHBgUERkdUIF1==


formula: (Ba.821 Sr.179) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.41932
b: 7.41932
c: 16.0402
alpha: 90
beta: 90
gamma: 90
cell_volume: 882.954
crystal_density: 3.493
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8AQHgfACC/GwDAHSwAAFcXAA==
atoms_y: wMYtAMDGLQBAQg8A4DY5AJCNPACwBAAAcMABAA==
atoms_z: AAAAAAAAAADgvwUA4FwJAGD6DgCQTggAkHkFAA==
atoms_occupancy: IBwyAODsCgAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: wLAHAMCwBwBAeAYAIL8CAMBFBABAAQUAIKcGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = .821

qdat:
AAAAAAAAAAAAAgAAAAAAgAABAAQAQAAQBAAAAAERAAgAiQECKAACQAAIkAgJAIQVEKgAKAAUoRKAFAg1AhsImSIAGsRYBoQoAUAFqTiWAgBSIxCCLCIBLUgNFGXgYj1DlJOBQHVKGBgWKdUHUs+CIwEg7YcEBgiSSlQgWX==


formula: Ba Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.43602
b: 7.43602
c: 16.1302
alpha: 90
beta: 90
gamma: 90
cell_volume: 891.910
crystal_density: 3.524
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwAQmR8AUOkbAHA7LACgmBcA
atoms_y: wMYtAEBCDwDgTzkA4KE8AAAAAACg6gEA
atoms_z: AAAAANDKBQCwZAkAQPcOAPBXCADwggUA
atoms_occupancy: AAk9AAAJPQAACT0AgIQeAAAJPQAACT0A
atoms_u_iso: wDMHAGDMBQCggAIAAGsDAMA/BQAgpwYA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural variations in the wesselsite-effenbergerite (Sr1-xBaxCuSi4O10)
 solid solution
 Sample: x = 1.000

qdat:
AAAAAAAAAAAAAgAAAAAAgAABAAgAQAAgCAAAAAIhABACEgIEiAAEgAASIBAyAQgqJUgBUABJgkoAaCDSCCYRMkwAaolQFhBQBQATpFJ4DAHUhkYIqIwGdRB0UZeBSKyeUo4FArUowFBUx7QaV14JFASD3BggKEJJOmGB64==


formula: Ti
compound: Great Tolbachik Fissure Eruption (Kamchatka)
formula_title: <missing>
a: 2.95
b: 2.95
c: 4.68
alpha: 90
beta: 90
gamma: 120
cell_volume: 35.271
crystal_density: 4.508
atoms_sites: ["Ti"]
atoms_x: VVgUAA==
atoms_y: q7AoAA==
atoms_z: QEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Natural analog of alpha-titanium in the exhalation products of
 the Great Tolbachik Fissure Eruption (Kamchatka)

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAABACAAAAAAAAAAAAACAAAAAAAAAAgAAAAAACAAAgAggAAAEAAAEAAAAEAAAAAAAgAEACAAAIAAIAQAIAgAAAEAABAAAQAAACAKAgAAAABBEABgAEBAIAAABIAgE==


formula: Mg Sb2 O6
compound: Synthetic
pub_title: The crystal structure of zinc metantimonate and similar compounds
formula_title: <missing>
a: 4.63
b: 4.63
c: 9.21
alpha: 90
beta: 90
gamma: 90
cell_volume: 197.434
crystal_density: 6.120
atoms_sites: ["Mg", "Sb", "O1", "O2"]
atoms_x: AAAAAAAAAABArRIAYH4SAA==
atoms_y: AAAAAAAAAABArRIAYH4SAA==
atoms_z: AAAAAEAkFAAAAAAAAAUUAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAACAAIAAAAAAgAgAAAAIAgAAAUBAAACBAAAGAAAAAwAAwwABxAAEMAAowAEQAFKADDAAMAEoAcoAmADIAVgDVAZwAQBUAawPgGQASB7BrAEAuAtBcBoDwCoEwBAXB8DgFASD0NwGAgOx4CgfCw==


formula: Tl (Cu1.55 Fe.45) Se2
compound: Bukov, Czechoslovakia
pub_title: New data on bukovite, thalcusite, chalcothallite and rohaite
formula_title: <missing>
a: 3.976
b: 3.976
c: 13.70
alpha: 90
beta: 90
gamma: 90
cell_volume: 216.577
crystal_density: 7.451
atoms_sites: ["Tl", "Cu", "Fe", "Se"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAA==
atoms_y: AAAAAICEHgCAhB4AAAAAAA==
atoms_z: AAAAAEBCDwBAQg8A4KoVAA==
atoms_occupancy: AAk9AGBNLwCguw0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAIAAAAAAAAAAAEAAEAAAAgAQAAIAAAABEAQAAACABAAAAqBQAQAAAAABQCACEAkAAMGAIICgAFCAEABAA0ICAAAAIIBIGABiAiBgBRAJCABjAAAAEIEAQBCCQYARAAIAwCAABEEiAEgEMBCCiAIhAAGI==


formula: Ag O
compound: Synthetic
formula_title: AgO
a: 5.8517
b: 3.4674
c: 5.4838
alpha: 90
beta: 107.663
gamma: 90
cell_volume: 106.022
crystal_density: 7.760
atoms_sites: ["Ag1", "Ag2", "O"]
atoms_x: AAAAAICEHgDQ/xEA
atoms_y: AAAAAAAAAADgLRUA
atoms_z: AAAAAICEHgAwWQ0A
atoms_occupancy: 0
atoms_u_iso: UBQAAJAaAACgDwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Low-temperature structures of CuO and AgO and their
 relationships to those of MgO and PdO
 Note: T = 9 K

qdat:
AAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAAEQEAAgAAEAAAAQQQAAAAAICAAIACSgAAIgCAQkACQAhEAQgCAgWAiCgAgFBAREAbw4AJgCAWACAQjDKAYCiIBRgMQhoUZAlOFEKnQsICSFA8NmkSEUYeGa5WyRCrrISl1kR==


formula: Ag2 S O4
compound: Synthetic
formula_title: Ag2SO4
a: 5.7960
b: 12.6670
c: 10.2238
alpha: 90
beta: 90
gamma: 90
cell_volume: 750.610
crystal_density: 5.518
atoms_sites: ["Ag", "S", "O"]
atoms_x: IKEHACChBwAA1P7/
atoms_y: IKEHACChBwAwfAMA
atoms_z: 0BQbACChBwAA5AwA
atoms_occupancy: 0
atoms_u_iso: QJwAAIDB//8QiwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Low-temperature structures of CuO and AgO and their
 relationships to those of MgO and PdO
 Note: T = 9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAIAAAAAIgAACAACAkAEAAIAAAAACSChAgACEMBCAAQgwgAIIBKgBJ0sgAkgC4AAIIwoSRIBI4kxAAKhxIRyCTIDAFSSCkhRAjEACBkSDoIGEEBELQCEAoMAGEBUYxYQCBQEFAkwABAYTB==


formula: (Zn.6 Al.4) O3.056 H2.912 C.2
compound: El Soplao cave, Cantabria, Spain
formula_title: <missing>
a: 3.06616
b: 3.06616
c: 22.6164
alpha: 90
beta: 90
gamma: 120
cell_volume: 184.138
crystal_density: 2.821
atoms_sites: ["Zn", "Al", "O1", "H", "C", "O2", "Wat"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAFVYFABA9QYAQPUGAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAKuwKADACvn/wAr5/w==
atoms_z: AAAAAAAAAADABRcA4A8aAMCjHgDgdB4A4HQeAA==
atoms_occupancy: AJ8kAABqGAAACT0AAAk9AIAaBgCAGgYAgKMEAA==
atoms_u_iso: 8BgBAPAYAQCATAEAgEwBALDuAQCw7gEAsO4BAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Zaccagnaite-3R, a new Zn-Al hydrotalcite polytype
 from El Soplao cave (Cantabria, Spain)
 Note: polytype zaccagnaite-3R

qdat:
AAAAAAAAAAAAABAAAAAAAAAAAAABAAAAAAAAAAACECAEACAAAAAgAAQAAAAABAAAAAAAICAAABAAAAAkggQAAIAQAAAEAAAAAAAAAAAAFAhAAQCAAAQAAAIQAEAAAEAAAAAAAAAACIAEAANIgBBAAEAAAAAAABhIAggAEA==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6837
b: 3.4226
c: 5.1288
alpha: 90
beta: 99.54
gamma: 90
cell_volume: 81.080
crystal_density: 6.516
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPAICJGQA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: iFkAAEBqAAA=
atoms_aniso_u22: 0HoAAHCtAAA=
atoms_aniso_u33: 8EYAAIBXAAA=
atoms_aniso_u12: qCAAAAAAAAA=
atoms_aniso_u13: 8BQAAOAuAAA=
atoms_aniso_u23: IA0AAAAAAAA=
pub_title:
 A refinement of the crystal structure of copper(II) oxide,
 with a discussion of some exceptional E.s.d.'s

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAQAAAAAAAAAAAAAgAQAACAIAAAAAABCAwAAAJABAAAAQAASAAAEAAAAAAAAgiAAAAIAAABYQAFQEQAcAQIAAQQGAEsIAEQEwAIAAABgFEQAAoKaCGICQKiAAAD==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6832
b: 3.4288
c: 5.1297
alpha: 90
beta: 99.3086
gamma: 90
cell_volume: 81.287
crystal_density: 6.500
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPABAhGgA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: MJgAANjbAAA=
atoms_aniso_u22: mGEBAIiLAAA=
atoms_aniso_u33: IN8AAJhgAgA=
atoms_aniso_u12: 2M3//wAAAAA=
atoms_aniso_u13: GG8AAEhZ//8=
atoms_aniso_u23: gOT//wAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 0 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAgAAAAAAAAAAAABAAgAAEAQAAAAAABEBgAAASACAAAAQAAmAAAIAAIAAAADBEAAAAIAAACggALAIQA4BAgAAggIASoQgggJgAgCAACAMESACgNEEYQRApWAAAM==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6776
b: 3.4593
c: 5.1264
alpha: 90
beta: 98.9645
gamma: 90
cell_volume: 81.938
crystal_density: 6.448
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPABCYGwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: kOwAAEj6CAA=
atoms_aniso_u22: qDgBAOA4AAA=
atoms_aniso_u33: sEQBAGCABgA=
atoms_aniso_u12: 8EsAAAAAAAA=
atoms_aniso_u13: wMsAAJC+/P8=
atoms_aniso_u23: uFoBAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 10 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAABAAAAAAAAAAAAACAEAAAgAgAAAAAAIICAAAAoACAAACAAESAACQACAAAAAUFAAAAAgAAAMIAAYBBAURAIAAQgIQBwiQCgBkABAgAAQGARQAYA8EiBIQWsEAACF==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6839
b: 3.4734
c: 5.1226
alpha: 90
beta: 98.7300
gamma: 90
cell_volume: 82.374
crystal_density: 6.414
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPAJDQHAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: gO0AAHjNCgA=
atoms_aniso_u22: SPgAANgWAgA=
atoms_aniso_u33: YDABABCABgA=
atoms_aniso_u12: 4Nn//wAAAAA=
atoms_aniso_u13: oLkAAFC5+/8=
atoms_aniso_u23: 8HcBAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 25 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAACAAAAAAAAAAAAAEAIAACABAAAAAAAQIMAAABgACAAAEAAJEAAQgAQAAAABIYAAAACAAAARAABgECERIBAABEBBAFAlAKAIoAQBAADAwBGABAHIoQBAhTgQAAQN==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6797
b: 3.4768
c: 5.1193
alpha: 90
beta: 98.6440
gamma: 90
cell_volume: 82.347
crystal_density: 6.416
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPAFA0HAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: YKkAAHgPCgA=
atoms_aniso_u22: wPgAAOiwAgA=
atoms_aniso_u33: ODABACg1BwA=
atoms_aniso_u12: qAwAAAAAAAA=
atoms_aniso_u13: 6MsAABgB+/8=
atoms_aniso_u23: OE4BAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 30 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAACAAAAAAAAAAAAAEAIAACABAAAAAAAQIMAAABgACAAAEAAREAAQgAQAAAABIYAAAACAAAA5AADQECERIBAABICBAFAqAMAQoAQCAADBwBGADALRQQDAjTgIAAgX==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6844
b: 3.4792
c: 5.1215
alpha: 90
beta: 98.6836
gamma: 90
cell_volume: 82.513
crystal_density: 6.403
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPANBGGwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: qO0AALhJCAA=
atoms_aniso_u22: SAwBAADmAAA=
atoms_aniso_u33: +MoAAOC3CAA=
atoms_aniso_u12: iOUAAAAAAAA=
atoms_aniso_u13: 0FwAAHCUAAA=
atoms_aniso_u23: 2BECAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 32 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAEAAAAAAAAAAAAAIAQAACABAAAAAAAgQMAAABAACAAAEAAREAAQgAQAAAABIYAAAACAAAAyAADgECIiQBAABIECAOAqAIARIAQCAACCwCEADATRggDBCVAQAAgU==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6732
b: 3.4770
c: 5.1190
alpha: 90
beta: 98.5625
gamma: 90
cell_volume: 82.250
crystal_density: 6.424
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPANCRGwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: EKkAAEAaCgA=
atoms_aniso_u22: +AsBAJiPAAA=
atoms_aniso_u33: cPMAAMiiCAA=
atoms_aniso_u12: ICYAAAAAAAA=
atoms_aniso_u13: IJQAAAgx/v8=
atoms_aniso_u23: SFwBAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 34 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAACAAAAAAAAAAAAAIAQAACABAAAAAAAgIMAAABgACAAAEAARCAAQgAQAAAABIYAAAABAAAAZAADIECEQoBAABICBAFAqAMAQoAICAAChwBCABAJQwIDBCTAEAAQV==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6791
b: 3.4805
c: 5.1183
alpha: 90
beta: 98.5981
gamma: 90
cell_volume: 82.418
crystal_density: 6.411
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPADCbGwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: UNwAAHAvCwA=
atoms_aniso_u22: aMkAAFA/AgA=
atoms_aniso_u33: wBsBABgZBgA=
atoms_aniso_u12: UI3//wAAAAA=
atoms_aniso_u13: WN4AAAi3+v8=
atoms_aniso_u23: 0CQBAAAAAAA=
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 36 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAEAAAAAAAAAAAAAIAQAACABAAAAAAAgIMAAABAACAAAEAAREAAggAQAAAABIQAAAACAAAAyAADQECIhQBAABIECAOAqAIAQoAQCAADCwBEADAjRggFBCVAIAAgW==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6791
b: 3.4805
c: 5.1183
alpha: 90
beta: 98.5981
gamma: 90
cell_volume: 82.418
crystal_density: 6.411
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPADCbGwA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A crystallographic contribution to the mechanism of a mechanically
 induced solid state reaction
 Note: milling time = 37 min (combustion)

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAEAAAAAAAAAAAAAIAQAACABAAAAAAAgIMAAABAACAAAEAAREAAggAQAAAABIQAAAACAAAAyAADQECIhQBAABIECAOAqAIAQoAQCAADCwBEADAjRggFBCVAIAAgW==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6833
b: 3.4208
c: 5.1294
alpha: 90
beta: 99.567
gamma: 90
cell_volume: 81.033
crystal_density: 6.520
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAAAAAAA=
atoms_y: QEIPALCBGQA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: MCoAACA1AAA=
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: kBoAAEA4AAA=
atoms_aniso_u22: oEEAAIBXAAA=
atoms_aniso_u33: MCoAAJAaAAA=
atoms_aniso_u12: MBEAAAAAAAA=
atoms_aniso_u13: wBIAAAAZAAA=
atoms_aniso_u23: IAMAAAAAAAA=
pub_title:
 Low-temperature structures of CuO and AgO and their
 relationships to those of MgO and PdO
 Note: T = 11 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAQAAAAAAAAAAAAAgAQAACAIAAAAAABCAwAAAIgBAAAAQAASAAAGAAAAAAAAghAAAAEAAABYQAEwCQAUAQIAAQQCACsEAEQEQAIAAAAwDCQAAoKaBDICQLTAAAD==


formula: Cu O
compound: Synthetic
formula_title: <missing>
a: 4.6927
b: 3.4283
c: 5.1370
alpha: 90
beta: 99.546
gamma: 90
cell_volume: 81.500
crystal_density: 6.483
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAIBd//8=
atoms_y: sA4PAJB+GQA=
atoms_z: AAAAAKDhDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: IGcAAOBgAAA=
atoms_aniso_u22: 8IcAAPC5AAA=
atoms_aniso_u33: oFoAAGBUAAA=
atoms_aniso_u12: IBwAAMDg//8=
atoms_aniso_u13: YCIAAHAwAAA=
atoms_aniso_u23: AAAAADD4//8=
pub_title:
 CuO: x-ray single-crystal structure determination at 196 K and room temperature
 Note: T = room temperature

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAIAAAwAAAAAAAAAAAABAAQAAEAQAAAAAABIBgAAASACAAAAgAAkAAAIAAAAAAADBEEAAAQAAADggATAIgAwBggAAggIAJoQBQgIgAQCAAGAMJCACgJkEYgJApMAAAN==


formula: Cu O
compound: Synthetic
pub_title: CuO: x-ray single-crystal structure determination at 196 K and room temperature Note: T = 196 K
formula_title: <missing>
a: 4.6893
b: 3.4268
c: 5.1321
alpha: 90
beta: 99.653
gamma: 90
cell_volume: 81.302
crystal_density: 6.499
atoms_sites: ["Cu", "O"]
atoms_x: QEIPAFBM//8=
atoms_y: QBAPADB1GQA=
atoms_z: AAAAABB8DwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cu", "O"]
atoms_aniso_u11: 8FUAAPBVAAA=
atoms_aniso_u22: MHUAAJCwAAA=
atoms_aniso_u33: EEAAADBDAAA=
atoms_aniso_u12: cBcAADD4//8=
atoms_aniso_u13: IBwAANAgAAA=
atoms_aniso_u23: 0AcAADD4//8=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAYAAAAAAAAAAAAAgAQAAEAIAAAAAABEAwAAAJABAAAAQAASAAAEAAAAAAABgiCAAAIAAACwQAJgEQAYAwQAAggKAC0IIkQIwAIAAAAgGERAAwMcCIIEgSmAAAG==


formula: Mg1.96 Si O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 143 K
formula_title: <missing>
a: 8.0746
b: 8.0746
c: 8.0746
alpha: 90
beta: 90
gamma: 90
cell_volume: 526.457
crystal_density: 3.526
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwDQ3w4A
atoms_y: gIQeACChBwDQ3w4A
atoms_z: gIQeACChBwDQ3w4A
atoms_occupancy: gNA7AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: oEEAAFBfAADwPAAA
atoms_aniso_u22: oEEAAFBfAADwPAAA
atoms_aniso_u33: oEEAAFBfAADwPAAA
atoms_aniso_u12: oPb//wAAAADwCgAA
atoms_aniso_u13: oPb//wAAAADwCgAA
atoms_aniso_u23: oPb//wAAAADwCgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAABAAAAAgAAgAAABAACAAAAgACAAABAAQAAAgAIAAAgAQAACACAAAgAgAAQAQAAAAgAAgBAACAEAAIBAACAIABAEAAAC==


formula: Mg1.94 Si O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 193 K
formula_title: <missing>
a: 8.0756
b: 8.0756
c: 8.0756
alpha: 90
beta: 90
gamma: 90
cell_volume: 526.653
crystal_density: 3.512
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBg4Q4A
atoms_y: gIQeACChBwBg4Q4A
atoms_z: gIQeACChBwBg4Q4A
atoms_occupancy: QDQ7AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: kEwAAGBUAABwSQAA
atoms_aniso_u22: kEwAAGBUAABwSQAA
atoms_aniso_u33: kEwAAGBUAABwSQAA
atoms_aniso_u12: oPb//wAAAADQBwAA
atoms_aniso_u13: oPb//wAAAADQBwAA
atoms_aniso_u23: oPb//wAAAADQBwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAACAAAAAgAAgAAABAAEAAAAgACAAACAAQAAAgAIAAAgAQAACACAAAgAgAAQAQAAAAgAAgBAACAEAAQBAACAQABAEAAAE==


formula: Mg1.9 Si O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 350 K
formula_title: <missing>
a: 8.0860
b: 8.0860
c: 8.0860
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.690
crystal_density: 3.474
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwDQ3w4A
atoms_y: gIQeACChBwDQ3w4A
atoms_z: gIQeACChBwDQ3w4A
atoms_occupancy: wPs5AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: MHUAALCBAACQfgAA
atoms_aniso_u22: MHUAALCBAACQfgAA
atoms_aniso_u33: MHUAALCBAACQfgAA
atoms_aniso_u12: EPX//wAAAADwCgAA
atoms_aniso_u13: EPX//wAAAADwCgAA
atoms_aniso_u23: EPX//wAAAADwCgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAABAAAACAAEAAAAgAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAQAAgCAAEAgACAQAAAI==


formula: Mg1.9 Si O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 443 K
formula_title: <missing>
a: 8.0931
b: 8.0931
c: 8.0931
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.084
crystal_density: 3.465
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBg4Q4A
atoms_y: gIQeACChBwBg4Q4A
atoms_z: gIQeACChBwBg4Q4A
atoms_occupancy: wPs5AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: oIwAAICJAAAQiwAA
atoms_aniso_u22: oIwAAICJAAAQiwAA
atoms_aniso_u33: oIwAAICJAAAQiwAA
atoms_aniso_u12: YPD//wAAAABABgAA
atoms_aniso_u13: YPD//wAAAABABgAA
atoms_aniso_u23: YPD//wAAAABABgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEAAgAABAAgAABABAAAIAEAABABAAAgBAAAABAABAEAAIAgABACAAQBAAEAgAAAQ==


formula: Mg1.92 Si.98 O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 489 K
formula_title: <missing>
a: 8.0976
b: 8.0976
c: 8.0976
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.969
crystal_density: 3.457
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBg4Q4A
atoms_y: gIQeACChBwBg4Q4A
atoms_z: gIQeACChBwBg4Q4A
atoms_occupancy: AJg6AIDQOwAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: gKIAADCOAADQnQAA
atoms_aniso_u22: gKIAADCOAADQnQAA
atoms_aniso_u33: gKIAADCOAADQnQAA
atoms_aniso_u12: QO3//wAAAADg/P//
atoms_aniso_u13: QO3//wAAAADg/P//
atoms_aniso_u23: QO3//wAAAADg/P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAEABAAABAAgAACABAAAIAIAACACAABACAAAACAACAEAAIAgABAEAAQBAAIAgAAAQ==


formula: Mg1.92 Si O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 537 K
formula_title: <missing>
a: 8.1030
b: 8.1030
c: 8.1030
alpha: 90
beta: 90
gamma: 90
cell_volume: 532.032
crystal_density: 3.464
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwDQ3w4A
atoms_y: gIQeACChBwDQ3w4A
atoms_z: gIQeACChBwDQ3w4A
atoms_occupancy: AJg6AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: UKoAAEC1AABgnwAA
atoms_aniso_u22: UKoAAEC1AABgnwAA
atoms_aniso_u33: UKoAAEC1AABgnwAA
atoms_aniso_u12: cOX//wAAAACADAAA
atoms_aniso_u13: cOX//wAAAACADAAA
atoms_aniso_u23: cOX//wAAAACADAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAACAABAAAAEAAIAAACAAIAAAIABAAACABAAAEACAAAQAIAACAEAABACAAAAEAAEAIAAQBAACAIAAgCAAIAgAAAg==


formula: Mg1.88 Si.98 O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 586 K
formula_title: <missing>
a: 8.1084
b: 8.1084
c: 8.1084
alpha: 90
beta: 90
gamma: 90
cell_volume: 533.096
crystal_density: 3.419
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBA3g4A
atoms_y: gIQeACChBwBA3g4A
atoms_z: gIQeACChBwBA3g4A
atoms_occupancy: gF85AIDQOwAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: oL4AABC9AABAzgAA
atoms_aniso_u22: oL4AABC9AABAzgAA
atoms_aniso_u33: oL4AABC9AABAzgAA
atoms_aniso_u12: AOf//wAAAACADAAA
atoms_aniso_u13: AOf//wAAAACADAAA
atoms_aniso_u23: AOf//wAAAACADAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAgAAEAAAACAACAAAAEAAIAAACAAQAAAIACAAAEABAAAEACAAAQAQAAEAEAACACAAAAEAAEAQAAQBAACAQAAgCAAQBAAABA==


formula: Mg1.84 Si.95 O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 635 K
formula_title: <missing>
a: 8.1164
b: 8.1164
c: 8.1164
alpha: 90
beta: 90
gamma: 90
cell_volume: 534.676
crystal_density: 3.364
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwDQ3w4A
atoms_y: gIQeACChBwDQ3w4A
atoms_z: gIQeACChBwDQ3w4A
atoms_occupancy: ACc4AMD7OQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: cMYAAEC1AACw5QAA
atoms_aniso_u22: cMYAAEC1AACw5QAA
atoms_aniso_u33: cMYAAEC1AACw5QAA
atoms_aniso_u12: YNf//wAAAADwCgAA
atoms_aniso_u13: YNf//wAAAADwCgAA
atoms_aniso_u23: YNf//wAAAADwCgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAQAAAAAAQAAAgAAAAAgAAIAAAAEAACAAAAIAAQAAAEAAQAAAQACAAAEACAAAEAEAAAgAQAAEAIAAEAEAAAAIAAIAQAAgCAAEAgABAIAAQCAAACA==


formula: Mg1.88 Si.95 O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 685 K
formula_title: <missing>
a: 8.1279
b: 8.1279
c: 8.1279
alpha: 90
beta: 90
gamma: 90
cell_volume: 536.951
crystal_density: 3.374
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBg4Q4A
atoms_y: gIQeACChBwBg4Q4A
atoms_z: gIQeACChBwBg4Q4A
atoms_occupancy: gF85AMD7OQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: cBEBAAD6AABAGQEA
atoms_aniso_u22: cBEBAAD6AABAGQEA
atoms_aniso_u33: cBEBAAD6AABAGQEA
atoms_aniso_u12: gNr//wAAAABABgAA
atoms_aniso_u13: gNr//wAAAABABgAA
atoms_aniso_u23: gNr//wAAAABABgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAACAAAAAAAAEAAAAQAAAAAAQAAAgAAAABAAAQAAAAEAAEAAAAIAAgAAAEAAgAAAgAEAAAIACAAAQAIAABABAAAQAQAAIAIAAAAQAAQBAACAEAAIAgAEAQABAIAAAEA==


formula: Mg1.84 Si.93 O4
compound: Synthetic
pub_title: Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O Note: T = 736 K
formula_title: <missing>
a: 8.1430
b: 8.1430
c: 8.1430
alpha: 90
beta: 90
gamma: 90
cell_volume: 539.950
crystal_density: 3.317
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwBg4Q4A
atoms_y: gIQeACChBwBg4Q4A
atoms_z: gIQeACChBwBg4Q4A
atoms_occupancy: ACc4AEDDOAAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: UEABALAwAQAwVgEA
atoms_aniso_u22: UEABALAwAQAwVgEA
atoms_aniso_u33: UEABALAwAQAwVgEA
atoms_aniso_u12: cMz//wAAAABwFwAA
atoms_aniso_u13: cMz//wAAAABwFwAA
atoms_aniso_u23: cMz//wAAAABwFwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAQAAAAIAAIAAAAQABAAAAQABAAABAAIAAAQAIAAAgAQAACACAAAgAgAAQAgAAABAABAEAAEAQAAgEAAIBAACAQAAAQA==


formula: Mg1.88 Si.96 O4
compound: Synthetic
formula_title: <missing>
a: 8.0947
b: 8.0947
c: 8.0947
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.398
crystal_density: 3.423
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwCA5A4A
atoms_y: gIQeACChBwCA5A4A
atoms_z: gIQeACChBwCA5A4A
atoms_occupancy: gF85AACYOgAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: YIYAAECcAABwlAAA
atoms_aniso_u22: YIYAAECcAABwlAAA
atoms_aniso_u33: YIYAAECcAABwlAAA
atoms_aniso_u12: sOv//wAAAACADAAA
atoms_aniso_u13: sOv//wAAAACADAAA
atoms_aniso_u23: sOv//wAAAACADAAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 635 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEAAgAABAAgAACABAAAIAEAABACAABABAAAACAACAEAAIAgABAEAAQBAAEAgAAAQ==


formula: Mg1.86 Si.94 O4
compound: Synthetic
formula_title: <missing>
a: 8.1031
b: 8.1031
c: 8.1031
alpha: 90
beta: 90
gamma: 90
cell_volume: 532.051
crystal_density: 3.386
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwCA5A4A
atoms_y: gIQeACChBwCA5A4A
atoms_z: gIQeACChBwCA5A4A
atoms_occupancy: QMM4AIBfOQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: 4KsAABC9AABAzgAA
atoms_aniso_u22: 4KsAABC9AABAzgAA
atoms_aniso_u33: 4KsAABC9AABAzgAA
atoms_aniso_u12: cOX//wAAAACQGgAA
atoms_aniso_u13: cOX//wAAAACQGgAA
atoms_aniso_u23: cOX//wAAAACQGgAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 685 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAACAABAAAAEAAIAAACAAIAAAIABAAACABAAAEACAAAQAIAACAEAABACAAAAEAAEAIAAQBAACAIAAgCAAIAgAAAg==


formula: Mg1.84 Si.91 O4
compound: Synthetic
formula_title: <missing>
a: 8.1115
b: 8.1115
c: 8.1115
alpha: 90
beta: 90
gamma: 90
cell_volume: 533.708
crystal_density: 3.342
atoms_sites: ["Mg", "Si", "O"]
atoms_x: gIQeACChBwCg5w4A
atoms_y: gIQeACChBwCg5w4A
atoms_z: gIQeACChBwCg5w4A
atoms_occupancy: ACc4AMCKNwAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si", "O"]
atoms_aniso_u11: YNEAAODdAACABgEA
atoms_aniso_u22: YNEAAODdAACABgEA
atoms_aniso_u33: YNEAAODdAACABgEA
atoms_aniso_u12: oN3//wAAAACwHQAA
atoms_aniso_u13: oN3//wAAAACwHQAA
atoms_aniso_u23: oN3//wAAAACwHQAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 736 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAQAAAgAAAAAgAAIAAAACAACAAAAEAAQAAACAAQAAAIACAAAEABAAAEACAAAQAQAAEAEAACACAAAAIAAIAQAAQBAAEAQAAgEAAQCAAABA==


formula: Mg1.88 Si.97 O4
compound: Synthetic
formula_title: <missing>
a: 8.0947
b: 8.0947
c: 8.0947
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.398
crystal_density: 3.430
atoms_sites: ["Mg", "Si1", "Si2", "O"]
atoms_x: gIQeACChBwCAhB4AEOYOAA==
atoms_y: gIQeACChBwCAhB4AEOYOAA==
atoms_z: gIQeACChBwAAAAAAEOYOAA==
atoms_occupancy: gF85AMD7OQBAnAAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si1", "O"]
atoms_aniso_u11: YIYAAECcAAAgmQAA
atoms_aniso_u22: YIYAAECcAAAgmQAA
atoms_aniso_u33: YIYAAECcAAAgmQAA
atoms_aniso_u12: QO3//wAAAACADAAA
atoms_aniso_u13: QO3//wAAAACADAAA
atoms_aniso_u23: QO3//wAAAACADAAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 635 K, split Si model

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEAAgAABAAgAACABAAAIAEAABACAABABAAAACAACAEAAIAgABAEAAQBAAEAgAAAQ==


formula: Mg1.84 Si.98 O4
compound: Synthetic
formula_title: <missing>
a: 8.1031
b: 8.1031
c: 8.1031
alpha: 90
beta: 90
gamma: 90
cell_volume: 532.051
crystal_density: 3.402
atoms_sites: ["Mg", "Si1", "Si2", "O"]
atoms_x: gIQeACChBwCAhB4AoOcOAA==
atoms_y: gIQeACChBwCAhB4AoOcOAA==
atoms_z: gIQeACChBwAAAAAAoOcOAA==
atoms_occupancy: ACc4AAAnOADA1AEAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si1", "O"]
atoms_aniso_u11: ILIAAMDBAAAQ1gAA
atoms_aniso_u22: ILIAAMDBAAAQ1gAA
atoms_aniso_u33: ILIAAMDBAAAQ1gAA
atoms_aniso_u12: cOX//wAAAACQGgAA
atoms_aniso_u13: cOX//wAAAACQGgAA
atoms_aniso_u23: cOX//wAAAACQGgAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 685 K, split Si model

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAACAABAAAAEAAIAAACAAIAAAIABAAACABAAAEACAAAQAIAACAEAABACAAAAEAAEAIAAQBAACAIAAgCAAIAgAAAg==


formula: Mg1.8 Si.97 O4
compound: Synthetic
formula_title: <missing>
a: 8.1115
b: 8.1115
c: 8.1115
alpha: 90
beta: 90
gamma: 90
cell_volume: 533.708
crystal_density: 3.360
atoms_sites: ["Mg", "Si1", "Si2", "O"]
atoms_x: gIQeACChBwCAhB4AwOoOAA==
atoms_y: gIQeACChBwCAhB4AwOoOAA==
atoms_z: gIQeACChBwAAAAAAwOoOAA==
atoms_occupancy: gO42AMAZNQBADQMAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["Mg", "Si1", "O"]
atoms_aniso_u11: 4N0AALDlAAAAEwEA
atoms_aniso_u22: 4N0AALDlAAAAEwEA
atoms_aniso_u33: 4N0AALDlAAAAEwEA
atoms_aniso_u12: MN///wAAAACwHQAA
atoms_aniso_u13: MN///wAAAACwHQAA
atoms_aniso_u23: MN///wAAAACwHQAA
pub_title:
 Compressibility and thermal expansion of hydrous ringwoodite with 2.5(3) wt% H2O
 Note: at room T after heating to T = 736 K, split Si model

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAQAAAgAAAAAgAAIAAAACAACAAAAEAAQAAACAAQAAAIACAAAEABAAAEACAAAQAQAAEAEAACACAAAAIAAIAQAAQBAAEAQAAgEAAQCAAABA==


formula: Sr.966 Fe.001 Ba.001 S O4
compound: Saxony, Ngar Majunga, Madagascar
formula_title: <missing>
a: 6.87032
b: 8.36030
c: 5.34732
alpha: 90
beta: 90
gamma: 90
cell_volume: 307.139
crystal_density: 3.912
atoms_sites: ["Sr", "Fe", "Ba", "S", "O1", "O2", "O3"]
atoms_x: 0KgJANCoCQDQqAkAsD8LANCxBQCQcgIAAAsTAA==
atoms_y: yDsLAMg7CwDIOwsAQMgaAABUJAAwuBIAcMYZAA==
atoms_z: QEIPAEBCDwBAQg8AwMYtAMDGLQDAxi0AcHc7AA==
atoms_occupancy: wPU6AKAPAACgDwAAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0J0AANCdAADQnQAAEIsAAIAGAQAw8gAAAK8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural trends for celestite (SrSO4), anglesite (PbSO4), and barite (BaSO4):
 confirmation of expected variations within SO4 groups

qdat:
AAAAAAAAAAAAAAAAAAAAAAAQBgABAAEAAgAIQAIUAAoBggEAIiQYQAACoACAyl4CgawICCFqMEUUSAPThaUujjTWYPyUrs5Bbpbd7EeKNP/Cnfx9VS9s59s28dm2/t2/3Tff+tla63c+f2++P+G/e+/9+vXzf///77Lf33==


formula: Pb S O4
compound: Synthetic
formula_title: <missing>
a: 6.95802
b: 8.48024
c: 5.39754
alpha: 90
beta: 90
gamma: 90
cell_volume: 318.486
crystal_density: 6.325
atoms_sites: ["Pb", "S", "O1", "O2", "O3"]
atoms_x: 0DQKAFA2CwAQ0QUAoOQCACDcEgA=
atoms_y: sHYLAKCfGgCQIyQAAMASAHCUGQA=
atoms_z: QEIPAMDGLQDAxi0AwMYtALB9OwA=
atoms_occupancy: 0
atoms_u_iso: 4CgBACCAAABQQAEAEGwBAIDtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural trends for celestite (SrSO4), anglesite (PbSO4), and barite (BaSO4):
 confirmation of expected variations within SO4 groups

qdat:
AAAAAAAAAAAAAAAAAAAAAAAgGAAEAAQAEABBABBgADAEEAgCIYCEAAAyABAERsBQGkGBCiyKCKWJALjgqEtKTm5obhq0sWE2xb58Idsr1oQ/9p5lV/Z65Z3i9mj/Pv8td19nffVb7fr7RPHem/+f8+/n35e//127s7b/lr==


formula: Ba.985 Sr.007 Mg.002 Ca.002 S O4
compound: Elk Creek, South Dakota, USA
formula_title: <missing>
a: 7.15505
b: 8.88101
c: 5.45447
alpha: 90
beta: 90
gamma: 90
cell_volume: 346.599
crystal_density: 4.447
atoms_sites: ["Ba", "Sr", "Mg", "Ca", "S", "O1", "O2", "O3"]
atoms_x: OKUJADilCQA4pQkAOKUJAOixCwAQmQYAAO4CAFDtEgA=
atoms_y: CEILAAhCCwAIQgsACEILADi8GgAg2iMAsHMTAICiGQA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAMDGLQDAxi0AwMYtAHAsOwA=
atoms_occupancy: oB48AGBtAABAHwAAQB8AAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: AK8AAACvAAAArwAAAK8AAFBfAAAgFgEAgKIAAGCGAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural trends for celestite (SrSO4), anglesite (PbSO4), and barite (BaSO4):
 confirmation of expected variations within SO4 groups

qdat:
AAAAAAAAAAAAAAAAAAAAAAECQABAAIAEABAgAiIAQgTAAggZILAAAmQEAAPHFCmyiDgMWQhhILCz1CVwuDWmFPkFGfSvZZKXWZDOq3Zsdn7H/FxvnbJy/vX3f/v5992/9b+/3y96n192/+9/vubvvevP///8//+//8f6/V==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9541
b: 7.9494
c: 5.7186
alpha: 90
beta: 90
gamma: 90
cell_volume: 225.211
crystal_density: 2.956
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAAABHQA=
atoms_y: 8FUZAPBVGQDgkS4AwGs4AECHKQA=
atoms_z: cGEuAHBhLgBgkfr/cCL6/9Co+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: IMsAACDLAABg6gAAYOoAAMDaAAA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: 4CgBAOAoAQCAOAEA4KUBAEAZAQA=
atoms_aniso_u22: wNoAAMDaAACghgEAYG0AACDLAAA=
atoms_aniso_u33: YG0AAGBtAAAAAAAA4KsAAECcAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAACBOAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAEAfAAA=
atoms_aniso_u23: UPv//1D7//9g8P//YPD//wAAAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 184 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIAgABAAAAACAIAAAIEIQgBIBAACgAAkFBCKBAAUAgOMIlUAQYARpIhKAARknM0uCUEXYhTJDESJOggSYSbqpMLTtNpATWfmFhSa9Vcd1rSvKX7qtft35Yyc/GttWfO0/ejd1673pr8F7==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9564
b: 7.9536
c: 5.7253
alpha: 90
beta: 90
gamma: 90
cell_volume: 225.698
crystal_density: 2.950
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAMD6HAA=
atoms_y: 8FUZAPBVGQBAmy4AwGs4ACCEKQA=
atoms_z: AGMuAABjLgCgsPr/8C76/6Cw+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: wNoAAMDaAAAA+gAAYOoAAGDqAAA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: QBkBAEAZAQAAdwEAoIYBAOAoAQA=
atoms_aniso_u22: APoAAAD6AAAAdwEAAH0AAMDaAAA=
atoms_aniso_u33: oIwAAKCMAAAAAAAAQJwAACDLAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAGBtAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u23: QAYAAEAGAADgsf//gMH//6APAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 224 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIAgABAAAAACAIAAAIEYQgBIBAACgABEFBCKBAAUAgMMIlkAQYARLZhKAARFHMlMEYIe5hlLGEmbbAgUokbyrYNneL6A2ctuKiUu1pcvf62vSv6vZd+/6xW9+KtXa/c5v0mfNs1mzXYJ1==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9579
b: 7.9595
c: 5.7328
alpha: 90
beta: 90
gamma: 90
cell_volume: 226.230
crystal_density: 2.943
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAID0HAA=
atoms_y: QFEZAEBRGQBAgi4AEGc4APCLKQA=
atoms_z: wFwuAMBcLgBAwPr/sCj6/4Ct+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: QJwAAECcAABAnAAAwNoAAAB9AAA=
atoms_aniso_label: ["Ca", "Sr", "O1", "O2"]
atoms_aniso_u11: oAkBAKAJAQAA9AEAYG0AAA==
atoms_aniso_u22: IE4AACBOAAAAAAAAwF0AAA==
atoms_aniso_u33: AH0AAAB9AADgqwAAgLsAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAYPD//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAYPD//w==
atoms_aniso_u23: YPD//2Dw//8gTgAAwOD//w==
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 265 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIAgABAAAAAEAIAAAYEQggBIDAACgABIJCESBAAoAgMIQlkAwoAhSRiMAATNONlcE4IszCmSKIkaeBg0ok2y2YbOefWAk8/cPEtd7r42f+1WTvs/S79dMjr/uTb2/tu7/dM/e15N2t4nn==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9596
b: 7.9644
c: 5.7416
alpha: 90
beta: 90
gamma: 90
cell_volume: 226.795
crystal_density: 2.935
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAOD9HAA=
atoms_y: YFQZAGBUGQBAgi4AsF04AECHKQA=
atoms_z: wFwuAMBcLgAAofr/EDL6/6Cw+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: YOoAAGDqAACgCQEAQBkBAAD6AAA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: wFcBAMBXAQCgCQEAAPQBAMDaAAA=
atoms_aniso_u22: APoAAAD6AACgAwIAAH0AAOAoAQA=
atoms_aniso_u33: oIwAAKCMAAAAAAAAYOoAAMDaAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAIA+AAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAEAfAAA=
atoms_aniso_u23: wPn//8D5//+Awf//oA8AAGDw//8=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 300 K, low-temperature experiment

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIBAABAAAAAEAIAAAQEQggBICAACgABILCESCAAoAgcYRKkAwoAjmREYAAiOOJJcFoI9TEqSUJMWcBBpQl+jUovccf0Bt9qUVJdbrW7u/712m94+y7uXInX/82bs/bV36+5fu7zJ1XQnP==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9615
b: 7.9629
c: 5.7428
alpha: 90
beta: 90
gamma: 90
cell_volume: 226.886
crystal_density: 2.934
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAJACHQA=
atoms_y: 8FUZAPBVGQCAoS4A4G44APCLKQA=
atoms_z: AGMuAABjLgDgz/r/ACT6/7C++v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: oAkBAKAJAQCgCQEA4CgBAKAJAQA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: QBkBAEAZAQCgCQEAIMUBAAB9AAA=
atoms_aniso_u22: APoAAAD6AABAEwIAIE4AAKAJAQA=
atoms_aniso_u33: oAkBAKAJAQAAAAAAAHcBAECWAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAMBdAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAEAfAAA=
atoms_aniso_u23: AOf//wDn//+APgAAAAAAAOAuAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 300 K, high-temperature experiment

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIBAABAAAAAEAIAAAQEQggBICAACgABQLCEUCAAoBAcYhKkBgwBDmREYAAieMZKYFoI91EqSUJM2cBhpQl/lUovcc/0Bt9qUWJebrWr+9712ndp+1fuXInX+9Wb1/bV3q+5/+yzL1fRGX==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9638
b: 7.9698
c: 5.7545
alpha: 90
beta: 90
gamma: 90
cell_volume: 227.651
crystal_density: 2.924
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPADD5HAA=
atoms_y: SFMZAEhTGQBQdy4AoE84AJCCKQA=
atoms_z: AGMuAABjLgBg3Pr/wDb6//DE+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: wCUBAMAlAQAA+gAAIEgBACBIAQA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: gDgBAIA4AQDA1AEAIMUBACDLAAA=
atoms_aniso_u22: IMsAACDLAACgCQEAgD4AAAD6AAA=
atoms_aniso_u33: AHcBAAB3AQAAAAAAIMUBAKADAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAB9AAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u23: IAMAACADAACgDwAAYPD//3AwAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 359 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAIBAABAAAAAIAIAAAwExAgBICAAEgACQKEEkCAAwBAYQhVIBhQBDKjEQAAiaYbK4JwIp2I0UoRYs4DDRRJ/m5Re44/sCn6+oWS87WVL9d/b8pbq/Vu9uRfP/8q3Neuvrttz/dj27yekcf==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9667
b: 7.9775
c: 5.7680
alpha: 90
beta: 90
gamma: 90
cell_volume: 228.539
crystal_density: 2.913
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPALDsHAA=
atoms_y: uFEZALhRGQAAlS4AQEY4AACBKQA=
atoms_z: cGEuAHBhLgBgDvv/wDb6/8DM+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: AHcBAAB3AQDgKAEAIMUBAECWAQA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: QJYBAECWAQBAkAIAYOQBAKCGAQA=
atoms_aniso_u22: oAkBAKAJAQAgywAAoIwAAKAJAQA=
atoms_aniso_u33: wNQBAMDUAQAAAAAAwM4CAOAiAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAECcAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u23: 8AoAAPAKAACAwf//wOD//4A+AAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 415 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAIBAABAAAAAIAQAAAwIxBABQGAAFAACgWIFEEABgBAYRCVIDCQCHUlIgABE8oqVoNQTpyRUtQyp4wCFihV/LyS+x6tYFOz+xsmx+unbndnXtz/N+pZmZmkTu5Xaez8t29Nr7v2tdpdIv/==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9692
b: 7.9873
c: 5.7796
alpha: 90
beta: 90
gamma: 90
cell_volume: 229.395
crystal_density: 2.902
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAJDpHAA=
atoms_y: wFMZAMBTGQAwdC4AkEE4AACBKQA=
atoms_z: UF4uAFBeLgAw/fr/8Ef6/5DU+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: oIYBAKCGAQCAOAEAIMUBAIC1AQA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: QJYBAECWAQCArwIAwFECAECWAQA=
atoms_aniso_u22: gDgBAIA4AQAA+gAAQJwAAAB3AQA=
atoms_aniso_u33: gLUBAIC1AQCgDwAAAHECAOAiAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAACDLAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAEAfAAA=
atoms_aniso_u23: wPn//8D5//9g8P//AAAAABAnAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 471 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQBAACAAAAAQAQAAAwJSBACQGAAFAACgWIJIEACgBA4xCpQFCgEGlqRgABJZY2bIdQm3khlahlLpwGLFCn6OkW9R12oKdXtjVNx69GXO7OXXj8r3T7szLOXdye4t35+9r1r9f+brjWld/==


formula: (Ca.997 Sr.003) C O3
compound: natural, unknown locality
formula_title: <missing>
a: 4.9723
b: 7.9983
c: 5.7931
alpha: 90
beta: 90
gamma: 90
cell_volume: 230.391
crystal_density: 2.890
atoms_sites: ["Ca", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPACDrHAA=
atoms_y: kFEZAJBRGQBAUC4A8DE4ABCPKQA=
atoms_z: oFkuAKBZLgBQAPv/8GD6/6Di+v8=
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQA=
atoms_u_iso: IMUBACDFAQBgZwEA4CICAEATAgA=
atoms_aniso_label: ["Ca", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: IMUBACDFAQBAlgEAQJACAEAZAQA=
atoms_aniso_u22: YGcBAGBnAQBg5AEA4CgBACBCAgA=
atoms_aniso_u33: gDICAIAyAgAgywAAgK8CAADuAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAKCMAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u23: wPn//8D5//+gkv//YPD//0AfAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 527 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQBAACAAAAAQAQAABQRSBACgKAAJAAFAqQKIIADACAxiCxQJEgINLERgACK6xceQ6gqlmDJ0jGXTgMVJC3SdItrTttQapm7GqrnV9c+PyIkeP5P5d31pM99vk/x9br77bvfV34X9L6U3f==


formula: (Ba.981 Sr.019) C O3
compound: Hexham, Northumberland, England
formula_title: <missing>
a: 5.3193
b: 8.9056
c: 6.4353
alpha: 90
beta: 90
gamma: 90
cell_volume: 304.850
crystal_density: 4.279
atoms_sites: ["Ba", "Sr", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPALAkHAA=
atoms_y: 2GgZANhoGQAgNC4AsP82AIC/KQA=
atoms_z: YA0uAGANLgCAKvv/oJf6/9Dz+v8=
atoms_occupancy: IOA7AOAoAQAACT0AAAk9AAAJPQA=
atoms_u_iso: kOIAAJDiAADgKAEAQEsBACAvAQA=
atoms_aniso_label: ["Ba", "Sr", "C", "O1", "O2"]
atoms_aniso_u11: 4PYAAOD2AACAtQEAoIYBAGDqAAA=
atoms_aniso_u22: cMYAAHDGAADA2gAAYOoAAOAoAQA=
atoms_aniso_u33: YOoAAGDqAAAgywAAYGcBAAB3AQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: QAYAAEAGAADA4P//oA8AAAAAAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAQAAEAEAAQAAAEACAAAhJQgCESBAgCAQhLEgIQSAAUoqNQSAkk0nAiAAg23JCZQWDtQ4xqFL6KUqGzuwWMV/PZLtxpHegfR+v0N2dN8/97vh3bb+T+u5N/2v//cl168/b4avj/PWuZP+/r/Xb/7==


formula: (Sr.853 Ca.147) C O3
compound: Dreisteinfurt, Westphalia, Germany
formula_title: <missing>
a: 5.0914
b: 8.3519
c: 5.9901
alpha: 90
beta: 90
gamma: 90
cell_volume: 254.716
crystal_density: 3.667
atoms_sites: ["Sr", "Ca", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPAOCZHAA=
atoms_y: sGMZALBjGQBgOi4AQLA3AECHKQA=
atoms_z: 0DguANA4LgBAwPr/gGL6/6DJ+v8=
atoms_occupancy: IBA0AOD4CAAACT0AAAk9AAAJPQA=
atoms_u_iso: sP4AALD+AABg6gAAwNoAALDMAAA=
atoms_aniso_label: ["Sr", "Ca", "C", "O1", "O2"]
atoms_aniso_u11: cBEBAHARAQBAlgEA4KsAAIC7AAA=
atoms_aniso_u22: ABMBAAATAQCAOAEAAPoAAGDqAAA=
atoms_aniso_u33: wNoAAMDaAAAAAAAAwNoAAIC7AAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAMDg//8=
atoms_aniso_u23: kAEAAJABAAAg0f//oJL//yDR//8=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAgAgABAAAAAgBAAAEUEgCAMCQAQQAAgOIiEEASAAVpCTRAhQhCq8EgAAo264ZmhFMPOFVQiYerNBOAPvNhRv7fXELI415QRv+OP97rTYtz3/wbeuN3M/xLnWu97Z3/v21/23aHr/+n3+31==


formula: Pb Ca.001 C O3
compound: Tsumeb, Namibia
formula_title: <missing>
a: 5.1820
b: 8.4953
c: 6.1436
alpha: 90
beta: 90
gamma: 90
cell_volume: 270.458
crystal_density: 6.563
atoms_sites: ["Pb", "Ca", "C", "O1", "O2"]
atoms_x: QEIPAEBCDwBAQg8AQEIPABBHHAA=
atoms_y: kHQZAJB0GQAAri4A0LE3AADlKQA=
atoms_z: CAYuAAgGLgAAiPr/cDv6/zCy+v8=
atoms_occupancy: YPk8AKAPAAAACT0AAAk9AAAJPQA=
atoms_u_iso: 0M8AANDPAABg6gAAwFcBAGA1AQA=
atoms_aniso_label: ["Pb", "Ca", "C", "O1", "O2"]
atoms_aniso_u11: 0M8AANDPAACgjAAA4KUBAMBXAQA=
atoms_aniso_u22: IOQAACDkAACgAwIAwNoAACBIAQA=
atoms_aniso_u33: EL0AABC9AABAHwAAQJYBAAD6AAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAOAuAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAKAPAAA=
atoms_aniso_u23: kAEAAJABAAAAAAAAoJL//6APAAA=
pub_title:
 Crystal structure and thermal expansion of aragonite-group carbonates
 by single-crystal X-ray diffraction
 Note: T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAgAACAEAAQAAAAgAQAACGEoBAECIAIIADAZgoIIAoAAw0QoiQGCQcrgqAAFY5XCk8I0F3CVwxIu6VUHAOeuyc6Xe+kzhzXiLi1Rfn/d1Ni9N7lL92B8tuZNv1d+3e/fuXbd8/LGw71uw+O/u97==


formula: U P O9 (Na H6)
compound: Lake Boga Granite, Victoria, Australia
formula_title: <missing>
a: 6.9935
b: 6.9935
c: 17.5101
alpha: 90
beta: 90
gamma: 90
cell_volume: 856.402
crystal_density: 3.428
atoms_sites: ["U", "P", "O1", "O2", "O3", "Na4", "Wat4"]
atoms_x: QEIPAMDGLQBAQg8AQEIPAPDjKwAgjwoAII8KAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAICjBACATTwAgE08AA==
atoms_z: 2AYDAAAAAABANAkAwMk5AOBUGwBg+xIAYPsSAA==
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQBAQg8AwMYtAA==
atoms_u_iso: 0DMBADAkAQBAEwIAoAMCAIAZAgBguggAYLoIAA==
atoms_aniso_label: ["U", "P", "O1", "O2", "O3"]
atoms_aniso_u11: kOIAAMCPAABg5AEAwNQBAOCfAgA=
atoms_aniso_u22: kOIAAMCPAABg5AEAwNQBAIC7AAA=
atoms_aniso_u33: wNQBABBNAgAAcQIAIEICAGDeAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAACDR//8=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAACDR//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 The crystal structure of metanatroautunite, Na[(UO2)(PO4)](H2O)3,
 from the Lake Boga Granite, Victoria, Australia
 Note: z-coordinate of U changed from .40959 to match reported bond lengths

qdat:
AAAAAAAAAAAAgAAAAAAAAQAAoAAAAAgAwAABAAIAACIAgACLDACAIgAEkAAJAgAVGABpgJASAoAAuIEkgAoAKEg8wRWAokKkHqAMAJEGAB0E2kiBgByFUBSFKGQGhhQiFoog0D2fiaDEYA0SoRGAyDZCnR+WhwIRgfQogY==


formula: Fe Ti3 O7
compound: Synthetic
formula_title: FeTi3O7
a: 9.9522
b: 2.7397
c: 5.9953
alpha: 90
beta: 90
gamma: 90
cell_volume: 163.468
crystal_density: 6.328
atoms_sites: ["Fe1", "Ti1", "Ti2", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAACANQ4AAAAAANBjEgDguycAIAQ2AA==
atoms_y: AAAAAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_z: oJYoACCDDAAAsDYA4DT//2AMJQBgnA0AQI8XAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure and high-temperature phase transitions in FeTiO3
 and a new dense FeTi3O7 structure
 Note: P = 61 GPa, T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAIgAAAAAAAAAAAAAggAACBAwAAAAgAEAABECEAAAECQAQBgAAQBAAQhIDEIAYIEAg0CCQgAsQBI4MIDAQAAwERSVE0IBBgqIQkBIgIIKrgAYZRBgkk2LAIFACBojIcKoCOCQEDcaCDkWQKCuQ6J==


formula: Ti S
compound: Synthetic
pub_title: Zur Kristallstruktur der Titansulfide
formula_title: <missing>
a: 3.417
b: 3.417
c: 26.455
alpha: 90
beta: 90
gamma: 120
cell_volume: 267.503
crystal_density: 4.466
atoms_sites: ["Ti1", "Ti2", "S1", "S2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: gIQeAEASFwAAAAAAQMsNAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAABAAAAAAAAAAACAAAAAAAAAAACIABAEAAAAgAEAAAAAQAAAAAAAIEAACAAAABQEEAAgEAAAQAAAAAAAAAAACgiACBAACAAAARABAAAgAAAAAAAAACQBAADEQCEACAAAAAAADEgIgAgAAAAAAMkBEAQAASAgA==


formula: Fe Sb2 O4
compound: <missing>
formula_title: <missing>
a: 8.5758
b: 8.5758
c: 5.8983
alpha: 90
beta: 90
gamma: 90
cell_volume: 433.787
crystal_density: 5.564
atoms_sites: ["Fe", "Sb", "O1", "O2"]
atoms_x: AAAAAGCuCgCAQikA4AoGAA==
atoms_y: gIQeAIACCgAAvgoA4LsnAA==
atoms_z: QEIPAAAAAABAQg8AAAAAAA==
atoms_occupancy: 0
atoms_u_iso: QBkBAIA+AAAA3AUAoA8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Advances in data reduction of high-pressure X-ray powder diffraction data from
 two-dimensional detectors: a case study of schafarzikite (FeSb2O4)
 Note: P = 0.5 GPa

qdat:
AAAAAAAAAAAAAAAAAIAAAAAAIAAIAAQAEAEEAACEAAEQhAAEBEIBkICAEECBIiJECRAAQgCyIYKYYSQ0RloFChYhRtGIhrGqBiEciNqi6jFSoc3JkZhRUztCVUTZk7z0WNal+aaJy2Zybpk+fk/xnW7c7tE8fMrZKiRIpV==


formula: Fe Sb2 O4
compound: <missing>
formula_title: <missing>
a: 5.7792
b: 8.3134
c: 8.4545
alpha: 90
beta: 91.879
gamma: 90
cell_volume: 405.976
crystal_density: 5.945
atoms_sites: ["Fe", "Sb1", "Sb2", "O1", "O2", "O3", "O4"]
atoms_x: AKwNAMBj//9AZR4AYJwNACBrEACgCQEAgIQeAA==
atoms_y: AAAAAIB/CgBAZDMAoIoqACBTFADAvAUAAHwVAA==
atoms_z: AEYeAMCkCQAgDAsA4PIJAIASMQAAgSkAAF8FAA==
atoms_occupancy: 0
atoms_u_iso: 4C4AAMBXAQBADQMAwNQBAICpAwCAqQMAgKkDAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Advances in data reduction of high-pressure X-ray powder diffraction data from
 two-dimensional detectors: a case study of schafarzikite (FeSb2O4)
 Note: P = 4.2 GPa, this is denoted as Phase II

qdat:
AAAAAAAAAAAAAAAAACQAAAgABSABgAAwACAIIAIJSAADSwYABkIRIsZTYCEwkFqWRMZKgBKMH7ZvF6XFQZ8/bBYPO17n/U6OrX5f5c+3nm7+1WebZT/+5/t7z35T+/vs/fr7Wq/Pv9Pv/r3if9+v8z/Pjvv/9fj7921fuX==


formula: Fe Sb2 O4
compound: <missing>
formula_title: <missing>
a: 7.8498
b: 7.8498
c: 5.7452
alpha: 90
beta: 90
gamma: 90
cell_volume: 354.016
crystal_density: 6.817
atoms_sites: ["Fe", "Sb1", "Sb2", "O1", "O2", "O3"]
atoms_x: AAAAAID99f8ABRQAoJApAKDlBgDgeh0A
atoms_y: gIQeAEBmCQAg2ycAgA4IAIDRJgDAAw8A
atoms_z: wIwNAAAAAAAAAAAAgG0NAAAAAAAAAAAA
atoms_occupancy: 0
atoms_u_iso: YG0AAAD6AACAtQEAoA8AAKAPAACgDwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Advances in data reduction of high-pressure X-ray powder diffraction data from
 two-dimensional detectors: a case study of schafarzikite (FeSb2O4)
 Note: P = 10.5 GPa, this is denoted as Phase III

qdat:
AAAAAAAAAAAAAIAAAABAAACAAASAABAAIAAgECBAghQAgQgQQAAEEIQhKBgGJAIACAmJgwkBBAQMkXDBkwQRYIoIgkII5YYxSxDGMWJyRjGM446kN+jP0SM/rO5wanUTZwt7n+aM85dtN5pi9P2hRWb5j9I/qUnFOjdRXQ==


formula: Cu6 Hg3 As4 S12
compound: not given
pub_title: Isotypy in aktashite Cu6Hg3As4S12 and nowackiite Cu6Zn3As4S12
formula_title: <missing>
a: 13.730
b: 13.730
c: 9.329
alpha: 90
beta: 90
gamma: 120
cell_volume: 1523.024
crystal_density: 5.454
atoms_sites: ["Cu1", "Cu2", "Hg", "As1", "As2", "S1", "S2", "S3", "S4"]
atoms_x: gKMEADDlFwDA6xIAoD0iAAAAAACQwhYAsPIbACA9BwBAbQwA
atoms_y: ENQRAACxIQDwzw0AQN0KAAAAAACwfAUAgB8aABCHCQDg/RwA
atoms_z: 4C4AAEAZAQCQfgAAAAAAAADdOwAgMAUAQAcEAPCVBgCQ3QUA
atoms_occupancy: 0
atoms_u_iso: 4MkAAOjBAADgfQEAcJQAAJApAAAQWQAAKEsAAJiAAADgagAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIIAAAABAAAQBIAEAEAICAAAgBAoBBAEFAAwIKCFAigBghgBgjAGCMIgigIIwkEYDEwmEwMBiQmBkRMTBCRMmDBixYMkUTDJlkgkyywyyywkllhJLWEssYSlnCcpQhNWJSECkywEZAHHIAUwBEAIBAAJA==


formula: Pb Nb2 O6
compound: Synthetic
pub_title: Etude structurale du metaniobate de plombe rhomboedrique II. - Positions des atomes
formula_title: <missing>
a: 10.501
b: 10.501
c: 11.555
alpha: 90
beta: 90
gamma: 120
cell_volume: 1103.474
crystal_density: 6.623
atoms_sites: ["Pb1", "Pb2", "Pb3", "Nb", "O1", "O2", "O3", "O4", "O5"]
atoms_x: AAAAAAAAAAAAAAAAUBMVAOCkFgCA6SIAQOcyAKDwGQBA9QYA
atoms_y: AAAAAAAAAAAAAAAAYDoVAEAqEwCAHxoAwCEKAGAYIwDAEzYA
atoms_z: AAAAALDLFQCQ0ygAUPEJAAD6AAAgEgoAADUMAKDHCwCg3wcA
atoms_occupancy: 0
atoms_u_iso: +FwAAPhcAAD4XAAAmIoAAMiLAQDAUQIAwFECAMBRAgDAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAACAAAAAgEAABAAQAIABACEEAAgBAAEggICoIEBgBIKQABKJIHAEGCCGggLAoWQBhCPBB0CNojBB6AbqEFGKlwDijymOnELYKwQpADtGE4ryGMfTMOBWFUjnA6jIivAEMLWRLQcZHBlJCpwgKiIkZnSIg4==


formula: Mo O3
compound: Synthetic
formula_title: <missing>
a: 3.9624
b: 13.860
c: 3.6971
alpha: 90
beta: 90
gamma: 90
cell_volume: 203.041
crystal_density: 4.709
atoms_sites: ["Mo", "O1", "O2", "O3"]
atoms_x: mDAFAMAfAgAwzh8AMKIeAA==
atoms_y: SC8GAECADQAYYAUAEJ4aAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAA==
atoms_occupancy: 0
atoms_u_iso: wF0AACDLAACgjAAAYG0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: March model

qdat:
AAAAAAAAAAAAAAAQAAAAAAAAAAAAAIQAAAAAIAAAAAAAAIAQAAAABIAgCECAlBAAQgAQACBAECBSAFAgqABQAYQAgBCAQhEAEAQAoQCgEChgRHkBQcIhAoUAxmgCArAgbAigAgQDUFBgBBIkAESAEAAahAQzCRiUQ1Digl==


formula: Mo O3
compound: Synthetic
formula_title: <missing>
a: 3.9624
b: 13.860
c: 3.6971
alpha: 90
beta: 90
gamma: 90
cell_volume: 203.041
crystal_density: 4.709
atoms_sites: ["Mo", "O1", "O2", "O3"]
atoms_x: kC4FAOAiAgAQyx8AgJ0eAA==
atoms_y: MC4GADiDDQBgYwUAMKEaAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAA==
atoms_occupancy: 0
atoms_u_iso: YG0AACDLAABAnAAAYG0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Generalized spherical-harmonic model

qdat:
AAAAAAAAAAAAAAAQAAAAAAAAAAAAAIQAAAAAIAAAAAAAAIAQAAAABIAgCECAlBAAQgAQACBAECBSAFAgqABQAYQAgBCAQhEAEAQAoQCgEChgRHkBQcIhAoUAxmgCArAgbAigAgQDUFBgBBIkAESAEAAahAQzCRiUQ1Digl==


formula: Ca C O3
compound: Synthetic
formula_title: <missing>
a: 4.99026
b: 4.99026
c: 17.0684
alpha: 90
beta: 90
gamma: 120
cell_volume: 368.103
crystal_density: 2.709
atoms_sites: ["Ca", "C", "O"]
atoms_x: AAAAAAAAAADgpg8A
atoms_y: AAAAAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ca", "C", "O"]
atoms_aniso_u11: YBwBAHDfAADgKAEA
atoms_aniso_u22: YBwBAHDfAAAQngEA
atoms_aniso_u33: 0AEBADALAQAgkwEA
atoms_aniso_u12: MI4AALhvAAAIzwAA
atoms_aniso_u13: AAAAAAAAAACgv///
atoms_aniso_u23: AAAAAAAAAABAf///
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Generalized spherical-harmonic model

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAEABAAAAAgAABAAAAgAAAJBAAAAAAAAIIgACoAQCAAAAQQACEAAgAgESABCEAAAAKAA0AAAABJAGAggEAiAEgAAACQCgBAIJAGRAAA5AUIAAEQCAEAFQEkIEEAKAAAqBhAAEA==


formula: Ti.507 Ni.493
compound: Synthetic
formula_title: TiNi
a: 3.00896
b: 3.00896
c: 3.00896
alpha: 90
beta: 90
gamma: 90
cell_volume: 27.243
crystal_density: 3.243
atoms_sites: ["Ti", "Ni"]
atoms_x: gIQeAAAAAAA=
atoms_y: gIQeAAAAAAA=
atoms_z: gIQeAAAAAAA=
atoms_occupancy: 4PEeACAXHgA=
atoms_u_iso: gD4AABACAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Annealed

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAAQAAAAAAAAAAAAEAAAAAAAAAAAgAAAAAAAAAEAAAAAAAAAQAAAAAAAAQAAAAAAACAAAAAAACAAAAAAAIAA==


formula: Ti.507 Ni.493
compound: Synthetic
formula_title: TiNi
a: 3.01302
b: 3.01302
c: 3.01302
alpha: 90
beta: 90
gamma: 90
cell_volume: 27.353
crystal_density: 3.230
atoms_sites: ["Ti", "Ni"]
atoms_x: gIQeAAAAAAA=
atoms_y: gIQeAAAAAAA=
atoms_z: gIQeAAAAAAA=
atoms_occupancy: 4PEeACAXHgA=
atoms_u_iso: EJUAAKCVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Aged

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAQAAAAAAAAAAAAIAAAAAAAAAABAAAAAAAAAAIAAAAAAAAAgAAAAAAAAgAAAAAAAIAAAAAAAEAAAAAAAgAA==


formula: Ti Ni
compound: Synthetic
formula_title: TiNi
a: 7.34100
b: 7.34100
c: 5.26996
alpha: 90
beta: 90
gamma: 120
cell_volume: 245.951
crystal_density: 6.476
atoms_sites: ["Ti", "Ti", "Ti", "Ni", "Ni", "Ni"]
atoms_x: AAAAACDQFABVWBQAAAAAABDhEwBVWBQA
atoms_y: AAAAAFCX//+rsCgAAAAAAKDj/v+rsCgA
atoms_z: AAAAAEBvFABgZwEAgIQeAOA7NACgPSIA
atoms_occupancy: 0
atoms_u_iso: AGQAAABkAAAAZAAAMPIAADDyAAAw8gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Aged

qdat:
AAAAAAAAAAAAAAAAEAABAAAAABAAEAAAAgBAAAECAAAiAAABAoACAIAAAgAqIBCIABgAREAFABEEAogEAQcAWKgRBICGALIBQBBYzCRILCERkLIgAAUdDgjQNIiKJJBhDh2RRYTQaDAwTRyiiiaPoiJaRlFGUU5xgmcJTx==


formula: Ti Ni
compound: Synthetic
formula_title: TiNi
a: 2.87580
b: 4.12644
c: 4.6325
alpha: 90
beta: 90
gamma: 96.964
cell_volume: 54.567
crystal_density: 6.486
atoms_sites: ["Ti", "Ni"]
atoms_x: QEEkACD2/f8=
atoms_y: kOARAABC9f8=
atoms_z: QEIPAMDGLQA=
atoms_occupancy: 0
atoms_u_iso: oAMCABCkAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Annealed

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQACAAAAAAQAQAQAAAQIAAAAAQAAAAAAIEAQAQAEIAABgAAqACCAAQAAgEBIAIgAiABgAoBCIAAAAgBZACh0ARgAUEAEABABJCUBALCGQBgMEELOgCoEQAgguQiEhCbKa5EIY==


formula: Ti Ni
compound: Synthetic
formula_title: TiNi
a: 2.8894
b: 4.1334
c: 4.6321
alpha: 90
beta: 90
gamma: 96.929
cell_volume: 54.917
crystal_density: 6.445
atoms_sites: ["Ti", "Ni"]
atoms_x: gGwiAND6/f8=
atoms_y: 4PQRANAw9f8=
atoms_z: QEIPAMDGLQA=
atoms_occupancy: 0
atoms_u_iso: EKQAANBSAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Texture and structural refinement using neutron diffraction data from
 molybdite (MoO3) and calcite (CaCO3) powders and a Ni-rich Ni50.7Ti49.30 alloy
 Note: Aged

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAEAAAAAAgAQAgAAAgAAAAAAQAAAAAAQQAQAgAEgAAEgABQAAIABAACAEEgAhACEAGABoBIgAAAEAD0AKFQCFABQAAgAKAJCEoEBcCLAFAkghLcgShhABIDwkIUFEWoi4Ihh==


formula: K3 Na U C3 O12 H2
compound: Jachymov, Czech Republic
formula_title: <missing>
a: 9.3000
b: 9.3000
c: 8.2940
alpha: 90
beta: 90
gamma: 120
cell_volume: 621.242
crystal_density: 3.252
atoms_sites: ["K", "Na", "U", "C", "O1", "O2", "O3", "O4", "Wat5"]
atoms_x: oNURAFVYFACrsCgAIF08AFAQOwAwujMAq7AoAJDRBwAAAAAA
atoms_y: AAAAAKuwKABVWBQAAJMmAMAsHQAwciYAVVgUAGBTLgAAAAAA
atoms_z: AAAAAMDGLQDAxi0AwMYtAMDGLQDAxi0AIOY6AMDGLQBA7wcA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQCAhB4A
atoms_u_iso: AD8CAOClAQDQAQEAwFcBAECWAQBgZwEAYOQBAECWAQBgVQQA
atoms_aniso_label: ["K", "Na", "U", "C", "O1", "O2", "O3", "O4", "Wat5"]
atoms_aniso_u11: QJACACDFAQDQ6AAAIEgBAECcAABAGQEAwNQBAGBnAQDgEAUA
atoms_aniso_u22: gDICACDFAQDQ6AAAAPoAAIA4AQCAMgIAwNQBAAB3AQDgEAUA
atoms_aniso_u33: YOQBAMBXAQDQMwEAgLUBAADuAgDgIgIAQBMCAEANAwBADQMA
atoms_aniso_u12: IBYBAHDfAAAwdQAAoIwAAAB9AACgCQEAYOoAAAB9AAAAcQIA
atoms_aniso_u13: MEMAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u23: oIwAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
pub_title:
 The crystal chemistry of the uranyl carbonate mineral grimselite,
 (K,Na)3Na[(UO2)(CO3)3](H2O), from Jachymov, Czech Republic
 Note: Sample B

qdat:
AAAAAAAAAAAAAgAAAAQAAAEAAQgAJAAAABIAKAAgggCAAglAEAESwMIIDBgEJQgBOgQGZCkBcMQJDA2wgT4wJ4TCYsShRPHCqgUxo9Nc7wWwKOqpiqpHarOX0nxl6o3nrHni1i/bu34fLYzSNu2qfn1N8N2uU6zHcm78e1==


formula: Fe Si2
compound: Synthetic
pub_title: A note on the compositions and crystal structures of MnB2, Mn3Si, Mn5Si3 and FeSi2
formula_title: <missing>
a: 2.684
b: 2.684
c: 5.128
alpha: 90
beta: 90
gamma: 90
cell_volume: 36.941
crystal_density: 5.035
atoms_sites: ["Fe", "Si"]
atoms_x: AAAAAICEHgA=
atoms_y: AAAAAICEHgA=
atoms_z: AAAAAMB6EAA=
atoms_occupancy: 0
atoms_u_iso: sE8AALBPAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAAAAgBAAAgAAAAAAAAAAQEABAAIAAAAAACAAACAAAAAgACCEAAAAQQEEAAAAAIAEQAAgAAAEAAIIAQgAAgiBEAAEIggQAEAgAQAYAARAACASgAIEBQAIAAIAIQEAARITIBE==


formula: Mn5 Si3
compound: Synthetic
pub_title: A note on the compositions and crystal structures of MnB2, Mn3Si, Mn5Si3 and FeSi2
formula_title: <missing>
a: 6.91
b: 6.91
c: 4.814
alpha: 90
beta: 90
gamma: 120
cell_volume: 199.064
crystal_density: 5.988
atoms_sites: ["Mn1", "Mn2", "Si"]
atoms_x: VVgUAGBkDgCAkiQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: WEMAAFhDAABYQwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAEAAAAAAAAAAAAIAAAAgAIAAAAAEAAJAAAAQEgABAAAACAAUIACAQAgAgACAKAAIwAEgAAAlCgBwUFAQAGEBJCIIAgiECIAHBKBCBKYAAQGYNDQohAmCxFgQKCNiiBhVgkiIgWI0ScwSA2yQoFhZhh==


formula: Mn B2
compound: Synthetic
pub_title: A note on the compositions and crystal structures of MnB2, Mn3Si, Mn5Si3 and FeSi2
formula_title: MnB2
a: 3.007
b: 3.007
c: 3.037
alpha: 90
beta: 90
gamma: 120
cell_volume: 23.782
crystal_density: 5.346
atoms_sites: ["Mn", "B"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAICEHgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAiAAAAAAACAAAAAAAAAEAAAAAAAAAAgAAAAEAAAAAAAhAAAAAAAACAAACEAAAAAgAAAAABAoAAAEAAAAEQAAAAEEAABAAAAAEA==


formula: Mn3 Si
compound: Synthetic
pub_title: A note on the compositions and crystal structures of MnB2, Mn3Si, Mn5Si3 and FeSi2
formula_title: Mn3Si
a: 5.722
b: 5.722
c: 5.722
alpha: 90
beta: 90
gamma: 90
cell_volume: 187.346
crystal_density: 6.839
atoms_sites: ["Mn1", "Mn2", "Si"]
atoms_x: gIQeAEBCDwAAAAAA
atoms_y: gIQeAEBCDwAAAAAA
atoms_z: gIQeAEBCDwAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAACAAAAAAAAAAAAAABAAAAAAAACAAIAAAAAAAAAQAAAAABABAAAAAAACAAAAAQAAAAAAAEAAAAIBAAAAABAAAAgEAAAABAAACAgAAAAgAACAAAAAIAACBAAAAIAAEEAAACAA==


formula: La (Ta Ti) O6
compound: Synthetic
formula_title: <missing>
a: 10.9420
b: 7.5831
c: 5.4614
alpha: 90
beta: 90
gamma: 90
cell_volume: 453.156
crystal_density: 6.797
atoms_sites: ["La", "Ta", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: 0PUbALBGJwCwRicAwOEcABCiEQAwvxUAECQmAA==
atoms_y: wMYtABDRHgAQ0R4AYFscAGDZOQDAxi0AwMYtAA==
atoms_z: 8HsCADAYHAAwGBwAQIcQAND1NADAABwAEHEVAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: CMAAAMB2AADAdgAA0M8AACi0AADY0QAASKgAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural studies of the aeschynite-euxenite transformation in
 the series Ln(TiTa)O6 Ln = lanthanide

qdat:
AAAAAAAAAAAAAAAAAAAQAEACAEASAAIAACEgAQKECBBAQiCZQFAkAIwYoMM2nMRKMRWZQjlmIc5CWZFnc91ihnXzc5sdMoM7PPVqptj/9mzRoU3f/a999t//Uyuvfv+31+rtKdNt99c39L+ae07PtT/+9rP7z6/Xvvcp/f==


formula: Ce (Ta Ti) O6
compound: Synthetic
formula_title: <missing>
a: 10.9694
b: 7.5288
c: 5.3829
alpha: 90
beta: 90
gamma: 90
cell_volume: 444.554
crystal_density: 6.947
atoms_sites: ["Ce", "Ta", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: wAAcAEBIJwBASCcAAAEdAKCjEQAQrRUAQAMmAA==
atoms_y: wMYtAMDVHgDA1R4A0FkcACChOQDAxi0AwMYtAA==
atoms_z: kKQCABAVHAAQFRwAoHcQAOADNQAwmxsAoCcVAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: iIYAAPjFAAD4xQAAEFkAAJCIAACIhgAAyBkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural studies of the aeschynite-euxenite transformation in
 the series Ln(TiTa)O6 Ln = lanthanide

qdat:
AAAAAAAAAAAAAAAAAAAQACADACAJAACAABCIAIRgiAJIIlgxJBIUAIUDUJFz2agzAsMNGKXyZGapKLNL5bz2jGblbRZp9jseWe/b8aa/159Mf3e/V/3avz7/49L/s9z7dfv/fud9//59f5/f9va/tdde78+71t/b/v/r03==


formula: Pr (Ta Ti) O6
compound: Synthetic
formula_title: <missing>
a: 10.9511
b: 7.5288
c: 5.3829
alpha: 90
beta: 90
gamma: 90
cell_volume: 443.813
crystal_density: 6.970
atoms_sites: ["Pr", "Ta", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: kO8bALBGJwCwRicAAOgcAKCjEQCwyxUAQAMmAA==
atoms_y: wMYtACDfHgAg3x4A0FkcAMCXOQDAxi0AwMYtAA==
atoms_z: wIMCAHAFHABwBRwAUDEQAEDbNACwdRsAoCcVAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: aJwAAMB2AADAdgAA0M8AAKjZAACIhgAASKgAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural studies of the aeschynite-euxenite transformation in
 the series Ln(TiTa)O6 Ln = lanthanide

qdat:
AAAAAAAAAAAAAAAAAAAQACADACAJAACAABCIAIRgiAJIEVgpJBIWAEUDKJDz2WwxAsOHGLWyZGa1GLrK4772TDXV5ZZptjmeWWW7aeK//ddmfS3fv/3W/7/v49H78976/f/9Pudv3/5/f9/+9u6/vbdfr8uv1W7b/v/vy3==


formula: Nd (Ta Ti) O6
compound: Synthetic
formula_title: <missing>
a: 10.9771
b: 7.5051
c: 5.3602
alpha: 90
beta: 90
gamma: 90
cell_volume: 441.596
crystal_density: 7.055
atoms_sites: ["Nd", "Ta", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: ANUbAABCJwAAQicAEPYcAECaEQDg3BUAMA4mAA==
atoms_y: wMYtAADcHgAA3B4AgF4cAECLOQDAxi0AwMYtAA==
atoms_z: IKYCAND1GwDQ9RsAkDcQANAONQDAahsA8KUUAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: kCkAAMB2AADAdgAAaDMAAChVAACoJQAAOEUAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgACACgBAJAACAABCIAIQgSAFEESwYkgoWAIKBKQipsqwSgSKGRKroulGqpOzEk3Y2IzPhz1SetQsO3Nfe3Nr6x33Sn2cv5698n8/f3Gy9/V8ut79fntTby/9/Lv3+v93v+3rz3fi3T/39b/Xrtp==


formula: Tb (Ta Ti) O6
compound: Synthetic
formula_title: <missing>
a: 10.977
b: 7.414
c: 5.2380
alpha: 90
beta: 90
gamma: 90
cell_volume: 426.287
crystal_density: 7.538
atoms_sites: ["Tb", "Ta", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: QA0cAKA4JwCgOCcAoPccAOCQEQDQahUAYAYmAA==
atoms_y: wMYtAMDuHgDA7h4AAO4bAHA4OQDAxi0AwMYtAA==
atoms_z: 8P4BALDyGwCw8hsAkJsQAHDNNQDgIhsAoPsTAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: wIkBAMB2AADAdgAA4CgBAODJAAAAvgAA0OIBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAAQCEAICIAAgAAhBACQEiQAkIoFFAxCWECBIGwAiKK5hFANg4zAxUchZODhw8PTp1oxcSfDiGyy70t9eb9ql/3ozujfPOs8z95e57+Lffrumf54dXmzTu5/uXt1/tmff83OXpvuzTm+r/v/d/3==


formula: Ho (Ti Ta) O6
compound: Synthetic
formula_title: <missing>
a: 14.6236
b: 5.5637
c: 5.2030
alpha: 90
beta: 90
gamma: 90
cell_volume: 423.323
crystal_density: 7.685
atoms_sites: ["Ho", "Ti", "Ta", "O1", "O2", "O3"]
atoms_x: AAAAACBECgAgRAoA4Fs3ABBtBQCwvQ8A
atoms_y: kCoOAMCzEwDAsxMAwEAiAFDXBQCgwAgA
atoms_z: QEIPAAAyMgAAMjIAMHwcAHDaNwAwTSgA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: aD0AAPjFAAD4xQAAyNcAADhPAAAIdAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIAAAAAQAAAAAAAGAAgAAAgACACNACoAyCJAIAoBFAWA4BQMDQGJDFwELxWGBMsnI4WHlQ4xOCkxw4IGYLFmKHqKwr5HLKuONc06pzHuMdBxzGwy/me53iUzmwpvF3m5qt7K9mNmY1cmpU/2rG5oydOHt==


formula: Tm (Ti Ta) O6
compound: Synthetic
formula_title: <missing>
a: 14.5706
b: 5.5339
c: 5.1832
alpha: 90
beta: 90
gamma: 90
cell_volume: 417.933
crystal_density: 7.847
atoms_sites: ["Tm", "Ti", "Ta", "O1", "O2", "O3"]
atoms_x: AAAAAMA6CgDAOgoAcHY3ALBKBQDgzg8A
atoms_y: QC8OALC+EwCwvhMA0GciAOCmBQDQbQgA
atoms_z: QEIPAOAuMgDgLjIAUJgcAAD1NwDwyScA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: aJwAAPjFAAD4xQAAgI4AANhyAADgKAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIAAAAAQAAAAAAACAAQAAAQABABOgBUAZBEgEASASgJgcAoDAoBkQx4BC4XBgTLRiODhw0OcTw5MMODA3Bx45g9R6F9I47XRxznFOMM9ZhoPe9XGN87rO2TyKbGrYWcbrd7svqZXRhMjf/t/N6Ztj16cX==


formula: Yb (Ti Ta) O6
compound: Synthetic
formula_title: <missing>
a: 14.5478
b: 5.5289
c: 5.1683
alpha: 90
beta: 90
gamma: 90
cell_volume: 415.704
crystal_density: 7.955
atoms_sites: ["Yb", "Ti", "Ta", "O1", "O2", "O3"]
atoms_x: AAAAANBICgDQSAoAkGA3AHBEBQBw0A8A
atoms_y: 0P4NABCWEwAQlhMAIK4iACB7BQAQEAgA
atoms_z: QEIPAFAUMgBQFDIA0KQcABA1OADAbScA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: MKwAAPjFAAD4xQAASJ4AAMhuAACgggAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIAAAAAIAAAAAAADAAQAAAQABAAmQA0AMgigCAKARQEgOAUDA0AiIRMABcLhwRlkyHBw4aPFJ4U2FHBgSg0UZQeo+CtkMsq4UszTmnGes4qHHOdhn/M9zuF6jNhy5JuN/Vf68yuGmY391N2Z27G5sTNmF==


formula: Lu (Ti Ta) O6
compound: Synthetic
formula_title: <missing>
a: 14.5288
b: 5.5226
c: 5.1572
alpha: 90
beta: 90
gamma: 90
cell_volume: 413.797
crystal_density: 8.023
atoms_sites: ["Lu", "Ti", "Ta", "O1", "O2", "O3"]
atoms_x: AAAAAPAyCgDwMgoAwHE3APA3BQCw1g8A
atoms_y: kN8NACCLEwAgixMAQMoiAHBdBQCgEQgA
atoms_z: QEIPAHAXMgBwFzIAcOYcAJAPOABglicA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: CMAAAPjFAAD4xQAAOKQAAEieAABApgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAIAAAAAIAAAAAAADAAIAAAQAAgAmQA6AMgiQBAJAJIEwOAKBgaAxIYsAg8KwwIjk5HBocWHnI4aTDDgwJw6KcoOYfBO6OUWacWZxzTlPsccjzjNQz/ne9zhW7no1ck/ntreY1ebHbIWu523e+0zP+fvxx==


formula: Eu2 Ta2 O7
compound: Synthetic
formula_title: Eu2Ta2O7
a: 3.9542
b: 27.142
c: 5.692
alpha: 90
beta: 90
gamma: 90
cell_volume: 610.893
crystal_density: 8.457
atoms_sites: ["Eu1", "Eu2", "Ta1", "Ta2", "O1", "O2", "O3", "O4", "O5"]
atoms_x: AAAAAAAAAACAhB4AgIQeAICEHgAAAAAAgIQeAAAAAACAhB4A
atoms_y: aJURABBIGwDgvxQAgCMbAIDSEQAgTRUAUGUYAGDFGwCAhB4A
atoms_z: QEIPAMDGLQDAxi0AQEIPAEBfHwDAxi0AoNIeAEBCDwCAhB4A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Eu1", "Eu2", "Ta1", "Ta2", "O1", "O2", "O3", "O5"]
atoms_aniso_u11: YIYAALCzAAAgZwAA0GsAACBIAQBAnAAAYGcBAEANAwA=
atoms_aniso_u22: QEsBAPDSAADgkgAA0J0AAKAJAQCAOAEAQBkBAECcAAA=
atoms_aniso_u33: YE4BAODdAACgpQAAEIsAAGBnAQDARQQAgDgBAECcAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAGD2/v8AAAAAgD4AAOAuAAA=
pub_title:
 Crystal structures of dieuropium(II) ditantalum heptoxide,
 Eu2Ta2O7 and europium(II) ditantalum hexoxide, EuTa2O6

qdat:
AAAAAAACAAAAAAAEAAAAgAAQgABABEBAFAQAhHEBAAiGAEBIgIAABsASCZQBCIIQ0kIokAIEAEgQBQolsDOhgGiCKCCioMRBFmGGEBBAAA0pOguHVyeQKgCCECmoGEUAIzBknjawtNTEcRUHFEgagipFy3CUaRhaWrJdGh==


formula: Eu Ta2 O6
compound: Synthetic
formula_title: <missing>
a: 11.02
b: 7.640
c: 5.610
alpha: 90
beta: 90
gamma: 90
cell_volume: 472.322
crystal_density: 8.576
atoms_sites: ["Eu", "Ta", "O1", "O2", "O3", "O4"]
atoms_x: IHQCAIiwCADAcjsAwA8NAADKCACAtBYA
atoms_y: QEIPAJDJPADgIgIAAO4CAEBCDwBAQg8A
atoms_z: MOEgABBNAgAgfQ0AoAgWAGAFOwDgPicA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Eu", "Ta", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: wNoAACCAAAAA+gAAQJwAAMDUAQDgKAEA
atoms_aniso_u22: 8IcAAAB9AAAAfQAAAH0AAGBtAABAHwAA
atoms_aniso_u33: gNQAAPC5AAAA+gAAAPoAAAD6AACgCQEA
atoms_aniso_u12: AAAAAAAAAAAAAAAAYPD//wAAAAAAAAAA
atoms_aniso_u13: oA8AACADAABAHwAAQB8AAIA+AAAAAAAA
atoms_aniso_u23: AAAAAAAAAADA4P//gMH//wAAAAAAAAAA
pub_title:
 Crystal structures of dieuropium(II) ditantalum heptoxide,
 Eu2Ta2O7 and europium(II) ditantalum hexoxide, EuTa2O6

qdat:
AAAAAAAAAAAAAAAAAAAgAgAUAgCIAAgAAIkACI0AJBICkYZoAgkgBMJgpimwqklQMUqqUscyy0KossK2v1QpXHH8+1P6O7/07r9S3L9/3blEb76//e/P7f6rZ3u1Lze6nXs663/7v7++5v8+u1b9P/dbv3v//t79bv791d==


formula: (Ca.982 Sr.018) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8422
b: 8.7904
c: 13.1344
alpha: 90
beta: 90
gamma: 90
cell_volume: 674.521
crystal_density: 3.103
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAADgrxAAAAAAAAAAAAAAAAAA
atoms_y: EF4UABBeFABAQg8AIOA7AED0AgBAKxcA4HsIAPABJwCgKyUA
atoms_z: QEIPAEBCDwAAAAAAkBwIAEBCDwDwKwcAMPkDAPD4AgBAQg8A
atoms_occupancy: wO87AEAZAQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU76

qdat:
AAAAAAAAAAAAAAAAgAAAAEAhAQBACAABQBABAAERhAAhAJEDoIIQEMAiEICDyCaDcgGOzAkGg9ArkwMTqH0WQK9MC8HhBcxrnHVcEf+o2AW3DpaM3ZDHSbie83eMe2uoNY+Oap1ZsBg7jZmPu+R7BzHdji0DdwmAeq0OpZ==


formula: (Ca.971 Sr.029) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8417
b: 8.7904
c: 13.1345
alpha: 90
beta: 90
gamma: 90
cell_volume: 674.468
crystal_density: 3.108
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAADQoRAAAAAAAAAAAAAAAAAA
atoms_y: gEMUAIBDFABAQg8AUNg7AJDvAgBAKxcAMHcIAJARJwAAHCUA
atoms_z: QEIPAEBCDwAAAAAAQCEIAEBCDwCwJQcAwPoDAMAAAwBAQg8A
atoms_occupancy: 4EM7ACDFAQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU77

qdat:
AAAAAAAAAAAAAAAAgAAAAEAhAQBACAABQBABAAERhAAhAJEDoIIQEMAiEICDyCaDcgGOzAkGg9ArkwMTqH0WQK9MC8HhBcxrnHVcEf+o2AS2jpeM1ZDHSbCe83eMe3uoNY+OaptZsBA7jZmPu+RrBzHdji0DdwmAeq0Opd==


formula: (Ca.965 Sr.035) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8415
b: 8.7916
c: 13.1360
alpha: 90
beta: 90
gamma: 90
cell_volume: 674.614
crystal_density: 3.110
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAABgoxAAAAAAAAAAAAAAAAAA
atoms_y: AFAUAABQFABAQg8AkN47AADuAgBAKxcAgHIIADAIJwAAHCUA
atoms_z: QEIPAEBCDwAAAAAAIB4IAEBCDwDwKwcAwPoDABD8AgBAQg8A
atoms_occupancy: IOY6AOAiAgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU78

qdat:
AAAAAAAAAAAAAAAAgAAAAEAhAQBACAABQBABAAERhAAhAJEDoIQQEMAiEICDyCaDcgGOzAkGg9ArkwMSqH0WQK9MC8HhBcxrnHVcEX+o0AXWjpeM1ZDHibie83eMe6uoNY2OaptZsBg7jpkPu+R7BzHdji0DdwmAeq0Opd==


formula: (Ca.979 Sr.021) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8419
b: 8.7940
c: 13.1393
alpha: 90
beta: 90
gamma: 90
cell_volume: 675.014
crystal_density: 3.102
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAACwhRAAAAAAAAAAAAAAAAAA
atoms_y: MEgUADBIFABAQg8A8M47AMDOAgCQJhcAEI0IAPDPJgCA3SQA
atoms_z: QEIPAEBCDwAAAAAAoBEIAEBCDwCgFwcAQCAEADAYAwBAQg8A
atoms_occupancy: 4MA7ACBIAQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU79

qdat:
AAAAAAAAAAAAAAAAgAAAAEAhAQBACAABQBABAAERhAAhAJEDoIQQEMAiEICDyCaDcgGMjBEHhdBLkwMW6H0WQK+ME8HhBcx1nHVcEXuo8AX3DpaM3RCHibC+83aUe6uoPY2OSpVxsDgzjpkbu+R6BSLelk0DZwmAfy0Mp9==


formula: (Ca.889 Sr.111) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8439
b: 8.8112
c: 13.1618
alpha: 90
beta: 90
gamma: 90
cell_volume: 677.724
crystal_density: 3.131
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAADgyBAAAAAAAAAAAAAAAAAA
atoms_y: IFMUACBTFABAQg8AAPY7AOAcAwCgAhcA4HsIAEAvJwDA/CQA
atoms_z: QEIPAEBCDwAAAAAA0CIIAEBCDwBwUQcAAOgDAKD9AgBAQg8A
atoms_occupancy: oEI2AGDGBgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU63

qdat:
AAAAAAAAAAAAAAABAAAAAEAhAgBACAABQCABAAITCAAiARMFQQQgIcAiIYCGkC0C8gEdmCIKh2CVJQsVcOkuQd6UI8PDC9hlOKpoJ39hoA93GS85TiKNE3H+1V85899w/wqc1idloHBmFXk/ItTsDiPtLpICRgqA+jkIh7==


formula: (Ca.807 Sr.193) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8457
b: 8.8286
c: 13.1834
alpha: 90
beta: 90
gamma: 90
cell_volume: 680.387
crystal_density: 3.157
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAAAAmhAAAAAAAAAAAAAAAAAA
atoms_y: gEMUAIBDFABAQg8AwO87AICvAgAgQRcAAE0IAAAQJwDgRCYA
atoms_z: QEIPAEBCDwAAAAAA0FQIAEBCDwDw+QYAwEUEAOAcAwBAQg8A
atoms_occupancy: YEExAKDHCwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU62

qdat:
AAAAAAAAAAAAAAABAAAAAEBCAgCAEAABgCABAAITCABiARMHQQggIUAiQYEGkF0E0gIpGCQXB8CvSQ4e4dJcg744T4eCF2C1afTYztbBwB/uOt973EUeIlPfsr575txh3x65WCXLIGH8bva+ZuXYDsr1XRICzBKB5jEZj3==


formula: (Ca.82 Sr.18) Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.8433
b: 8.8169
c: 13.1726
alpha: 90
beta: 90
gamma: 90
cell_volume: 678.650
crystal_density: 3.159
atoms_sites: ["Ca", "Sr", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAABgihAAAAAAAAAAAAAAAAAA
atoms_y: ADcUAAA3FABAQg8AAN07AKD9AgAgQRcAwKoIAKAfJwBAOyUA
atoms_z: QEIPAEBCDwAAAAAAwBQIAEBCDwDwKwcAQAcEAKD9AgBAQg8A
atoms_occupancy: gAwyAID8CgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of synthetic lawsonite solid-solution series CaAl2
 [(OH)2/(Si2O7)](H2O)-SrAl2[(OH)2/(Si2O7)](H2O) and the Cmcm-P2_1/m phase transition
 Note: Run #AU83

qdat:
AAAAAAAAAAAAAAABAAAAAEBCAgCAEAABQCABAAITCAAiARMHQQQgIcAiIYEGkC0G0gEdGCIOh2C9RQsd0PouQ78UJ8NDC1CtOOpoZ/5hoA/1Knc5TiONI3Grq185cu5wtxqY1iZloHDmNXs/ItTsDkW9LpICRBKBcjkMh7==


formula: Ca Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.849
b: 8.790
c: 13.132
alpha: 90
beta: 90
gamma: 90
cell_volume: 675.152
crystal_density: 3.091
atoms_sites: ["Ca", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAEBCDwAAAAAAAAAAAMD3EAAAAAAAAAAAAAAAAAA=
atoms_y: cIAUAEBCDwCQKTwAwM4CAPBIFwCgVgkA8M8mAACfJAA=
atoms_z: QEIPAAAAAADgswcAQEIPAKDlBgBQmAMA0NwCAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A high-pressure study of lawsonite using angle-dispersive
 powder-diffraction methods with synchrotron radiation
 Note: Run #BN82, P = 0 GPa

qdat:
AAAAAAAAAAAAAAAAgAAAAEAhAQBACAABQBABAAERhAAiAJEDoQIQEMAiEICDyCaDcgGMzAkGhZAvEwMT6HyWQK5MCcPiBdRrHHXcEd+o8AXXDp8d3ZGNhvie02eM+7/Yf5qesrXxoDhzjzsf+8SzDyN3HloCZwqAvz4Mqz==


formula: Ca Al2 Si2 O10 H4
compound: Synthetic
formula_title: <missing>
a: 5.714
b: 8.592
c: 12.871
alpha: 90
beta: 90
gamma: 90
cell_volume: 631.898
crystal_density: 3.303
atoms_sites: ["Ca", "Al", "Si", "O1", "O2", "O3", "O-H4", "Wat5"]
atoms_x: AAAAAEBCDwAAAAAAAAAAAODIEAAAAAAAAAAAAAAAAAA=
atoms_y: IFMUAEBCDwBgGDwAIDYEACBBFwCgUAoAoCUmAAAiJAA=
atoms_z: QEIPAAAAAAAQxQcAQEIPALBwBwDgHAMAIDwDAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A high-pressure study of lawsonite using angle-dispersive
 powder-diffraction methods with synchrotron radiation
 Note: Run #BN89, P = 9.8 GPa

qdat:
AAAAAAAAAAAAAAAAIAAAAAgEICAIAIAAFAEACAAITCAAhAImBoIIIEFAJCCAgsgWQykAy0YEgeGkF+UgwpUPIqga6cCqPRBeolnjmnBNdKOgH94dbxn9IJWLMN7xK0RtNbga46ecrNYkBQ9xYyn9Vsegcpvo4kgZuCwD+q==


formula: Pb Al2 Si2 O10 H4
compound: Synthetic
pub_title: Synthesis of Pb-zoisite and Pb-lawsonite
formula_title: PbAl2Si2O7(OH)2*H2O
a: 5.85
b: 9.03
c: 13.31
alpha: 90
beta: 90
gamma: 90
cell_volume: 703.107
crystal_density: 4.547
atoms_sites: ["Pb", "Al", "Si", "O1", "O2", "O3", "O4", "O-H5", "Wat6"]
atoms_x: wJv+/yB3DgCwPP//4KUBAGBlKwCgjAAAQKj+/+DODwDAdfz/
atoms_y: sJ8UACCjDwDw0gAAYGcBAOCeFwAAPzQAgD0VAABqGABANSYA
atoms_z: QEIPAGDw//8gIzUAQEIPANDbFwDwfDgAYI45AAD1BQBAQg8A
atoms_occupancy: 0
atoms_u_iso: UMMAAJCwAACQZQAAQBkBAECcAABAnAAAIE4AAMBdAABAlgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAgCAAAEAACRAAMAgCIFAIADSCkRBgz4FGISBg8BewM0oRnxOYK+EXWkeKkO+s56rhff63nk/avXfvfv1dxfpv9Lf96Pem8v9d//f2/52/1e+fp/d+///f7737P3/7p9V73/+9y/23/++vH6/v3d5/1917==


formula: La (Nb Ti) O6
compound: Synthetic
pub_title: Solving structural problems of ceramic materials Compound 1
formula_title: LaNbTiO6
a: 11.2041
b: 8.85114
c: 5.27180
alpha: 90
beta: 115.3282
gamma: 90
cell_volume: 472.544
crystal_density: 5.281
atoms_sites: ["La", "Nb", "Ti", "O1", "O2", "O3"]
atoms_x: gIQeAJhSEACYUhAAcBAWAPAzJwAAECcA
atoms_y: AGIqAKgQOACoEDgAEAM4APAJLgCgrSAA
atoms_z: QEIPABCd5P8QneT/MAT+/8DtAQBQ0ycA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: 8IwAAKiEAACohAAAoCMAAKAjAACgIwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAACAAAACAACAAAAAAIEIQAAAgAAAIAQgQEaABCCQgAAgIAEjAjAFMJAAAggxIoBAhkKCRSEBAotoEU4IVKIJSELYZDYNnggA47ikyGLAs5q8G0D6ORE1+rzCKlqywEGUYgTdnaMveCpgowik0m3q9PWjU==


formula: La.924 (Nb1.228 Ti.772) O6
compound: Synthetic
pub_title: Solving structural problems of ceramic materials Compound 2
formula_title: <missing>
a: 10.96305
b: 7.58996
c: 5.46833
alpha: 90
beta: 90
gamma: 90
cell_volume: 455.015
crystal_density: 5.480
atoms_sites: ["La", "Nb", "Ti", "O1", "O2", "O3", "O4"]
atoms_x: qPobAEBNJwBATScAYAodAIC5EQBgtxUAYB8mAA==
atoms_y: wMYtADjWHgA41h4AgEUcANClOQDAxi0AwMYtAA==
atoms_z: 8HECAIBFHACARRwAgI0QAADl9/8Q4xsAcHoVAA==
atoms_occupancy: gGU4AMB5JQBAjxcAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: MBsAAJBHAACQRwAAyBkAAMgZAADIGQAAyBkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAQAIAGAEAiAAIAAEEgAQaECBDAQmERQFBEAJQRIYY1OUxSUikRQlLGQ5bEu6Jm81tmiurWZ7I7JQZ2ee/M7XH/7LmjQ1uv/S77/9/+p3df/f0vr9/8Uqbf757/3f918v29ev7t7tcnnn//+7Zf//==


formula: La.741 (Nb1.778 Ti.222) O6
compound: Synthetic
pub_title: Solving structural problems of ceramic materials Compound 3
formula_title: La0.37Nb0.889Ti0.111O3
a: 7.80411
b: 7.82272
c: 7.92310
alpha: 90
beta: 90
gamma: 90
cell_volume: 483.700
crystal_density: 5.146
atoms_sites: ["La", "Nb", "Ti", "O1", "O2", "O3", "O4", "O5"]
atoms_x: gIQeAKDcLQCg3C0AMGcsABBSLwCAhB4AgIQeAMDGLQA=
atoms_y: YKQtAICEHgCAhB4AgIQeAICEHgCAhB4AAAk9AMDGLQA=
atoms_z: AAAAAEgMEABIDBAAAAAAAICEHgCA5A4A4F0NAJBcDgA=
atoms_occupancy: IDotAKBCNgBgxgYAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: wCsAAIhjAACIYwAAAF8AAABfAAAAXwAAAF8AAABfAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAQAAAAAgAAAQAAFAABAAEAAAACgCQAIAsAQBABgABGBYRAobgMCAAkiDOOAJAYAJQiU5sMECH3MXDfAAEGP3aGMJ6B7g3OB9e2eYJn0+y8crmX/GZt5vjZk1f/3Mn3vvqm/f9w7jTPmO//Hrf53Rt6XjF+==


formula: Sr Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: SrNb2O6
a: 10.9862
b: 7.7223
c: 5.5944
alpha: 90
beta: 90.372
gamma: 90
cell_volume: 474.612
crystal_density: 5.170
atoms_sites: ["Sr", "Nb1", "O1", "O2", "O3", "O4"]
atoms_x: UIUCADCpCAAwgf7/wN0MAHD6CADggQcA
atoms_y: QEIPAEC7//+AMgIAoP0CAEBCDwDAvfD/
atoms_z: wPsgAIAyAgDg2g0AIEcWAEAr/v8ATQgA
atoms_occupancy: 0
atoms_u_iso: EBcBABANAQAgsgAAMAEBADhPAAAgsgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAYAgBQAAgAAQIABESAEgUCThRICQUIASUJQ13IdhIYSM+IWp+gjbHUzFnLs8ia57Nk+txjml/+/v78b9/vxY4x/7/vvb79v9dX87u3a+Nv5cz3X//t//L/7x+f//7dtv5z+tf/V27f2/38/z==


formula: (Sr.9 La.1) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.9La0.1Nb2O6
a: 11.021
b: 7.675
c: 5.584
alpha: 90
beta: 90.19
gamma: 90
cell_volume: 472.327
crystal_density: 5.267
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAYAgCIAAgAAIUABEyAIgUCMwpYBQUQAsGRIxmkziUYKM0op6VESdJqtWfvbdQk9I6Wew1Kxu+/u5V3Pd999ZexO9b+/5/1+9Nu3f787+9/t/12vv98n3/3/P1fe3+f77/+35t/59677W/095==


formula: (Sr.8 La.2) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.8La0.2Nb2O6
a: 11.042
b: 7.665
c: 5.584
alpha: 90
beta: 90
gamma: 90
cell_volume: 472.613
crystal_density: 5.336
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: ANQwAAA1DAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAYAgCIAAgAAIkACEyAIgoCUQmoBgYgBIGhJhGolkkwMNMpS2ZES8TzZsVt68hk3S68/hfWZ9/ff36teV75V72U7/e+36fn9fe1TX/+7/3eL+3rv/++29//372/+v75t/v32777f+/7r7/s3b==


formula: (Sr.7 La.3) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.7La0.3Nb2O6
a: 11.046
b: 7.653
c: 5.571
alpha: 90
beta: 90
gamma: 90
cell_volume: 470.945
crystal_density: 5.427
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: gLkqAIBPEgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAYAQCIAAgAAIkABCxAIQYCMQVUAwYgBIGRFRnllkkYGFKox+YiKWR5Mke8v0RibKbd/x/tI3/9P76btb99qvXSd/6/36vz+/u3pn//T/5vl/b17//Pr/b3359+/v1v+f7/X68+f/f3r+91c/==


formula: (Sr.6 La.4) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.6La0.4Nb2O6
a: 11.055
b: 7.658
c: 5.578
alpha: 90
beta: 90
gamma: 90
cell_volume: 472.229
crystal_density: 5.485
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: AJ8kAABqGAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAYAgCIAAgAAIkACFSAIgoCUQWYAgYgBIGhJRnplokYENMpS+ZkS8Trds3c90ykXa+6/hdeZ97be38r+f/tf9uUu9b+r/fn//9vzO7+37bPJ//lW//f3++v/77f/X798/32r958/+/vdz7q71==


formula: (Sr.9 La.1) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.9Nd0.1Nb2O6
a: 11.018
b: 7.672
c: 5.575
alpha: 90
beta: 90.25
gamma: 90
cell_volume: 471.251
crystal_density: 5.279
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAQAYAQBIAAgAAIUABExAIQUBKwlMAwUQAsCJIxnkTSUYGEskV3dEabJZsqdl9XQits5OeoetZ2vln97TG0/88s+Qu2f/XY/f/+mn9398bvVv3f67V/7e35+r3v/ufLXP9/fX66u/V9v/5jf7l8==


formula: (Sr.8 La.2) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.8Nd0.2Nb2O6
a: 11.042
b: 7.644
c: 5.563
alpha: 90
beta: 90
gamma: 90
cell_volume: 469.545
crystal_density: 5.371
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: ANQwAAA1DAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAgAIAQCIAAgAAIUABCpAIQYCMYVUAwMgBEFQlJ3kk0kUGFGUw7cyKdRpM2b+e6ZSPpPdfo9rMb79u7+N/N+/l+3KW9t/d7f5/v1b13ve6/93y9ry3//X2/vv582/7m6vdP79q7O/fun7vrf6ud==


formula: (Sr.7 La.3) Nb2 O6
compound: Synthetic
pub_title: Synthesis and characterisation of reduced niobates [Sr1-xLnxNb2O6, Ln = La, Nd]
formula_title: Sr0.7La0.3Nb2O6
a: 11.053
b: 7.640
c: 5.556
alpha: 90
beta: 90
gamma: 90
cell_volume: 469.176
crystal_density: 5.448
atoms_sites: ["Sr", "La", "Nb", "O1", "O2", "O3", "O4"]
atoms_x: UIUCAFCFAgAwqQgAMIH+/8DdDABw+ggA4IEHAA==
atoms_y: QEIPAEBCDwBAu///gDICAKD9AgBAQg8AwL3w/w==
atoms_z: wPsgAMD7IACAMgIA4NoNACBHFgBAK/7/AE0IAA==
atoms_occupancy: gLkqAIBPEgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EBcBABAXAQAQDQEAILIAADABAQA4TwAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAQAIAQCIAAgAAISABDJAIQYCMYTUAwMgBEDQlJ1jk0icGHGUQ+8SOdRts2buf6WSPePc7oVskf/We3+KrN9/V3rJW/v/7/PXvv1Jz3v/5//rp/qxfu/r1/e39+/fbj6ffn1/29nf7vj1ryv5Xf==


formula: Li P
compound: Synthetic
pub_title: Zur Struktur von LiP und KSb
formula_title: LiP
a: 5.582
b: 4.940
c: 10.255
alpha: 90
beta: 118.15
gamma: 90
cell_volume: 249.334
crystal_density: 2.020
atoms_sites: ["Li1", "Li2", "P1", "P2"]
atoms_x: 8CANAJDGDQBQURMAoJ0SAA==
atoms_y: QKgXANBDKACAozYAUI0JAA==
atoms_z: sCIUANDJAQAw0hEAIN4GAA==
atoms_occupancy: 0
atoms_u_iso: EIUBAKCGAQCgvgAAQLUAAA==
atoms_aniso_label: ["Li1", "Li2", "P1", "P2"]
atoms_aniso_u11: IGEBANB+AQCQsAAAILIAAA==
atoms_aniso_u22: 0EwBACBIAQCQyQAAQLUAAA==
atoms_aniso_u33: YMsBAKCfAQAAyAAA8KAAAA==
atoms_aniso_u12: ABkAADDf///wCgAAUPv//w==
atoms_aniso_u13: IOQAACCAAABwYgAAYDsAAA==
atoms_aniso_u23: oN3//+AVAACgDwAAAAAAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAIAQQAAAAAgIAAACAAQACAMCgAIEIAAwAkBAAoAIgiBRHAAqACASGyQAWEDQoLQBFWg3MUQGikTpKawIMBakoA/mUDoUPA9DvrBg30oKkrd6JtOvRFf5/QAnZ2cGW0wJLzZattnk+la9qS3FtT==


formula: K Sb
compound: Synthetic
pub_title: Zur Struktur von LiP und KSb
formula_title: KSb
a: 5.582
b: 4.940
c: 10.255
alpha: 90
beta: 118.15
gamma: 90
cell_volume: 249.334
crystal_density: 8.570
atoms_sites: ["K1", "K2", "Sb1", "Sb2"]
atoms_x: UFwNADCeDgCwqhMAyHkTAA==
atoms_y: YFoYAMCyKADQ3zYA4CQKAA==
atoms_z: YEAUAFDvAQDIexEAwIMHAA==
atoms_occupancy: 0
atoms_u_iso: cPIBAAAmAgCQkQEAYIABAA==
atoms_aniso_label: ["K1", "K2", "Sb1", "Sb2"]
atoms_aniso_u11: wO0BAIB9AgBwjgEA8JoBAA==
atoms_aniso_u22: IN4BAHDZAQAgkwEAMG8BAA==
atoms_aniso_u33: MB4CAPD+AQBAyAEAUFkBAA==
atoms_aniso_u12: sLn//9A5AAAA5///sDYAAA==
atoms_aniso_u13: wNoAAJCwAACA1AAAQGoAAA==
atoms_aniso_u23: ALX///Dx///Q7v//YPD//w==
qdat:
AAAAAAAAAAAAAAAAAAAAAIAQQAAAAAgIAAACAAQACAMCgAIEIAAwAkBAAoAIgiBRHAAqAGASGyAAWEBQoLQBFWg3MUQGikTpKagIMBakoA/mUDoUHA9DPLBg30oKErd6JtHvRFf5/QAnZ2MGW04ZLzZattnk+la9qS3FtT==


formula: Mo O3
compound: Synthetic
pub_title: Least squares refinement of the crystal structure of molybdenum trioxide
formula_title: <missing>
a: 3.9628
b: 13.855
c: 3.6964
alpha: 90
beta: 90
gamma: 90
cell_volume: 202.949
crystal_density: 4.711
atoms_sites: ["Mo", "O1", "O2", "O3"]
atoms_x: iEoFACB7HgDAzx8A0EYCAA==
atoms_y: IDQGAOiOGgCoSAUAYIMNAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAA==
atoms_occupancy: 0
atoms_u_iso: eC0AABhvAAA4fAAAILwAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAQAAAAAAAAAAAAAIQAAAAAIAAAAAAAAIAQAAAABIAgCECAlBAAQgAQACBACCBSAFAgqABQAYQAgBCAIhEAEAIA4QCQEChgZHkBQcIhAoUAxmgCAqggXAigAgIDUFAgBBIkAESAEAAWhAQzCRiUQ2Dhgl==


formula: K.876 Na.071 Al2.889 S2 O14 H6
compound: Hungary
formula_title: <missing>
a: 6.9859
b: 6.9859
c: 17.481
alpha: 90
beta: 90
gamma: 120
cell_volume: 738.825
crystal_density: 2.751
atoms_sites: ["KA", "NaA", "Al", "S", "O1", "O2", "O3", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACwVg0AeLIHAAA7CwA=
atoms_y: AAAAAAAAAACAhB4AAAAAAAAAAABQqfL/iE34/wDF9P8=
atoms_z: AAAAAAAAAACAhB4AeGsSALB0FwBQSvz/mJEIAGDGBgA=
atoms_occupancy: gHc1AGBVBADgxjoAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: YGcBAGBnAQBAnAAAgLsAACBIAQCgCQEAYOoAAKCAAgA=
atoms_aniso_label: ["KA", "NaA", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: 4KUBAOClAQBgbQAAgLsAAKCGAQCAOAEA4KsAAA==
atoms_aniso_u22: AAAAAAAAAACgjAAAAAAAAAAAAACAOAEA4KsAAA==
atoms_aniso_u33: oAkBAKAJAQDA2gAA4KsAAOCrAAAA+gAAgDgBAA==
atoms_aniso_u12: IMsAACDLAADgLgAAwF0AACDLAADA2gAAIE4AAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQB8AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQB8AAA==
pub_title:
 Thermal expansion of alunite up to dehydroxylation
 and collapse of the crystal structure
 Note: T = 300 C

qdat:
AAAAAAAAAAAAAAAAAAoAAgAAAAAAAEgAAACwiAAAAAQAAJRIAAAigBKgAAAQgCaUAAJAAUwAAQBeIACYC4AAQANYAJAHIACBdQAgDAAJBsgCgFAAAOwCgoAAh6AUB4AgYAKHACAeAYMgEPwGDAEFkDBkCBYGDAKXAQKABU==


formula: K.876 Na.071 Al2.892 S2 O14 H6
compound: Hungary
formula_title: <missing>
a: 6.9897
b: 6.9897
c: 17.574
alpha: 90
beta: 90
gamma: 120
cell_volume: 743.564
crystal_density: 2.734
atoms_sites: ["KA", "NaA", "Al", "S", "O1", "O2", "O3", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACQWA0AQLMHAOA3CwA=
atoms_y: AAAAAAAAAACAhB4AAAAAAAAAAABwp/L/wEz4/yDI9P8=
atoms_z: AAAAAAAAAACAhB4AsGUSAMhmFwCIRPz/wJEIAPDHBgA=
atoms_occupancy: gHc1AGBVBACA1joAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: gLUBAIC1AQCAuwAAwNoAAAB3AQAgSAEAoAkBAADuAgA=
atoms_aniso_label: ["KA", "NaA", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: APQBAAD0AQAAfQAAwNoAACDFAQAAdwEAIMsAAA==
atoms_aniso_u22: AAAAAAAAAABAnAAAAAAAAAAAAAAAdwEAIMsAAA==
atoms_aniso_u33: gDgBAIA4AQCgCQEAYOoAAMDaAACAOAEAAHcBAA==
atoms_aniso_u12: APoAAAD6AACAPgAAYG0AAGDqAACgCQEAIE4AAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACgDwAAQB8AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAACgDwAAQB8AAA==
pub_title:
 Thermal expansion of alunite up to dehydroxylation
 and collapse of the crystal structure
 Note: T = 400 C

qdat:
AAAAAAAAAAAAAAAAABIAAgAAAAAAAEgAAAFSCAAAAAgAASSIAACDACTAAAAggFmkAAhABVQAAQC6IAEYJwAAgAaoATAOIACC+gBADAARCogFgdAAAbgEhIABDSAkDoAg4ASNACAqAYMgEegSGAILILDICDwKHASdAgUADU==


formula: K.876 Na.071 Al2.916 S2 O14 H6
compound: Hungary
formula_title: <missing>
a: 6.9916
b: 6.9916
c: 17.621
alpha: 90
beta: 90
gamma: 120
cell_volume: 745.958
crystal_density: 2.730
atoms_sites: ["KA", "NaA", "Al", "S", "O1", "O2", "O3", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACAWQ0AgLQHAFA2CwA=
atoms_y: AAAAAAAAAACAhB4AAAAAAAAAAACApvL/gEv4/7DJ9P8=
atoms_z: AAAAAAAAAACAhB4A8GESABhiFwBoQfz/EJIIAAC9BgA=
atoms_occupancy: gHc1AGBVBACAUzsAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: YOQBAGDkAQAgywAAYOoAAECWAQDAVwEAQBkBACC5AwA=
atoms_aniso_label: ["KA", "NaA", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: 4CICAOAiAgCgjAAAAPoAAMDUAQCghgEAIMsAAA==
atoms_aniso_u22: AAAAAAAAAADgqwAAAAAAAAAAAACghgEAIMsAAA==
atoms_aniso_u33: YGcBAGBnAQDgKAEAAPoAAKAJAQBgZwEAQJYBAA==
atoms_aniso_u12: oAkBAKAJAQAgTgAAYG0AAGDqAABAGQEAIE4AAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACgDwAAQB8AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAACgDwAAQB8AAA==
pub_title:
 Thermal expansion of alunite up to dehydroxylation
 and collapse of the crystal structure
 Note: T = 450 C

qdat:
AAAAAAAAAAAAAAAAABIAAgAAAAAAAIgAAAJSCAAAAAgAAiUIAACFAEVAAABBAJGkAAiACmQAAQEqIAIwKwAAgATIATAaIAEC2gCQFAARFpAFgeAAAWgFCIABFSAoDoAgwAiVAEBcAQcgIfgUGAINIKFICHQSOAk2AgUAFY==


formula: K.876 Na.071 Al2.796 S2 O14
compound: Hungary
formula_title: <missing>
a: 6.9935
b: 6.9935
c: 17.640
alpha: 90
beta: 90
gamma: 120
cell_volume: 747.168
crystal_density: 2.663
atoms_sites: ["KA", "NaA", "Al", "S", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACgVw0AILoHAA==
atoms_y: AAAAAAAAAACAhB4AAAAAAAAAAABgqPL/4EX4/w==
atoms_z: AAAAAAAAAACAhB4AIF8SALBbFwDQOPz/MJAIAA==
atoms_occupancy: gHc1AGBVBACA4jgAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oAMCAKADAgBAlgEAwNQBAKCAAgDgIgIAQBMCAA==
atoms_aniso_label: ["KA", "NaA", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: IMUBACDFAQDgqwAA4CgBAOAiAgAA9AEAAPoAAA==
atoms_aniso_u22: AAAAAAAAAAAgywAAAAAAAAAAAAAA9AEAAPoAAA==
atoms_aniso_u33: QJACAECQAgDASwMA4BwDACA8AwAA7gIA4BYEAA==
atoms_aniso_u12: wNoAAMDaAAAgTgAAoIwAAEAZAQAgSAEAYG0AAA==
atoms_aniso_u13: AAAAAAAAAACgDwAAAAAAAAAAAACgDwAAoA8AAA==
atoms_aniso_u23: AAAAAAAAAACgDwAAAAAAAAAAAACgDwAAoA8AAA==
pub_title:
 Thermal expansion of alunite up to dehydroxylation
 and collapse of the crystal structure
 Note: T = 500 C

qdat:
AAAAAAAAAAAAAAAAABIAAgAAAAAAAIgAAAJSEAAAAAgAAkUIAAEFAElAAABBAJGkAAiACqQAAQEqIAIwKwAAgAjQAjAaIAEF2gCQGAAiFJAJguAAAWgFCQABFSBIDoAgwAkVAEBcAQZAIvgUKAQNQSHQCHQWOAk2BAoAGY==


formula: Ca6 Al6.772 Fe.228 O16.748 Cl.624
compound: Ettringer Bellerberg volcano near Mayen, Eifel district, Germany
formula_title: <missing>
a: 12.0320
b: 12.0320
c: 12.0320
alpha: 90
beta: 90
gamma: 90
cell_volume: 1741.861
crystal_density: 2.768
atoms_sites: ["Ca", "Al1", "Fe1", "Al2", "O1", "O2", "O2a", "Cl"]
atoms_x: wGkIAKj8AACo/AAA4Gc1APgoAgDoOQsAoEQMAGDjFgA=
atoms_y: AAAAAKj8AACo/AAAAAAAAMAkGwDoOQsAkGMRAAAAAAA=
atoms_z: QEIPAKj8AACo/AAAQEIPAMgpCQDoOQsAcHAGAEBCDwA=
atoms_occupancy: AAk9AGCOOQCgegMAAAk9AAAJPQCgPDcAwLwFAACyDAA=
atoms_u_iso: qFwAAIBIAACASAAA8DIAAGhqAACQeQAAoHMAAMCPAAA=
atoms_aniso_label: ["Ca", "Al1", "Fe1", "Al2", "O1", "O2", "O2a", "Cl"]
atoms_aniso_u11: gGsAAIBIAACASAAAqCoAABh5AACQeQAAoIwAAEA4AAA=
atoms_aniso_u22: MGYAAIBIAACASAAAKDcAAABfAACQeQAA8CMAAIC7AAA=
atoms_aniso_u33: IEQAAIBIAACASAAAKDcAACBnAACQeQAAwKgAAIC7AAA=
atoms_aniso_u12: AAAAABgQAAAYEAAAAAAAAPjk///g4///wBIAAAAAAAA=
atoms_aniso_u13: AAAAABgQAAAYEAAAAAAAAMjJ///g4///IAMAAAAAAAA=
atoms_aniso_u23: mAgAABgQAAAYEAAAAAAAALgLAADg4///8CMAAAAAAAA=
pub_title:
 A reinvestigation of mayenite from the type locality, the Ettringer Bellerberg
 volcano near Mayen, Eifel district, Germany

qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAEABAAAAgBACAIAACAQAAACAgIAAgIEBAgQAAECCCBBBABBABCCEAIIQhCEAIBCEIQCEABEQiEQEIgIAEREBABEAAkQEQAgAAgAAAgAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Mn3 Fe2 Si3 O12
compound: Calculated structure
pub_title: Parameterization of energy and interactions in garnets: End-member properties
formula_title: <missing>
a: 11.8288
b: 11.8288
c: 11.8288
alpha: 90
beta: 90
gamma: 90
cell_volume: 1655.092
crystal_density: 4.437
atoms_sites: ["Mn", "Fe", "Si", "O"]
atoms_x: IKEHAAAAAABg4xYAwD0CAA==
atoms_y: AAAAAAAAAAAAAAAAqCIDAA==
atoms_z: QEIPAAAAAABAQg8A+BsoAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAACAAAgAAAAAAAQAIAAAEAEAIAQAAEAgAAAEAgIAAgICBAgQAACBAggQQQAQQAQQggBCCEIIQBAEIQhAIQAEIhEQgIRAIAIhEBACIAAiIEQAgAAQAAAQAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAA==


formula: Pb2 As O3 Cl2 H
compound: Lavrion, Greece
formula_title: Pb2(AsO2OH)Cl2
a: 6.4235,
b: 5.5399,
c: 9.321
alpha: 90
beta: 90.767
gamma: 90
cell_volume: 331.663
crystal_density: 6.100
atoms_sites: ["Pb1", "Pb2", "As1", "O2", "O-H1", "Cl1", "Cl2"]
atoms_x: OKIRAJBeIACANy8AAFQkAMBJLQBwpA4A8CQ2AA==
atoms_y: QEIPAEBCDwBAQg8AYNEAAEBCDwBAQg8AQEIPAA==
atoms_z: sPMaANA4MwDwFRMAsGcVAMAzBwDw/wUAoEsoAA==
atoms_occupancy: 0
atoms_u_iso: QM4AALD+AADwoAAAYOoAAGBnAQAwPQEA8B0BAA==
atoms_aniso_label: ["Pb1", "Pb2", "As1", "O2", "O-H1", "Cl1", "Cl2"]
atoms_aniso_u11: wHYAAKDwAAAQWQAAAH0AAAD6AACAuwAAwNoAAA==
atoms_aniso_u22: MMAAAEAZAQBQqgAAoIwAAMBRAgBAlgEAIMsAAA==
atoms_aniso_u33: YDUBAOD2AAAA4QAAwNQBAAD6AADAVwEAQJYBAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: MBEAAJAzAABQFAAAAAAAAOAuAACAPgAAgD4AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAYPD//wAAAAAAAAAAAAAAAA==
pub_title:
 Pb2(AsO2OH)Cl2, a new phase from the Lavrion ancient slags, Greece:
 occurrence and characterization

qdat:
AAAAAAAAAAAQAAAAIAAAgAkAAgAEgIAACCCAADCFAQSAwgAwhgrKEJRBQJCpUzCwActPgviBoBJvdKbTHHPz1EvSy1jFh283q1Gbv7v1PS2W4/0dJ+3/vc+n7g3+brdv1OLv/rz/vP+ndu/jv6bv/O9+//n/Ld36v/fvX7==


formula: Mg O H F
compound: Synthetic
formula_title: Mg(OH)F
a: 10.1299
b: 3.0723
c: 4.676
alpha: 90
beta: 90
gamma: 90
cell_volume: 145.527
crystal_density: 2.753
atoms_sites: ["Mg", "O", "H", "F"]
atoms_x: oBEIANCRGwBwcDgAcH4MAA==
atoms_y: wMYtAMDGLQDAxi0AQEIPAA==
atoms_z: 0C4fAIC0LwCA6DcAkJwtAA==
atoms_occupancy: 0
atoms_u_iso: 8CMAAFAUAAAwRAQAUF8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structure of magnesium hydroxide fluoride, Mg(OH)F:
 a topological intermediate between brucite- and rutile-type structures

qdat:
AAAAAAAAAAAAAAAAAAAACAAACAAAAAEAAAAAAAQBBIQABCggAIAQAEEAIQgAgggAIBgA0BJQEAyJkARBAEThRSgQIEQOwAhCMDjAiFEMeRGQD0IRWl1RSmBqwSppQBUKkQAGHvJApXE2Ti0NqsRXgOCnvrhg4VgVfmRZWS==


formula: Zn O H F
compound: Synthetic
formula_title: Zn(OH)F
a: 10.2280
b: 3.1125
c: 4.7165
alpha: 90
beta: 90
gamma: 90
cell_volume: 150.148
crystal_density: 4.485
atoms_sites: ["Zn", "O", "H", "F"]
atoms_x: wG4IAKBnGwAgVjkAgHMMAA==
atoms_y: wMYtAMDGLQDAxi0AQEIPAA==
atoms_z: kG0gAOAIMADQGzcAwD0vAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structure of magnesium hydroxide fluoride, Mg(OH)F:
 a topological intermediate between brucite- and rutile-type structures
 Note: transformed from Serier et al (2007)

qdat:
AAAAAAAAAAAAAAAAAAAAEAAAEAAAAAQAAAAAABAIIiAAIUEABACAAggBCEAIIEACAYAJASoCANCrAYBACRQwpQIEFIHYAShUDRAVDIMtBKgDogjfRaVc0DegxsegGZTSgA4dcWDGqJovHCmbMmSFYSusocnmJFH4qW0iUO==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7850
b: 9.1324
c: 5.1924
alpha: 90
beta: 101.751
gamma: 90
cell_volume: 454.271
crystal_density: 5.160
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABQVxIAcDgHABBlFwCg7xUA
atoms_y: oG43AOB9EACQqwUAQH4FACCpDgDQCAQA
atoms_z: QEIPAEBCDwBQKg0AoHUIAJAmFwAgxjcA
atoms_occupancy: 0
atoms_u_iso: IDUAAAAyAAAAMgAAwEQAALA2AACgKAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 4 K

qdat:
AAAAAAAAAAAAAAABAAAAABAgAAACAABCAACAQAAAQQCCABQUAINAAAIJNAJAACCYEDgQRNARSMACcoAQ4sMo0NqMAEmTsAu6iVBg3mBJ2UccJp7fFzDaP0WYMhiPeLFn8ZLxWDbCoT3WT4fCJEjZW3BNmh3pOkmhnHD5nd==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7840
b: 9.1338
c: 5.1924
alpha: 90
beta: 101.753
gamma: 90
cell_volume: 454.291
crystal_density: 5.160
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADAVRIAkDsHAMBpFwCA7BUA
atoms_y: MHA3AJCCEACQqwUAYIEFALCqDgDQCAQA
atoms_z: QEIPAEBCDwBQKg0AUHoIANAsFwAgxjcA
atoms_occupancy: 0
atoms_u_iso: IDUAAIA+AADwPAAAkEwAAHAwAAAwKgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 15 K

qdat:
AAAAAAAAAAAAAAABAAAAABAgAAACAABCAACAQAAAQQCCABQUAINAAAIJNAJAACCYECgQRNARSMACcoAQ4sMo0NqMAEmTsAu6jlBQ3mBV2cccJpbfFzDaP0WYNBiPeLFn8ZLxWBbCoT3UTYfCZEjZW3BNmh3pOkmhnHD5nd==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7840
b: 9.1342
c: 5.1924
alpha: 90
beta: 101.754
gamma: 90
cell_volume: 454.309
crystal_density: 5.160
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAVxIA0EEHAABwFwDw6hUA
atoms_y: UHM3ACCEEAAgrQUAoIcFALCqDgDwCwQA
atoms_z: QEIPAEBCDwAwJw0A4HsIAPAvFwDAvDcA
atoms_occupancy: 0
atoms_u_iso: gCUAAIA+AAAAMgAAwEQAALAdAADwIwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 30 K

qdat:
AAAAAAAAAAAAAAABAAAAABAgAAACAABCAACAQAAAQQCCABQUAINAAAIJNAJAACCIECgQRNARSMACcoAQ4sMo0NyMAEmTsAu6jlBQXmBV2cccJpbfFzDaP0WYNBiPeLFn8ZLxWBbCoT3UTYfCZEjZW3BNmhXpOkmhnHD5nd==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7838
b: 9.1349
c: 5.1929
alpha: 90
beta: 101.750
gamma: 90
cell_volume: 454.385
crystal_density: 5.159
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACAVBIAQEAHAJBxFwDQ5xUA
atoms_y: 4HQ3ACCEEADAowUAEIYFAGCvDgCQAgQA
atoms_z: QEIPAEBCDwBwLQ0AMJAIAHA8FwCguTcA
atoms_occupancy: 0
atoms_u_iso: QB8AAFAtAADwPAAAgFcAAJAaAAAAGQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 50 K

qdat:
AAAAAAAAAAAAAAABAAAAABAgAAACAABCAACAQAAAQQCCABQUAINAAAIJNAJAACCYECgQSNARSMACUoAQ4sMo0OyMAEmTsAu6ilBQ3mCZ2cccJpbfFzDaO0WYNBiNeLFn8ZTxWDbCoT/Uj4fCZFjZW3BNmhXpOkmhlHD5nf==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7848
b: 9.1369
c: 5.1936
alpha: 90
beta: 101.764
gamma: 90
cell_volume: 454.569
crystal_density: 5.157
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABQUhIAYEMHAMBpFwCw5BUA
atoms_y: MHA3ALCFEABQpQUAgIQFALCqDgCwBQQA
atoms_z: QEIPAEBCDwDAKA0AUJMIALBCFwDAvDcA
atoms_occupancy: 0
atoms_u_iso: 8CMAABAnAABAOAAAIE4AAOAVAABwMAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 100 K

qdat:
AAAAAAAAAAAAAAABAAAAABBAAAACAABCAACAgAAAQQCCABQUAINAAAIJNAJAACCYECgQSNARSMACUoAQ4sIo0PyMAEmTsAv9ClBg3kCa2cccJq/bHTHcO0WYVBiVeTHnsZTx2DbCoT/Uj4fCZFjZW7BNmhnpOkuhlHD6mf==


formula: Fe Ge O3
compound: Synthetic
formula_title: FeGeO3
a: 9.7993
b: 9.1491
c: 5.1991
alpha: 90
beta: 101.891
gamma: 90
cell_volume: 456.122
crystal_density: 5.139
atoms_sites: ["Fe1", "Fe2", "Ge", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAIVBIAaEUHAABwFwAw5xUA
atoms_y: EG03AHB/EAAwogUAoIcFAJCnDgAQ9gMA
atoms_z: QEIPAEBCDwAgMg0AUJMIAMBQFwCAzzcA
atoms_occupancy: 0
atoms_u_iso: AEsAAPBVAAAQWQAAIIAAAOBgAABwYgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic and low-temperature structural behavior of clinopyroxene-type FeGeO3:
 A neutron diffraction, magnetic susceptibility, and Fe Mossbauer study
 T = 298 K

qdat:
AAAAAAAAAAAAAAABAAAAABBAAAACAABCAACAgAAAQQCCABQUAIWAAAIJJAJAAEEYEFgQSJAyiMACVIAApYIp0X2IAEsWoBX9GpCgvkCc8Ys0qy6bPSHsPkmYZCkf6iHLopjjWDzEwT9Uj4+CpNDbG/DdGhGxXE1CmHNqmb==


formula: As S
compound: Synthetic
pub_title: The dual behavior of the beta-As4S4 altered by light
formula_title: <missing>
a: 9.967
b: 9.355
c: 8.921
alpha: 90
beta: 102.520
gamma: 90
cell_volume: 812.025
crystal_density: 3.501
atoms_sites: ["As1", "As2", "S1", "S2", "S3"]
atoms_x: sAQAANBc9v8AAAAAAAAAAGCi8/8=
atoms_y: cH7z/zBc5/8QWPz/sGze/3BX7f8=
atoms_z: EGADAMD7BwBAQg8AQEIPAJCcFAA=
atoms_occupancy: 0
atoms_u_iso: oP0CAECQAgAA9AEAILkDAOAiAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAAAAkIAgIAAAAEgBAQsAAkAAIkghCMAUDBgyiEkB0SAAkRkejCwaAkbYCCk4qETIMuK3C6Rkm4qbfpqf9Ffja9sfrzbPzs/O7/3s+Xl3lt3avb97zh964vY3J8f9ZvK6toSPVohjjeuTkC0eKZks4==


formula: Fe Si2
compound: Synthetic
pub_title: Om jarn-kisellegeringarnas byggnad
formula_title: <missing>
a: 2.69
b: 2.69
c: 5.08
alpha: 90
beta: 90
gamma: 90
cell_volume: 36.759
crystal_density: 5.060
atoms_sites: ["Fe", "Si"]
atoms_x: AAAAAICEHgA=
atoms_y: AAAAAICEHgA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAAAAAgAQAAgAAAAAAAAAAgCABAABAAAAAACAAAAgAAABAAEAFAAAAgQEAQAAAAIAAYAAAgAABAAAQAgIAABECAgAATBAIAATAAQABIAFAAIAggIAYAQEBIAIECAgAAEhBAgz==


formula: Ca C O3
compound: Synthetic
pub_title: Microtwinning hypothesis for a more ordered vaterite model
formula_title: <missing>
a: 8.4721
b: 7.1575
c: 4.1265
alpha: 90
beta: 90
gamma: 90
cell_volume: 250.227
crystal_density: 2.657
atoms_sites: ["Ca", "C", "O1", "O2"]
atoms_x: gIQeAEBCDwCwKRcAQEIPAA==
atoms_y: gIQeAAAQJwDw9SgAgCchAA==
atoms_z: AAAAAICWGwBAZiIAgKsLAA==
atoms_occupancy: 0
atoms_u_iso: IHABAIBpAgCAaQIAgGkCAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAIABAAAAAAIAAAAAAAAYAECAQAAAMEGBAABEAAAAMIBAAAQACMMBgYAAARgBCBAZgAEIAABQJEQQMGYcsAARhABg2zCCAAJaACAyYwgAdqTEPgGYADgwCHtnEAFmyI9uFgB7gGH0wg==


formula: C2 H5 O N
compound: Synthetic
formula_title: <missing>
a: 11.513
b: 11.513
c: 12.883
alpha: 90
beta: 90
gamma: 120
cell_volume: 1478.852
crystal_density: 1.194
atoms_sites: ["C1", "C2", "H1", "H2", "H3", "H4", "H5", "O", "N"]
atoms_x: qBcdAIjRFABQ0w4AYIYZAHDHHQDwBiIAYIcdAFi3DgCoYRQA
atoms_y: sO0HAHg8AAAw1vT/UFH6/1CBCwDAnQYAQKULAKD2///g5Pn/
atoms_z: WDICACBlAgBgewYAsIkHADBqBgBwJAIAYC7+/zjc//9QjAUA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["C1", "C2", "H1", "H2", "H3", "H4", "H5", "O", "N"]
atoms_aniso_u11: kGUAAFBGAABg6gAAYOoAACBCAgCgCQEA4CICABBZAABgbQAA
atoms_aniso_u22: IGcAAHBJAABg6gAAIEgBAMDUAQBAlgEAwNQBAOBgAADwbgAA
atoms_aniso_u33: 0J0AALBoAACAtQEA4KUBAKADAgBAfgUA4CICAACvAACgpQAA
atoms_aniso_u12: wBIAAJAaAADgLgAAQJwAAGDw///gqwAAwOD//6AoAABwMAAA
atoms_aniso_u13: cP7//3D+//+gDwAA4LH//yBOAACAPgAAYHP//wDn//8w+P//
atoms_aniso_u23: kAEAAJABAAAgTgAAgD4AAMDm/v/gLgAAgDgBABAOAADQIAAA
pub_title:
 Neutron diffraction at 23 K and ab initio molecular-orbital studies of
 molecular structure of acetamide
 Note: T = 23 K

qdat:
AAAAAAAAAAAAAAAAAAQIAAAAAAEAAgEEQAQAIACAAQBBAgEAVRAAgQikQBghDRAoIDggNIjSBwgKRMAOoGkqgHpGQKQ8g6WUKQVJUNAZSIdB0cj1MKoVSo6MBWWHR4AOhqodDlQ4ONAVogGKFHRNQEaUGMAmCKhBhgBCJE==


formula: Cu3 V2 O11 H6
compound: Synthetic
pub_title: T = 323 K
formula_title: <missing>
a: 10.657
b: 5.887
c: 7.228
alpha: 90
beta: 95.035
gamma: 90
cell_volume: 451.719
crystal_density: 3.489
atoms_sites: ["Cu1", "Cu2", "V", "O1", "O2", "O3", "O4", "Wat5", "H"]
atoms_x: AAAAAEBCDwBYy///AAAAAODiFACwaQQAgNkUAOC6CgDAXBUA
atoms_y: AAAAAEBCDwCAhB4AgIQeAICEHgAweRAAAAAAAAAAAACAhB4A
atoms_z: AAAAAAAAAADYfA8AgIQeAAAhBwCgYwsAQE0JANDEHwCQbw8A
atoms_occupancy: 0
atoms_u_iso: MMAAAKjFAACABgEA4J8CAACvAACAzgEAQOcAAFA0AwBg0QAA
atoms_aniso_label: ["Cu1", "Cu2", "V", "O1", "O2", "O3", "O4", "Wat5"]
atoms_aniso_u11: ILIAAHDGAACQsAAAgDgBAFDDAADQMwEAQAABAABlBAA=
atoms_aniso_u22: wHYAAGBUAADgpQEA4AoGAMArAABg/QEA4HkAAADoAwA=
atoms_aniso_u33: ECEBALAwAQCgvgAAQJwAAKAiAQBARQIAgDgBAMBXAQA=
atoms_aniso_u12: AAAAAIDz//8AAAAAAAAAAAAAAAAQWQAAAAAAAAAAAAA=
atoms_aniso_u13: 0DkAAIDz///wIwAAgD4AAIAlAADQawAAEA4AAIA+AAA=
atoms_aniso_u23: AAAAAJABAAAAAAAAAAAAAAAAAADADAEAAAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAEAAAACIAAAAEAAAQAAAAEEUAEECAATAAhAAkAgEQIEoCQQBo0oAAAAShRaKRgiNgBJwsBMFCm0AkFYlXsxRHHAojgNnvyz2DibvBIbZPJqRHzV5jS+kdCtWqwW5Z3K5P8SPsXHPzuVnl+r41ix4XTSkX==


formula: Ca3 Si S1.82 O25.66 H30
compound: Bellerberg, near Kottenheim, Eastern Eifel area,
formula_title: <missing>
a: 11.1548
b: 11.1548
c: 10.5702
alpha: 90
beta: 90
gamma: 120
cell_volume: 1139.036
crystal_density: 1.888
atoms_sites: ["Ca", "Si", "S", "Wat1", "Wat2", "Wat3", "O-H4", "O5", "O6"]
atoms_x: oMcLAAAAAABVWBQAwM0XAKBcCABVWBQAEEIIAFVYFACAqwsA
atoms_y: QD7//wAAAACrsCgA0DAOAEB/8P/QDf//4MwHAKuwKADQbiUA
atoms_z: QEIPAAAAAAAAAAAAQEIPAEBCDwCQ+xkAYEkGAGCj9//gCQIA
atoms_occupancy: AAk9AAAJPQDAijcAAAk9AAAJPQAACT0AAAk9AIB9NADAbDwA
atoms_u_iso: qBsAAKjZAABIngAAqNkAAOAoAQDAdgAA+MUAAEgbBgDoGAQA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kottenheimite, Ca3Si(OH)6(SO4)2*12H2O, a new member of the ettringite group
 from the Eifel area, Germany
 Rhineland-Palatinate, Germany

qdat:
AAAAAAAAAABAAACAAABBASCBAAAICIICEAhQBERSIoEJkQALIyCYEkyTIbRWKTYeChiblCcXaFgxWm1SnNWD7aiq7r7yuXOrv78fDf1fc8/6bX/7qz/Xu+m6z57/PvWpXcsXa/XfX5a0Nvo67vNZlo/fg1C7RpzWqjYxE1==


formula: Ag7.998 Sn (S3.897 Te2.103)
compound: Lengenbach Quarry, Binntal, Canton Valais, Switzerland
formula_title: <missing>
a: 11.0003
b: 11.0003
c: 11.0003
alpha: 90
beta: 90
gamma: 90
cell_volume: 1331.109
crystal_density: 6.860
atoms_sites: ["Ag1", "Ag2", "Sn", "SX1", "TeX1", "SX2", "TeX2", "SX3", "TeX3"]
atoms_x: EIgNABA1GgBAQg8AYOMWAGDjFgAAAAAAAAAAAMDGLQDAxi0A
atoms_y: AAAAABA1GgBAQg8AYOMWAGDjFgAAAAAAAAAAAMDGLQDAxi0A
atoms_z: AAAAAACBLgBAQg8AYOMWAGDjFgAAAAAAAAAAAMDGLQDAxi0A
atoms_occupancy: YNEZAGDFGwAACT0AgGYjAICiGQDAui8AQE4NAOCFMAAggwwA
atoms_u_iso: oMsCAJDWAgCgNQIAYBADAGAQAwCg/QIAoP0CAKD9AgCg/QIA
atoms_aniso_label: ["Ag1", "Ag2", "Sn", "SX1", "TeX1", "SX2", "TeX2", "SX3", "TeX3"]
atoms_aniso_u11: wM4CAJDWAgCgNQIAYBADAGAQAwCg/QIAoP0CAKD9AgCg/QIA
atoms_aniso_u22: EMoCAJDWAgCgNQIAYBADAGAQAwCg/QIAoP0CAKD9AgCg/QIA
atoms_aniso_u33: EMoCAJDWAgCgNQIAYBADAGAQAwCg/QIAoP0CAKD9AgCg/QIA
atoms_aniso_u12: AAAAAAAAAAAAAAAAIAMAACADAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAJABAAAAAAAAIAMAACADAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u23: cP7//5ABAAAAAAAAIAMAACADAAAAAAAAAAAAAAAAAAAAAAAA
pub_title:
 Te-rich canfieldite, Ag8Sn(S,Te)6, from Lengenbach Quarry, Binntal,
 Canton Valais, Switzerland: Occurrence, description and crystal structure

qdat:
AAAAAAAAAAAAAAAAEAAgAAAAAAAgAAAEAgAAAAQAAEEAAACAAEAAABAAIQAAQAEQAAgAiAAQAQAAQAkABAEgAQCQAIBAAICQAgEgAAkAICACAoAgSAIEAIEAAEgIFAAKAAQBAACAgAIAgAACAAQAEAAAAACAAAAAAAAABA==


formula: Mg1.5 S O5 H
compound: Nepa deposit of potassium salts, Eastern Siberia, Russia
pub_title: Crystalline structure of a new natural Mg-sulfate Mg3[SO4]2(OH)2
formula_title: <missing>
a: 5.254
b: 5.254
c: 12.971
alpha: 90
beta: 90
gamma: 90
cell_volume: 358.058
crystal_density: 2.774
atoms_sites: ["Mg", "S", "O1", "O2", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_y: AAAAAMDGLQAAvR8AQEIPAOD9HAA=
atoms_z: gIQeACChBwAAhgsAYOMWAICuFwA=
atoms_occupancy: wMYtAAAJPQAACT0AAAk9AEBCDwA=
atoms_u_iso: IHABAOhsAABQ/wAAwCoBAJAXAwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAIMAAAAAABAAAAAoAAAACIAAAAoAAA4AAAEgAAAAAA4AAJAAAFAAMAAWgAAQAMAAhAAEACgAegAAAGACwAFAGAAoACAMALABgBADwAADgAgAAGAPACAYBYAQGASAADAMAMBgeAIC==


formula: Rb Al S2 O20 H24
compound: Synthetic
pub_title: Refinement of the alum structures. III. X-ray study of the a alums, K, Rb and NH4Al(SO4)2*12H2O
formula_title: <missing>
a: 12.243
b: 12.243
c: 12.243
alpha: 90
beta: 90
gamma: 90
cell_volume: 1835.116
crystal_density: 1.885
atoms_sites: ["Rb", "Al", "S", "O(1)", "O(2)", "Wat(1)", "Wat(2)"]
atoms_x: gIQeAAAAAADwFRMA8BQPAEBcEwCwwAIAUA4BAA==
atoms_y: gIQeAAAAAADwFRMA8BQPAHAbEADglAgAwBj//w==
atoms_z: gIQeAAAAAADwFRMA8BQPAFDcGQBwKBIAIHwJAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Rb", "Al", "S", "O(1)", "O(2)", "Wat(1)", "Wat(2)"]
atoms_aniso_u11: SFECAJAoAQAwTAEAIGwFACCwAgCozgEAeIIAAA==
atoms_aniso_u22: SFECAJAoAQAwTAEAIGwFAADXBQDwYwEAiNoBAA==
atoms_aniso_u33: SFECAJAoAQAwTAEAIGwFAPDCAQDYvQAAOJoAAA==
atoms_aniso_u12: 0G8BAHiCAADAuP//YJgCAGD3AgDgCwAAQEcAAA==
atoms_aniso_u13: 0G8BAHiCAADAuP//YJgCAChC//8g9P//+LEAAA==
atoms_aniso_u23: 0G8BAHiCAADAuP//YJgCADhWAwDgCwAACE7//w==
qdat:
AAAAAAAAAAAAAABAAQAQAgAAQCAAICBAgAQIIIQQQBBCEAhAIRCIiARESIgREiJAkCBIEkkkCUUkEkpISUEhSUoSVKAqVClCiRSiVUiqFFUEFVRFVBVYIlEQooRCRCgAMSAIAJAgAAIgAAAIAAAAQAAAAAAAAAAAAAAAAA==


formula: N Al S2 O20 H24
compound: Synthetic
pub_title: Refinement of the alum structures. III. X-ray study of the a alums, K, Rb and NH4Al(SO4)2*12H2O
formula_title: <missing>
a: 12.240
b: 12.240
c: 12.240
alpha: 90
beta: 90
gamma: 90
cell_volume: 1833.767
crystal_density: 1.627
atoms_sites: ["N", "Al", "S", "O(1)", "O(2)", "Wat(l)", "Wat(2)"]
atoms_x: gIQeAAAAAAAg3BIAgLIOAGAtEwCAyAIAgB8BAA==
atoms_y: gIQeAAAAAAAg3BIAgLIOAHDpDwDwcAgA8Pf+/w==
atoms_z: gIQeAAAAAAAg3BIAgLIOAFB4GQCQKxIAoG8JAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["N", "Al", "S", "O(1)", "O(2)", "Wat(l)", "Wat(2)"]
atoms_aniso_u11: sLsCAEg0AQAoQAEAIC4HAGDYAwB4gAIAMO0AAA==
atoms_aniso_u22: sLsCAEg0AQAoQAEAIC4HABjgBwCwHAEA8KMCAA==
atoms_aniso_u33: sLsCAEg0AQAoQAEAIC4HAMC2AQDIYwEAODsAAA==
atoms_aniso_u12: MO0AABhHAAB4ggAAwBn+/+CmBQD4UgAAaIn//w==
atoms_aniso_u13: MO0AABhHAAB4ggAAwBn+/8C2AQC4agAAYNz//w==
atoms_aniso_u23: MO0AABhHAAB4ggAAwBn+/2AWBwDouP//2F4AAA==
qdat:
AAAAAAAAAAAAAABAAQAQAgAAQCAAICBAgAQIIIQQQAhCEAhAIRCIiARESIgJESJAkCBIEkkUCUSiEkpIKSEhSUoSUqAqUiVChRKhVUiqFFUEE1RFVBVUIjEQooRCJCgAKRAEAJAgAAEgAAAIAAAAQAAAAAAAAAAAAAAAAA==


formula: Hg2 I O
compound: Synthetic
pub_title: Structure of mercury(I,II) iodide oxide, Hg2OI
formula_title: <missing>
a: 17.603
b: 6.981
c: 6.701
alpha: 90
beta: 101.61
gamma: 90
cell_volume: 806.615
crystal_density: 8.961
atoms_sites: ["Hg1", "Hg2", "I", "O"]
atoms_x: GAoaAJDyDgBQ9AYAQHsSAA==
atoms_y: iFkUACDaBQCwShQAENUVAA==
atoms_z: +IsNALjbDAB4uhMA0LIJAA==
atoms_occupancy: 0
atoms_u_iso: ANEBABB2AQAYzQEA8CIBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAQAAAQAAAAAAGIAAAAAkBIBgANQCAgAEDAYAQGAGCQwIAWQIAyxgJCQhrgA3GKGYoJUCelg0qBYSWIzxITQJPkgJHYWuLEyV2KosOY6kXkjKG7yuWUvRLQf6bib2+zTp0rtBe4HiqFalG2Nsux+u1Fj95tw==


formula: (Al.5 Nb.5) O2
compound: Synthetic
formula_title: AlNbO4
a: 12.1545
b: 3.7350
c: 6.4884
alpha: 90
beta: 107.62
gamma: 90
cell_volume: 280.735
crystal_density: 4.351
atoms_sites: ["Al1", "Nb1", "Al2", "Nb2", "O1", "O2", "O3", "O4"]
atoms_x: UNELAFDRCwCQQQYAkEEGAOBJCABAcQMAcBAWAOAAEAA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: oGESAKBhEgDAqSwAwKksALCaAABAMRYAEDgSAABCJwA=
atoms_occupancy: ANQwAAA1DAAANQwAANQwAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: cMYAAHDGAAC4agAAuGoAALDMAAAQUwEAMNkAAHAXAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability, cation ordering, and local
 relaxation along the AlNbO4-Al0.5Cr0.5NbO4 join
 Note: Sample label: N00

qdat:
AAAAAAAAAAAAAAAAAggAAAAAAAAAIEAAABAIQAAgAAAgICBAAABAAQQAVAFhAkBAAECAAQyEYAASIAgSAIEIHhhAKAUNYBAENkBI4WCABLoEMGQhQeJC4zECUCgZCyTAtQIQMMw4FxBAXJhgl4CpWVJIrBYgpRxycG+QA8==


formula: Al.94 Nb O4 Cr.06
compound: Synthetic
formula_title: AlNbO4
a: 12.1620
b: 3.7454
c: 6.4910
alpha: 90
beta: 107.64
gamma: 90
cell_volume: 281.772
crystal_density: 4.370
atoms_sites: ["Al1", "Nb1", "Al2", "Nb2", "O1", "O2", "O3", "O4", "Cr2"]
atoms_x: oO8LAKDvCwAoRQYAKEUGAIByCABwggMA0BkWAAAEEAAoRQYA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_z: iIMSAIiDEgAAsCwAALAsAIDtAADgchYAwAoSAIBnJwAAsCwA
atoms_occupancy: ANQwAAA1DACAiwgAANQwAAAJPQAACT0AAAk9AAAJPQCAqQMA
atoms_u_iso: UPUAAFD1AAAAfQAAAH0AAAD6AADw0gAAIP0AAEC1AAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability, cation ordering, and local
 relaxation along the AlNbO4-Al0.5Cr0.5NbO4 join
 Note: Sample label: N06

qdat:
AAAAAAAAAAAAAAAAAggAAAAAAAAAIIAAABAIQAAgAAAgICBAAABAAQQAmAFBAkCAAIECAQ2IoAAWIBAUAQEQLhiBSAYa4CAQVIBRYmEABiQEINAjA8SI5GEFIEhROYdDJgKgIwxoRxCA8pmCPQFDM05grJQiNDjpIbZABw==


formula: Al.875 Nb O4 Cr.125
compound: Synthetic
formula_title: AlNbO4
a: 12.1724
b: 3.7550
c: 6.4957
alpha: 90
beta: 107.67
gamma: 90
cell_volume: 282.894
crystal_density: 4.391
atoms_sites: ["Al1", "Nb1", "Al2", "Nb2", "O1", "O2", "O3", "O4", "Cr2"]
atoms_x: uPoLALj6CwBQSgYAUEoGAKBcCADAfQMAQP8VAOAAEABQSgYA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_z: KKcSACinEgDAuCwAwLgsACDkAADAVhYAMAkSAPB+JwDAuCwA
atoms_occupancy: ANQwAAA1DADgkwQAANQwAAAJPQAACT0AAAk9AAAJPQAgoQcA
atoms_u_iso: 8OsAAPDrAAB4XwAAeF8AACDkAAAArwAAcFwBABCLAAB4XwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability, cation ordering, and local
 relaxation along the AlNbO4-Al0.5Cr0.5NbO4 join
 Note: Sample label: N12

qdat:
AAAAAAAAAAAAAAAAAggAAAAAAAAAQIAAABAQQABAAAAgIEBAAACAAgQBGALCAkEAAQECAg6QwAAcQCAoAgIgVhoCiAo6wCAgXQCiYsIADKQIIaBGBskRyKEMgZESuw1KZAUgxBlIjhED5ZkEogaHGzLB2WhkcCiUJqRADw==


formula: Al.76 Nb O4 Cr.24
compound: Synthetic
formula_title: AlNbO4
a: 12.1881
b: 3.7726
c: 6.5033
alpha: 90
beta: 107.70
gamma: 90
cell_volume: 284.872
crystal_density: 4.428
atoms_sites: ["Al1", "Nb1", "Nb2", "O1", "O2", "O3", "O4", "Cr1", "Cr2"]
atoms_x: WBQMAFgUDACgVAYA0FQIAABrAwBwEBYA0AsQAFgUDACgVAYA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_z: AO0SAADtEgCQsSwA4MQAAABEFgDQMRIAIHcnAADtEgCQsSwA
atoms_occupancy: AGMuAAA1DAAA1DAAAAk9AAAJPQAACT0AAAk9AABxAgAANQwA
atoms_u_iso: gAYBAIAGAQBwSQAAUFkBABAIAQCwmgAAgIkAAIAGAQBwSQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability, cation ordering, and local
 relaxation along the AlNbO4-Al0.5Cr0.5NbO4 join
 Note: Sample label: N25

qdat:
AAAAAAAAAAAAAAAABAgAAAAAAAAAQQAAABAggABAAABAQECAAACAAgQEEApCBIIAAgQCAh0gwAA0QEAwBASBHDgEEBTqgICAeAGIxUQAE0gQZYCkNaMG6EI0BigkUjzJSAiEcCkJaCIkU9gapA4YMkcC3yFlQEOgbLwAWh==


formula: Al.76 Nb O4 Cr.24
compound: Synthetic
formula_title: AlNbO4
a: 12.1886
b: 3.7748
c: 6.5033
alpha: 90
beta: 107.72
gamma: 90
cell_volume: 285.018
crystal_density: 4.425
atoms_sites: ["Al1", "Nb1", "Nb2", "O1", "O2", "O3", "O4", "Cr1", "Cr2"]
atoms_x: eBwMAHgcDAAoVAYA0FQIAFBmAwCABRYAgCkQAHgcDAAoVAYA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_z: 4AcTAOAHEwBAuywAAK8AAJBeFgAw1xEAQJMnAOAHEwBAuywA
atoms_occupancy: AGMuAAA1DAAA1DAAAAk9AAAJPQAACT0AAAk9AABxAgAANQwA
atoms_u_iso: wFcBAMBXAQBAHwAAgAYBADBDAACwswAAgIkAAMBXAQBAHwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability, cation ordering, and local
 relaxation along the AlNbO4-Al0.5Cr0.5NbO4 join
 Note: Sample label: N37

qdat:
AAAAAAAAAAAAAAAABAgAAAAAAAAAQQAAABAggACAAABAIECAAACAAgQEEApCBEQAAgQCAhygwAAUQEAwBAKCHBgEEBTqgICAeAGIxUQAE0gQZYCkVaMG6EI0Bigk0jxJSAiEYDkKaCIkY7grJB4YEoMC7SEmQEPAaLwA1h==


formula: Ge O2
compound: Synthetic
formula_title: GeO2
a: 4.9858
b: 4.9858
c: 5.6473
alpha: 90
beta: 90
gamma: 120
cell_volume: 121.574
crystal_density: 4.286
atoms_sites: ["Ge", "O"]
atoms_x: EJgbANAmGAA=
atoms_y: AAAAADBtEgA=
atoms_z: AAAAALCVBQA=
atoms_occupancy: 0
atoms_u_iso: wHYAAIDtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure refinement of GeO2 polymorphs at high pressures and
 temperatures by energy-dispersive spectra of powder diffraction
 Note: P = 0.0001 GPa T = 293 K
 Note: quartz structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAIAAAAAEAAAAAAAAAAAgAIAgAEAAAgAACgAAACgAAAABAACAABBQgAAgAACAAhQgECIADAAAhAghABBADCCAIAAAZjBCAARAkAISAIQhMMSAIgmQgMBEFiEQABESGTAYEiE0C0KIgQKQJEQ==


formula: Ge O2
compound: Synthetic
formula_title: GeO2
a: 4.9113
b: 4.9113
c: 5.6099
alpha: 90
beta: 90
gamma: 120
cell_volume: 117.187
crystal_density: 4.447
atoms_sites: ["Ge", "O"]
atoms_x: MIIbAMDmFwA=
atoms_y: AAAAALCrEgA=
atoms_z: AAAAAFBaBQA=
atoms_occupancy: 0
atoms_u_iso: wHYAADABAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure refinement of GeO2 polymorphs at high pressures and
 temperatures by energy-dispersive spectra of powder diffraction
 Note: P = 1.69 GPa T = 293 K
 Note: quartz structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAABAAAAAAAAAAACACAEAAIAACAAAiAAAARAAAQABAAIAABEgQACAAACAAJgIBECACQAAMAEQIAiAAsAIAgAAhLKAgABhAgIUEAkAjMKCAoQOAUIGBBwggAkBwyRIIBMowI4hIEFCAF==


formula: Ge O2
compound: Synthetic
formula_title: GeO2
a: 4.8546
b: 4.8546
c: 5.5943
alpha: 90
beta: 90
gamma: 120
cell_volume: 114.178
crystal_density: 4.564
atoms_sites: ["Ge", "O"]
atoms_x: oGcbANDbFwA=
atoms_y: AAAAAODuEgA=
atoms_z: AAAAAAAUBQA=
atoms_occupancy: 0
atoms_u_iso: SJ4AAOAoAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure refinement of GeO2 polymorphs at high pressures and
 temperatures by energy-dispersive spectra of powder diffraction
 Note: P = 3.55 GPa T = 293 K
 Note: quartz structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAAAAAQAAAAAAAAAAAQAgAgABAAAQAAQQAAAEIAABAAEABAAAChAgBAAAACAAKAIBACAEgABIACAIAgABkACAQAAAdiAgABYAJAGBAYAGxBAYBAGhCAwSAaAICCAGTFCAgDTFBDwCAKEI==


formula: Ge O2
compound: Synthetic
formula_title: GeO2
a: 4.8310
b: 4.8310
c: 5.5680
alpha: 90
beta: 90
gamma: 120
cell_volume: 112.539
crystal_density: 4.631
atoms_sites: ["Ge", "O"]
atoms_x: YEgbAIDHFwA=
atoms_y: AAAAABAZEwA=
atoms_z: AAAAAFD2BAA=
atoms_occupancy: 0
atoms_u_iso: ILIAAAgVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure refinement of GeO2 polymorphs at high pressures and
 temperatures by energy-dispersive spectra of powder diffraction
 Note: P = 4.58 GPa T = 293 K
 Note: quartz structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAIAAAAAAAAAAAIAQAIAAgAAEAAIIAAACCAAAQABAAQAAAkQIAIAAAAgADgCAYAQAkAAJAAQBAEAAMgAQCAAADkQEAALABEAYEBgArIECgMAaEIDBIAsAgIIAZMcIBAXGKCNgIAUY==


formula: Ge O2
compound: Synthetic
formula_title: GeO2
a: 4.9097
b: 4.9097
c: 5.6249
alpha: 90
beta: 90
gamma: 120
cell_volume: 117.424
crystal_density: 4.438
atoms_sites: ["Ge", "O"]
atoms_x: 0HgbAIDgFwA=
atoms_y: AAAAALCSEgA=
atoms_z: AAAAAJBgBQA=
atoms_occupancy: 0
atoms_u_iso: ILIAADABAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure refinement of GeO2 polymorphs at high pressures and
 temperatures by energy-dispersive spectra of powder diffraction
 Note: P = 2.9 GPa T = 493 K
 Note: quartz structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAABAAAAAAAAAAACACAEAAIAACAABCAAAAhAAAQABAAQAABEgQAEAAACAAJAIBIBACQAAIAEgIAoABIAIAgACBSIBAABAAggUEBQAiIKCCIgUAQIMEBiBACIBghRAIBEihCxBQECKAF==


formula: Ag Mn As S3
compound: Uchucchacua polymetallic deposit, Lima Department, Peru
formula_title: <missing>
a: 5.4496
b: 5.4496
c: 32.949
alpha: 90
beta: 90
gamma: 90
cell_volume: 978.524
crystal_density: 4.533
atoms_sites: ["Ag", "Mn1", "Mn2", "As", "AsSb", "S1", "S2", "S3"]
atoms_x: YPUsABAkDQCQXSsAUIgOAFCIDgDw9AsAcLcoAODgDAA=
atoms_y: gE4OABAkDQCQXSsAQAstAEALLQCgvCoAIEYrAJD3CQA=
atoms_z: MCMCACChBwAgoQcAQO8CAEDvAgAQTQcAMP8CAFDpAgA=
atoms_occupancy: AAk9AAAJPQAACT0AQHAxAMCYCwAACT0AAAk9AAAJPQA=
atoms_u_iso: kCcCAGBnAQDgpQEAkEYBAJBGAQDAiQEAwNQBACDFAQA=
atoms_aniso_label: ["Ag", "Mn1", "Mn2", "As", "AsSb", "S1", "S2", "S3"]
atoms_aniso_u11: 4CICAOClAQAA9AEAUA4BAFAOAQBAlgEAoIYBAECQAgA=
atoms_aniso_u22: QBMCAOClAQAA9AEAoIYBAKCGAQBAEwIAwM4CAAB3AQA=
atoms_aniso_u33: 0EYCAIC7AAAA+gAAcEMBAHBDAQDA2gAAQBkBAIA4AQA=
atoms_aniso_u12: MMb//8BdAADA4P//kLb//5C2//+gkv//QKL//+Cx//8=
atoms_aniso_u13: EIsAAAAZAABg8P//0DkAANA5AADAXQAAoA8AAGDw//8=
atoms_aniso_u23: EJH//wDn//+gDwAAIOr//yDq//9AHwAAoA8AAKAPAAA=
pub_title:
 Manganoquadratite, AgMnAsS3, a new manganese-bearing sulfosalt from the Uchucchacua
 polymetallic deposit, Lima Department, Peru: Description and crystal structure

qdat:
AAAAAAAAAAAACAAAAAAUQEAgAkA4BIgFAAEQAQEkECB0pBQhIBgCAEMRCCmhjVhiKBAQEKkRBBAgR0kdpk8wUI9IhCECAAAAco3JMQgnSREIKVAi1SJOts1iIXS2ViIgB1JIiAHZ9Wf19WREAAPMkSbKSJs/ckWykiAte/==


formula: K.78 N.22 H.88 P O4
compound: Synthetic
formula_title: <missing>
a: 7.4398
b: 7.4398
c: 7.0454
alpha: 90
beta: 90
gamma: 90
cell_volume: 389.967
crystal_density: 2.205
atoms_sites: ["K", "N-NH4", "H-NH4", "P", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAKBWCQA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAMA/BQA=
atoms_z: gIQeAICEHgCAhB4AAAAAAGDABwA=
atoms_occupancy: gJsvAIBtDQAAtjUAAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["K", "N-NH4", "H-NH4", "P", "O"]
atoms_aniso_u11: IE4AACBOAAAgTgAAgD4AAIA+AAA=
atoms_aniso_u22: IE4AACBOAAAgTgAAgD4AAIA+AAA=
atoms_aniso_u33: 4KsAAOCrAADgqwAAoIYBAIA4AQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAIDB//8=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAEAfAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Structure refinements of the mixed crystal K0.78(NH4)0.22H2PO4
 in the temperature range from 20 K to 250K
 Note: T = 20 K

qdat:
AAAAAAAAAAAAAAAAAAAAEAAAAAAAQAAAAABBAAABAAAAFACAAAAABECAIAAFAEAgABCEACAGgQICASACCBQIEEDIgggIARIEEAAOCMINEhQ4SQApKIEBhCDVQQyECLksKILECGVSBaA0XIUdElbDMCocSlM6aIjxUMBNyU==


formula: Ti O2
compound: Synthetic
pub_title: Structural and thermal parameters for rutile and anatase
formula_title: <missing>
a: 4.5937
b: 4.5937
c: 2.9587
alpha: 90
beta: 90
gamma: 90
cell_volume: 62.435
crystal_density: 4.249
atoms_sites: ["Ti", "O"]
atoms_x: AAAAADCaEgA=
atoms_y: AAAAADCaEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ti", "O"]
atoms_aniso_u11: QGoAAEBRAAA=
atoms_aniso_u22: wPn//8Dg//8=
atoms_aniso_u33: AAAAAAAAAAA=
atoms_aniso_u12: QGoAAEBRAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: 4EcAALA2AAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAQAACABAAAgAAAAAAAAAAgAEAAAAABAgEAAAhAAIAQAQAAQAEAQAAgBCAAAEgggAAAAmAAgAAgEQDAJAEBAQAICIgAAAiQAiECAAHASQQgYGAOABAgCBEBACQYKIg==


formula: Ti O2
compound: Synthetic
pub_title: Structural and thermal parameters for rutile and anatase
formula_title: <missing>
a: 3.7845
b: 3.7845
c: 9.5143
alpha: 90
beta: 90
gamma: 90
cell_volume: 136.268
crystal_density: 3.894
atoms_sites: ["Ti", "O"]
atoms_x: AAAAAAAAAAA=
atoms_y: AAAAAAAAAAA=
atoms_z: AAAAAPCyDAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ti", "O"]
atoms_aniso_u11: QFEAANC2AAA=
atoms_aniso_u22: AAAAAAAAAAA=
atoms_aniso_u33: AAAAAAAAAAA=
atoms_aniso_u12: QFEAADAqAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: YG0AAIBwAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAghAAAAAAAAAAIAAAAACBAAAAAAASAAAAABAIAABBCAAAAgJQAAAAAAABCIABAggAAACCAAIiABBCUAAABAAiAAQAIAACAACBACIRAAAAAAkAhCAACEAJAAgDAAA==


formula: Fe3 C
compound: Synthetic
pub_title: Strukturuntersuchungen an Karbiden des Eisens, Wolframs und Chroms mit thermischen Neutronen
formula_title: <missing>
a: 4.514
b: 5.078
c: 6.729
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.243
crystal_density: 7.732
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: oJEUACAN9v9gThoA
atoms_y: IAwLAICvAgCgvPj/
atoms_z: YNgDAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAABAAAAAQAAAAAAAAAQAAAAIAAgBiAQABAAAEAAwBgBAAAkAAAACAAOBAMAEIAAABQAKABIihIBAOgEiJIE4AACBHSaQBAIEQRQNBWYACgQASTqEBgRG0REUQcU/EMogCsZDvKhicjjMCmw==


formula: Fe3 C
compound: Synthetic
pub_title: The crystal structure of cementite, Fe3C
formula_title: <missing>
a: 4.5144
b: 5.0787
c: 6.7297
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.294
crystal_density: 7.729
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: IFMUAGAxCgDArxwA
atoms_y: YCsLAABxAgCAiwgA
atoms_z: oPcDAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAABAAAAAQAAAAAAAAAQAAAAIAAgBiAQABAAAEAAwBgBAAAkAAAACAAOBAMAEIAAABQAMABIihIBAOgEiJYEwAACBHUaQBAIEgRQNCWYAGgwASTyEBgRG0REUQcU+EMogGsZD/Kii0jjMCmw==


formula: Fe3 C
compound: Synthetic
pub_title: Comparison of X-ray and neutron-diffraction refinements of the structure of cementite Fe3C
formula_title: <missing>
a: 5.090
b: 6.748
c: 4.523
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.353
crystal_density: 7.677
atoms_sites: ["Fed", "Fec", "C"]
atoms_x: QFoLAIAyAgBAUjYA
atoms_y: YNgDAEBCDwBAQg8A
atoms_z: AAUUAIAANABAdxsA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIQACCEggACkAAIAAwBAAoCBIAQFAUAAUjASgYWAEVDgAVgDQdKQKwpAJEh0O0CBFAvp5gURsnBDi7VZiGqhID9foxKIid5XPtzI/aL00hO30f26O+lu/xN+4==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.733
c: 4.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.388
crystal_density: 7.725
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: kDwLAAANAgDgkzYA
atoms_y: MHwDAEBCDwBAQg8A
atoms_z: kFEUABBTMwDwexsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAACggAIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 4.2 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAwAACAAAAAAQAAgAEIABBCQQABiAAEAAwAgAkBAsAICgKAAKRgJwELACKhwAKgBcKTIFYWgEiIaH5BAiQN66oHI1TQRZPWe5Du40B338YSiRv2ZS6Y8e/BM6ImuZH97Cr5b3eTvW==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.733
c: 6.513
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.856
crystal_density: 5.351
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: QEELAMAGAgAQjDYA
atoms_y: 0HIDAEBCDwBAQg8A
atoms_z: EEUUAKBUMwDgbRsA
atoms_occupancy: 0
atoms_u_iso: IMsAACDLAADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 20 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAEQQAAAAAQACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAgKAIApUgZ0hsICA3VMXAvGUWgGBvOiuNKogx2oDpateeFu5FHk3fOxXeb706255vFNv7cniN0z3/WV6nfK3LG3X929b73==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.734
c: 6.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.855
crystal_density: 5.352
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 4DcLAKADAgBQkjYA
atoms_y: 8HUDAEBCDwBAQg8A
atoms_z: 4EwUAPBPMwBAdxsA
atoms_occupancy: 0
atoms_u_iso: oAkBAKAJAQCggAIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 40 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAEQQAAAAAQACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAgKAIApUgZ0hsICA3VMXAvGUXAGBvOiuMqogx2oDpateeFq5FHk3fOxXWb726255vFPv7cviN0z3/eV6nfK3LG33929b73==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.735
c: 6.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.888
crystal_density: 5.351
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: wDQLAHALAgAAlzYA
atoms_y: MHwDAEBCDwBAQg8A
atoms_z: oEYUAJBGMwDwYhsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAAAAcQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 60 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAEQQAAAAAQACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAgKAIApYgZ0hsICA3VMXAvGUXAGBvOiuMqogz2oDJateeFq5FHk3fOxnWb726255vFLt7cviN1z3/eV6nfK/LG3f97dT/3==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.735
c: 6.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.888
crystal_density: 5.351
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: ID4LAAANAgDAdzYA
atoms_y: 8HUDAEBCDwBAQg8A
atoms_z: oEYUAKBUMwCgZxsA
atoms_occupancy: 0
atoms_u_iso: IMsAACDLAADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 80 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAEQQAAAAAAACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAAKAIApYgZ0hsICA3VMXAvGUXAGBuOiuMqogz2oDJateeFq5FHk3fOxnWbr26255vFLt7cviN1z3/eV6nfK/LG3ft7dT/3==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.736
c: 6.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.921
crystal_density: 5.350
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: MDMLALARAgBgoDYA
atoms_y: sIgDAEBCDwBAQg8A
atoms_z: EF4UAFAnMwDQXxsA
atoms_occupancy: 0
atoms_u_iso: IMsAACDLAACAMgIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 100 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAEQQAAAAAQACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAgKAIApYgZ0hsICA3VMXAuGUnAGBvOiuMqpgz2oDJqteaFu5HHk3fOxnmbr26255vFLt7cvid1z3/cV6n/L/VG3ft7fz/3==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.738
c: 6.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.987
crystal_density: 5.348
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: UDYLAGAWAgCwmzYA
atoms_y: cIIDAEBCDwBAQg8A
atoms_z: IFMUACAvMwBAXhsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 120 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAQAAAIQQAAAAAQACQAAyABAAICCMEmAAAAAJgQFIJAUAKykAgKAIAqYgZ0hsICA3dMXA6GUnAGBvOi+Mqxgz2oDJqteaFO5HHlXfPRnm7/26255vJLt7cvif1z3fc37n/L/VE3f9rfz/3==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.740
c: 4.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.548
crystal_density: 7.717
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: sD8LAGAWAgCgpjYA
atoms_y: kIUDAEBCDwBAQg8A
atoms_z: AFAUALBJMwBwbxsA
atoms_occupancy: 0
atoms_u_iso: IMsAACDLAADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 140 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAACAAAAAAQABgAEIABBCgQABiAAEAAwAgAoBAsAICgMAAORgJgMLACKhwAKgBYKVIFQcgEiIcH5BAkQX66oHI1TghZNWe5F3w0B338QWkRL0ZT+Q0f/DNaJEu5H+1G2pd38ZvW==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.742
c: 4.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.594
crystal_density: 7.714
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: ADsLAIAZAgCQsTYA
atoms_y: 0IsDAEBCDwBAQg8A
atoms_z: QFYUABA6MwBwVhsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAABgYQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 160 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAACAAAAAAQABgAEIABBCgQABkAAEAAwAgAoBAsAICgMAAOhgJgMLACKhQASgBYKVIFQcgFiQcH5BAkQX6ywHI1VghRNWe5F3w0C230QWkRL0ZS+RYe/FPaJEu5H+1G6pf385v2==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.743
c: 4.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.617
crystal_density: 7.713
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: ADsLAPAXAgCwtDYA
atoms_y: AIQDAEBCDwBAQg8A
atoms_z: UEsUAKA7MwAAcRsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAABgYQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 180 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAACAAAAAAQABgAEIABBCgQABkAAEAAwAgAoBAsAICgMAAOhgRgELACKhQASgBQKVIFQcgFiQcH5BAkQXqywHI1VghRdWe5F3w0Cm34QSkRL0RSuRYe/FPaJEu5H+1G+pb385v2==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.746
c: 4.512
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.686
crystal_density: 7.710
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: QEELAIAZAgBQqzYA
atoms_y: 4IADAEBCDwBAQg8A
atoms_z: 8EEUAGA1MwCAZBsA
atoms_occupancy: 0
atoms_u_iso: YOoAAGDqAADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 200 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAACAAAAAAQABgAEIABBCgQABkAAEAAwAgAoBBIAICgMAAOhgRgMLACKhQATgBYKVIFQcgFiQ8H5BAkQXa0wFQ1Vghxeae5F3wkDm34QaoRL0zSuR4e/FeaJEvZH+9G+qdn05X2==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.747
c: 4.513
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.743
crystal_density: 7.707
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: ID4LANAUAgDQnjYA
atoms_y: sIgDAEBCDwBAQg8A
atoms_z: MEgUANBMMwBQbBsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AADAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 220 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAEIABBCgQABkAAEAAwAgAoBBIAICgUAAOhgRgMLACKhQATgDYKlIFQcgFiQ0LxBAkQnU0wFQ1Vghxeae5H3xkDm/4QrIRL0zWuR4e/FeaREvZH+9G/yen07X6==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.748
c: 4.513
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.766
crystal_density: 7.706
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: sD8LAPAXAgBwrjYA
atoms_y: gJADAEBCDwBAQg8A
atoms_z: oEYUAEAyMwDgbRsA
atoms_occupancy: 0
atoms_u_iso: oAkBAKAJAQBAEwIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 240 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAEIABBCgQABkAAEAAwAgAoBBIAICgUAAOhgRgMLACKhQATgDYKlIFQcgFiQ0LxBAkQnU0wFQ1Vghxeae5H3xkDm/4QrIRL0zUuR4e/JWqREvZH+9G3yen07X6==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.750
c: 4.514
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.846
crystal_density: 7.702
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: QEELAMAfAgBg0jYA
atoms_y: EJIDAEBCDwBAQg8A
atoms_z: UEsUAEAyMwAwaRsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAAAA9AEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 260 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABBCgQABkAAEAAwAgAoBBIAICgUAAMhARgMPACShQATgDYKlIFQcgFiQ0LxBAkQn00wFQ1lhBxeaepHnxkDm/4QrIRL0zkuy4e9JWqREuZP/tHXSeu07X6==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.753
c: 4.514
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.915
crystal_density: 7.699
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: sD8LAFAhAgCwzTYA
atoms_y: UJgDAEBCDwBAQg8A
atoms_z: gFwUAKAiMwCgThsA
atoms_occupancy: 0
atoms_u_iso: YOoAAGDqAACgAwIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 280 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABBEgQABkAAEAAwAgAoBBIAIDAUAAMhARgMPACShQATgD4KlIFQcgFiQ4LxBAkQn10gFg1lhBxeaapHnxkCu/4wrIhL01kuy4d9J2qREu5P/2LXUav1Tna==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.081
b: 6.754
c: 4.515
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.942
crystal_density: 7.697
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: YEQLAKAcAgCA1TYA
atoms_y: IKADAEBCDwBAQg8A
atoms_z: wGIUABAhMwCwQxsA
atoms_occupancy: 0
atoms_u_iso: gLsAAIC7AAAgxQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCCggABkAAEAAwAgAoBBIAICgUAAMhARgMPACShQATgD4KlIFwcgFCQ4LxBAkQn10gFg1lhBxey6pHnxEGsf4wrIRL03suyoc8p0qREu5P/2L3Uav1Tna==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.081
b: 6.755
c: 4.515
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.965
crystal_density: 7.696
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 0EILADAeAgDgxTYA
atoms_y: gJADAEBCDwBAQg8A
atoms_z: IFMUANAaMwBgehsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAACAtQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 320 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCCggABEAAEAAwAgAoBBIAICgUAAMhARgMPACSjQAVgD4KlIFwcgFCQ4LxBAkQn10gGg1phBxey6pHnxEGsfwwrIjL03suyoc8p0qREq5P/2L3Uav1Tvq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.081
b: 6.756
c: 4.517
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.056
crystal_density: 7.691
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: QEELABAbAgBg0jYA
atoms_y: AJ0DAEBCDwBAQg8A
atoms_z: cGcUAKAJMwCAZBsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AACAtQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 340 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCEggABEAAEAAwAgAoBBIAIFAUAAMhARgMPACSjQAVgCoKlQFwcgFCR4LxBAkQn14gGg2qhBSey7pFnREGsfwwrIjKs3o2zo98psqiFe6f72L3Uc312tq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.080
b: 6.757
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.083
crystal_density: 7.690
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: cFILAJAnAgAA+zYA
atoms_y: kJ4DAEBCDwBAQg8A
atoms_z: sFQUAAATMwCwXBsA
atoms_occupancy: 0
atoms_u_iso: wNoAAMDaAABgZwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 360 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCCggABEAAEAAwAgAoBBIAQEgUAAMhAhAMOgCSjQAVgCwKpQFwcgHCR4KxBAkQn14gGg3LBBSey7pFnRCGsfwwqIjKs3I3zw98psqiFe6f92SzU83p3tq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.080
b: 6.759
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.129
crystal_density: 7.688
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 0EILAOAiAgDQ6TYA
atoms_y: AJ0DAEBCDwBAQg8A
atoms_z: sG0UALD+MgBwbxsA
atoms_occupancy: 0
atoms_u_iso: QBkBAEAZAQBAlgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 380 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCEggABEAAEAAwAgAoBBIAQEgYAAMhAjAMOgCSjQAVgGwKpQFwUgHCR4KxBAkRH14gGg3LCBSey7pFnRCGsfwwqQjes3I3zw98ptKiFe6f9WSzY83p3tq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.080
b: 6.760
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.152
crystal_density: 7.687
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 8F4LAJAnAgAw2jYA
atoms_y: MJUDAEBCDwBAQg8A
atoms_z: MEgUAKAiMwCAfRsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AAAAdwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 400 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCEggABEAAEAAwAgAoBBIAQEgYAAMhAjAMOgCSjQAVgGwKpQGgUgHCR4LRBAkRH14gGg3LCBScy7pNnRCG8fxQqQjes7I3Tw98ptKiFe6f9aS3Y83p3tq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.079
b: 6.761
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.144
crystal_density: 7.687
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: YF0LAAAmAgCABzcA
atoms_y: kJ4DAEBCDwBAQg8A
atoms_z: AFAUANABMwAgWxsA
atoms_occupancy: 0
atoms_u_iso: YOoAAGDqAAAgSAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 420 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCEggABEAAEAAwAgAoBBIAQEgYAAMhAjAMKgCSjQAVgHwKpQGwUgHCR4LRBAkRH14gGg3LCBScz7pNnRCG8fxQqQjesbI3Tw98ptOiFe6f/WSzY82p3tq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.078
b: 6.763
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.159
crystal_density: 7.686
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: IFcLAEAsAgDwBTcA
atoms_y: kJ4DAEBCDwBAQg8A
atoms_z: UGQUACDkMgBwbxsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AABAGQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 440 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCEggABEAAEAAwAgAoBBIAQEgYAAMhAhAMKgCSiQAVgHQKpQHQVAHCRwLxBAkRHV4wGg3LCBScx7pNmxCM8fxQyQjesbI/Vw98xtOiFe6X/WSzY8np1ul==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.077
b: 6.764
c: 4.518
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.152
crystal_density: 7.687
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: EGILAFAhAgCw/zYA
atoms_y: sKEDAEBCDwBAQg8A
atoms_z: AGkUAIDtMgCAZBsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AABg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 460 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCCggABEAAEABwAgAoBBIAQEgYAAMhAhAMKgCSSQAVQHQKpQHQVAHCRwLxBAkRHWYwGgvTCBSMx7pNmxCM8fxQyQjesbIvVw98xtOiHd6T/WizY8nltul==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.078
b: 6.766
c: 4.519
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.263
crystal_density: 7.681
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: IHALAMAfAgAAFDcA
atoms_y: 4JkDAEBCDwBAQg8A
atoms_z: MEgUABAIMwCgZxsA
atoms_occupancy: 0
atoms_u_iso: YOoAAGDqAACgCQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 480 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCFAgADEAAEABwAgAoBCIAQEgYAAMhAjAMKgCSiQAWgHwKpQHg1AHCRwLhBAoRHW4wGg3TCDicx7pNHTCM8XhRSQmesbY/Vg98xtPENd6X/qjSQ5npV+p==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.077
b: 6.767
c: 4.520
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.289
crystal_density: 7.680
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 4IILACApAgBQDzcA
atoms_y: UJgDAEBCDwBAQg8A
atoms_z: EEUUANAaMwAwaRsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AABg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 500 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIABCFAgADEAAIABwAgAoBCYAQEgYAAMhAjAMKgCkSQAWQHwKpQHg1AHCRwLhBAoRHWYwHBPTCDicx7pNHTCM8XiRSQmasdY/Vg98x9PELV83/qjTR5nJV+l==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.080
b: 6.770
c: 4.522
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.519
crystal_density: 7.669
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: wH8LAMAfAgDAJjcA
atoms_y: wJYDAEBCDwBAQg8A
atoms_z: IFMUAOD2MgDQXxsA
atoms_occupancy: 0
atoms_u_iso: APoAAAD6AAAgywAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 520 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIACCFAgADEAAIABgBAAwBCYAQFAYAANBAjAUcgCkmQAWgHwKpQLg1APEiwKhBAoSPWogPBdSEDiZj7pNNjEI4XiRWgmt03Z+rg3YjadEN5sn6tFmx5vJbdq==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.082
b: 6.772
c: 4.522
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.626
crystal_density: 7.663
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: MH4LAEATAgDQNDcA
atoms_y: sIgDAEBCDwBAQg8A
atoms_z: gEMUALD+MgAwaRsA
atoms_occupancy: 0
atoms_u_iso: gDgBAIA4AQBAGQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 540 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAAAgAACAAAAAAQABgAIIACCFAgADEAAIABgBAAwBCYAQFAYAAZBAjAUdACkmgAWgHwOxQLg1APEjwKiBAoiPUpgNBeSECiZj6xVNjEJY/iRkhKt03Z+rg3ZjaeIW7sn7VGmx7vTr9T==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.083
b: 6.775
c: 4.523
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.760
crystal_density: 7.657
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 8JALAGAWAgDQNDcA
atoms_y: EJIDAEBCDwBAQg8A
atoms_z: 8EEUAAD6MgAAWBsA
atoms_occupancy: 0
atoms_u_iso: 4CgBAOAoAQDA2gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 560 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAABgAACAAAAAAQABgAIIACCFAgADEAAIABgBAAwBCYAQFAYAAZBAiAUdACkkgAUgGwNRQLg1AOEjQKiCBQiPUxgNBeSEDEpj2xbOlEZ4/ihkhM95Vp+rA3ZD8eIW7pn3ZGmxrOTu/V==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.085
b: 6.776
c: 4.524
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.879
crystal_density: 7.651
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: 4JsLAGAWAgAQOzcA
atoms_y: UH8DAEBCDwBAQg8A
atoms_z: MC8UAEAyMwCgZxsA
atoms_occupancy: 0
atoms_u_iso: wFcBAMBXAQDgKAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 580 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAABgAACAAAAAAQACgAIQACCFAgADEAAIABgBAAwBCYAQFAYAAZDAiAYdAEkkgAkgOwVRQLhqAOEjQOiCBQiPdxgNBumEHEpn3SaOmEZ4/ChkhNe5ep9TA2xH0WIWzZH3ZGuxreXu2V==


formula: Fe3 C
compound: Synthetic
formula_title: <missing>
a: 5.087
b: 6.779
c: 4.526
alpha: 90
beta: 90
gamma: 90
cell_volume: 156.078
crystal_density: 7.641
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: kKALABAbAgBATDcA
atoms_y: wH0DAEBCDwBAQg8A
atoms_z: IDoUALAXMwCQWRsA
atoms_occupancy: 0
atoms_u_iso: YGcBAGBnAQAA+gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermal expansion and crystal structure of cementite, Fe3C, between 4 and 600 K
 determined by time-of-flight neutron powder diffraction
 Note: T = 600 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAABAABgAACAAAAAAQACgAIQACCFAgACEAAIABgBAAwCCQAQJAwAAZCBCAYVAEpEgAsgPgVSQLBqAOElgXiCBRCOtSgWCumIHEpF3SaKmEaxvChIiVbp7T1SBuzH0aIszZP6REtjXeXK+Z==


formula: (Fe2.7 Mn.3) C
compound: <missing>
pub_title: On the cementite structure
formula_title: <missing>
a: 5.0598
b: 6.7462
c: 4.5074
alpha: 90
beta: 90
gamma: 90
cell_volume: 153.857
crystal_density: 7.740
atoms_sites: ["FeG", "MnG", "FeS", "MnS", "C"]
atoms_x: gBULAIAVCwBwPQIAcD0CACCHNQA=
atoms_y: oBAEAKAQBABAQg8AQEIPAEBCDwA=
atoms_z: 4JcUAOCXFAAgSDMAIEgzAIAZGwA=
atoms_occupancy: gO42AIAaBgCA7jYAgBoGAAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["FeG", "MnG", "FeS", "MnS", "C"]
atoms_aniso_u11: oA8AAKAPAAAwKgAAMCoAAOAiAgA=
atoms_aniso_u22: MCoAADAqAACgKAAAoCgAACBOAAA=
atoms_aniso_u33: AEsAAABLAABgVAAAYFQAAMBXAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: EA4AABAOAACQAQAAkAEAAIA+AAA=
atoms_aniso_u23: IAMAACADAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAwAABAAAAAAIAAwAEEAAhBgQABiAACAA4AQAMAQkAECQKAAGQwIgFHQApJoAFoBcCyUB4NQBgkcC4QQKER1uMBoV0wgUjMeaJZsYinD8SMyFlulbHVMG/EPRohrrm/dk6dPs5Jr2==


formula: Cd Cu As O5 H
compound: Synthetic
pub_title: CdCu(OH)(AsO4), the first Cd member of the adelite-descloizite structure type
formula_title: CdCu(OH)(AsO4)
a: 7.415
b: 5.890
c: 9.016
alpha: 90
beta: 90
gamma: 90
cell_volume: 393.768
crystal_density: 5.598
atoms_sites: ["Cd", "Cu", "As", "O1", "O2", "O3", "O4", "H"]
atoms_x: uHcHAICEHgBIGTUA8HU1ALAqAgBwsSkAYM4mAIAwLAA=
atoms_y: QEIPAAAAAADAxi0AEDUfAMDGLQDAxi0AQEIPAEBCDwA=
atoms_z: 4B4LAAAAAACw5gkAUDEQAGAvAgBADQMAoFsEAICvAgA=
atoms_occupancy: 0
atoms_u_iso: yOYAAMCFAAA4cgAA8NIAAIBqAQDg3QAAkH4AAIA+AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAIAAQAQAEAQQAEAEIAMECAQiCEAhIFIcAAnAALAMSER6kJCGoKhCmCV4fpYUKPF28E3l06JFvFOz6h2W8Z03cz2df6z7zf6H7/769/m/97Pqn++/+ur/+3v39+//6dbdn3/36/s/9t/zXu7+u/793==


formula: Fe3 C
compound: Synthetic
pub_title: Determination of the position of carbon in cementite by the neutron diffraction method
formula_title: <missing>
a: 4.525
b: 5.088
c: 6.74
alpha: 90
beta: 90
gamma: 90
cell_volume: 155.176
crystal_density: 7.686
atoms_sites: ["Fe1", "Fe2", "C"]
atoms_x: IFMUAKDO9f8AcQIA
atoms_y: YCsLAABxAgBAmxUA
atoms_z: oPcDAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAABAAAAAgAAAAAAAAAQAAAAIABACkAgABAAAEAAwDACAABIAAAAEAAcCAYAIQAAABgAUAFRFCQCAZAJESQKwAAECNJ4gEAgRAjgqFJwAOBAApLoQGAiNrIIpCpzcJSSAOjkOqZEKxKUQOfA==


formula: K Pb2 Cl5
compound: Challacollo silver mine, Iquique, Atacama desert, Chile
formula_title: <missing>
a: 8.864
b: 7.932
c: 12.491
alpha: 90
beta: 90.153
gamma: 90
cell_volume: 878.230
crystal_density: 4.771
atoms_sites: ["K", "Pb1", "Pb2", "Cl1", "Cl2", "Cl3", "Cl4", "Cl5"]
atoms_x: 8OsAAODYHgCQ8g4AUIUCAEBxHAAwmA8AgKYQAHBGDQA=
atoms_y: UJ4CAPAyPAAQFjkAoM8SAHAWFQBw+ggAoGIgAFBdKgA=
atoms_z: 8KAyAICYCgAQIh4AMF0EALArBgBg+xIAEL4dALBlDQA=
atoms_occupancy: 0
atoms_u_iso: eAgCAHgIAgB4CAIAeAgCAHgIAgB4CAIAeAgCAHgIAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The new mineral challacolloite, KPb2Cl5, the natural occurrence of a
 technically known laser material

qdat:
AAAAAAAAAAABAAACBCACEIACIAIiIgRJAEAMkhpYEoS06kRIJ17jldR/Hzlmc+dy6fHl+c7f732vX3Xz933///71/+8+//nftv//f9/lff////7+/ff//v3+3/7f//8/f3s1///831f0X/37v/9rvz/xu/on7n+fu9r59x==


formula: Ca C O3
compound: Synthetic
pub_title: Ab-initio-Strukturbestimmung von Vaterit mit automatischer Beugungstomographie
formula_title: <missing>
a: 12.170
b: 7.120
c: 9.470
alpha: 90
beta: 118.37
gamma: 90
cell_volume: 722.026
crystal_density: 2.762
atoms_sites: ["Ca1", "Ca2", "C1", "C2", "O1", "O2", "O3", "O4", "O5"]
atoms_x: QEIPABDXBABQNgsAAAAAAICdBQAANQwAoHoDAEC5EAAAAAAA
atoms_y: QEIPAPAOEAAA7RcA4Mw5AEB9GgDgCRsA4G00AIDSEQCg3wcA
atoms_z: AAAAABC4HgDA/Q8AQEIPAIAOCABgWhgA8GEXAKAsEABAQg8A
atoms_occupancy: 0
atoms_u_iso: 4BwDAIAyAgAA7gIAwM4CAMC8BQAgKgYAICoGACA2BABgVQQA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAACAEAAAAQQAAAIAAhAIIAAGREAAAASABUwIgAggiAHzEQBggojIACLrpKAwoi4ITAlciCMmQcZILdWeDtJ0C0kUsNR0lOpyfkS69t389ZWEPmrk96We3m+jcj1N7b92HM5jaf/Y1ynV+bMKnJ35WXU==


formula: Ca C O3
compound: <missing>
pub_title: Uber Vaterit und seine Struktur
formula_title: <missing>
a: 4.13
b: 7.15
c: 8.48
alpha: 90
beta: 90
gamma: 90
cell_volume: 250.410
crystal_density: 2.655
atoms_sites: ["Ca", "C", "O1", "O2"]
atoms_x: AAAAACCVCQBgvxwAAAAAAA==
atoms_y: AAAAAOC1KADgtSgA4LUoAA==
atoms_z: AAAAAEBCDwBAQg8AwDMHAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAQAAAACAAAQIAAAAAAAAIBCAAABCAAAICARCQAIEOBAABEEgCQQIBEJBYACkEDAYUICRADBlQ5sAGBFgjQxNc4MKIUskMxxK5xnzDOUQ5kSXHeYwmCUsXMPhGUcvMpvFtHMyEU3YXkTKDfrsWs5H==


formula: Ca C O3
compound: Synthetic
formula_title: <missing>
a: 4.1291
b: 7.1581
c: 8.4764
alpha: 90
beta: 90
gamma: 90
cell_volume: 250.533
crystal_density: 2.654
atoms_sites: ["Ca", "C", "O1", "O2"]
atoms_x: AAAAAKDYBACgtxYAgKH8/w==
atoms_y: AAAAAMBtJwAg8yMAYMIoAA==
atoms_z: AAAAAEBCDwBAQg8AsHAHAA==
atoms_occupancy: 0
atoms_u_iso: gEwBAPBSAwDwUgMA8FIDAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Microtwinning hypothesis for a more ordered vaterite model
 Note: Meyer (1959) model, not preferred

qdat:
AAAAAAAAAAAAAAAAAAAQAAAACAAAQIABAAAIAAIBCAAAAigQAICARCQEIEMBAABEEgBgcIBEJBQBGkMDiYkKCRADDlR54AGJGhlwqN95MKYcskcxxJ5xnzDGYY5UWvWsZ1mEVq/M/BE0b3F5/lZH9mE0/+38XMrfvM2s5N==


formula: Ca C O3
compound: Synthetic
formula_title: <missing>
a: 4.1304
b: 4.1304
c: 8.4749
alpha: 90
beta: 90
gamma: 120
cell_volume: 125.213
crystal_density: 2.655
atoms_sites: ["Ca", "C", "O1", "O2"]
atoms_x: AAAAACAtKwAgGSYAEKs1AA==
atoms_y: AAAAAEBRGQBAKQ8AIE0uAA==
atoms_z: AAAAAMDGLQAg5yUAwMYtAA==
atoms_occupancy: AAk9AEhYFABIWBQASFgUAA==
atoms_u_iso: EGwBAGAMAgBgDAIAYAwCAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Microtwinning hypothesis for a more ordered vaterite model
 Note: Kamhi (1963) model, not preferred

qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAIABAAAAAAIAAAAAAAAQAICAAAAAIEEBAAAEAAAAIIBAAAQACEECAIAAARABCBAZAAEIAABQBEAQMEQYIAAhBABgkRACAAJUACAiQggAVCREHAEQADAgCFJGEAAkgIUkBABTAEGohA==


formula: Mn V2 O4
compound: Synthetic
pub_title: Magnetisme - Etude par diffraction des neutrons du compose spinelle MnV2O4
formula_title: <missing>
a: 8.52
b: 8.52
c: 8.52
alpha: 90
beta: 90
gamma: 90
cell_volume: 618.470
crystal_density: 4.743
atoms_sites: ["Mn", "V", "O"]
atoms_x: AAAAAKAlJgAwsxcA
atoms_y: AAAAAKAlJgAwsxcA
atoms_z: AAAAAKAlJgAwsxcA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAIAAAAIAAAIAAEAAEAAQAAABABABABAEAIAgAAQCAQEAgICAAQECBAAQIAECCCBCBACCCCEEIAQhBCEIAhCIAhAIRCIhAIiEREAiIiIgIiIEQEiJEQIkSJACRIkCRIIgkSJIJIkkEkgkEkgEApEoIKSQElJ==


formula: Al O2 H.08
compound: Tveidalen, Langesundsfjorden, Norway
pub_title: Hydrogen atoms in boehmite: A single crystal X-ray diffraction and molecular orbital study
formula_title: <missing>
a: 3.693
b: 12.221
c: 2.865
alpha: 90
beta: 90
gamma: 90
cell_volume: 129.304
crystal_density: 3.034
atoms_sites: ["Al", "O1", "O2", "H"]
atoms_x: QEIPAEBCDwBAQg8AgCsYAA==
atoms_y: YJrs/5CuEQAQ8AQAwFECAA==
atoms_z: AAAAAAAAAAAAAAAAAAAAAA==
atoms_occupancy: AAk9AAAJPQAACT0AAHECAA==
atoms_u_iso: ABJ6AAASegAAEnoAgIQeAA==
atoms_aniso_label: ["Al", "O1", "O2"]
atoms_aniso_u11: ADIAADAqAAAAZAAA
atoms_aniso_u22: MEMAAOBgAADwVQAA
atoms_aniso_u33: cEkAACBnAABwSQAA
atoms_aniso_u12: AAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAAQAAAAAAAAAAACAAAAIAAAIAAAAAAAAAAAAIAAAACAAQAAAAAAIAEAAAAQAgEABACAUAAGAABoAAEAgQAACAQACAQBAAAAgAGIDQAAEAgAAAEAQQAAAAEABAgAAQAAwAYAQIQQQYABAgBBABEGAAAw==


formula: Cu2 Se
compound: Synthetic
formula_title: <missing>
a: 5.694
b: 5.694
c: 5.694
alpha: 90
beta: 90
gamma: 90
cell_volume: 184.609
crystal_density: 7.414
atoms_sites: ["Cu1", "Cu2", "Se"]
atoms_x: QEIPAMBiFAAAAAAA
atoms_y: QEIPAMBiFAAAAAAA
atoms_z: QEIPAMBiFAAAAAAA
atoms_occupancy: APkVAADECQAACT0A
atoms_u_iso: gCYEACAwBQDAzRcA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray study of the average structures of Cu2Se and Cu1.8S in the
 room temperature and the high temperature phases
 Note: Sample: Cu2Se (low), T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAABAAAAAAAAAAAAAAAgAAAAAAAAgACAAAAAAAAAEAAAAAAQAQAAAAAAAQAAAAEAAAAAAAAgAAABAIAAAAAIAAAEAgAAAAIAAAICAAAACAAAIAAAAAQAAECAAAAQAAQIAAAEA==


formula: Cu2 Se
compound: Synthetic
formula_title: <missing>
a: 5.787
b: 5.787
c: 5.787
alpha: 90
beta: 90
gamma: 90
cell_volume: 193.803
crystal_density: 7.062
atoms_sites: ["Cu1", "Cu2", "Se"]
atoms_x: QEIPAECnEwAAAAAA
atoms_y: QEIPAECnEwAAAAAA
atoms_z: QEIPAECnEwAAAAAA
atoms_occupancy: ABAnAEB+BQAACT0A
atoms_u_iso: IDYEAEAHBABAkAIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray study of the average structures of Cu2Se and Cu1.8S in the
 room temperature and the high temperature phases
 Note: Sample: Cu2Se (high) Model 1, T = 433 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAQAAAAAAAAAAAAAAQAAAAAAAAgACAAAAAAAAAIAAAAABAAgAAAAAACAAAAAgAAAAAAAIAAAAgCAAAAAEAAACAgAAAAIAAAQEAAAAIAAAgAAAABAAAQQAAAEAABBAAABAABB==


formula: Cu1.95 Se
compound: Synthetic
formula_title: <missing>
a: 5.787
b: 5.787
c: 5.787
alpha: 90
beta: 90
gamma: 90
cell_volume: 193.803
crystal_density: 6.953
atoms_sites: ["Cu1", "Cu2", "Cu3", "Se"]
atoms_x: QEIPAOA5EwCAhB4AAAAAAA==
atoms_y: QEIPAOA5EwAAAAAAAAAAAA==
atoms_z: QEIPAOA5EwAAAAAAAAAAAA==
atoms_occupancy: wK8cAABTBwBADQMAAAk9AA==
atoms_u_iso: oHoDAOAQBQCgzQoAIL8CAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray study of the average structures of Cu2Se and Cu1.8S in the
 room temperature and the high temperature phases
 Note: Sample: Cu2Se (high) Model 2, T = 433 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAQAAAAAAAAAAAAAAQAAAAAAAAgACAAAAAAAAAIAAAAABAAgAAAAAACAAAAAgAAAAAAAIAAAAgCAAAAAEAAACAgAAAAIAAAQEAAAAIAAAgAAAABAAAQQAAAEAABBAAABAABB==


formula: Cu1.84 S
compound: Synthetic
formula_title: <missing>
a: 5.564
b: 5.564
c: 5.564
alpha: 90
beta: 90
gamma: 90
cell_volume: 172.251
crystal_density: 5.745
atoms_sites: ["Cu1", "Cu2", "S"]
atoms_x: QEIPAMDlEwAAAAAA
atoms_y: QEIPAMDlEwAAAAAA
atoms_z: QEIPAMDlEwAAAAAA
atoms_occupancy: AL0fAIAaBgAACT0A
atoms_u_iso: IDYEAGDkAQCgjAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray study of the average structures of Cu2Se and Cu1.8S in the
 room temperature and the high temperature phases
 Note: Sample: Cu1.8S (low), T = 300 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAACAAAAAAAAAAAAAAAQAAAAAAAAEAAQAAAAAAAAAIAAAAAAgAQAAAAAAAQAAAABAAAAAAAAEAAAAIAgAAAAAgAAAEBAAAAAIAAAICAAAABAAAEAAAAAEAAAgQAAABAAAggA==


formula: Cu1.84 S
compound: Synthetic
formula_title: <missing>
a: 5.582
b: 5.582
c: 5.582
alpha: 90
beta: 90
gamma: 90
cell_volume: 173.928
crystal_density: 5.690
atoms_sites: ["Cu1", "Cu2", "S"]
atoms_x: QEIPAECnEwAAAAAA
atoms_y: QEIPAECnEwAAAAAA
atoms_z: QEIPAECnEwAAAAAA
atoms_occupancy: AIEpAICpAwAACT0A
atoms_u_iso: oGgGAIC1AQAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray study of the average structures of Cu2Se and Cu1.8S in the
 room temperature and the high temperature phases
 Note: Sample: Cu1.8S (high), T = 393 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAEAAAAAAAAAAAAAAAgAAAAAAAAQAAgAAAAAAAAAgAAAAABAAgAAAAAAAgAAAAEAAAAAAAAQAAAAgEAAAAACAAAAgIAAAAAgAAAgIAAAAIAAAQAAAAAQAAECAAAAQAAEEAA==


formula: (Be2.859 Cu.141) (Al1.884 Fe.116) Si6 O18.44 Li.12 H.88
compound: Synthetic
formula_title: <missing>
a: 9.2502
b: 9.2502
c: 9.2184
alpha: 90
beta: 90
gamma: 120
cell_volume: 683.107
crystal_density: 2.709
atoms_sites: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2", "Wat", "LiM"]
atoms_x: gIQeAICEHgCrsCgAq7AoANCfFwBYzBIAiGMeAAAAAAAAAAAA
atoms_y: AAAAAAAAAABVWBQAVVgUABgYBwDoYw4ASOEIAAAAAAAAAAAA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAANkIAEBCDwAAAAAA
atoms_occupancy: oCo6AGDeAgDAfjkAQIoDAAAJPQAACT0AAAk9AADbGgAAUwcA
atoms_u_iso: gIkAAICJAADwVQAA8FUAABBZAAAgywAAgKIAAADiBADARQQA
atoms_aniso_label: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2"]
atoms_aniso_u11: 4MQAAODEAABQXwAAUF8AAMBdAACAuwAAAMgAAA==
atoms_aniso_u22: IE4AACBOAABQXwAAUF8AAFBfAADAqAAAMKcAAA==
atoms_aniso_u33: wF0AAMBdAACgQQAAoEEAAGBUAADgKAEA4JIAAA==
atoms_aniso_u12: ECcAABAnAABwMAAAcDAAAJAzAABQeAAA8G4AAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEMP//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAYNf//w==
pub_title:
 Gemmological investigation of a synthetic blue beryl: a multi-methodological study
 Note: Sample: M2-1

qdat:
AAAAAAAAAAAAAgAAAAAAAACAAAQAAAAAgAGAIAAQAIAAAMAYEADAIAAAAwQBgoAAwMMBQ4QDBjAQUgGGMDHABDmAHEHHcOKgQ7CuIM7BPIYrjcgDcf8FfiOh9Q7sX81od8Dgb8zBmx/lbJsbs/APmyNcuTfWQlk8bweO18==


formula: (Be2.856 Cu.144) (Al1.882 Fe.118) Si6 O18.49 Li.12 H.98
compound: Synthetic
formula_title: <missing>
a: 9.2489
b: 9.2489
c: 9.2211
alpha: 90
beta: 90
gamma: 120
cell_volume: 683.115
crystal_density: 2.715
atoms_sites: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2", "Wat", "LiM"]
atoms_x: gIQeAICEHgCrsCgAq7AoANCfFwCAxxIAUF8eAAAAAAAAAAAA
atoms_y: AAAAAAAAAABVWBQAVVgUALgYBwAYYQ4AQN8IAAAAAAAAAAAA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAYNgIAEBCDwAAAAAA
atoms_occupancy: ABs6AADuAgAgbzkA4JkDAAAJPQAACT0AAAk9AEDoHQAAUwcA
atoms_u_iso: kJcAAJCXAAAwXAAAMFwAAHBiAAAQ1gAAAK8AAEB+BQBADQMA
atoms_aniso_label: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2"]
atoms_aniso_u11: gLsAAIC7AADgYAAA4GAAAABkAAAw2QAA8NIAAA==
atoms_aniso_u22: wF0AAMBdAADgYAAA4GAAAMBdAADwuQAAgLsAAA==
atoms_aniso_u33: IIAAACCAAADQUgAA0FIAALBoAAAgLwEAYJ8AAA==
atoms_aniso_u12: ADIAAAAyAABwMAAAcDAAAJAzAABwlAAAcHsAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAkLb//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAINH//w==
pub_title:
 Gemmological investigation of a synthetic blue beryl: a multi-methodological study
 Note: Sample: M2-2

qdat:
AAAAAAAAAAAAAgAAAAAAAACAAAQAAAAAgACAIAAQAIAAAIAYEACAIAAAAwQAgoAAwMMBQ4QDBjAQUgGGMDHABDGAHEHHcOMgQzCuIM7BPIYzDcgDMd8FfiOh9Q7sXsVoZ8Dgb8zBmx/lbIsbs/APmyNcuTfNglk2bweO98==


formula: (Be2.829 Cu.171) (Al1.892 Fe.108) Si6 O18.48 Li.12 H.96
compound: Synthetic
formula_title: <missing>
a: 9.2483
b: 9.2483
c: 9.2193
alpha: 90
beta: 90
gamma: 120
cell_volume: 682.893
crystal_density: 2.721
atoms_sites: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2", "Wat", "LiM"]
atoms_x: gIQeAICEHgCrsCgAq7AoACCgFwDgwRIAKGQeAAAAAAAAAAAA
atoms_y: AAAAAAAAAABVWBQAVVgUAPgZBwCwXw4AGOQIAAAAAAAAAAAA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAA+NYIAEBCDwAAAAAA
atoms_occupancy: YI45AKB6AwBAvTkAwEsDAAAJPQAACT0AAAk9AABMHQAAUwcA
atoms_u_iso: IJkAACCZAACgWgAAoFoAAABkAADA2gAA0LYAAEB+BQBAfgUA
atoms_aniso_label: ["Be", "Cu", "Al", "Fe", "Si", "O1", "O2"]
atoms_aniso_u11: wNoAAMDaAAAAZAAAAGQAAHBiAADQ6AAAUNwAAA==
atoms_aniso_u22: wF0AAMBdAAAAZAAAAGQAAFBfAAAgsgAA0LYAAA==
atoms_aniso_u33: YG0AAGBtAADgRwAA4EcAAGBtAACQLQEAkLAAAA==
atoms_aniso_u12: 4C4AAOAuAAAAMgAAADIAAJAzAABQkQAAcHsAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgMH//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAINH//w==
pub_title:
 Gemmological investigation of a synthetic blue beryl: a multi-methodological study
 Note: Sample: M2-3

qdat:
AAAAAAAAAAAAAgAAAAAAAACAAAQAAAAAgACAEAAQAIAAAMAYEADAIAAAAwQAgoAAwMMAw4QDBjAQUQGGMDHABDmAHEHHMOMgQzCuIMbBHIYrjcQDMf8FdiOh9Q7sTsTodsDgb8zAmxvlZI8bs/APmyNcuTfNQlk+boeO98==


formula: Cu O H Cl
compound: Synthetic
pub_title: Verfeinerung der Kristallstruktur von Kupfer(II)-hydroxichlorid, Cu(OH)Cl
formula_title: <missing>
a: 5.555
b: 6.671
c: 6.127
alpha: 90
beta: 114.88
gamma: 90
cell_volume: 205.978
crystal_density: 3.741
atoms_sites: ["Cu", "O", "H", "Cl"]
atoms_x: 2HwPAEA0CQBA0QwAIKQTAA==
atoms_y: kDEHANCDFQDAXBUAoPYYAA==
atoms_z: GA3+/9BBBwCA3g8AYP7s/w==
atoms_occupancy: 0
atoms_u_iso: KLQAAECmAAAoxwEAyM0AAA==
atoms_aniso_label: ["Cu", "O", "Cl"]
atoms_aniso_u11: OHcAAMiWAADYmgAA
atoms_aniso_u22: eJYAAGiXAAA4CAEA
atoms_aniso_u33: aPsAACDBAACYrQAA
atoms_aniso_u12: +AcAAHDl//8AAAAA
atoms_aniso_u13: WD4AAPBGAADAMAAA
atoms_aniso_u23: AOL//xD6///4AgAA
qdat:
AAAAAAAAAAAAAAAAAAAABAAAEAgAAAAIAAAADCAABEAAEBAAAgSEkACAACCQIgJAKERACDEQAVhIAgRAKTCQEIZiFAAiEQ4FmBQI4EAhSpiCFZCFAw5E6MaiHGmUWGI+EYxVZa2ViPMWxTXCD8cajHPf7FFwx3ug2+Zute==


formula: Ce P O5 H2
compound: Synthetic
pub_title: Crystal structures of a series of rare earth phosphates
formula_title: <missing>
a: 7.055
b: 7.055
c: 6.439
alpha: 90
beta: 90
gamma: 120
cell_volume: 277.551
crystal_density: 4.543
atoms_sites: ["Ce", "P", "O1", "O2", "Wat"]
atoms_x: gIQeAICEHgDAOBsAQNAhAAAAAAA=
atoms_y: gIQeAICEHgDg+AgAIBA0AAAAAAA=
atoms_z: gIQeAAAAAACg3hwAoN4cAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAQAAAAAAAAAAACAAAAIABAAAAAAAgIAABAAGAAABAQAKBBAAAACIEBBEAACABAGIAEAgQiAAAqCCEABEACCQBEhkQAAyAQIBIBQUAiCIgAFEIIAAIFAQRVAAkRIBQBFAlEMIFMpAoKKjQ2hAoLQEMa==


formula: Ce P O4
compound: Synthetic
formula_title: <missing>
a: 6.76
b: 7.00
c: 6.44
alpha: 90
beta: 103.63
gamma: 90
cell_volume: 296.159
crystal_density: 5.272
atoms_sites: ["Ce", "P", "O1", "O2", "O3", "O4"]
atoms_x: gNIRAIDSEQDg4AwAwNMWAOCAHACAFAcA
atoms_y: gIUJAICFCQDAbDwA4LYTAMA/BQDgVw4A
atoms_z: 4BAFACB2IwBg0RkAAFIcACCxLgAAgSkA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structures of a series of rare earth phosphates
 Note: O3-y has been modified to a realistic value

qdat:
AAAAAAAAAAAAAAAAgAAAABEAAAAAADABAFIQCAAEIAQiBAADAIQKIEAgoAUHIBwDEWQ5UAET4JABGA/WjYjAUwkEjR99YPDzJG5OdGzHRL5lnN8z1qFc3v5q/3rlr369J9w/cLr3meu7dT9269/dt7PNr+b/3/9b3f3Lh/==


formula: Fe Se
compound: Synthetic
formula_title: <missing>
a: 3.636
b: 3.636
c: 5.946
alpha: 90
beta: 90
gamma: 120
cell_volume: 68.077
crystal_density: 6.576
atoms_sites: ["Fe", "Se"]
atoms_x: AAAAAFVYFAA=
atoms_y: AAAAAKuwKAA=
atoms_z: AAAAAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Rontgenographische Daten der Mischphasen im System Pyrit (FeS2) -
 Ferroselit (FeSe2)/Pyrrhotin (FeS) - Achavalit (FeSe)

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAACAAAAAAAAAAEAAAAAAAACAAAAEAAAEABAEAAAAIAAgAAAAAAgAAgCAgAARABAACAACAAAAAAAJACAAQAAAAgQQAFgACAAAgAgQgAGAgRAAQBggABQEEYAIBAAAFAQgAAA==


formula: Fe (Se.5 S.5)
compound: Synthetic
formula_title: <missing>
a: 3.521
b: 3.521
c: 5.901
alpha: 90
beta: 90
gamma: 120
cell_volume: 63.356
crystal_density: 5.837
atoms_sites: ["Fe", "Se", "S"]
atoms_x: AAAAAFVYFABVWBQA
atoms_y: AAAAAKuwKACrsCgA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: AAk9AICEHgCAhB4A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Rontgenographische Daten der Mischphasen im System Pyrit (FeS2) -
 Ferroselit (FeSe2)/Pyrrhotin (FeS) - Achavalit (FeSe)

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAACAAAAAAAAAAIAAAAAAAAAEAAAIAAAAAIAgAAAAAIAAAAAAAABAAAAAGAAQAEAAAAAgAIEAAgABQAAAAAAgAAgAQwCgBAAAAABAAAEAgAgAAAAIQABAIBAAAEBCAIAMAA==


formula: Cr N
compound: north Chile iron meteorite
formula_title: <missing>
a: 4.148
b: 4.148
c: 4.148
alpha: 90
beta: 90
gamma: 90
cell_volume: 71.370
crystal_density: 6.143
atoms_sites: ["Cr", "N"]
atoms_x: AAAAAICEHgA=
atoms_y: AAAAAICEHgA=
atoms_z: AAAAAICEHgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Orientation relationships of carlsbergite in schreibersite and kamacite
 in the north Chile iron meteorite

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAAAAAABAAAAAAAAAACAAAAAAAAAAAAAAAAAABAAAAAAAAEAAAAAAACAAAAAA==


formula: Cd Se
compound: Synthetic
pub_title: The structure and Bijvoet ratios of cadmium selenide
formula_title: <missing>
a: 4.299
b: 4.299
c: 7.010
alpha: 90
beta: 90
gamma: 120
cell_volume: 112.198
crystal_density: 5.665
atoms_sites: ["Cd", "Se"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAFj/FgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Cd", "Se"]
atoms_aniso_u11: 6CABAGDvAAA=
atoms_aniso_u22: 6CABAGDvAAA=
atoms_aniso_u33: eF4BANi9AAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAQBABAAAAAAAAAgAAAAAACAAABAAAQQQAAAACAAAAAAAAgAIBAAABQAAAIABAAGAAAEgAAEAAAFkAAHAAIABAEEAAMACEAQDUAAwAJgEAcAAoAIAADIADACYCBaABgCQED4AaAQBAQA==


formula: Be O
compound: Synthetic
formula_title: <missing>
a: 2.6983
b: 2.6983
c: 4.3776
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.602
crystal_density: 3.009
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAANATFwA=
atoms_occupancy: 0
atoms_u_iso: wHYAADhFAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: sIEAANhAAAA=
atoms_aniso_u22: sIEAANhAAAA=
atoms_aniso_u33: sGgAAGBKAAA=
atoms_aniso_u12: 2EAAAIgiAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 High-pressure and high-temperature crystal chemistry of beryllium oxide
 Note: Crystal no. 1 in air

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAABAABAAAAAAAAAAAAAAEAAAAAAAAAAACAAAAAACAAAACAQBAAAAAAAACAAAAAAAAAAAABAAAEAAgAAAAADAAAAAAEAAAEAAACEAAAAAEIAAAAQAAAAACEYAA==


formula: Be O
compound: Synthetic
formula_title: <missing>
a: 2.6983
b: 2.6983
c: 4.3776
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.602
crystal_density: 3.009
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAMAFFwA=
atoms_occupancy: 0
atoms_u_iso: 4GoAAFBBAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: IGwAANhAAAA=
atoms_aniso_u22: IGwAANhAAAA=
atoms_aniso_u33: IGcAAEhEAAA=
atoms_aniso_u12: QDgAAIgiAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 High-pressure and high-temperature crystal chemistry of beryllium oxide
 Note: Crystal no. 2 in air

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAABAABAAAAAAAAAAAAAAEAAAAAAAAAAACAAAAAACAAAACAQBAAAAAAAACAAAAAAAAAAAABAAAEAAgAAAAADAAAAAAEAAAEAAACEAAAAAEIAAAAQAAAAACEYAA==


formula: Be O
compound: Synthetic
formula_title: <missing>
a: 2.6983
b: 2.6983
c: 4.3776
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.602
crystal_density: 3.009
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAGAVFwA=
atoms_occupancy: 0
atoms_u_iso: KEsAAHg3AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure and high-temperature crystal chemistry of beryllium oxide
 Note: Crystal no. 1 in cell

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAABAABAAAAAAAAAAAAAAEAAAAAAAAAAACAAAAAACAAAACAQBAAAAAAAACAAAAAAAAAAAABAAAEAAgAAAAADAAAAAAEAAAEAAACEAAAAAEIAAAAQAAAAACEYAA==


formula: Be O
compound: Synthetic
formula_title: <missing>
a: 2.6983
b: 2.6983
c: 4.3776
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.602
crystal_density: 3.009
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAIAYFwA=
atoms_occupancy: 0
atoms_u_iso: KEsAAHgtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure and high-temperature crystal chemistry of beryllium oxide
 Note: Crystal no. 2 in cell


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: P = 1.1 GPa
formula_title: <missing>
a: 2.6928
b: 2.6928
c: 4.3705
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.445
crystal_density: 3.027
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAALAQFwA=
atoms_occupancy: 0
atoms_u_iso: 2GgAAEBHAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAABAABAAAAAAAAAAAAAACAAAAAAAAAAABAAAAAABAAAABAIAgAAAAAAABAAAAAAAAAAAAAgAABAAQAAAAAAwAAAAABAAABAAAAiAAAAACCAAAACAAAAABBKAA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: P = 2.2 GPa
formula_title: <missing>
a: 2.6883
b: 2.6883
c: 4.3614
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.297
crystal_density: 3.043
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAOAhFwA=
atoms_occupancy: 0
atoms_u_iso: EFkAAGA7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAAgAAAAAAAAAAAAABAAAAAAAAAAAAgAAAAABAAAAAgEAQAAAAAAAAgAAAAAAAAAAAAQAAAgAEAAAAAAYAAAAABAAAAgAAAQgAAAAAhAAAABAAAAAAQhgA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: P = 3.8 GPa
formula_title: <missing>
a: 2.6832
b: 2.6832
c: 4.3524
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.137
crystal_density: 3.061
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAPAWFwA=
atoms_occupancy: 0
atoms_u_iso: wHYAAGA7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAQAAgAAAAAAAAAAAAAAgAAAAAAAAAAAgAAAAAAQAAAAQCAIAAAAAAAAQAAAAAAAAAAAAEAAAQACAAAAAAEAAAAAAQAAAIAAAEIAAAAAIQAAAAQAAAAAEIoA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: P = 4.0 GPa
formula_title: <missing>
a: 2.6825
b: 2.6825
c: 4.3525
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.124
crystal_density: 3.062
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAPAvFwA=
atoms_occupancy: 0
atoms_u_iso: uHQAAHg3AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAQAAQAAAAAAAAAAAAAAgAAAAAAAAAAAgAAAAAAQAAAAQCAIAAAAAAAAQAAAAAAAAAAAAEAAAIACAAAAAAEAAAAAAIAAAEAAAEIAAAAAIQAAAAQAAAAAEIoA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: P = 5.0 GPa
formula_title: <missing>
a: 2.6776
b: 2.6776
c: 4.3454
alpha: 90
beta: 90
gamma: 120
cell_volume: 26.981
crystal_density: 3.079
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAANATFwA=
atoms_occupancy: 0
atoms_u_iso: mIAAAEhJAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAQAAQAAAAAAAAAAAAAAgAAAAAAAAAAAQAAAAAAQAAAAIBAEAAAAAAAAIAAAAAAAAAAAACAAAEABAAAAAADAAAAAAIAAACAAACEAAAAACEAAAAIAAAAABCEA==


formula: Be O
compound: Synthetic
formula_title: <missing>
a: 2.6983
b: 2.6983
c: 4.3776
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.602
crystal_density: 3.009
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAADAEFwA=
atoms_occupancy: 0
atoms_u_iso: KFUAAIgxAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: aFYAAIAvAAA=
atoms_aniso_u22: aFYAAIAvAAA=
atoms_aniso_u33: 8FoAAKA8AAA=
atoms_aniso_u12: SCsAAPAZAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 High-pressure and high-temperature crystal chemistry of beryllium oxide
 Note: Crystal no. 3 in mount


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: T = 543 K
formula_title: <missing>
a: 2.7002
b: 2.7002
c: 4.3851
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.689
crystal_density: 3.000
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAFAHFwA=
atoms_occupancy: 0
atoms_u_iso: yG4AAEhJAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: gHAAADhFAAA=
atoms_aniso_u22: gHAAADhFAAA=
atoms_aniso_u33: kGoAABhMAAA=
atoms_aniso_u12: QDgAALAiAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAABAACAAAAAAAAAAAAAAEAAAAAAAAAAAEAAAAAAEAAAAEAgCAAAAAAAAEAAAAAAAAAAAACAAAEABAAAAAAGAAAAAAIAAAIAAAEQAAAAAQQAAAAgAAAAAEJIAA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: T = 763 K
formula_title: <missing>
a: 2.7050
b: 2.7050
c: 4.3927
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.835
crystal_density: 2.984
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAHAKFwA=
atoms_occupancy: 0
atoms_u_iso: oIIAAAhXAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: UIIAAOBWAAA=
atoms_aniso_u22: UIIAAOBWAAA=
atoms_aniso_u33: MHoAALhbAAA=
atoms_aniso_u12: KEEAAHArAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAACAACAAAAAAAAAAAAAAIAAAAAAAAAAAIAAAAAAIAAAAIAgEAAAAAAAAIAAAAAAAAAAAAEAAAIACAAAAAAMAAAAAAQAAAQAAAIQAAAAAhAAAABAAAAAAQjAAA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: T = 963 K
formula_title: <missing>
a: 2.7109
b: 2.7109
c: 4.3999
alpha: 90
beta: 90
gamma: 120
cell_volume: 28.003
crystal_density: 2.966
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAJANFwA=
atoms_occupancy: 0
atoms_u_iso: SKgAAKh6AAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: aKEAANB1AAA=
atoms_aniso_u22: aKEAANB1AAA=
atoms_aniso_u33: 6LcAAKh6AAA=
atoms_aniso_u12: +FIAABg9AAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAACAAEAAAAAAAAAAAAAAQAAAAAAAAAAAIAAAAAAQAAAAQBAIAAAAAAAAQAAAAAAAAAAAAIAAAgAIAAAAAAoAAAAABAAABAAAAhAAAAACCAAAAEAAAAABCKAAA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: T = 1073 K
formula_title: <missing>
a: 2.714
b: 2.714
c: 4.405
alpha: 90
beta: 90
gamma: 120
cell_volume: 28.099
crystal_density: 2.956
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAAGAVFwA=
atoms_occupancy: 0
atoms_u_iso: ELgAAJiAAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: OLMAAOB+AAA=
atoms_aniso_u22: OLMAAOB+AAA=
atoms_aniso_u33: sMcAAKCCAAA=
atoms_aniso_u12: QGAAAKBBAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAEAAEAAAAAAAAAAAAAAQAAAAAAAAAAAQAAAAAAQAAAAQCAIAAAAAAAAgAAAAAAAAAAAAQAABAAQAAAAAAgAAAAACAAABAAAAkAAAAAEEAAAAIAAAAACEYAAA==


formula: Be O
compound: Synthetic
pub_title: High-pressure and high-temperature crystal chemistry of beryllium oxide Note: T = 1183 K
formula_title: <missing>
a: 2.7178
b: 2.7178
c: 4.4078
alpha: 90
beta: 90
gamma: 120
cell_volume: 28.196
crystal_density: 2.946
atoms_sites: ["Be", "O"]
atoms_x: VVgUAFVYFAA=
atoms_y: q7AoAKuwKAA=
atoms_z: AAAAABAaFwA=
atoms_occupancy: 0
atoms_u_iso: 4MkAAHiMAAA=
atoms_aniso_label: ["Be", "O"]
atoms_aniso_u11: WMUAAFCMAAA=
atoms_aniso_u22: WMUAAFCMAAA=
atoms_aniso_u33: UNcAAACMAAA=
atoms_aniso_u12: yGQAAChGAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAEAAEAAAAAAAAAAAAAAQAAAAAAAAAAAgAAAAAAgAAAAgEAQAAAAAAABAAAAAAAAAAAAAgAACAAQAAAAABgAAAAAEAAACAAACEAAAAAEIAAAAQAAAAAIIwAAA==


formula: Ca6 Al7 O16 Cl
compound: Synthetic
pub_title: Crystal structure of Ca12Al14O32Cl2 and luminescence properties of Ca12Al14O32Cl2:Eu2+
formula_title: <missing>
a: 12.0095
b: 12.0095
c: 12.0095
alpha: 90
beta: 90
gamma: 90
cell_volume: 1732.107
crystal_density: 2.764
atoms_sites: ["Ca", "Al1", "Al2", "O1", "O2", "Cl"]
atoms_x: aIUIAKgLAQDgZzUAKBwCADg/CwBg4xYA
atoms_y: AAAAAKgLAQAAAAAAEDkbADg/CwAAAAAA
atoms_z: QEIPAKgLAQBAQg8AYB4JADg/CwBAQg8A
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQBIWBQA
atoms_u_iso: QJwAAGBtAADAXQAAQJwAAKCMAABgZwEA
atoms_aniso_label: ["Ca", "Al1", "Al2", "O1", "O2", "Cl"]
atoms_aniso_u11: ILIAANBrAAAgTgAAUHgAAHCUAACgjAAA
atoms_aniso_u22: ILIAANBrAAAgZwAAILIAAHCUAAAgxQEA
atoms_aniso_u33: UF8AANBrAAAgZwAAQJwAAHCUAAAgxQEA
atoms_aniso_u12: AAAAAHD+//8AAAAA0NX//xDc//8AAAAA
atoms_aniso_u13: AAAAAHD+//8AAAAAcMz//xDc//8AAAAA
atoms_aniso_u23: gCUAAHD+//8AAAAAkAEAABDc//8AAAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACABAAAAgBACAEAABAIAAACAQEAAQICBAgIAACCBBAgggAggAhBCAEIIQQhAEAQiEIBCABCIBCIBEQCACIiAgAiAARECIAQAAQAAAQAAAAAAAASAAAAAAAAAAAAAAAAAAAAAAAA==


formula: K2 Ca C2 O6
compound: Synthetic
formula_title: <missing>
a: 5.3822
b: 5.3822
c: 18.156
alpha: 90
beta: 90
gamma: 120
cell_volume: 455.481
crystal_density: 2.606
atoms_sites: ["K", "Ca", "C", "O"]
atoms_x: AAAAAAAAAAAAAAAAgGgIAA==
atoms_y: AAAAAAAAAAAAAAAAgJf3/w==
atoms_z: 2MUMAAAAAABY6CMAANwjAA==
atoms_occupancy: 0
atoms_u_iso: mD4BAPi7AADwwwAAqDgBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 On the aplanarity of the CO3 group in buetschliite, dipotassium calcium
 dicarbonate, K2Ca(CO3)2: a further refinement of the atomic arrangement

qdat:
AAAAAAAAAAAAAAAAAIAAAAAQAIAAAAAAQACAEABAAAEAAIYAAAEIgIAAAAACMBABFAgIACABAQAJABABARBAQQgAAAmABUIAAAWICgggEAhAKAAAEiCIiAgsAWIAAWIWIAAEQIBAiRESIIEAMAAJISQACAECCGQlAAYCkA==


formula: Ca.66 Al F5
compound: Hekla volcano, Iceland
pub_title: Jakobssonite, CaAlF5, a new mineral from fumaroles at the Eldfell and Hekla volcanoes, Iceland
formula_title: <missing>
a: 8.601
b: 6.2903
c: 7.2190
alpha: 90
beta: 114.61
gamma: 90
cell_volume: 355.091
crystal_density: 2.776
atoms_sites: ["Ca", "Al", "F1", "F2", "F3"]
atoms_x: AAAAAAAAAAAAAAAAQBMCAED/LgA=
atoms_y: ADQhAAAAAADA+zkAAPIrAAAVOwA=
atoms_z: QEIPAAAAAABAQg8AgE08AMAZNQA=
atoms_occupancy: gEgoAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 6GwAAOhiAACo2QAA+MUAADABAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAABAABAAgIAABAAAAADEAAQAAMADAEACAIICAAAzQACAEgoCpBQBhADAYAgkIENhAEwicAISCAnjAcBdNAZQIyGMwaOIGNE9BGBzBIUL5UkXmZfBQ5/AjFlEryPesXrDiSF7QvY1Z2S4wb==


formula: Fe As S
compound: La Roche-Balue Quarry, Loire-Atlantique, France
formula_title: <missing>
a: 5.7612
b: 5.6841
c: 5.7674
alpha: 90
beta: 111.721
gamma: 90
cell_volume: 175.456
crystal_density: 6.164
atoms_sites: ["Fe", "As", "S"]
atoms_x: KE4RABAACQDw+ycA
atoms_y: iJv//9j3BwBwAAgA
atoms_z: SPYRAOgPNQAwmRMA
atoms_occupancy: 0
atoms_u_iso: MPIAAHD4AADAJQEA
atoms_aniso_label: ["Fe", "As", "S"]
atoms_aniso_u11: MPIAAOD2AACQFAEA
atoms_aniso_u22: gO0AAOD2AADAJQEA
atoms_aniso_u33: cPgAACD9AAAQOgEA
atoms_aniso_u12: QAYAACADAADA+f//
atoms_aniso_u13: MFwAAMBdAACAcAAA
atoms_aniso_u23: sAQAAOD8//+QAQAA
pub_title:
 Stoichiometric arsenopyrite, FeAsS, from La Roche-Balue Quarry,
 Loire-Atlantique, France: Crystal structure and Mossbauer study

qdat:
AAAAAAAAAAAAAAAAAAAEAAAAAABAAAAAAAAABQAQACAYAAAAABAAAyAAAACAAFgAiAAKAIBAACMAQCYAOCAOAQEJgsAAAARBADTOkYAJGAQEQQkCfBKYAIjOxQt3ARE4QHtQChbOOt+wBHEAIB8eD7PAGFAO/EDRr3FKNz==


formula: Pt2 Hg Se3
compound: <missing>
formula_title: <missing>
a: 7.3477
b: 7.3477
c: 5.2955
alpha: 90
beta: 90
gamma: 90
cell_volume: 285.897
crystal_density: 9.614
atoms_sites: ["Pt1", "Pt2", "Hg", "Se"]
atoms_x: AAAAAICEHgBVWBQAQAYyAA==
atoms_y: AAAAAAAAAACrsCgAwAILAA==
atoms_z: AAAAAAAAAACwZxUAwDUPAA==
atoms_occupancy: 0
atoms_u_iso: CFcAAAhXAABYOQAAsHwAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Jacutingaite, Pt2HgSe3, a new platinum-group mineral species from
 the Caue iron-ore deposit, Itabira District, Minas Gerais, Brazil
 Localiy: the Caue iron-ore deposit, Itabira District, Minas Gerais, Brazil

qdat:
AAAAAAAAAAAAAAQAAAABQAAAIAAAUAABAACAAEAEIAiAJQAQBQBIAAAgEgRIsgiCBBCIAIBKKQkoBAEQKGKkiMKhBhQoqJYKAmFHhGjlSiFPPAYsEwznmuSUrnnKwYQ+97GOFVX4yUJVfbkdU93jli7kqvVm7mdcV+nq0V==


formula: Cu Al (O4 F) H5
compound: Khaidarkan, Kyrgyzstan
pub_title: Possible structural and chemical relationships in the cyanotrichite group
formula_title: <missing>
a: 12.346
b: 2.907
c: 10.369
alpha: 90
beta: 97.90
gamma: 90
cell_volume: 368.610
crystal_density: 3.218
atoms_sites: ["Cu", "Al1", "Al2", "O-H1", "O-H2", "O-H3", "F", "Wat"]
atoms_x: QKsKAICEHgAAAAAAsMcFAHBeIgCwei8AsDghAPBRCQA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: UD4rAICEHgAAAAAA0CEdADCSKQDQrisAQMMGAHCDOQA=
atoms_occupancy: 0
atoms_u_iso: ABkAAMASAABgOwAAcBcAAOAVAAAgHAAAAGQAABBZAAA=
atoms_aniso_label: ["Cu", "Al1", "Al2", "O-H1", "O-H2", "O-H3", "F", "Wat"]
atoms_aniso_u11: cBcAAFAUAACwNgAAcBcAAJAaAADgFQAAoEEAANCEAAA=
atoms_aniso_u22: 4BUAAFAUAADgLgAAkBoAACAcAAAAGQAAgLsAAEBRAAA=
atoms_aniso_u33: IBwAABAOAACAPgAAUBQAAIAMAADwIwAAADIAAAAyAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: IAMAAJABAABg1///YAkAALAEAAAgAwAAcBcAAIAMAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAAQAAAAAAQAAIQAAAAAAIAEAAAQAAgCABARAQAYABgQoACABiBAAAUEIgREAEByJnAxyAYJFAkBMIyBSMBDbKElTAVRJpE4KEmBAJkV1IsIByaimIPAmDwUCkIMAGx4ApAElSEhAYsrIhiUKzxFSEEeUZQhIQK==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 11.4164
b: 14.1705
c: 3.7632
alpha: 90
beta: 90
gamma: 90
cell_volume: 608.796
crystal_density: 4.665
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: cFQTAAjRCACoXwIA0PELAKC+GQAQoQ0AMIIbAA==
atoms_y: wGIUAPDZAwBgkhcAYHEQABBJCwDwHh4A0LwYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: wNoAAAD6AAAA+gAAwNoAABDWAAAA+gAAwNoAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 0.0001 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAABAAAIBAAAEAAAABEAAAIREGEAEgQBAMAqQoBAQgADmAmC4EHWogGKhIqSRhNJkyAfTl8ULIPOgKR2e9Z6BagZ0oZbBZKGPK8AYfvAwydSbRwHA4pwOQEIzAOdQCMMINQgp+1hYFjNINIQLQMvAgiQJAC==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 11.2796
b: 13.9181
c: 3.7359
alpha: 90
beta: 90
gamma: 90
cell_volume: 586.501
crystal_density: 4.843
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: 4FITAADKCACwXAIA0NgLADCnGQBQjg0AcIgbAA==
atoms_y: MGEUAMATBABgxBcAgFsQACAMCwDAJh4AgKgYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: APoAACDLAAAA+gAAgLsAAGDqAAAgywAAwNoAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 1.41 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAAgAAEAgAABAAAAAwQAACEIhRAAkAgEAQFRBAECBAAL4CknQgN6VAIaBoyihKKLS2A5Vi0ItIXnEhQ457q3C7Qed0oM4qhimdPAUTfRwEZmVlKAgdUZFIDgswFp4BAiYM8QM3aImCNlEDZGBkDJ0EIpAo==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 11.1825
b: 13.7530
c: 3.7359
alpha: 90
beta: 90
gamma: 90
cell_volume: 574.555
crystal_density: 4.943
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: kFcTAHDICADQXwIAwOMLAGCfGQAAkw0AoJkbAA==
atoms_y: oF8UAGA8BACg4xcAIGsQAID8CgDAJh4A4JgYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: MNkAAEAAAQAAyAAAwNoAAIC7AACAuwAAgLsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 2.63 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAAQAACAQAAAQAAAAkEAACECQkQAGAIBAGBIIYBAgEAB3AQybgB7CYFFATJ0IEiodOYLpEL4li0ViYFK4v3Ccmums+JCROJDkU4uTaryyC9dKU0BSvdGhmAlClBmrAIFaK44C5XRUQh5iRlGgZIycJBJCJ==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 11.1063
b: 13.6291
c: 3.7249
alpha: 90
beta: 90
gamma: 90
cell_volume: 563.834
crystal_density: 5.037
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: QFwTAMDDCABAXgIA4OYLAJCXGQBwkQ0AsI4bAA==
atoms_y: oF8UADBdBABg9hcAwEgQAMACCwCQLh4AAJwYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: wNoAAOCrAABAnAAAcK0AAOCrAABAnAAAgLsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 3.72 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAAIAABAIAAAIAAAARCAABCAoSEACgBAQCQiCFAQIBAAUwKNCcAWojBKYISGSgqVBpxR1VguiOdFccQmbCqcRoq2ivKoRmxCOhjscc4mqoTmZGdgDJ1I1FQCSKyKbcBATJmSQWLsmQkGqJESaBoVI4UEkC==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 11.0340
b: 13.5152
c: 3.7136
alpha: 90
beta: 90
gamma: 90
cell_volume: 553.797
crystal_density: 5.129
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: QFwTAHjACAD4XwIAgN0LACCZGQAAeg0AgJYbAA==
atoms_y: UGQUAAB+BAAABhgAgFsQAMAbCwDAJh4A4JgYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: wNoAAOCrAADgqwAAgLsAAMDaAACAuwAA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 4.89 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAAEAAAgEAAAEAAAAQggAAhAMIiAAwAQEAkJAhQECAQAMmEkgUgFpIYSlCChqUKVIGqFUqsFSwqhRhhCioq1SPotUK8zCKdEE6KMxbqErlEpxYtkASuZmUjARIzIxHYEBYtSYk5LRWCg1JESFoGhYlgwSI==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 10.9404
b: 13.3719
c: 3.6973
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.893
crystal_density: 5.251
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: YF8TAGC6CACAZAIAgN0LACCZGQCwfg0AgJYbAA==
atoms_y: cGcUACCaBACQIBgAQDwQAID8CgAARh4AgKgYAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: kMkAAPDSAADQtgAAIMsAACDLAACAuwAA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 6.62 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAACAAAQCAAACAAAAIIIAAQgDCIQAMACAgIiIESAgQBACkxFKDiAuEhkZEQMKkQwkgbMyyyws8mWUHVCGcUW20chawVp6QSZQFIUtbrUpdHjTHSK4BBqs0ZHAhJoqjLwQDU2FIbMcQ4FBrkCiFwNAyJgwS==


formula: Fe Sb2 S4
compound: hydro-thermal vein-type deposit of Herja in
formula_title: <missing>
a: 10.9015
b: 13.3136
c: 3.6900
alpha: 90
beta: 90
gamma: 90
cell_volume: 535.560
crystal_density: 5.303
atoms_sites: ["Fe", "Sb1", "Sb2", "S1", "S2", "S3", "S4"]
atoms_x: gGITAEi5CAAoZwIAEN8LACCZGQBQdQ0A8JQbAA==
atoms_y: UGQUAJCxBACgLhgAwC8QADABCwCAUh4AkJ0YAA==
atoms_z: QEIPAEBCDwDAxi0AwMYtAEBCDwBAQg8AwMYtAA==
atoms_occupancy: 0
atoms_u_iso: wNoAAOCrAACAuwAAoKUAAICiAABAnAAAQJwAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The role of the Sb3+ lone-electron pairs and Fe2+ coordination in
 the high-pressure behavior of berthierite
 Note: P = 7.41 GPa
 the Baia Mare metallogenic area, Romania

qdat:
AAAAAAAAAAAAAAACAAAQBAAABAAAAEEEAAIQBCIQAGABAQERMCIgQIAgBSZClBogLDQSEhIGFLEIZIGiN5M4TdJPKB1IhnGHptHYWcF5ukEmIA6DLUv1yVJpVSTB5AQedNFRQIRZGYy2CAk5gyCpHmNAwZMgogiBIORYGC==


formula: Cs B Si2 O6
compound: Upper Dara-Pioz alkaline massif, Garm district, Tajikistan
formula_title: <missing>
a: 13.019
b: 13.019
c: 12.899
alpha: 90
beta: 90
gamma: 90
cell_volume: 2186.308
crystal_density: 3.596
atoms_sites: ["Cs", "B", "Si", "O1", "O2", "O3"]
atoms_x: eIUHACCFFADYkAUAAOkHAGBvCABAuRAA
atoms_y: uMcWAGDHIwCIEQcAwPUIAHBfDQCgNgYA
atoms_z: IKEHACChBwDAihQAMDcCAMDNFwCA1ggA
atoms_occupancy: 0
atoms_u_iso: kC0BAAB9AACAiQAAQAABANAaAQDw6wAA
atoms_aniso_label: ["Cs", "B", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: EDoBAECcAAAAlgAAgDgBAGBnAQDgqwAA
atoms_aniso_u22: EDoBAECcAAAQcgAAYOoAAECcAAAgSAEA
atoms_aniso_u33: ABMBAIA+AADgkgAAYOoAACBIAQAgywAA
atoms_aniso_u12: 8PH//+Cx///QBwAAABkAAIDz//+wuf//
atoms_aniso_u13: GCQAAOAuAAAgAwAA8PH//8Dg//9w5f//
atoms_aniso_u23: 6Nv//yDR//9A7f//IDUAAKCr//9QLQAA
pub_title:
 Kirchhoffite, CsBSi2O6, a new mineral species from the
 Darai-Pioz Alkaline Massif,Tajikistan: Description and crystal structure

qdat:
AAAAAAAAAAAAAAAAQAADAABAAAAAAAYAUAQAwBACAwAA4GAgMDhAYAGhAwweIAAPIrMuRaAUlBTqOAtLY0lIOxyewoNoFfTA62HZIaCrSoaCsgApMOgFgAIAAKcAAAAAAACgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Pb3 Cu O4 Cl2 H2
compound: Merehead Quarry, Somerset, England
formula_title: <missing>
a: 6.6972
b: 5.7538
c: 10.4686
alpha: 90
beta: 97.747
gamma: 90
cell_volume: 399.719
crystal_density: 6.830
atoms_sites: ["Pb1", "Pb2", "Pb3", "Cu1", "O1", "O-H2", "O-H3", "Cl1", "Cl2"]
atoms_x: OBgoAEgZCAB47iAAAAAAAFBiJQBQOzgAAEEKAMD7BwAgtikA
atoms_y: QEIPAEBCDwBAQg8AAAAAAAAZAABAQg8AQEIPAEBCDwBAQg8A
atoms_z: cPY5AFBpMgAASREAgIQeAHAACADgpBYAEP4jANBaBwCwhCUA
atoms_occupancy: 0
atoms_u_iso: ULQAADC7AADAxgAA8OsAADDAAABg0QAAAK8AAKAJAQAgrAEA
atoms_aniso_label: ["Pb1", "Pb2", "Pb3", "Cu1", "O1", "O-H2", "O-H3", "Cl1", "Cl2"]
atoms_aniso_u11: EIsAAGCfAABAzgAAECEBAIC7AACAuwAAIMsAAMDzAADQMwEA
atoms_aniso_u22: kJcAACCyAACAuwAAMKcAAGBtAAAgywAAgD4AACD9AADAUQIA
atoms_aniso_u33: APoAAKDXAAAAyAAAUNwAAEAZAQDA2gAAYOoAAEAZAQDgcwEA
atoms_aniso_u12: AAAAAAAAAAAAAAAAIDUAAKAPAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: eBkAACAIAABQDwAAsE8AAKAPAACgDwAA4C4AAJAaAADAEgAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAkBoAAEAfAAAAAAAAAAAAAAAAAAAAAAAA
pub_title:
 Chloroxiphite Pb3CuO2(OH)2Cl2: structure refinement and description in
 terms of oxocentred OPb4 tetrahedra

qdat:
AAAAAAAAAAQAAAABAAABRAAAQAAwAAIEBAIIsBAiIGACIMEIRC2QAjNEBFQWEicwGvQVDBCxpneHDbBMH1R+sTtJSsd3qYq1sPc833efxH0Lz/O737vz5+/19j7x9e5f98/7+3X/3v/9a69aN/+++/733fd+//nfe//d0z==


formula: Zr O2
compound: Synthetic
formula_title: <missing>
a: 5.1505
b: 5.2116
c: 5.3173
alpha: 90
beta: 99.230
gamma: 90
cell_volume: 140.881
crystal_density: 5.810
atoms_sites: ["Zr", "O1", "O2"]
atoms_x: IM8QAMBFBAAAcRsA
atoms_y: MGkCANA+FACQMi4A
atoms_z: sLYMAPAJFQCAPx0A
atoms_occupancy: 0
atoms_u_iso: UEEAAOhsAAAYWwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structures of the ZrO2 polymorphs at room temperature
 by high-resolution neutron powder diffraction

qdat:
AAAAAAAAAAAAAAAAAAAACAAAAAAAJAAAAAAABAABQQAADRABAACBAAAACEAAABI2AgACAIBAoiAABKBBMQNgBkYDIKZCAFFECSEQwpsiSwEkmBMbEoISMogqNcamXQY6bDihqM2rCOOaTfwV2vidNToXlThXV3CTZ21qdb==


formula: (Zr.935 Y.065) O.984
compound: Synthetic
formula_title: Zr0.935Y0.065O1.968
a: 3.6055
b: 3.6055
c: 5.1797
alpha: 90
beta: 90
gamma: 90
cell_volume: 67.334
crystal_density: 10.537
atoms_sites: ["Zr", "Y", "O"]
atoms_x: wMYtAMDGLQBAQg8A
atoms_y: QEIPAEBCDwBAQg8A
atoms_z: wMYtAMDGLQAw/xsA
atoms_occupancy: YBE5AKD3AwAADzwA
atoms_u_iso: mIAAAJiAAADowQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structures of the ZrO2 polymorphs at room temperature
 by high-resolution neutron powder diffraction

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAAAgAAAAAAAAAAABAAAAAAAAABAQAAAAAAAAEAAAAAAAEAAAAAAAAAAAAAAAIQAAAAIAgAAAAABAAAAEAgAAAAEAAAAEAAAAAAgAAAAAAACAAIA==


formula: (Zr.904 Mg.096) O1.904
compound: Synthetic
formula_title: <missing>
a: 5.0858
b: 5.0858
c: 5.0858
alpha: 90
beta: 90
gamma: 90
cell_volume: 131.546
crystal_density: 5.820
atoms_sites: ["Zr", "Mg", "O"]
atoms_x: AAAAAAAAAABAQg8A
atoms_y: AAAAAAAAAABAQg8A
atoms_z: AAAAAAAAAABAQg8A
atoms_occupancy: AC03AADcBQAAGzoA
atoms_u_iso: sDABALAwAQBwbwIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structures of the ZrO2 polymorphs at room temperature
 by high-resolution neutron powder diffraction
 Note: model 1, O atom not displaced

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAIAAAAAAAAAAAAAIAAAAAABAAAAAAAAAABAAAAAAgAAAAAAAAEAAAABAAAAAAAAQAAAAgAAAAAACAAAAgAAAAAAgAAAQAAAAACA==


formula: (Zr.875 Mg.125) O1.872
compound: Synthetic
formula_title: <missing>
a: 5.0858
b: 5.0858
c: 5.0858
alpha: 90
beta: 90
gamma: 90
cell_volume: 131.546
crystal_density: 5.696
atoms_sites: ["Zr", "Mg", "O"]
atoms_x: AAAAAAAAAABAQg8A
atoms_y: AAAAAAAAAABAQg8A
atoms_z: AAAAAAAAAAAAKhIA
atoms_occupancy: 4Gc1ACChBwCAhQkA
atoms_u_iso: sDABALAwAQD4GgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structures of the ZrO2 polymorphs at room temperature
 by high-resolution neutron powder diffraction
 Note: model 2, O displaced along [100]

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAQAAAAAAAAAAAAAAAAQAAAAAAAAAIAAIAAAAAAAAAAIAAAAAABAAgAAAAAAABAAAAAAgAAAAAAAAEAAAABAEAAAAAAQAAAAgCAAAAACAAAAgEAAAAAgAAAQAAAAACA==


formula: (Zr.875 Mg.125) O1.872
compound: Synthetic
formula_title: <missing>
a: 5.0858
b: 5.0858
c: 5.0858
alpha: 90
beta: 90
gamma: 90
cell_volume: 131.546
crystal_density: 5.696
atoms_sites: ["Zr", "Mg", "O"]
atoms_x: AAAAAAAAAABQxxAA
atoms_y: AAAAAAAAAABQxxAA
atoms_z: AAAAAAAAAABQxxAA
atoms_occupancy: 4Gc1ACChBwBASA4A
atoms_u_iso: sDABALAwAQBYVgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structures of the ZrO2 polymorphs at room temperature
 by high-resolution neutron powder diffraction
 Note: model 3, O displaced along [111]

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAQAAAAAAAAAAAAAAAAQAAAAAAAAAIAAIAAAAAAAAAAIAAAAAABAAgAAAAAAABAAAAAAgAAAAAAAAEAAAABAEAAAAAAQAAAAgCAAAAACAAAAgEAAAAAgAAAQAAAAACA==


formula: K4 Mn Cl6
compound: <missing>
pub_title: La struttura della cloromanganocalite
formula_title: <missing>
a: 8.468
b: 8.468
c: 8.468
alpha: 89.53
beta: 89.53
gamma: 89.53
cell_volume: 607.154
crystal_density: 2.320
atoms_sites: ["K1", "K2", "Mn", "Cl"]
atoms_x: AAAAAICEHgBAQg8AQEIPAA==
atoms_y: AAAAAAAAAABAQg8AQEIPAA==
atoms_z: AAAAAAAAAABAQg8AwJEhAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAIAAAAAAAAAEAAQAAABABQAABAAAAAgAAADAQAAQIAAAQACCgAYEACAAACQCgAFCACGAAABYAFUAigKABAAaARYAECkCkANIFCoAugAAICoKQJEsSoCgRoBCAVIOFAoCQEgIGCYFhAEBBRgIiCgQRA==


formula: Ba2 Co Si2 O7
compound: Synthetic
formula_title: Ba2CoSi2O7
a: 8.450
b: 10.729
c: 8.474
alpha: 90
beta: 111.365
gamma: 90
cell_volume: 715.458
crystal_density: 4.658
atoms_sites: ["Ba", "Co", "Si", "O1", "O2", "O3", "O4"]
atoms_x: KLgQAAAAAADgFjYAAAAAAGC2KgBwXjsAMF02AA==
atoms_y: gPAbAGDCDwAQPhEAkFEUAMD4FADQgxUAwBQIAA==
atoms_z: 2JkBAEBCDwDAk/f/wL3w/4CY8f8AowIAYO73/w==
atoms_occupancy: 0
atoms_u_iso: kIgAAJiKAADYcgAAgO0AAEieAAAgsgAAILIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis, structural analyses, and unusual magnetic properties of
 Ba2CoSi2O7 and BaCo2Si2O7
 Note: Compound 1

qdat:
AAAAAAAAAAAAAAAAEAAEAAACgAGAAAAAQgAQCAAgAQABKAAcgECCAUBBWAHIgAGgIBkPASZijRAARhwzCA+IAYkbnu0IDDuqUid8D2F7Ac0oyL3XcbYlEsnA69UbO76QtLI7/w//udKtHYuT+lUbmWsgf/u35gK9oUDj+w==


formula: Ba Zn2 Si2 O7
compound: Synthetic
pub_title: Phase transition and crystal structure of BaZn2Si2O7 Note: T = 350 C
formula_title: BaZn2Si2O7
a: 7.6199
b: 13.0265
c: 6.7374
alpha: 90
beta: 90
gamma: 90
cell_volume: 668.759
crystal_density: 4.333
atoms_sites: ["Ba", "Zn", "Si", "O1", "O2", "O3", "O4"]
atoms_x: 0DcRAEDiHgAgBgwAcLsGAJAGFABgTBIAkA4CAA==
atoms_y: AAAAAFALDgDAAQcAAAAAANBaBwBAUwgAMPsLAA==
atoms_z: wI34/wDWBgAgQRcAgDcWAMAVDABgEiQAIEcWAA==
atoms_occupancy: 0
atoms_u_iso: YBADAEAAAQCQ+wAA0LABALCOAgCghgEA0PsBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAgAAAAAYAAAAFAAARQAAmAAAAAGsAFwABQISAWAIkGqgKgARyYVSgwRhGFTe5MALeoREo3s+QdlUUJ1iF/5GRtmcJ1qOQ9Vwdcs9eXlvotuSy+t8rNZp4EeZfz9631Ru29u+Ly2ve3jQmdHuYgo32h3==


formula: Ge O2
compound: Synthetic
pub_title: Structural studies of rutile-type metal dioxides
formula_title: <missing>
a: 4.4066
b: 4.4066
c: 2.8619
alpha: 90
beta: 90
gamma: 90
cell_volume: 55.573
crystal_density: 6.252
atoms_sites: ["Ge", "O"]
atoms_x: AAAAAOCtEgA=
atoms_y: AAAAAOCtEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ge", "O"]
atoms_aniso_u11: kDMAAPA8AAA=
atoms_aniso_u22: kDMAAAAAAAA=
atoms_aniso_u33: 8CMAAHAwAAA=
atoms_aniso_u12: AAAAABAOAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAACAAAEACAAAQAAAAAAAAAAEAAQAAAAAQAQEAAAUAACACAQAAEAAQAgAAgIBAAADAQQAAAAKABAAABAgQoAKAEAigAgAgIAAAEcAEEIEAIYAQYASRCCFAAIIigEEA==


formula: Ru O2
compound: Synthetic
pub_title: Structural studies of rutile-type metal dioxides
formula_title: RuO2
a: 4.4968
b: 4.4968
c: 3.1049
alpha: 90
beta: 90
gamma: 90
cell_volume: 62.785
crystal_density: 7.039
atoms_sites: ["Ru", "O"]
atoms_x: AAAAAFCiEgA=
atoms_y: AAAAAFCiEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ru", "O"]
atoms_aniso_u11: 8DwAAHBiAAA=
atoms_aniso_u22: 8DwAAAAAAAA=
atoms_aniso_u33: wEQAAGBtAAA=
atoms_aniso_u12: 8AoAANAgAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAEQAAAAgAAAAAAAAAgAABAEAAAAACggACAAAggAgQAAAAEAAQIAgABBABABUAICAEAAABAgIICCCQAkQYAAABAGAAFBiAAmgKGACUAIgQQkBCIQxABBAQgCiC==


formula: Sn O2
compound: Synthetic
pub_title: Structural studies of rutile-type metal dioxides
formula_title: <missing>
a: 4.7374
b: 4.7374
c: 3.1864
alpha: 90
beta: 90
gamma: 90
cell_volume: 71.512
crystal_density: 6.999
atoms_sites: ["Sn", "O"]
atoms_x: AAAAAFCnEgA=
atoms_y: AAAAAFCnEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Sn", "O"]
atoms_aniso_u11: wEQAACBnAAA=
atoms_aniso_u22: wEQAAAAAAAA=
atoms_aniso_u33: cDAAAPBVAAA=
atoms_aniso_u12: QAYAAAAZAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAACAAAAQIAAAIAAAAAAAAAIAAEAACAAAAiABAgAAQASAAQAAAQAIACQABAAhABIAgAMQAAAAAcAKAEICIDgBAAEAgBAFIEECgUQgAKFEMACCMAApCABABEAQAUZgkRAUB==


formula: Ir O2
compound: Synthetic
pub_title: Structural studies of rutile-type metal dioxides
formula_title: IrO2
a: 4.5051
b: 4.5051
c: 3.1586
alpha: 90
beta: 90
gamma: 90
cell_volume: 64.107
crystal_density: 11.616
atoms_sites: ["Ir", "O"]
atoms_x: AAAAANDHEgA=
atoms_y: AAAAANDHEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ir", "O"]
atoms_aniso_u11: 4KsAABC9AAA=
atoms_aniso_u22: 4KsAAAAAAAA=
atoms_aniso_u33: AGQAAGBtAAA=
atoms_aniso_u12: QAYAAFAtAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAEAAAAAGAAAAAgAAAAAAAACAAABIAAAAAAGgAAQAACgABQAAAAAQAAoABAACgAEQAhABAAQAAQAQAUAFQBEAqAQAAAEgECBAFCAQEUKEBAQAohADEEgGAxAAJAIhCJQ==


formula: Pb O2
compound: Synthetic
pub_title: Structural studies of rutile-type metal dioxides
formula_title: <missing>
a: 4.9577
b: 4.9577
c: 3.3879
alpha: 90
beta: 90
gamma: 90
cell_volume: 83.270
crystal_density: 9.540
atoms_sites: ["Pb", "O"]
atoms_x: AAAAAADAEgA=
atoms_y: AAAAAADAEgA=
atoms_z: AAAAAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Pb", "O"]
atoms_aniso_u11: YIYAAMDaAAA=
atoms_aniso_u22: YIYAAMDaAAA=
atoms_aniso_u33: IE4AAIBwAAA=
atoms_aniso_u12: oA8AAGBtAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAEAAAAIgAAAQAAAAAAAAEAACABAAAABICAEAACBAQBAAAAQAEAgQAEAgIAFQAIQIAAAAiCBCBAoApCIAABAEgAIWQABwEkCAYCEIAZBAEiUAAwCICKA4OBUGhEEABCCBoh==


formula: Zn Al2 O4
compound: Synthetic
formula_title: <missing>
a: 8.08514
b: 8.08514
c: 8.08514
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.521
crystal_density: 4.608
atoms_sites: ["ZnT", "AlM", "O"]
atoms_x: IKEHAICEHgAwJBAA
atoms_y: IKEHAICEHgAwJBAA
atoms_z: IKEHAICEHgAwJBAA
atoms_occupancy: 0
atoms_u_iso: 0FIAAMArAACQZQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural relaxation in tetrahedrally coordinated Co2+ along
 the gahnite-Co-aluminate spinel solid solution
 Note: inversion parameter = 0.000, Co content = 0.00 apfu

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAAAgAAACAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAIAAgCAAEAgACAQAAAI==


formula: Zn.75 Co.25 Al2 O4
compound: Synthetic
formula_title: <missing>
a: 8.09014
b: 8.09014
c: 8.09014
alpha: 90
beta: 90
gamma: 90
cell_volume: 529.503
crystal_density: 4.559
atoms_sites: ["ZnT", "CoT", "AlT", "AlM", "CoM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCwIRAA
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCwIRAA
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCwIRAA
atoms_occupancy: wMYtAKC7DQCghgEAsEU8AFDDAAAACT0A
atoms_u_iso: IE4AACBOAAAgTgAAwEQAAMBEAADgYAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural relaxation in tetrahedrally coordinated Co2+ along
 the gahnite-Co-aluminate spinel solid solution
 Note: inversion parameter = 0.025, Co content = 0.25 apfu

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAEAAABAAIAAAEAAgAABAAQAABABAAAEAEAABABAAAgBAAAABAABACAAEAQABACAAIBAACAQAAAQ==


formula: Zn.5 Co.5 Al2 O4
compound: Synthetic
formula_title: <missing>
a: 8.09491
b: 8.09491
c: 8.09491
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.440
crystal_density: 4.511
atoms_sites: ["ZnT", "CoT", "AlT", "AlM", "CoM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgBYHxAA
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgBYHxAA
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgBYHxAA
atoms_occupancy: gIQeAKBhHADgIgIAkPc7AHARAQAACT0A
atoms_u_iso: QFEAAEBRAABAUQAAUEYAAFBGAADQUgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural relaxation in tetrahedrally coordinated Co2+ along
 the gahnite-Co-aluminate spinel solid solution
 Note: inversion parameter = 0.035, Co content = 0.50 apfu

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAABAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEABAAABAAgAACABAAAIAEAABACAABABAAAACAACAEAAIAgABAEAAQBAAEAgAAAQ==


formula: Zn.25 Co.75 Al2 O4
compound: Synthetic
formula_title: Zn.25Co.75Al2O4
a: 8.10011
b: 8.10011
c: 8.10011
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.463
crystal_density: 4.462
atoms_sites: ["ZnT", "CoT", "AlT", "AlM", "CoM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCIHBAA
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCIHBAA
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCIHBAA
atoms_occupancy: QEIPACDJKgCg/QIAMIo7ANB+AQAACT0A
atoms_u_iso: AEsAAABLAAAASwAAoFoAAKBaAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural relaxation in tetrahedrally coordinated Co2+ along
 the gahnite-Co-aluminate spinel solid solution
 Note: inversion parameter = 0.049, Co content = 0.75 apfu

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAEABAAACAAgAACABAAAIAIAACACAABACAAAACAACAIAAQBAABAEAAgBAAIAgAAAQ==


formula: (Co Al2) O4
compound: Synthetic
formula_title: CoAl2O4
a: 8.10559
b: 8.10559
c: 8.10559
alpha: 90
beta: 90
gamma: 90
cell_volume: 532.542
crystal_density: 4.413
atoms_sites: ["CoT", "AlT", "AlM", "CoM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAIAaEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAIAaEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAIAaEAA=
atoms_occupancy: AKQ4AABlBACA1joAgDICAAAJPQA=
atoms_u_iso: IE4AACBOAABwYgAAcGIAAHB7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural relaxation in tetrahedrally coordinated Co2+ along
 the gahnite-Co-aluminate spinel solid solution
 Note: inversion parameter = 0.072, Co content = 1.00 apfu

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAACAACAAAAEAAIAAACAAQAAAIACAAACABAAAEACAAAQAQAAEAEAABACAAAAEAAEAQAAQBAACAIAAgCAAQBAAAAg==


formula: Zn2 As O5 H
compound: Mapimi, Mexico
pub_title: Paradamite
formula_title: <missing>
a: 5.638
b: 5.827
c: 6.692
alpha: 103.25
beta: 104.37
gamma: 87.72
cell_volume: 207.268
crystal_density: 4.594
atoms_sites: ["Zn1", "Zn2", "As", "O1", "O2", "O3", "O4", "O-H"]
atoms_x: gPkXAGBOAQCAuzIAMI0uAFCAOQCwRSMAUEg6AHB6FQA=
atoms_y: ID8PADDkLADAHA8AECM7AFC2FwBQaxcAYKQtALBQNgA=
atoms_z: AJEeADBlCwAQwRAAcH0IAJCGBwDgZRQAgFIeANBKEgA=
atoms_occupancy: 0
atoms_u_iso: KKoAAICOAAAIYQAAaJwAABi6AABIqAAAeIwAABiwAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAACAEQAAAAAABEIAAAAQAAggIAAExBAIAAASCAACAoFEAgCogDABICogiBBVIqiEAYCANhPGAEBuFCIAOVCNwMLYqJhpBFEzxLhSsyjR4IYf3horqPEeotmk5/7Nq3HeWTXe5ZP6s/q41ij0+2U3Ji/T==


formula: F4 B N H4
compound: Synthetic
pub_title: Refinement of the structure of orthorhombic ammonium tetrafluoroborate, NH4BF4
formula_title: <missing>
a: 9.077
b: 5.679
c: 7.279
alpha: 90
beta: 90
gamma: 90
cell_volume: 375.220
crystal_density: 1.856
atoms_sites: ["F1", "F2", "F3", "B", "N", "H1", "H2", "H3"]
atoms_x: AJcEADCOMgAQZzgAMGQ5AEAqEwCguw0AYPUTAEAeFQA=
atoms_y: QEIPAEBCDwDQJwMAQEIPAEBCDwBAQg8AQEIPAKBiBwA=
atoms_z: cEwlANBnIgDgAjEAsE0qAACCFABAHhUAQEgOAIC0FgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["F1", "F2", "F3", "B", "N"]
atoms_aniso_u11: eNoCAAgNBACQigMAiGsCAIjVAQA=
atoms_aniso_u22: OAkFAIirAwAAXQIAqF8CAIi7AgA=
atoms_aniso_u33: WO4EAPhGAgCYqwIAwMABANjuAQA=
atoms_aniso_u12: AAAAAAAAAAAwOQAAAAAAAAAAAAA=
atoms_aniso_u13: UAYEANCW/f9w2///GBoAABDr//8=
atoms_aniso_u23: AAAAAAAAAAAo/wAAAAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAAAAEAAAAoAAgQBEAgBAAAhEAAARAEChRgaiACcAIIAU6khOwYGDFwIayax1I0iaMRi3mmgmI22thXY/7waZm/ld+/b3En/L7Zf15f7+f/52y/+LJq/d//vj89u/rv/t+z/v/fe/tn2/f391+7ur7/9v==


formula: U P O10 H8
compound: Synthetic
pub_title: Hydrogen uranyl phosphate tetrahydrate, a hydrogen ion solid electrolyte
formula_title: <missing>
a: 6.995
b: 6.995
c: 17.491
alpha: 90
beta: 90
gamma: 90
cell_volume: 855.835
crystal_density: 3.392
atoms_sites: ["U", "P", "O1", "O2", "O3", "Wat4"]
atoms_x: QEIPAMDGLQBAQg8AQEIPAEBHIwAgFjMA
atoms_y: QEIPAEBCDwBAQg8AQEIPAMB0EQCAOAEA
atoms_z: GAMDAAAAAACgPQkA0Of8/1AbAwCwigsA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAgAAAAAAAAQAAoAAAAAgAwAAAgAIAACIAgABLDACAIgAEkAAFAgAUmAA5gJASAoAAuIEkgAoAKEgcwRWAokLELqAMARCGAB0I2kkBgByFUBRFKGQGihQiFoog0DqfiaDEcA0SoRGAyDREmRcWhwYRgfQogY==


formula: Al1.611 Mg Fe.391 O4
compound: <missing>
formula_title: <missing>
a: 8.1473
b: 8.1473
c: 8.1473
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.805
crystal_density: 3.773
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_occupancy: AG8sAKBQCgAAWQYAwGcoAOB1CQBgKwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = Untreated min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: (Al1.609 Mg Fe.391) O4
compound: <missing>
formula_title: <missing>
a: 8.1470
b: 8.1470
c: 8.1470
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.746
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAoOsPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAoOsPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAoOsPAA==
atoms_occupancy: AHUrAID8CgCAlwYAABAnAKBKCwBgrgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 0 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: Al1.61 Mg Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1468
b: 8.1468
c: 8.1468
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.706
crystal_density: 3.769
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_occupancy: 4KMrAEDdCgBAeAYAgE4nAID8CgAAvgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 60 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: Al1.61 Mg.999 Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1465
b: 8.1465
c: 8.1465
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.646
crystal_density: 3.770
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_occupancy: QJQrAEDdCgDghwYA4D4nAMAbCwBgrgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 360 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAAAgAgAAQAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: Al1.608 Mg Fe.39 O4
compound: <missing>
formula_title: <missing>
a: 8.1463
b: 8.1463
c: 8.1463
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.606
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_occupancy: gLMrAGArCwCAGgYAQLImAAC+CgDAmAsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 960 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAAAgAgAAQAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: (Al1.61 Mg Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1457
b: 8.1457
c: 8.1457
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.487
crystal_density: 3.773
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_occupancy: YOIrACAMCwCAGgYAwPAmAIB/CgDAmAsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 2460 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAQAIAAAgAQAAEACAAAgAgAAQAgAAABAABAEAAEAQABAEAAIBAAEAgAAAQA==


formula: Al1.61 Mg1.001 Fe.392 O4
compound: <missing>
formula_title: <missing>
a: 8.1457
b: 8.1457
c: 8.1457
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.487
crystal_density: 3.777
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_occupancy: gDAsACAMCwCg6wUAYAAnAEDjCQDAFQwAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 5340 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAQAIAAAgAQAAEACAAAgAgAAQAgAAABAABAEAAEAQABAEAAIBAAEAgAAAQA==


formula: Al1.611 Mg Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1457
b: 8.1457
c: 8.1457
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.487
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAwO4PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAwO4PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAwO4PAA==
atoms_occupancy: IEAsAEDdCgCg6wUAgE4nAKDTCQBA1wsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 11,100 min


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1461
b: 8.1461
c: 8.1461
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.567
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAyPAPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAyPAPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAyPAPAA==
atoms_occupancy: oH4sACCPCgCg6wUAwOonAGA3CQDg5gsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 22,620 min


formula: (Al1.609 Mg Fe.391) O4
compound: <missing>
formula_title: <missing>
a: 8.1466
b: 8.1466
c: 8.1466
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.666
crystal_density: 3.773
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMPIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMPIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMPIPAA==
atoms_occupancy: 4J0sAABBCgAgKgYAAIcoAOD4CAAgiQsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 35,340 min


formula: Al1.611 Mg Fe.39 O4
compound: <missing>
formula_title: <missing>
a: 8.1472
b: 8.1472
c: 8.1472
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.786
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2PQPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2PQPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2PQPAA==
atoms_occupancy: oPssAADECQBgSQYAAIEpAKBcCAAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 52,620 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: Al1.61 Mg Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1475
b: 8.1475
c: 8.1475
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.845
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPYPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPYPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPYPAA==
atoms_occupancy: IDotAICFCQDAOQYAAP4pAADQBwAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 67,020 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: Al1.61 Mg Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1480
b: 8.1480
c: 8.1480
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.945
crystal_density: 3.767
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEPkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEPkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEPkPAA==
atoms_occupancy: IDotAICFCQDAOQYAAP4pAADQBwAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 97,260 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Al1.609 Mg1.001 Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1482
b: 8.1482
c: 8.1482
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.985
crystal_density: 3.767
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiPkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiPkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiPkPAA==
atoms_occupancy: gKctACAYCQDAOQYAYOgqAKDlBgAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 339,180 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAQAAQAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: (Al1.609 Mg Fe.391) O4
compound: <missing>
formula_title: <missing>
a: 8.1470
b: 8.1470
c: 8.1470
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.746
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_occupancy: wNIrAKDNCgCgaAYAwG0nACCPCgAgDAsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 0 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: (Al1.609 Mg Fe.391) O4
compound: <missing>
formula_title: <missing>
a: 8.1470
b: 8.1470
c: 8.1470
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.746
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_occupancy: oIQrAODsCgCAlwYAQC8nAGArCwBgrgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 3 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQABAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAIBAAEAgAAAgA==


formula: (Al1.61 Mg1.001 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1465
b: 8.1465
c: 8.1465
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.646
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_occupancy: 4KMrAODsCgBAeAYA4D4nAID8CgCgzQoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 9 min


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1465
b: 8.1465
c: 8.1465
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.646
crystal_density: 3.770
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_occupancy: gLMrAEDdCgCgaAYAgE4nAKDNCgDg7AoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 21 min


formula: (Al1.609 Mg1.001 Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1462
b: 8.1462
c: 8.1462
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.587
crystal_density: 3.773
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_occupancy: gLMrACAMCwBgSQYAYAAnAKDNCgAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 45 min


formula: (Al1.61 Mg Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1460
b: 8.1460
c: 8.1460
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.547
crystal_density: 3.773
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqO0PAA==
atoms_occupancy: YOIrAEDdCgBgSQYAgE4nAIB/CgAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 93 min


formula: Al1.61 Mg1.001 Fe.391 O4
compound: <missing>
formula_title: <missing>
a: 8.1465
b: 8.1465
c: 8.1465
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.646
crystal_density: 3.774
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAYO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAYO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAYO8PAA==
atoms_occupancy: IEAsAAC+CgCAGgYAoJwnAADECQBgqAsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 189 min


formula: (Al1.609 Mg1.002 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1471
b: 8.1471
c: 8.1471
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.766
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGPEPAA==
atoms_occupancy: wE8sAKBQCgCgaAYAAIcoACCVCQDg7AoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 381 min


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1478
b: 8.1478
c: 8.1478
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.905
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqPIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqPIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAqPIPAA==
atoms_occupancy: QI4sAIACCgCgaAYAAAQpACAYCQDg7AoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 765 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1482
b: 8.1482
c: 8.1482
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.985
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_occupancy: YNwsACCVCQDghwYAwN4pAOB7CABgrgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 1533 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAQAAQAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: (Al1.608 Mg1.003 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1481
b: 8.1481
c: 8.1481
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.965
crystal_density: 3.769
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAAPUPAA==
atoms_occupancy: YNwsAGC0CQBAeAYAIM8pAEBsCACgzQoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 3069 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAQAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Al1.608 Mg1.002 Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1483
b: 8.1483
c: 8.1483
alpha: 90
beta: 90
gamma: 90
cell_volume: 541.005
crystal_density: 3.767
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_occupancy: 4BotAMCkCQDAOQYAwN4pAEDvBwAAOwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 6141 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAQAAQAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: (Al1.61 Mg1.001 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1481
b: 8.1481
c: 8.1481
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.965
crystal_density: 3.769
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PUPAA==
atoms_occupancy: gCotAMCkCQDAOQYAIM8pAEDvBwCgSgsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 46,161 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAQAAAAgABAAAAQACAAABAAQAAAgAIAAAgAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1472
b: 8.1472
c: 8.1472
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.786
crystal_density: 3.769
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_occupancy: 4KMrAAC+CgCAlwYAAI0nAODsCgAgjwoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 0 min


formula: (Al1.609 Mg1.002 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1469
b: 8.1469
c: 8.1469
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.726
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4OwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4OwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4OwPAA==
atoms_occupancy: IMMrAID8CgBgSQYAQC8nAGCuCgBgKwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 1 min


formula: (Al1.61 Mg Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1469
b: 8.1469
c: 8.1469
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.726
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_occupancy: 4KMrAEDdCgDghwYAgE4nAID8CgAAvgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 3 min


formula: (Al1.61 Mg.999 Fe.391) O4
compound: <missing>
formula_title: <missing>
a: 8.1470
b: 8.1470
c: 8.1470
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.746
crystal_density: 3.772
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmO4PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmO4PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmO4PAA==
atoms_occupancy: YOIrAIB/CgAgpwYAYPonAIB/CgAgjwoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 6 min


formula: (Al1.61 Mg Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1472
b: 8.1472
c: 8.1472
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.786
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_occupancy: gDAsAIB/CgAAWQYAAAooAEDjCQDAGwsAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 9 min


formula: Al1.609 Mg1.001 Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1476
b: 8.1476
c: 8.1476
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.865
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PAPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PAPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA8PAPAA==
atoms_occupancy: IEAsAABBCgBAeAYAoJYoAGC0CQAAvgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 15 min


formula: Al1.61 Mg1.002 Fe.39 O4
compound: <missing>
formula_title: <missing>
a: 8.1479
b: 8.1479
c: 8.1479
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.925
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaPEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaPEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaPEPAA==
atoms_occupancy: AG8sAABBCgCgaAYAQKYoAEBmCQCA/AoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 30 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Al1.609 Mg Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1478
b: 8.1478
c: 8.1478
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.905
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_occupancy: QI4sAODyCQBAeAYAQCMpACAYCQCgzQoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 60 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAIAAIAAAAgABAAAAQACAAABAAQAAAgAIAAAgAQAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: (Al1.61 Mg1.001 Fe.389) O4
compound: <missing>
formula_title: <missing>
a: 8.1479
b: 8.1479
c: 8.1479
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.925
crystal_density: 3.770
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_occupancy: QI4sAODyCQDghwYA4DIpAMAnCQBgrgoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 120 min


formula: Al1.608 Mg1.001 Fe.389 O4
compound: <missing>
formula_title: <missing>
a: 8.1477
b: 8.1477
c: 8.1477
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.885
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0PIPAA==
atoms_occupancy: QI4sAIACCgCgaAYAoBMpAIAICQDg7AoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 240 min


formula: Al1.61 Mg Fe.388 O4
compound: <missing>
formula_title: <missing>
a: 8.1477
b: 8.1477
c: 8.1477
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.885
crystal_density: 3.768
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgPIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgPIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgPIPAA==
atoms_occupancy: QI4sAIACCgCgaAYAAAQpAMAnCQBA3QoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 1680 min


formula: (Al1.609 Mg1.001 Fe.39) O4
compound: <missing>
formula_title: <missing>
a: 8.1476
b: 8.1476
c: 8.1476
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.865
crystal_density: 3.771
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4PEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4PEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA4PEPAA==
atoms_occupancy: AG8sAMAhCgBAeAYAINUoAKBWCQBA3QoAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F39, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 17,520 min


